This book presents the proceedings of the 3rd edition of the International Conference on Theoretical, Applied and Experi
785 122 38MB
English Pages XII, 341 [345] Year 2020
Table of contents :
Front Matter ....Pages ixii
Front Matter ....Pages 11
HighSpeed ModeI Delamination (Tianyu Chen, Christopher M. Harvey, Simon Wang, Vadim V. Silberschmidt)....Pages 38
Characterization of Dynamic Fractures for Compressed PMMA Material (C. Huang)....Pages 913
Tensile Behavior of a Titanium Alloy Additively Manufactured via Selective Electron Beam Melting (Yinling Zhang, Shoujiang Qu, Aihan Feng, Daolun Chen)....Pages 1419
The Rule of Mixtures on the Elastic Buckling Response of Rectangular GLARE FML Plates Under Shear Stresses (Costas D. Kalfountzos, George S. E. Bikakis, Efstathios E. Theotokoglou)....Pages 2025
Evaluating Bonding Characteristics of Joggled Lap CFRP Using Acoustic Emission Techniques (Claudia Barile, Caterina Casavola, Giovanni Pappalettera, Carmine Pappalettere, Paramsamy Kannan Vimalathithan)....Pages 2631
Experimental Study of Low Concentration Diffusible Hydrogen Effect on Mechanical Behaviour of Carbon Steel (I. M. Dmytrakh, R. L. Leshchak, A. M. Syrotyuk)....Pages 3237
Effects of Temperature on Tensile and Fracture Behavior of Dissimilar Metal Welded Joint for Nuclear SafeEnd (Lei Wang, Yang Liu, Xiu Song, Jiahua Liu)....Pages 3843
A Multiattribute Information Based Method of Material Strength Distribution Fitting (Liyang Xie, Bo Qin, Ningxiang Wu)....Pages 4451
Performance of a Carburizing Bearing Steel After Surface Nanosized (Yanhui Wang, Fucheng Zhang, Zhinan Yang, Hezong Li, Qian Yang)....Pages 5257
Residual Strength and Toughness of Nano and Micro Scale Fiber Reinforced Cementitious Composites (Panagiotis A. Danoglidis, Maria S. KonstaGdoutos, Emmanuel E. Gdoutos)....Pages 5863
Experimental and Numerical Strategy for the Determination of Mechanical Properties Related to Human Cortical Bone Fracture (J.L. Tailhan, Y. GodioRaboutet, C. Boulay)....Pages 6469
Effect of External Field Treatment on the Microstructure and Deformation Behavior of NickelBase Superalloy (Yang Liu, Lei Wang, Xiu Song, Yao Wang)....Pages 7075
Dynamic Speckle Contrast Imaging for Surface Defect Detection (Rishikesh Kulkarni, Shanta Patil, Pramod Rastogi)....Pages 7681
Experimental Investigation of the Elastic Modulus of Timber by Using Density and Fiber Orientation (WeiChung Wang, TzuYu Kuo)....Pages 8285
Effect of pH on Microstructure and Properties of UltrasonicAssisted Electroless NiP Coatings (Jingjing Cao, Xiaoyu Wang, Yifan Zhao, Guofang Kong)....Pages 8687
Tailoring the Toughness and Electrochemical Capacitance of CNT Reinforced Mortars (Maria S. KonstaGdoutos, Panagiotis A. Danoglidis, Myrsini E. Maglogianni)....Pages 8889
Front Matter ....Pages 9191
The Creep Resistance of ShortFibre Reinforced Metal Matrix Composites (Vaclav Sklenicka, Kveta Kucharova, Milan Svoboda, Petr Kral, Marie Kvapilova, Jiri Dvorak)....Pages 9399
Adhesive Joint Fracture Under Combined Pulsed and Vibrational Loading (Yuri Petrov, Andrey Logachev, Nickolay Granichin, Grigory Volkov)....Pages 100105
Study on the Fracture Mechanism of the P91 Steel During Small Punch Tensile Testing (Hezong Li, Hao Chen, H. K. AlAbedy, Wei Sun)....Pages 106111
Damage Accumulation and Growth Models for the CreepFatigue Interaction (A. V. Tumanov, V. N. Shlyannikov)....Pages 112116
Crack Growth and Plastic, Fracture Process and Damage Zones Behavior Under Mixed Mode Loading (Valery Shlyannikov, Daria Fedotova)....Pages 117123
Front Matter ....Pages 125125
Parametric Resonance of a Microbeam with Flexible Support Under Fringing Field Excitation (Zhichong Wang)....Pages 127132
Measurement of Elastic Nonlinearities Using the Fundamental Edge Wave Mode (James Martin Hughes, Andrei Kotousov, ChingTai Ng)....Pages 133139
Unsteady Axisymmetric ElectroMagnetoElastic Oscillations of a Continuous Cylinder Under the External Displacement Field (Vladimir Vestyak, Vasily Scherbakov)....Pages 140144
Development of Micromechanical Models of Fatigue Damage (James Vidler, Andrei Kotousov, ChingTai Ng)....Pages 145150
Research on Springback of 5A02 Aluminum Alloy Considering Thickness Normal Stress in Hydroforming (Peicheng Jiang, Lihui Lang, Sergei Alexandrov)....Pages 151157
On the Friction Test for Metal Forming Applications (Sergei Alexandrov, Marko Vilotic, Dragisa Vilotic)....Pages 158161
From the Linear Theory of Elasticity to Bending Equations for Beams with Variable CrossSection (Boris Gusev, Vasily Saurin)....Pages 162163
On Different Representations of Equations for Beam with Variable CrossSection (Vladimir Poliakov, Vasily Saurin)....Pages 164165
Shear Residual Stresses Induced by Torsional Loading (D. Pérez Gallego, J. Ruiz Hervías, D. A. Cendón Franco)....Pages 166167
Elastoplastic Analysis of Reentrant Cell Formation in Auxetic Foams Under Compression and Heat Treatment (YunChe Wang, TsaiWen Ko, HsiangWei Lai)....Pages 168169
Analytical Modeling of the ThermoMechanical Behavior of a FrictionPendulum Seismic Isolator (Todor Zhelyazov)....Pages 170171
Front Matter ....Pages 173173
Damage Accumulation and Limit State of Welded Pipelines with CorrosionErosion Metal Loss Due to UltraLowCycle Fatigue (Alexey Milenin, Elena Velikoivanenko, Galina Rozynka, Nina Pivtorak)....Pages 175180
Unsteady ElasticDiffusion Oscillations of a Simply Supported Kirchhoff Plate Under the Distributed Transverse Load Action (O. A. Afanasieva, A. V. Zemskov)....Pages 181186
A Dynamic Contact Problem of Torsion that Reduces to the Singular Integral Equation with Two Fixed Singularities (V. Popov, O. Kyrylova)....Pages 187192
Some Dynamic Problems for Layered Composites (Sergey Pshenichnov)....Pages 193197
The Influence of Geometric Parameters on the Bearing Capacity of TransformableVolume Structure (L. M. Lobanov, V. S. Volkov, O. V. Makhnenko, S. M. Kandala, Y. V. Borovyk)....Pages 198203
The Influence of Mixed Conditions on the Stress Concentration in the Neighborhood of Interfacial Inclusions in an Inhomogeneous Transversely Isotropic Space (Oleksandr Kryvyi, Yurii Morozov)....Pages 204209
On an Approach to the Thermoelastic Analysis of Nonhomogeneous Solids (Roman Kushnir, Yuriy Tokovyy)....Pages 210215
The Stress State Near the Corner Point of the Interface of Piecewise Homogeneous Plane in the Presence of Interfacial Shear Cracks (V. M. Nazarenko, A. L. Kipnis)....Pages 216221
Coupled Nonstationary Longitudinal Vibrations of an Infinite Electromagnetoelastic Rod (Thong D. Pham, Dmitry V. Tarlakovskii, Vladimir A. Vestyak)....Pages 222227
The Effect of Cracks Interaction in Materials Under Loading Along Cracks (Viacheslav Bogdanov, Vladimir Nazarenko)....Pages 228234
Safe Loading of the Orthotropic Plate with Periodic System of Collinear Cracks (Olga Bogdanova)....Pages 235241
Boundary Element Analysis of Partially Debonded ShellLike Rigid Inclusions in Anisotropic Medium (Heorhiy Sulym, Nataliia Ilchuk, Iaroslav Pasternak)....Pages 242247
The Transmission of an Acoustic Wave Through a Composite Plate with Energy Dissipation in a Material Taken into Account Based on ThreeDimensional Equations of Elasticity Theory (V. N. Paimushin, R. K. Gazizullin)....Pages 248253
Vibration of the Plate with Integral Layer Damping: Experimental and Theoretical Studies (V. N. Paimushin, V. A. Firsov, V. M. Shishkin, R. K. Gazizullin)....Pages 254260
Thermomagnetoelectroelasticity of Bimaterial Solids with High Temperature Conducting Interface and Thin Internal Inhomogeneities (Andrii Vasylyshyn, Iaroslav Pasternak, Heorhiy Sulym)....Pages 261267
Fracture of Composite Materials Under Compression Along Cracks (Mykhailo Dovzhyk, Viacheslav Bogdanov, Vladimir Nazarenko)....Pages 268272
Development of Welded Elements of the Railway Freight Car Bogie with Increased Characteristics of Fatigue Resistance and Survivability (L. Lobanov, O. Makhnenko, A. Pustovoy, S. Solovey)....Pages 273279
Electron Beam Additive Technology Optimization Using Mathematical Modeling (Oleh Makhnenko, Nikita Ananchenko, Stepan Kandala, Andriy Babenko)....Pages 280286
Nonstationary Contact Problems for Thin Shells and Solids (Grigory Fedotenkov, Dmitry Tarlakovskii)....Pages 287292
Shear Buckling Mode and Failure of Sandwich Specimen Facing Layer Under FourPoint Bending (V. N. Paimushin, M. V. Makarov, S. A. Kholmogorov, M. A. Shishov)....Pages 293300
Model of LowCycle Deformation of Stainless Steel Under Soft Loading (Vasilii Gorokhov, Sergei Kapustin, Yuriy Churilov, Dmitriy Kazakov, Dmitriy Zhegalov)....Pages 301304
Creep and LongTerm Strength of Structures (Ivan Volkov, Leonid Igumnov, Svetlana Litvinchuk)....Pages 305308
Mathematical Modeling of Nonlinear Dynamic Deformation and Failure of MetalPlastic Shells of Revolution (Leonid Igumnov, Nikolai Abrosimov, Nadezhda Novoseltseva, Vasilii Gorokhov)....Pages 309311
Impact of Transient Pressure on a HalfSpace with Membrane Type Coating (Elena Mikhailova, Grigory Fedotenkov, Dmitry Tarlakovskii)....Pages 312315
Front Matter ....Pages 317317
Some Considerations on Stress Intensity Factor at Atomic Scale (Pasquale Gallo)....Pages 319324
Initial Intergranular Cracking of NiBase Superalloys Due to the Degradation of the Crystallinity of Grain Boundaries Under CreepFatigue Loading (Wataru Suzuki, Yifan Luo, Kenta Ishihara, Kens Suzuki, Hideo Miura)....Pages 325331
Characterization of Microstructurally Small Fatigue Crack Behavior (Evgenii Malitckii, Heikki Remes, Pauli Lehto, Sven Bossuyt)....Pages 332333
An AtomicLevel Unified Criterion for Brittle Fracture (Kai Huang, Takashi Sumigawa, Takahiro Shimada, Takayuki Kitamura)....Pages 334336
Fatigue of Micro/Nano Metals (Takayuki Kitamura, Takashi Sumigawa, Kai Huang)....Pages 337338
Back Matter ....Pages 339341
Structural Integrity 16 Series Editors: José A. F. O. Correia · Abílio M. P. De Jesus
Emmanuel Gdoutos Maria KonstaGdoutos Editors
Proceedings of the Third International Conference on Theoretical, Applied and Experimental Mechanics
Structural Integrity Volume 16
Series Editors José A. F. O. Correia, Faculty of Engineering, University of Porto, Porto, Portugal Abílio M. P. De Jesus, Faculty of Engineering, University of Porto, Porto, Portugal Advisory Editors Majid Reza Ayatollahi, School of Mechanical Engineering, Iran University of Science and Technology, Tehran, Iran Filippo Berto, Department of Mechanical and Industrial Engineering, Faculty of Engineering, Norwegian University of Science and Technology, Trondheim, Norway Alfonso FernándezCanteli, Faculty of Engineering, University of Oviedo, Gijón, Spain Matthew Hebdon, Virginia State University, Virginia Tech, Blacksburg, VA, USA Andrei Kotousov, School of Mechanical Engineering, University of Adelaide, Adelaide, SA, Australia Grzegorz Lesiuk, Faculty of Mechanical Engineering, Wrocław University of Science and Technology, Wrocław, Poland Yukitaka Murakami, Faculty of Engineering, Kyushu University, Higashiku, Fukuoka, Japan Hermes Carvalho, Department of Structural Engineering, Federal University of Minas Gerais, Belo Horizonte, Minas Gerais, Brazil ShunPeng Zhu, School of Mechatronics Engineering, University of Electronic Science and Technology of China, Chengdu, Sichuan, China Stéphane Bordas, University of Luxembourg, ESCHSURALZETTE, Luxembourg Nicholas Fantuzzi Bologna, Italy
, DICAM Department, Univ of Bologna, BOLOGNA,
The Structural Integrity book series is a high level academic and professional series publishing research on all areas of Structural Integrity. It promotes and expedites the dissemination of new research results and tutorial views in the structural integrity ﬁeld. The Series publishes research monographs, professional books, handbooks, edited volumes and textbooks with worldwide distribution to engineers, researchers, educators, professionals and libraries. Topics of interested include but are not limited to: – – – – – – – – – – – – – – – – – – – – – –
Structural integrity Structural durability Degradation and conservation of materials and structures Dynamic and seismic structural analysis Fatigue and fracture of materials and structures Risk analysis and safety of materials and structural mechanics Fracture Mechanics Damage mechanics Analytical and numerical simulation of materials and structures Computational mechanics Structural design methodology Experimental methods applied to structural integrity Multiaxial fatigue and complex loading effects of materials and structures Fatigue corrosion analysis Scale effects in the fatigue analysis of materials and structures Fatigue structural integrity Structural integrity in railway and highway systems Sustainable structural design Structural loads characterization Structural health monitoring Adhesives connections integrity Rock and soil structural integrity.
** Indexing: The books of this series are submitted to Web of Science, Scopus, Google Scholar and Springerlink ** This series is managed by team members of the ESIS/TC12 technical committee. Springer and the Series Editors welcome book ideas from authors. Potential authors who wish to submit a book proposal should contact Dr. Mayra Castro, Senior Editor, Springer (Heidelberg), email: [email protected]
More information about this series at http://www.springer.com/series/15775
Emmanuel Gdoutos Maria KonstaGdoutos •
Editors
Proceedings of the Third International Conference on Theoretical, Applied and Experimental Mechanics
123
Editors Emmanuel Gdoutos Ofﬁce of Theoretical and Applied Mechanic Academy of Athens Athens, Greece
Maria KonstaGdoutos Civil Engineering Department The University of Texas at Arlington Arlington, TX, USA
ISSN 2522560X ISSN 25225618 (electronic) Structural Integrity ISBN 9783030478827 ISBN 9783030478834 (eBook) https://doi.org/10.1007/9783030478834 © Springer Nature Switzerland AG 2020 This work is subject to copyright. All rights are reserved by the Publisher, whether the whole or part of the material is concerned, speciﬁcally the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microﬁlms or in any other physical way, and transmission or information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed. The use of general descriptive names, registered names, trademarks, service marks, etc. in this publication does not imply, even in the absence of a speciﬁc statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. The publisher, the authors and the editors are safe to assume that the advice and information in this book are believed to be true and accurate at the date of publication. Neither the publisher nor the authors or the editors give a warranty, express or implied, with respect to the material contained herein or for any errors or omissions that may have been made. The publisher remains neutral with regard to jurisdictional claims in published maps and institutional afﬁliations. This Springer imprint is published by the registered company Springer Nature Switzerland AG The registered company address is: Gewerbestrasse 11, 6330 Cham, Switzerland
Preface
This volume contains sixtyone sixpage papers/twopage abstracts presented at the “Third International Conference on Theoretical, Applied and Experimental Mechanics,” (ICTAEM_3) held in Athens, Greece, June 14–17, 2020. The papers/abstracts are arranged in three topics and two special symposia. The three topics are: “Materials: Properties, Manufacturing, Modelling” with sixteen contributions, “Fracture” with ﬁve contributions and “Miscellaneous (Computational Mechanics, Dynamics, Nanomaterials, Plasticity, Wave Propagation)” with eleven contributions. The two symposia are: “Symposium on Theoretical and Experimental Approaches in Mechanics of Solids with Nonhomogeneities and Defects,” by Roman Kushnir with twentyfour contributions and “Fracture Nanomechanics, Fatigue and Fracture at Small Scales (experiments and simulations)” by Pasquale Gallo with ﬁve contributions. The papers of the tracks have been contributed from open call, while the papers of the two symposia have been solicited by the organizers, to who we are greatly indebted. ICTAEM_3 will focus in all aspects of theoretical, applied and experimental mechanics including biomechanics, composite materials, computational mechanics, constitutive modeling of materials, dynamics, elasticity, experimental mechanics, fracture, mechanical properties of materials, micromechanics, nanomechanics, plasticity, stress analysis, structures, wave propagation. The attendees of ICTAEM_3 will have the opportunity to interact with the most outstanding world leaders and get acquainted with the latest developments in the area of mechanics. ICTAEM_3 will be a forum of university, industry and government interaction and exchange of ideas in an area of utmost scientiﬁc and technological importance. We are sure that besides the superb technical program, the attendees of ICTAEM_3 will enjoy the city of Athens. It is considered as the ancient capital of the world with a long fascinating history dating from the Neolithic Age, the city of the goddess of wisdom Athena, a center for the arts, learning and philosophy, home of Plato’s Academy and Aristotle’s Lyceum, the birthplace of democracy and of Western civilization, of the most intellectual and artistic ideas, the cradle of
v
vi
Preface
democracy, the host city of the ﬁrst modernday Olympic Games in 1896, and the Summer Olympics in 2004. More than a hundred participants attended ICTAEM_3. The participants of ICTAEM_3 came from 20 countries. Roughly speaking 14% came from Europe, 24% from the Far East, 7% from the Americas and 55% from other countries. We are happy and proud to have welcomed in the historic city of Athens wellknown experts who came to discuss problems related to the analysis and prevention of failure in structures. Presentation of technical papers alone is not enough for effective scientiﬁc communication. It is the healthy exchange of ideas and scientiﬁc knowledge, formal and informal discussions, together with the plenary and contributed papers that make a fruitful and successful meeting. Informal discussions, personal acquaintance and friendship play an important role. We very sincerely thank the authors who have contributed to this volume, the symposium/sessions organizers for their hard work and dedication and the referees who reviewed the quality of the submitted contributions. The tireless effort of the members of the organizing committee as well as of other numerous individuals, and people behind the scenes is appreciated. We are deeply indebted to Dr. Stavros Shiaeles for his hard work and dedication in the organization of the conference. Finally, a special word of thanks goes to Dr. Maria Shiaeles for her continuous collaboration and support. March 2020
Emmanuel Gdoutos Maria KonstaGdoutos
Contents
Materials: Properties, Manufacturing, Modelling HighSpeed ModeI Delamination . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Tianyu Chen, Christopher M. Harvey, Simon Wang, and Vadim V. Silberschmidt
3
Characterization of Dynamic Fractures for Compressed PMMA Material . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . C. Huang
9
Tensile Behavior of a Titanium Alloy Additively Manufactured via Selective Electron Beam Melting . . . . . . . . . . . . . . . . . . . . . . . . . . . Yinling Zhang, Shoujiang Qu, Aihan Feng, and Daolun Chen
14
The Rule of Mixtures on the Elastic Buckling Response of Rectangular GLARE FML Plates Under Shear Stresses . . . . . . . . . . Costas D. Kalfountzos, George S. E. Bikakis, and Efstathios E. Theotokoglou Evaluating Bonding Characteristics of Joggled Lap CFRP Using Acoustic Emission Techniques . . . . . . . . . . . . . . . . . . . . . . . . . . . Claudia Barile, Caterina Casavola, Giovanni Pappalettera, Carmine Pappalettere, and Paramsamy Kannan Vimalathithan
20
26
Experimental Study of Low Concentration Diffusible Hydrogen Effect on Mechanical Behaviour of Carbon Steel . . . . . . . . . . . . . . . . . . I. M. Dmytrakh, R. L. Leshchak, and A. M. Syrotyuk
32
Effects of Temperature on Tensile and Fracture Behavior of Dissimilar Metal Welded Joint for Nuclear SafeEnd . . . . . . . . . . . . . Lei Wang, Yang Liu, Xiu Song, and Jiahua Liu
38
A Multiattribute Information Based Method of Material Strength Distribution Fitting . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Liyang Xie, Bo Qin, and Ningxiang Wu
44
vii
viii
Contents
Performance of a Carburizing Bearing Steel After Surface Nanosized . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Yanhui Wang, Fucheng Zhang, Zhinan Yang, Hezong Li, and Qian Yang Residual Strength and Toughness of Nano and Micro Scale Fiber Reinforced Cementitious Composites . . . . . . . . . . . . . . . . . . . . . . . . . . . Panagiotis A. Danoglidis, Maria S. KonstaGdoutos, and Emmanuel E. Gdoutos
52
58
Experimental and Numerical Strategy for the Determination of Mechanical Properties Related to Human Cortical Bone Fracture . . . J.L. Tailhan, Y. GodioRaboutet, and C. Boulay
64
Effect of External Field Treatment on the Microstructure and Deformation Behavior of NickelBase Superalloy . . . . . . . . . . . . . . Yang Liu, Lei Wang, Xiu Song, and Yao Wang
70
Dynamic Speckle Contrast Imaging for Surface Defect Detection . . . . . Rishikesh Kulkarni, Shanta Patil, and Pramod Rastogi
76
Experimental Investigation of the Elastic Modulus of Timber by Using Density and Fiber Orientation . . . . . . . . . . . . . . . . . . . . . . . . . WeiChung Wang and TzuYu Kuo
82
Effect of pH on Microstructure and Properties of UltrasonicAssisted Electroless NiP Coatings . . . . . . . . . . . . . . . . . . . Jingjing Cao, Xiaoyu Wang, Yifan Zhao, and Guofang Kong
86
Tailoring the Toughness and Electrochemical Capacitance of CNT Reinforced Mortars . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Maria S. KonstaGdoutos, Panagiotis A. Danoglidis, and Myrsini E. Maglogianni
88
Fracture The Creep Resistance of ShortFibre Reinforced Metal Matrix Composites . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Vaclav Sklenicka, Kveta Kucharova, Milan Svoboda, Petr Kral, Marie Kvapilova, and Jiri Dvorak
93
Adhesive Joint Fracture Under Combined Pulsed and Vibrational Loading . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 100 Yuri Petrov, Andrey Logachev, Nickolay Granichin, and Grigory Volkov Study on the Fracture Mechanism of the P91 Steel During Small Punch Tensile Testing . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 106 Hezong Li, Hao Chen, H. K. AlAbedy, and Wei Sun
Contents
ix
Damage Accumulation and Growth Models for the CreepFatigue Interaction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 112 A. V. Tumanov and V. N. Shlyannikov Crack Growth and Plastic, Fracture Process and Damage Zones Behavior Under Mixed Mode Loading . . . . . . . . . . . . . . . . . . . . . . . . . . 117 Valery Shlyannikov and Daria Fedotova Miscellaneous (Computational Mechanics, Dynamics, Nanomaterials, Plasticity, Wave Propagation) Parametric Resonance of a Microbeam with Flexible Support Under Fringing Field Excitation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 127 Zhichong Wang Measurement of Elastic Nonlinearities Using the Fundamental Edge Wave Mode . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 133 James Martin Hughes, Andrei Kotousov, and ChingTai Ng Unsteady Axisymmetric ElectroMagnetoElastic Oscillations of a Continuous Cylinder Under the External Displacement Field . . . . . 140 Vladimir Vestyak and Vasily Scherbakov Development of Micromechanical Models of Fatigue Damage . . . . . . . . 145 James Vidler, Andrei Kotousov, and ChingTai Ng Research on Springback of 5A02 Aluminum Alloy Considering Thickness Normal Stress in Hydroforming . . . . . . . . . . . . . . . . . . . . . . . 151 Peicheng Jiang, Lihui Lang, and Sergei Alexandrov On the Friction Test for Metal Forming Applications . . . . . . . . . . . . . . 158 Sergei Alexandrov, Marko Vilotic, and Dragisa Vilotic From the Linear Theory of Elasticity to Bending Equations for Beams with Variable CrossSection . . . . . . . . . . . . . . . . . . . . . . . . . 162 Boris Gusev and Vasily Saurin On Different Representations of Equations for Beam with Variable CrossSection . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 164 Vladimir Poliakov and Vasily Saurin Shear Residual Stresses Induced by Torsional Loading . . . . . . . . . . . . . 166 D. Pérez Gallego, J. Ruiz Hervías, and D. A. Cendón Franco Elastoplastic Analysis of Reentrant Cell Formation in Auxetic Foams Under Compression and Heat Treatment . . . . . . . . . . . . . . . . . . 168 YunChe Wang, TsaiWen Ko, and HsiangWei Lai Analytical Modeling of the ThermoMechanical Behavior of a FrictionPendulum Seismic Isolator . . . . . . . . . . . . . . . . . . . . . . . . . 170 Todor Zhelyazov
x
Contents
Symposium on Theoretical and Experimental Approaches in Mechanics of Solids with Nonhomogeneities and Defects, by Roman Kushnir Damage Accumulation and Limit State of Welded Pipelines with CorrosionErosion Metal Loss Due to UltraLowCycle Fatigue . . . . . . . 175 Alexey Milenin, Elena Velikoivanenko, Galina Rozynka, and Nina Pivtorak Unsteady ElasticDiffusion Oscillations of a Simply Supported Kirchhoff Plate Under the Distributed Transverse Load Action . . . . . . . 181 O. A. Afanasieva and A. V. Zemskov A Dynamic Contact Problem of Torsion that Reduces to the Singular Integral Equation with Two Fixed Singularities . . . . . . . 187 V. Popov and O. Kyrylova Some Dynamic Problems for Layered Composites . . . . . . . . . . . . . . . . . 193 Sergey Pshenichnov The Inﬂuence of Geometric Parameters on the Bearing Capacity of TransformableVolume Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . . 198 L. M. Lobanov, V. S. Volkov, O. V. Makhnenko, S. M. Kandala, and Y. V. Borovyk The Inﬂuence of Mixed Conditions on the Stress Concentration in the Neighborhood of Interfacial Inclusions in an Inhomogeneous Transversely Isotropic Space . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 204 Oleksandr Kryvyi and Yurii Morozov On an Approach to the Thermoelastic Analysis of Nonhomogeneous Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 210 Roman Kushnir and Yuriy Tokovyy The Stress State Near the Corner Point of the Interface of Piecewise Homogeneous Plane in the Presence of Interfacial Shear Cracks . . . . . . 216 V. M. Nazarenko and A. L. Kipnis Coupled Nonstationary Longitudinal Vibrations of an Inﬁnite Electromagnetoelastic Rod . . . . . . . . . . . . . . . . . . . . . . . . 222 Thong D. Pham, Dmitry V. Tarlakovskii, and Vladimir A. Vestyak The Effect of Cracks Interaction in Materials Under Loading Along Cracks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 228 Viacheslav Bogdanov and Vladimir Nazarenko Safe Loading of the Orthotropic Plate with Periodic System of Collinear Cracks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 235 Olga Bogdanova
Contents
xi
Boundary Element Analysis of Partially Debonded ShellLike Rigid Inclusions in Anisotropic Medium . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 242 Heorhiy Sulym, Nataliia Ilchuk, and Iaroslav Pasternak The Transmission of an Acoustic Wave Through a Composite Plate with Energy Dissipation in a Material Taken into Account Based on ThreeDimensional Equations of Elasticity Theory . . . . . . . . . 248 V. N. Paimushin and R. K. Gazizullin Vibration of the Plate with Integral Layer Damping: Experimental and Theoretical Studies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 254 V. N. Paimushin, V. A. Firsov, V. M. Shishkin, and R. K. Gazizullin Thermomagnetoelectroelasticity of Bimaterial Solids with High Temperature Conducting Interface and Thin Internal Inhomogeneities . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 261 Andrii Vasylyshyn, Iaroslav Pasternak, and Heorhiy Sulym Fracture of Composite Materials Under Compression Along Cracks . . . 268 Mykhailo Dovzhyk, Viacheslav Bogdanov, and Vladimir Nazarenko Development of Welded Elements of the Railway Freight Car Bogie with Increased Characteristics of Fatigue Resistance and Survivability . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 273 L. Lobanov, O. Makhnenko, A. Pustovoy, and S. Solovey Electron Beam Additive Technology Optimization Using Mathematical Modeling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 280 Oleh Makhnenko, Nikita Ananchenko, Stepan Kandala, and Andriy Babenko Nonstationary Contact Problems for Thin Shells and Solids . . . . . . . . . 287 Grigory Fedotenkov and Dmitry Tarlakovskii Shear Buckling Mode and Failure of Sandwich Specimen Facing Layer Under FourPoint Bending . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 293 V. N. Paimushin, M. V. Makarov, S. A. Kholmogorov, and M. A. Shishov Model of LowCycle Deformation of Stainless Steel Under Soft Loading . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 301 Vasilii Gorokhov, Sergei Kapustin, Yuriy Churilov, Dmitriy Kazakov, and Dmitriy Zhegalov Creep and LongTerm Strength of Structures . . . . . . . . . . . . . . . . . . . . 305 Ivan Volkov, Leonid Igumnov, and Svetlana Litvinchuk
xii
Contents
Mathematical Modeling of Nonlinear Dynamic Deformation and Failure of MetalPlastic Shells of Revolution . . . . . . . . . . . . . . . . . . 309 Leonid Igumnov, Nikolai Abrosimov, Nadezhda Novoseltseva, and Vasilii Gorokhov Impact of Transient Pressure on a HalfSpace with Membrane Type Coating . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 312 Elena Mikhailova, Grigory Fedotenkov, and Dmitry Tarlakovskii Fracture Nanomechanics, Fatigue and Fracture at Small Scales (experiments and simulations) by Pasquale Gallo Some Considerations on Stress Intensity Factor at Atomic Scale . . . . . . 319 Pasquale Gallo Initial Intergranular Cracking of NiBase Superalloys Due to the Degradation of the Crystallinity of Grain Boundaries Under CreepFatigue Loading . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 325 Wataru Suzuki, Yifan Luo, Kenta Ishihara, Kens Suzuki, and Hideo Miura Characterization of Microstructurally Small Fatigue Crack Behavior . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 332 Evgenii Malitckii, Heikki Remes, Pauli Lehto, and Sven Bossuyt An AtomicLevel Uniﬁed Criterion for Brittle Fracture . . . . . . . . . . . . . 334 Kai Huang, Takashi Sumigawa, Takahiro Shimada, and Takayuki Kitamura Fatigue of Micro/Nano Metals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 337 Takayuki Kitamura, Takashi Sumigawa, and Kai Huang Author Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 339
Materials: Properties, Manufacturing, Modelling
HighSpeed ModeI Delamination Tianyu Chen1, Christopher M. Harvey1(&) , Simon Wang1,2 and Vadim V. Silberschmidt1 1
,
Loughborough University, Loughborough, Leicestershire LE11 3TU, UK [email protected] 2 Hebei University of Engineering, Handan 056038, China
Abstract. The analytical theory of modeI delamination propagation in double cantilever beams (DCBs) under high loading rates is developed by accounting for structural vibration and wave dispersion, and by using EulerBernoulli beam theory. The developed analytical theory is validated against experimental data and against ﬁnite element method (FEM) simulations, showing excellent agreement. It is shown that the developed analytical theory can accurately calculate energy release rate (ERR) for both stationary and propagating delamination, and that structural vibration can have a signiﬁcant effect on ERR. It is further shown how the theory can be used to postprocess experimental results from highspeed delamination tests to determine fracture toughness. Among other examples, the work is therefore expected to be useful to engineers and academic researchers to determine the initiation, arrest and propagation fracture toughness of laminated materials against delamination. The developed theory also provides useful benchmark solutions for the development of numerical codes. Keywords: Double cantilever beam Dynamic energy release rate Dynamic fracture toughness
1 Introduction Double cantilever beams (DCBs) have been widely used to determine the fracture toughness of materials under mode I loading conditions. A standard method has been established for modeI interlaminar fracture toughness testing with DCBs [1], but it is only applicable for quasistatic loading. Under dynamic loads, where inertia is signiﬁcant, there has been comparatively little research carried out. Moreover, what studies there have been did not consider structural vibration and consequently provided a ‘smoothed’ solution for energy release rate (ERR). Vibration, however, can be signiﬁcant under high loading rates, which causes ERR to oscillate with a spectrum of frequencies and amplitudes. For a stationary crack, the authors have presented an analytical solution for the ERR of a DCB under constant highrate opening [2], which is accurate for the ﬁrst vibration mode but not for high order vibration modes. Later, the authors developed the analytical solution for the same case, but including higher order vibration modes, for cyclic loading [3], and for cracks on elastic interfaces [4]. The improved representation © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 3–8, 2020. https://doi.org/10.1007/9783030478834_1
4
T. Chen et al.
of the uncracked region in the latter work captures the crack tip deformation more accurately, and consequently, the ERR also. The elastic interface in that work is also relevant for the study of crack process zones. It is worth noting that Ref. [4] uses a global energy balance approach and shows that the dispersive propagation of flexural waves must be considered in order to capture contributions to the ERR from higherorder vibration modes. Qualitatively, this is because not all the energy stored in the vibrating beam is immediately available to the crack tip to drive propagation at a point in time since waves propagate with a ﬁnite wave speed. Energy flow in and out of the crack tip region must be considered, which means accounting for the dispersive propagation of flexural waves. By contrast, if the conventional global energy balance approach is used, as in Refs. [5, 6], then when vibration is included, the ERR diverges as higher order vibration modes are added [2]. Whereas the previous work has been for either been stationary cracks [2–6], or for propagating cracks without vibration effects [5, 6], this article will present for the ﬁrst time the analytical theory for the ERR of a propagating crack with vibration effects at high loading rates. Among other examples, the complete theory is expected to be useful to engineers and academic researchers to determine the dynamic initiation and propagation fracture toughness of laminated materials. It also provides useful benchmark solutions for the development of numerical codes.
2 Analytical Theory for DCBs Under High Rates of Loading Consider the DCB geometry shown in Fig. 1a, where v is the constant opening rate applied from t ¼ 0, and vt is the opening displacement. The EulerBernoulli beam assumption applies since h a, where h is the thickness of one DCB arm, and a is the crack length. Figure 1b shows the coordinate system and the effective boundary conditions under which the crack tip is assumed to be clamped.
Fig. 1. (a) Symmetric double cantilever beam; (b) effective boundary condition
HighSpeed ModeI Delamination
2.1
5
ERR Solution for a Stationary Crack
According to Ref. [2], the deflection of the beam in Fig. 1b, which is effectively half a DCB, under constant opening rate is rﬃﬃﬃﬃﬃﬃ 1 3 qA X Ki x 3x wðx; tÞ ¼ va þ 1 vt ; / ða xÞ sinðxi tÞ þ EI i¼1 k3i i 2a3 2a 2
ð1Þ
where for the ith mode, /i ða xÞ is the mode shape, xi is the angular frequency, ki is determined by the frequency equation of tanhðki Þ tanðki Þ ¼ 0, and Ki is given as pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Ki ¼ ð1Þi r2i þ 1 þ r2i 1 with ri ¼ ½coshðki Þ cosðki Þ=½sinhðki Þ sinðki Þ. According to Freund [7], the dynamic ERR, is M 2 ða; tÞ a_ 2 1 2 ; G¼ bEI c0
ð2Þ
where c20 ¼ E=q. By combining Eqs. (1) and (2), the dynamic ERR for a stationary crack (that is, a_ ¼ 0) is i2 EI h ð2Þ w ða; tÞ b " #2 pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 1 9EIv2 t2 12 qAEI v2 t X Ki 4qAv2 X Ki ¼ þ sinðxi tÞ þ sinðxi tÞ ; ba2 ba4 k b k i¼1 i i¼1 i
G¼
ð3Þ
where b is the beam width, and A is the area of the beam’s crosssection. 2.2
ERR Solution for a Propagating Crack
Based on Eq. (2), and using the same technique as in Ref. [4] to account for the wave dispersion, the analytical ERR solution for a propagating crack is obtained as pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 9EIv2 t2 12 qAEI v2 t Ki 0 a_ 2 a_ 2 X a_ G¼ 1 2 þ 1 2 f sin 1 p xi t ; ð4Þ ba2 ba4 Ci c0 c0 i¼1 ki i where fi0 is a reduction factor for wave dispersion and CiP is the phase speed of the ith mode wave. The derivation of Eq. (4), with full details concerning each term, will be published shortly in a full journal article by the authors. 2.3
Limiting Speed of Crack Propagation
pﬃﬃﬃﬃﬃﬃﬃﬃﬃ In Eq. (4), the crack propagation speed a_ should be no greater than c0 ¼ E=q to retain a positive ERR. Another constraint on a_ is that it must be no greater than C1P , the ﬁrst mode wave phase speed, since the ﬁrst mode wave modulates all the other waves _ and carries the most vibrational energy. That is, if the crack propagates faster than a, the vibrational energy cannot be supplied to the crack tip to open the crack. This limit
6
T. Chen et al.
in 1D structures is the counterpart to Freund’s [7] limiting crack speed of CR (Rayleigh wave speed) in a semiinﬁnite space. The ratio of these two limiting speeds is C1p k1 1þm pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ r ; ¼ pﬃﬃﬃ CR 6 ð0:862 þ 1:14mÞ 1 m
ð5Þ
where r ¼ h=a is the aspect ratio of EulerBernoulli beam. Equation (5) shows limiting speed in DCBs is not only determined by material properties but also by the geometry. An examination of experimentally measured crack propagating speeds and the theoretical limiting crack speed predicted by Eq. (5) is given in Fig. 2.
Fig. 2. Comparison of measured crack propagation speeds under various loading rates [6]: (a) PEEK/carbonﬁber composite; (b) epoxy/carbonﬁber composite
3 Experimental and Finite Element Method Veriﬁcation There have been relatively few experimental studies of DCBs under high loading rates [8]. Nevertheless, there is a series of experiments reported by Blackman et al. [6] at high loading rates up to 15 ms−1. Considering their results for a loading rate of 10 ms−1, their crack length versus time results can be used to obtain the timevarying crack propagation speed a_ ðtÞ, and to calculate ERR using Eq. (3) for the stationary crack and Eq. (4) for the propagating crack. The results are presented in Fig. 3. In Fig. 3, the fracture toughness for initiation and arrest are adopted from Ref. [9], which numerically simulates the same tests from Blackman et al. [6]. It is seen that the ERR calculated using the developed theory, presented in Sect. 2, can accurately predict the fracture toughness for crack initiation under the dynamic regime. Moreover, the ERR for crack propagation is always above the arrest fracture toughness except for when crack arrest happens at around t ¼ 2:6 ms, as expected. There were not sufﬁcient data points from the experiments to accurately determine the crack propagation speed, and so the developed theory was instead further veriﬁed against FEM simulation results from Ref. [9]. The crack length versus time results from the simulation were used to obtain the timevarying crack propagation speed, a_ ðtÞ, and to calculate the ERR. Figure 4 compares the analytically predicted and the numerically simulated. Excellent agreement is seen for this case of 10 ms−1 opening.
HighSpeed ModeI Delamination
7
Fig. 3. Dynamic ERR for 10 ms−1 opening rate using experiment data
Fig. 4. Dynamic ERR for 10 ms−1 opening rate using FEM data
4 Conclusion Analytical solutions for the dynamic ERR of a DCB resulting from high loading rates, including vibration, are derived for both stationary and propagating cracks. These solutions are veriﬁed against experimental results and FEM simulations. It is shown that the developed theory can accurately predict ERR in comparison to numerical
8
T. Chen et al.
simulations; and can accurately determine the fracture toughness for crack initiation and crack arrest in comparison to both experiments and numerical simulations. To the best of the author’s knowledge, the theory presented here for the dynamic ERR of stationary and propagating cracks, including vibration, has not been solved before. These solutions are readily applicable to various engineering applications, and in particular, are expected to be useful to engineers and academic researchers to determine the initiation, arrest and propagation fracture toughness of laminated materials against delamination. The developed theory also provides useful benchmark solutions for the development of numerical codes.
References 1. ASTM D552801: Standard test method for mode I interlaminar fracture toughness of unidirectional ﬁberreinforced polymer matrix composites (2014) 2. Chen, T., Harvey, C.M., Wang, S., Silberschmidt, V.V.: Dynamic interfacial fracture of a double cantilever beam. Eng. Fract. Mech. (2018). https://doi.org/10.1016/j.engfracmech. 2018.11.033 3. Chen, T., Harvey, C.M., Wang, S., Silberschmidt, V.V.: Dynamic interfacial fracture of a thinlayered structure. Procedia Struct. Integrity 13, 613–618 (2018) 4. Chen, T., Harvey, C.M., Wang, S., Silberschmidt, V.V.: Dynamic delamination on elastic interface. Compos. Struct. 234, 111670 (2019) 5. Smiley, A.J., Pipes, R.B.: Rate effects on mode I interlaminar fracture toughness in composite materials. J. Compos. Mater. 21(7), 670–687 (1987) 6. Blackman, B.R.K., Kinloch, A.J., Wang, Y., Williams, J.G.: The failure of ﬁbre composites and adhesively bonded ﬁbre composites under high rates of test. J. Mater. Sci. 31(17), 4451– 4466 (1996) 7. Freund, L.B.: Dynamic Fracture Mechanics. Cambridge University Press, Cambridge (1990) 8. May, M.: Measuring the ratedependent mode I fracture toughness of composites  a review. Compos. Part A Appl. Sci. Manuf. 81, 1–12 (2016) 9. Liu, Y., van der Meer, F.P., Sluys, L.J.: Cohesive zone and interfacial thick level set modeling of the dynamic double cantilever beam test of composite laminate. Theor. Appl. Fract. Mech. 96, 617–630 (2018)
Characterization of Dynamic Fractures for Compressed PMMA Material C. Huang(&) Wuhan Textile University, Wuhan, People’s Republic of China [email protected]
Abstract. Polymethyl methacrylate (PMMA) is a quasibrittle material and dynamic behaviors usually present thermoplastic characteristic. But in some cases, PMMA breaks with the complete brittle characteristic. The complex behaviors need to be studied for a further understanding. A series of PMMA specimens are designed to study the behaviors on a Spilt Hopkinson Pressure Bar (SHPB) device. The complex behaviors are found to be dominated by the impulsive energy and there exists a critical energy for the specimens to create the complete brittle fracture. Keywords: Thermoplastic deformation
Brittle fracture Impulsive energy
1 Introduction Dynamic fractures of brittle materials usually present very complex modes and various theories are tried to explain the fracture mechanism from different points of view. The fractures are thought to involve many factors including loads, material properties, microstructures, geometries and so on. The concerning factors have been studied broadly in published literatures, but it is still difﬁcult to determine the factor that can play a dominant role in fractures. PMMA is generally recognized as a brittle material with the properties of light weight, high strength and transparency. When compressed statically, cylindrical specimen deforms in barrel shape like metal one and presents high ductility with the features of elastoplastic deformation. However, under SHPB impact loading the primary deformation is characterized by fractures and the material presents strong sensitive characteristics of dynamic behaviors. PMMA is composed of high molecule mass and glass transition occurs at the lower temperature. Under impact loading, thermoplastic deformations usually occur on fragment debris and affect the dynamic behaviors. In order to study the dynamic fracture characteristics, a series of cylindrical PMMA specimens are designed for SHPB experiments to test size effects on the fractures. The specimens are assigned with two diameters of 8 mm and 15 mm. The lengths of 8, 10, 12 and 14 mm are set for the 8 mm diameter specimens with the aspect ratios (L/D) of 1, 1.25, 1.5 and 1.75, respectively. The 15 mm diameter specimens are designed with the purpose to correlate size effects with the responses, the specimens are designated with the aspect ratios of 1, 1.27, 1.53 and 1.8 that equal to the 8 mm diameter specimens one by one. The specimen lengths are then determined as 15, 19, 23 and 27 mm. © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 9–13, 2020. https://doi.org/10.1007/9783030478834_2
10
C. Huang
In the meantime, the 8 length specimens present a monotonic length sequence which can be used to study length effects on dynamic fractures.
2 Size Effects on Dynamic Fractures To simplify the investigation of size effects, SHPB device sets identical incident loading to all the tested specimens. Under the identical loading, specimen size becomes the only variable in SHPB experiments and dynamic responses can be studied concerning the effects of specimen size. The experiment settings allow the size effects just resulting from the size itself and correlate the fracture modes with the size effects. Size effects on strengths of the specimens have been discussed and aspect ratio is validated as an important parameter to affect the strengths [1]. This paper focuses on dynamic fractures of the specimens. In the SHPB experiments, the 8 length specimens break in essential different modes. Figure 1 shows the fracture mode of a 27 mm length specimen that has the longest length with the largest volume in the 8 length specimens. In the experiments, impact (or front) end contacting incident bar is colored in black and the rear end is kept in original form to distinguish the fragment debris and make the specimen recovered easily. The fracture shows that large debris comes from the two ends of the specimen and the small and uniform debris primarily breaks from the middle section. The largest debris shows the rear end remained in cylindrical shape with little damages on the circumferential surface, while the impact end is broken into the relatively larger black fragment debris. The fracture difference between the front and rear ends may result from a slightly slowed propagation of stress wave to deliver the stress late to the rear end resulting in the rear stress relatively smaller than the front [2]. Moreover, the end debris is shown apparently larger than the debris from middle section. The fracture modes indicate that transverse deformation is conﬁned by the end friction signiﬁcantly even though grease is used to reduce the effect of friction. High conﬁnement increases debris size and reduces the amount of debris as the same effect applied by high conﬁnement pressure. The end debris shows a length range of 5– 10 mm indicating that the conﬁnement effect has the action range of 5–10 mm. It is worth mentioning that the rear end debris shows lots of adiabatic shear bands on the fracture surface characterizing the signiﬁcant thermoplastic deformations.
Fig. 1. Fracture of 25 mm specimen
Fig. 2. Fracture of 19 mm specimen
Characterization of Dynamic Fractures
11
The 19 mm length specimen breaks with the similar modes as the 27 mm one, but presents more characteristics of thermoplastic deformation. The rear end is broken in conical shape that is usually observed in high pressure conﬁnement as the transition of brittle to ductile fracture occurs [3]. Figure 2 shows the rear end debris with the clear adiabatic shear bands on the inclined surface. The surface is formed by a shear fracture indicating that the conﬁnement effect of friction is signiﬁcant in created complex stress state. The 5–10 mm lengths of the end debris verify the friction conﬁnement to act on the specimens within the length range. Moreover, in comparison with the 27 mm specimen, the 19 mm one shows the reductions of debris sizes as the specimen length decreases to lead to the rise of strain rate. The fractures present the characterized sensitivity of strain rate.
Fig. 3. Fracture of 15 mm specimen
With the further decrease of specimen length, the 15 mm length specimen shows a different fracture mode in comparison with the 19 and 27 mm specimens. As shown in Fig. 3, the specimen is broken completely with relatively uniform debris. In order to minimize the conﬁnement effect of friction, heavy grease is used on the end surfaces. But the end debris still has the 5–10 mm lengths indicating that the friction conﬁnement is changed little for the short specimen. The fracture is primarily under the action of complex stress state. Unlike the 19 and 27 mm specimens, fragment debris of the 15 mm one does not show signiﬁcant thermoplastic deformations. The specimen breaks with the reduced debris sizes showing the characteristic of brittle fracture. Here, the different fracture modes of the specimens can only be attributed to the length decrease. Figure 4 shows the fracture of a 14 mm length specimen. The specimen just has 1 mm length difference with the 15 mm specimen. In Fig. 4, the black debris breaks from the impact end with the characteristic of friction conﬁnement effect. The debris shows the lengths around 5 mm that is much less than the 15 mm specimen even though the two specimens break with the similar characteristic of brittle fracture. The debris difference may be concluded resulting from the effect of transverse size as the
12
C. Huang
two just have 1 mm length difference. If the transverse size is the right factor, aspect ratio may be a more desirable geometric parameter to present the effect of transverse size. The aspect ratio has shown the effects on strengths of the specimens [1]. The 14 mm length specimen has the identical aspect ratio with the 27 mm length specimen, but they show essentially different fracture modes. The 14 mm specimen breaks with brittle characteristic of uniform debris as the ends are broken into much smaller debris. If the fracture modes are determined by transverse size, the aspect ratio should present a little correlation with the fractures. There must exist other factor to dominate the fractures.
Fig. 4. Fracture of 14 mm specimen
Fig. 5. Fracture of 8 mm specimen
In comparison with the previous specimens, the 8 mm specimen breaks with smaller but more uniform debris as shown in Fig. 5. It can be concluded that under the identical loading condition, with the decrease of specimen sizes the reduced debris becomes more and more uniform and presents the strain rate sensitivity of fractures as the strain rate increases with the specimen length decrease. Moreover, the 15 mm length specimen indicates a transition from the thermoplastic to brittle fractures as the specimens with the length of 15 mm or less than break with the brittle characteristic.
3 Discussion and Conclusion The transition of fracture modes involves the size changes of both length and transverse diameter, but aspect ratio representing the geometric property of specimen is unable to show the correlation with the fracture modes. Under the identical loading condition, the impulsive energy applying to any given specimen is constant. With the reduction of sizes, specimen volume decreases synchronously and the impulsive energy accumulates the energy much more than the required for breaking the specimen. Impulsive energy appears to be the dominant factor to determine the fracture modes. In the performed SHPB experiments, the identical impulsive energy is applied to the specimens consistently. With the decrease of specimen volume, the impulsive energy exceeds the required fracture energy more and more. The exceeding impulsive energy breaks specimen in a much shorter time and brings the specimen a high deformation
Characterization of Dynamic Fractures
13
strain rate to result in the more uniform fracture. In the case of the fracture, the specimen does not have the time to perform thermoplastic deformation. For the PMMA specimens, the 15 mm one presents the initiation of brittle fracture indicating that the impulsive energy is the critical one to change thermoplastic fracture into brittle one. Under the impulsive energy, the other small size specimens are all broken in brittle fracture regardless of the effect of aspect ratios and with the decrease of specimen volumes, the fracture becomes more uniform with smaller debris. Therefore, impulsive energy is the dominant factor to determine the fracture modes of brittle material.
References 1. Huang, C.: A further exploration on loading strain rate In: Gdoutos, E. (eds.) Structural Integrity, Proceedings of the First International Conference on Theoretical, Applied and Experimental Mechanics, ICTAEM 2018, vol 5, pp. 161–163. Springer, Cham (2018) 2. Wang, Z.G., Meyer, L.W.: On the plastic wave propagation along the specimen length in SHPB test. Exp. Mech. 50(7), 1061–1074 (2010) 3. Rittel, D., Brill, A.: Dynamic flow and failure of conﬁned polymethylmethacrylate. J. Mech. Phys. Solids 56(4), 1401–1416 (2008)
Tensile Behavior of a Titanium Alloy Additively Manufactured via Selective Electron Beam Melting Yinling Zhang1,2, Shoujiang Qu1, Aihan Feng1(&), and Daolun Chen2(&) 1
2
School of Materials Science and Engineering, Tongji University, Shanghai 201804, China [email protected] Department of Mechanical and Industrial Engineering, Ryerson University, Toronto, ON M5B 2K3, Canada [email protected]
Abstract. Additive manufacturing or 3Dprinting of titanium alloys with a high strengthtoweight ratio holds signiﬁcant interest in the aerospace and biomedical industries. The purpose of this investigation was to determine microstructure and tensile deformation behavior of a 3Dprinted Ti6Al4V alloy via selective electron beam melting (SEBM). Plentiful multioriented alamellae were present in the prior columnar b grains, which were oriented in the building direction because of the presence of temperature gradients during 3Dprinting. The processing parameters selected in this study ensured superior strength and high ductility by controlling the thickness of alamellae, with both surpassing the values speciﬁed in the ASTM standard. The horizontally orientated 3Dprinted alloy demonstrated a certain extent of strain rate sensitivity which decreased with increasing strain, suggesting that dislocation slip was a predominant deformation mode, since the ﬁne and abundant multioriented alamellae could impede the formation of extension twinning. Fracture surface was observed to be characterized by typical dimples and some entrapped gas pores. Keywords: Selective electron beam melting properties
Ti6Al4V alloy Tensile
1 Introduction Ti6Al4V alloy has been widely applied to various aircraft components and biomedical industry due to their low density, high strength and excellent fracture toughness [1]. However, the geometrical sophistication of many parts is often difﬁcult to access for the traditional subtractive manufacturing methods along with the inferior machinability of titanium alloys [2]. Recently, additive manufacturing (AM), also known as 3D printing, has become an increasingly popular manufacturing process technique providing a great degree of design freedom and a huge potential for manufacturing optimized and customized components with complicated shapes ideally [3]. Selective electron beam melting © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 14–19, 2020. https://doi.org/10.1007/9783030478834_3
Tensile Behavior of a Titanium Alloy Additively Manufactured via SEBM
15
(SEBM) is one of the most popular AM processes due to the advantages such as the vacuum working environment to avoid impurity elements and relatively slow cooling rate to reduce the processinduced residual stresses [4]. However, studies on the deformation behavior of SEBMmanufactured Ti6Al4V alloy are still very limited. Hence, further research is necessary and urgent to evaluate the deformation characteristics of such a 3Dprinted titanium alloy, so as to warrant its safe and durable applications in the aerospace and medical industry.
2 Materials and Experimental Procedure 2.1
Additive Manufacturing Processing
Samples fabricated with prealloyed Ti6Al4V powders, with a chemical composition (wt%) of 6.40 Al, 4.12 V and balance Ti, were processed using SEBM in a vacuum atmosphere. The size of powders used had a size distribution from 45 to 105 µm which meet the speciﬁed requirement (45–150 µm). The samples were additively manufactured (or 3Dprinted) using an Arcam Q20 system, which was operated at a beam current of 35 mA, a layer thickness of 0.09 mm with a scan speed function of 24 and a line offset of 0.22 mm. The electron beam scanning was set to rotate at an angle of 66° for each layer to improve the bonding between layers with a more uniform distribution of heat combined with a lessened residual stress. The horizontally positioned cylinders with a size of Ф15 170 mm were ﬁrstly 3Dprinted, as shown in Fig. 1. Those cylinders were ﬁnally machined and polished into tensile specimens with a gauge length of Ф6 32 in the end.
Fig. 1. Schematic diagram of SEBM building strategy and sample positioning.
2.2
Experimental Procedure
Optical microscope (OM) and electron backscatter diffraction (EBSD) were used to analyze the oriented microstructure with an observational surface parallel to the building direction. The sample for the EBSD analysis was prepared ﬁrst by mechanical grinding, followed by electropolishing in an electrolyte containing 6% perchloric acid, 34% nbutanol and 60% methanol at 0.8 A and 253 K for *70 s. Uniaxial tensile tests
16
Y. Zhang et al.
were carried out under strain control at ambient temperature at varying strain rates from 1 10−4 s−1 to 1 10−2 s−1. Two samples were tested at a given strain rate to determine the yield strength (YS), ultimate tensile strength (UTS) and ductility (%EL). The fracture surfaces were examined using a scanning electron microscope (SEM).
3 Results and Discussion 3.1
Phase Constitution and Microstructure
Figure 2(a) shows the macrostructure of a SEBMprocessed Ti6Al4V alloy. As seen from the observational surface, columnar grains were basically oriented vertically along the building direction with elongated shapes, which had a morphology of priorb grains present above the transus temperature of *950 °C. It is obvious that the highlyoriented columnar morphology was created by the presence of high temperature gradients in the fast heating and cooling process of 3D printing. Almost the entire hightemperature priorb phase with a bodycentered cubic (bcc) crystal structure would unavoidably transform into a phase with a hexagonal closepacked (hcp) crystal structure during the subsequent cooling process (below the transus temperature). Besides, several pores could also be observed, which was due to the trapped gas in the powder bed during 3D printing. Figure 2(b) shows the EBSD result of inverse pole ﬁgure (IPF) orientation map. The black and white lines represent the highangle (with a misorientation angle of >15°) grain boundaries and the lowangle boundaries (with a misorientation angle inbetween 2° to 15°), respectively. The microstructure was characterized by plentiful multioriented alamellae which were generated following the Burgers orientation relationship (i.e., {110}b//(0001)a and b//a) during the solidstate phase transformation of titanium alloy [5]. Due to the crystal symmetry, up to six different a variants are possible to be present in each priorb grain [6].
Fig. 2. (a) Optical micrograph and (b) EBSD IPF orientation map of SEBMmanufactured Ti6Al4V alloy.
Tensile Behavior of a Titanium Alloy Additively Manufactured via SEBM
3.2
17
Tensile Properties
Typical tensile engineering stressstrain curves of the horizontally orientated SEBMmanufactured Ti6Al4V samples at varying strain rates are presented in Fig. 3(a). It can be seen that the stressstrain curves shifted higher as strain rate increased. The average value of the YS and UTS of the present SEBMmanufactured Ti6Al4V alloy determined at different strain rates is shown in Table 1. The obtained YS (870– 961 MPa) and UTS (957–998 MPa) are 5–16% and 7–12%, respectively, higher than the YS (825 MPa) and UTS (895 MPa) speciﬁed in the ASTM F2924 standard for the additive manufactured Ti6Al4V alloy with powder bed fusion. The obtained ductility of *13% is also higher than the speciﬁed value (6–10%) in this ASTM standard. The hardening capacity (Hc) of a material proposed by Afrin et al. [7] can be expressed as follows, Hc ¼ rUTS ry =ry
ð1Þ
where rUTS and ry represent the UTS and YS, respectively. The hardening capacity values obtained at different strain rates are also tabulated in Table 1, with an average value of *0.07. Strain hardening exponent (n) can also be used to describe the plastic deformation characteristics of a material, which could be evaluated via the following Hollomon equation [8], r ¼ Ken
ð2Þ
where r is true stress, e is true strain, and K is strength coefﬁcient. The experimental data of r and e in the uniform deformation stage from the yield point to the ultimate tensile point are chosen to evaluate the strain hardening exponent. The value of n in the present 3Dprinted alloy increased slightly with decreasing strain rate with an average of *0.06. This is in agreement with that of traditional Ti6Al4V ELI alloy with a n value of from *0.045 to *0.08 over a wide range of strain rates from 1 10−2 s−1 to 1 10−5 s−1. Strainrate sensitivity (SRS) is another important parameter reflecting the deformation behavior of materials. The effect of strain rate on the flow stress of the SEBMmanufactured Ti6Al4V alloy can be described using a power law [9], r ¼ C_em
ð3Þ
where r is flow stress, C is a constant and m is the SRS. A plot based on Eq. (3) at certain true strain values is shown in Fig. 3(b). It can be observed that the m value or the slope in Fig. 3(b) decreased as the true strain increased. It is known that the samples which were prone to extension twinning exhibited an increasing trend of SRS with increasing strain, whereas an opposite trend in the SRS was reported when twinning was not a favorable mode of deformation [10]. This suggests that the slip of dislocations was a predominant mode of deformation, rather than extension twinning in the present 3Dprinted Ti6Al4V alloy. It is likely as a result of the presence of ﬁne and abundant multioriented alamellae (Fig. 2(b)), which impede the formation of extension twinning.
18
Y. Zhang et al.
Table 1. Tensile properties of the horizontal SEBMmanufactured Ti6Al4V alloy determined at different strain rates at room temperature. Strain rate, s−1 1 10−2 1 10−3 1 10−4
ry, MPa 961 914 870
rUTS, MPa Elongation, % Hc N 998 14 0.04 0.04 971 15 0.06 0.06 957 11 0.1 0.08
Fig. 3. (a) Typical engineering stressstrain curves of the present SEBMmanufactured horizontal orientated Ti6Al4V alloy obtained at three strain rates; (b) strainrate sensitivity as a function of true strain.
3.3
Fractography
Figure 4 shows a typical example of the fracture surface of the present SEBMmanufactured Ti6Al4V alloy tested at a strain rate of 1 10−4 s−1. It can be observed that the fracture morphology of this alloy appeared pretty ductile, characterized by the presence of abundant dimples. In addition, a few circular pores also exist on the fracture surface, which appeared during the processing of 3Dprinting.
Fig. 4. A typical SEM image of the fracture surface of the present SEBMmanufactured horizontal orientated Ti6Al4V alloy tested at a strain rate of 1 10−4 s−1.
Tensile Behavior of a Titanium Alloy Additively Manufactured via SEBM
19
4 Conclusions Microstructure and tensile behavior of a horizontally oriented SEBMmanufactured Ti6Al4V alloy were evaluated. The following conclusions can be drawn: (1) The microstructure of asbuilt SEBM samples was observed to consist of predominantly oriented alamellar phase positioned inside the prior columnar b grains along the building direction. (2) The processing parameters selected in this study were suitable, leading to a superior strength coupled with high ductility of the present 3Dprinted alloy, with both values exceeding the speciﬁed strength and ductility in the relevant ASTM standard. The alloy demonstrated a certain extent of strain rate sensitivity which decreased with increasing strain. (3) Fracture surface examination showed a ductile mode of fracture in the tensile tested specimens, as characterized by abundant dimples and some entrapped gas pores. Acknowledgements. The authors are grateful for the ﬁnancial support provided by the National Natural Science Foundation of China (NSFC) (Grant No. 51871168) and the Natural Sciences and Engineering Research Council of Canada (NSERC) in the form of international research collaboration. The authors appreciated Q. L, A. M, J. A and R. C for kind assistances.
References 1. Cui, C., Hu, B.M., Zhao, L., Liu, S.: Titanium alloy production technology, market prospects and industry development. Mater. Des. 32(3), 1684–1691 (2011) 2. de Formanoir, C., Brulard, A., Vivès, S., Martin, G., Prima, F., Michotte, S., Rivière, E., Dolimont, A., Godet, S.: A strategy to improve the workhardening behavior of Ti6Al4V parts produced by additive manufacturing. Mater. Res. Lett. 5(3), 201–208 (2017) 3. Lavine, M.S.: Fast, continuous, 3D printing. Science 347(6228), 1325 (2015) 4. Galarraga, H., Lados, D.A., Dehoff, R.R., Kirka, M.M., Nandwana, P.: Effects of the microstructure and porosity on properties of Ti6Al4V ELI alloy fabricated by electron beam melting (EBM). Addit. Manuf. 10, 47–57 (2016) 5. Tan, X., Kok, Y., Tan, Y.J., Descoins, M., Mangelinck, D., Tor, S.B., Leong, K.F., Chua, C. K.: Graded microstructure and mechanical properties of additive manufactured Ti6Al4V via electron beam melting. Acta Mater. 97, 1–16 (2015) 6. Beladi, H., Chao, Q., Rohrer, G.S.: Variant selection and intervariant crystallographic planes distribution in martensite in a Ti6Al4V alloy. Acta Mater. 80, 478–489 (2014) 7. Afrin, N., Chen, D.L., Cao, X., Jahazi, M.: Strain hardening behavior of a friction stir welded magnesium alloy. Scr. Mater. 57, 1004–1007 (2007) 8. Hollomon, J.H.: Tensile deformation. Trans. AIME 162, 268–290 (1945) 9. Lin, X.Z., Chen, D.L.: Strain hardening and strainrate sensitivity of an extruded magnesium alloy. J. Mater. Eng. Perform. 17, 894–901 (2008) 10. Chun, Y.B., Davies, C.H.J.: Twinninginduced negative strain rate sensitivity in wrought Mg alloy AZ31. Mater. Sci. Eng. A 523, 5713–5722 (2011)
The Rule of Mixtures on the Elastic Buckling Response of Rectangular GLARE FML Plates Under Shear Stresses Costas D. Kalfountzos(&), George S. E. Bikakis, and Efstathios E. Theotokoglou Department of Mechanics, Laboratory of Strength of Materials, National Technical University of Athens, 9 Iroon Polytechniou, 15773 Zografou, Athens, Greece [email protected]
Abstract. Fiber Metal Laminates (FMLs) are hybrid composite materials consisting of alternating metal layers bonded to ﬁberreinforced prepreg layers. ARALL, CARALL and GLARE belong to this new family of materials. GLARE is the most successful FML up to now and is currently being used for the construction of primary aerospace structures. In this study, the elastic buckling response of rectangular GLARE FMLs subjected to shearing stresses is investigated using the ﬁnite element method and eigenvalue buckling analysis. Simply supported, clamped and mixed boundary conditions are considered. Using validated FEM models, the buckling coefﬁcientaspect ratio diagrams of seven GLARE grades are obtained along with the diagrams of three UD glassepoxy composites and monolithic 2024T3 aluminum. The rule of mixtures is evaluated and found to be a simple method to estimate approximately the elastic buckling stress of the GLARE plates. An approximate formula is derived for the estimation of the critical buckling coefﬁcient of the GLARE plates using the buckling coefﬁcients of their constituents. Keywords: Elastic buckling
Fibermetal laminates Rule of mixtures
1 Introduction Fiber Metal Laminates (FMLs) are hybrid composite materials consisting of alternating metallayers bonded to ﬁberreinforced preimpregnated (prepreg) layers. These materials are developed to fulﬁll the desire of aircraft manufacturers and airliners for reduction of direct operational costs and structural weight of aircrafts [1]. ARALL (Aramid Reinforced ALuminum Laminates), CARALL (CArbon Reinforced ALuminum Laminates) and GLARE (GLAssREinforced) belong to this new family of materials. GLARE is the most successful FML up to now and is currently being used for the construction of aerospace structures, such as the fuselage of the Airbus A380 air plane, the aircraft cargo floors of Boeing 777, aircraft engine cowlings and aircraft stiffeners with a wide variety of shapes [2–4]. FMLs combine signiﬁcant advantages of metal and ﬁberreinforced composites. Because of the intact bridging of ﬁbers, in the © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 20–25, 2020. https://doi.org/10.1007/9783030478834_4
The Rule of Mixtures on the Elastic Buckling
21
wake of the crack, which restrain crack opening, FMLs demonstrate high fatigue resistance [5]. They also have high fracture toughness [6], excellent impact resistance [7], low density, excellent moisture, corrosion and ﬁre resistance [8, 9], which make them ideal for multipurpose aerospace applications. The elastic buckling of thin plates has great practical importance and it is a classical problem of the strength of materials. Plate buckling must always be considered during the design of many engineering applications where stiffened thinwalled structures are employed. For the purpose of buckling analysis, the wall plates among stiffeners could be analyzed approximately as isolated rectangular plates. FMLs are mainly used for the construction of stiffened thinwalled aerospace structures and, therefore, the buckling strength of FML plates is very important [10, 11]. This study deals with the elastic buckling of rectangular FML plates subjected to shearing stresses, the calculation of their buckling coefﬁcients and the construction of diagrams showing their variation as a function of the plate aspect ratio. More specifically, the main objective of this study is the investigation of applicability of the rule of mixtures for the calculation of the average critical buckling stress of the examined GLARE plates. Furthermore, an approximation formula to predict the buckling coefﬁcients of FMLs is derived using the rule of mixtures for the buckling stresses.
Fig. 1. Finite element mesh of a rectangular 600 200 mm plate (a/b = 3) along with the applied shear loading.
2 Problem Deﬁnition and Finite Element Modeling Procedure A thin rectangular plate is considered, under pure shear loading consisting of alternating layers of 2024T3 aluminum and unidirectional (UD) glassepoxy bonded to form FML. The plate has length a, width b a, as it is illustrated in Fig. 1 and a relatively small thickness t. Since the plate is subjected to pure shear loading (Fig. 1) and each opposite parallel edge is not allowed to move in the direction of Nxy, it will buckle for a speciﬁc critical value of the applied load Nxy. The elastic buckling load will be predicted using the ﬁnite element method. ANSYS software [12] is employed for
22
C. D. Kalfountzos et al.
this purpose along with eigenvalue buckling analysis. From the FEM results the shear buckling coefﬁcient k will be determined for variable aspect ratio a/b and (k, a/b) curves of plates consisting of different materials will be constructed. In order to apply the rule of mixtures, three different material systems are considered, namely FMLs and their constituents, UD composites and monolithic aluminum. Also, three types of bc are considered, namely simply supported, clamped and TSLC. For the FEM modeling we use plane rectangular 4noded SHELL 181 elements, which are suitable for modeling the thin layered plates studied in this article. Each SHELL element has three translational and three rotational degrees of freedom per node. The material behavior of 2024T3 aluminum and UD glassepoxy is idealized using linear elastic material models with isotropic and orthotropic mechanical properties, respectively. The convergence of the critical buckling load Nxy predicted from the eigenvalue buckling analysis is always veriﬁed by comparison of results corresponding to ﬁne and very ﬁne mesh density. Furthermore, the ply stress levels corresponding to the critical value of Nxy are always below the linear elastic limits. Speciﬁcally, the von Mises stresses in aluminum layers and the stress components in prepreg layers are well below the proportional limit of aluminum and the composite ply strengths, respectively. The shear buckling coefﬁcient of aluminum plates is calculated by [13]: k¼
Nxy b2 p2 D
ð1Þ
where D is the bending stiffness of the isotropic plate. The shear buckling coefﬁcient of the laminates is calculated by [14]: k¼
Nxy b2 p ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ p2 D11 D22
ð2Þ
where Dii(i = 1, 2) are the bending stiffnesses of the laminate. The average critical buckling stress is calculated with the relation: rxyc ¼
Nxy t
ð3Þ
In order to validate our FEM procedure and the suitability of the applied simply supported bc, we have initially compared the FEM results with corresponding theoretical results [13] for monolithic aluminum plates. A very good agreement between our FEM results and the literature predictions has been observed. As a result, the validity of the implemented FEM modeling and the applied bc for the simply supported aluminum plates is ensured. As expected, the clamping of the plates is modeled by imposing zero transverse rotations along their edges in addition to the applied simply supported bc. The TSLC bc along the edges of the plates have been applied as follows: the Transverse edges are Simply supported and the Longitudinal edges are Clamped. For the validation of our FEM modeling of GLARE and composite laminates, we have compared the obtained FEM results with appropriate literature results [14]. A very
The Rule of Mixtures on the Elastic Buckling
23
good agreement between our FEM results and the literature predictions has been also observed for the analyzed UD composite laminates and the specially orthotropic GLARE grades. Consequently, the FEM modeling of the GLARE and composite laminates is validated.
3 Rule of Mixtures versus FEM Results We have investigated the applicability of the classical rule of mixtures for the calculation of the average critical buckling stress rgxyc of seven different GLARE grades. In ref. [15] other applications of the rule of mixtures can be found. Speciﬁcally, the stress rgxyc is calculated using the formula: rgxyc ¼ rcxyc ð1 MVF Þ þ raxyc MVF
ð4Þ
Where rcxyc and raxyc are the average critical buckling stresses of composite and aluminum plates, respectively, with the same dimensions, and MVF is the metal volume fraction of each plate. The composite plates also have the same ﬁber orientation angles, ﬁber volume fraction and ply thickness with the composite plies of each GLARE plate. In Fig. 2 the stresses calculated using Eq. (4) are compared with the detailed FEM calculations for GLARE 3 and GLARE 5 respectively. A good agreement between the accurate and the rule of mixtures (rgxyc , a/b) curves is found.
60
2024T3 aluminum GLARE 33/20.458 FEM GLARE 33/20.458 rule of mixtures
50
GLARE 53/20.292 FEM GLARE 53/20.292 rule of mixtures
σxyc (MPa)
40
UD glassepoxy crossply
30 20 10 0 0
1
2
3
a/b
4
5
6
Fig. 2. FEM versus rule of mixtures average critical buckling stresses of simply supported GLARE plates with crossply ﬁber orientation under pure shear.
24
C. D. Kalfountzos et al.
Using Eqs. (1–3), the average critical buckling stresses of aluminum, composite and GLARE plates can be calculated as a function of their buckling coefﬁcient, and by substitution in Eq. (4) a very useful relation is obtained: rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ D11C D22C D ð1 MVF Þ þ kA pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ MVF kG ¼ kC D11G D22G D11G D22G
ð5Þ
where DiiC are the bending stiffnesses of the composite plate, DiiG are the bending stiffnesses of the GLARE plate, kC is the buckling coefﬁcient of the composite plate, and kA is the buckling coefﬁcient of the aluminum plate. Equation (5) can be used in order to estimate approximately the buckling coefﬁcient of a simply supported, clamped or TSLC GLARE plate when kC and kA are known. In Fig. 3 the buckling coefﬁcients calculated using Eq. (5) are compared with FEM calculations for GLARE 3 plates with clamped, simply supported and mixed bc. A good agreement between exact and Eq. (5) based (kG, a/b) curves is found. A good agreement has also been found for the other considered GLARE plates of this study. Consequently, the validity of Eq. (5) is demonstrated for the approximate calculation of kG.
16
clamped GLARE 33/20.458 FEM clamped GLARE 33/20.458 equation(5)
14
ss GLARE 33/20.458 FEM ss GLARE 33/20.458 equation (5)
12
TSLC GLARE 33/20.458 FEM TSLC GLARE 33/20.458 equation (5)
10 k 8 6 4 2 0
1
2
3 a/b
4
5
6
Fig. 3. Exact versus approximate buckling coefﬁcients of GLARE 3 plates under pure shear with clamped, simply supported (ss) and mixed (TSLC) bc.
4 Conclusions This article deals with the elastic buckling of rectangular simply supported, clamped and TSLC FMLs subjected to pure shear loading. ANSYS FEM software is employed in combination with the eigenvalue analysis in order to predict the buckling coefﬁcient of the laminates. The implemented ﬁnite element models have been validated by comparison with appropriate theoretical results concerning simply supported bc.
The Rule of Mixtures on the Elastic Buckling
25
It is found that the rule of mixtures can be applied in order to estimate approximately the critical buckling stresses of the GLARE plates when the buckling stresses of plates having the same geometry and consisting of one constituent material, aluminum or UD glassepoxy, are known. The same ﬁber orientation angles, ﬁber volume fraction and ply thickness with the composite plies of the GLARE plates are necessary in order to apply the rule of mixtures. Based on the veriﬁed validity of the rule of mixtures, an approximate formula is derived for the estimation of the buckling coefﬁcient of the GLARE plates when the buckling coefﬁcients of plates consisting of the constituent materials are known.
References 1. Verolme, K.: The initial buckling behavior of flat and curved ﬁber metal laminate panels. Report LR785, Delft University of Technology (1995) 2. Gunnink, J.W., Vlot, A., De Vries, T.J., et al.: Glare technology development 1997–2000. Appl. Compos. Mater. 9(4), 201–219 (2002) 3. Woerden, H.J.M., Sinke, J., Hooijmeijer, P.A.: Maintenance of glare structures and glare as riveted or bonded repair material. Appl. Compos. Mater. 10(4–5), 307–329 (2003) 4. Vermeeren, C.A.J.R.: An historic overview of the development of ﬁbre metal laminates. Appl. Compos. Mater. 10(4–5), 189–205 (2003) 5. Sinmazçelik, T., Avcu, E., Bora, M.O., Çoban, O.: A review: ﬁbre metal laminates, background, bonding types and applied test methods. Mater.Des. 32(7), 3671–3685 (2011) 6. Castrodeza, E.M., Bastian, F.L., Perez Ipiña, J.E.: Critical fracture toughness, JC and d5C, of unidirectional ﬁbre–metallaminates. ThinWalled Struct. 41(12), 1089–1101 (2003) 7. Bikakis, G.S.E.: Simulation of the dynamic response of GLARE plates subjected to low velocity impact using a linearized spring–mass model. Aerosp. Sci. Technol. 64, 24–30 (2017) 8. Vogelesang, L.B., Vlot, A.: Development of ﬁbre metal laminates for advanced aerospace structures. J. Mater. Process. Technol. 103(1), 1–5 (2000) 9. Botelho, E.C., Silva, R.A., Pardini, L.C., Rezende, M.C.: A review on the development and properties of continuous ﬁber/epoxy/aluminum hybrid composites for aircraft structures. Mat. Res. 9(3), 247–256 (2006) 10. Bikakis, S.E., Kalfountzos, C.D., Theotokoglou, E.E.: Elastic buckling response of rectangular GLARE ﬁbermetal laminates subjected to shearing stresses. Aerosp. Sci. Technol. 87, 110–118 (2019) 11. Kounadis, A.N., Sophianopoulos, D.S.: Nonlinear dynamic buckling of a cylindrical shell panel model. AIAA J. 34, 2421–2428 (1996) 12. ANSYS: Structural Analysis Guide. ANSYS Inc. (2014) 13. Timoshenko, S.P., Gere, J.M.: Theory of Elastic Stability. Mc Graw Hill, Stanford (1961) 14. Gay, D., Hoa, S.V., Tsai, S.W.: Composite Materials Design and Applications. CRC Press LLC, Boca Raton (2003) 15. Moriniere, F.D., Alderliesten, R.C., Sadighi, M., et al.: An integrated study on the low velocity impact response of the GLARE ﬁbremetal laminate. Comp. Struct. 100, 89–103 (2013)
Evaluating Bonding Characteristics of Joggled Lap CFRP Using Acoustic Emission Techniques Claudia Barile(&) , Caterina Casavola , Giovanni Pappalettera Carmine Pappalettere , and Paramsamy Kannan Vimalathithan
,
Dipartimento di Meccanica Matematica e Management, Politecnico di Bari, Viale Japgia 182, 70126 Bari, Italy [email protected] Abstract. In this study, the carbon ﬁber reinforced plastics (CFRP) specimens bonded adhesively in joggled lap conﬁguration are tested for their bonding characteristics. The acoustic emission (AE) technique is used as a characterizing tool and peak amplitude is taken as the primary acoustic descriptor. The peak amplitude distributed in the time domain of the test is clustered by using an unsupervised pattern recognition algorithm (kmeans++ algorithm) to differentiate the different damage modes. Furthermore, the waveforms of the acoustic signals recorded were studied using wavelet packet transform (WPT). The frequency band associated with each damage mode is identiﬁed using the wavelet packet transform. It is identiﬁed that the dominant damage mode responsible for failure is the interfacial debonding and interlaminar crack growth through the thickness of the adhesive layer. Overall, the acoustic emission technique proved to be a powerful tool in evaluating the bonding characteristics of the tested CFRP joggled lap specimens. Keywords: Acoustic emission CFRP Bonding Wavelet packet transform Pattern recognition
1 Introduction The Carbon Fiber Reinforced Plastics (CFRP) has extensively been used in aerospace structures, especially in crucial aerospace structures such as the structures joining lower spar of the fuselage and bulkhead, fuselage and halfwing, etc. Thus, designing and testing a proper joint structure at these crucial parts have become essential. Acoustic Emission (AE) technique remains a powerful tool in characterizing damage progression in CFRP structures. AE technique records the transient elastic waves developed due to the stressing of a material under loading [1]. The corresponding signals recorded by a transducer (e.g. PZT) are ﬁltered, preampliﬁed and stored for further analysis. Since these generated elastic waves are very sensitive even to the grain movement, microcracks or micromatrix cracking, they are very efﬁcient in analyzing the various features of the damage progression.
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 26–31, 2020. https://doi.org/10.1007/9783030478834_5
Evaluating Bonding Characteristics of Joggled Lap CFRP
27
2 Materials and Methods 2.1
Materials
CFRP laminates used in this study comprise highstrength stitched carbon ﬁbers reinforced in epoxy resin and cured by autoclave method. The average resin percentage in each laminate is 43% and the ply thickness is 0.244 mm. The adhesive used for bonding the upper and lower laminates has a shear and peel strength of 25 MPa and 65 MPa, respectively. The upper adherend consists of 8 plies with a thickness of 2 mm and the lower ply with 6 plies and 1.5 mm. The adhesive layer coated to join the upper and lower laminate has a length of 26 mm and a thickness of 3.67 mm. The adhesive was cured at a temperature of 100 °C to 150 °C for about 1 h. 2.2
Testing Methods
The testing was carried out as per ASTM D5868 standard at a crosshead displacement rate of 13 mm/min in 100 kN INSTRON servohydraulic machine. To record the acoustic activities during testing, two AE sensors, R30a with an operating frequency of 150 kHz to 450 kHz were fastened to the surface of the specimen. The sensors are placed exactly 40 mm from the middle of the specimens. The recorded AE signals are preampliﬁed by 40 dB through 2/4/6 AST preampliﬁer. The waveforms are recorded at a sampling rate of 1 MSPS. 2.3
Unsupervised Pattern Recognition Technique
In this research work, kmeans++ unsupervised pattern recognition algorithm is used to cluster the peak amplitude distribution for the entire load history. The kmeans++ works on the principle of selecting speciﬁc number of centroids; then it assigns the datapoints to each cluster based on the minimum distance between each datapoint and the centroid. Detailed step by step procedure of this technique can be found elsewhere [2]. The peak amplitudes recorded during the testing of all three specimens were classiﬁed into three clusters. 2.4
Wavelet Packet Transform
Wavelet Packet Transform (WPT) decomposes the recorded waveform into low and highfrequency components, approximation and detail, respectively, while retaining the orthogonality, smoothness and the localization properties of the parent wavelet. A desired level of decomposition (i) can be assigned to the WPT technique and the total number of WPT components are 2i. The frequency content of the WPT and the decomposition are carried out in Wavelet Toolbox in MATLAB [3]. The decomposition level for this study is set at i = 3.
28
C. Barile et al.
3 Results and Discussions 3.1
Mechanical Test Results
The mechanical test results are presented in Table 1. All the specimens have suffered damage in two different stages and accordingly, the peak loads at those junctures are termed as peak load at initial rupture and ﬁnal rupture. The mechanical results of all three specimens having same material and geometric conﬁgurations show different peaks loads at initial and ﬁnal rupture. JLS 1 specimen signiﬁcantly has carried more load before its initial rupture than JLS 2 and JLS 3 specimens. JLS 2, in particular, has a very poor strength both at the initial and ﬁnal rupture. The differences in these peak loads, despite their similar design conﬁguration is because these three specimens have two adherends each, bonded together using a highstrength adhesive manually. The application of the adhesive, its surface area, thickness, curing conditions could differ between the three specimens. This is the reason why the three specimens have different peak loads at rupture. Table 1. Mechanical properties of specimens. Specimen Peak load (kN) Initial rupture Final rupture JLS 1 6.02 4.09 JLS 2 2.67 3.89 JLS 3 3.86 5.57 Mean 4.18 4.52 Std. Dev. 1.70 0.92
3.2
Acoustic Emission Test Results
The peak amplitudes recorded during the test are clustered using kmeans++ unsupervised pattern recognition technique and are presented in Fig. 1. The peak amplitude for all three JLS specimens, clustered into 3 groups, is presented and discussed. The clustered peak amplitude data shows clearly the differences in damage progressions between the three specimens. In JLS 1 specimen, there is very few events in cluster 1 (higher amplitude cluster) during the initial stages of loading. The peak amplitude accumulates in cluster 1 only at the end of the test around 1.8 s. Similarly, there are very few events in cluster 2 as well until 0.9 s duration. This clearly indicates that no major damage occurred in the specimen until the material reaches 0.9 s. The amplitudes in cluster 3 indicate low amplitude signals, which normally represent microcracking, which is the only major damage mode in JLS 1, until 0.9 s. This occurrence can be connected with the fact that JLS1 shows higher strength compared with JLS 2 and JLS 3.
Evaluating Bonding Characteristics of Joggled Lap CFRP
29
Fig. 1. Peak amplitude clustered by kmeans++ algorithm for JLS 1, 2 and 3
Looking at JLS 2, amplitude commenced to accumulate in cluster 1 and 2 at a very early stages, indicating major damages in the specimen at a very early stages of loading. This is the reason for the poor peak load even at the initial rupture. JLS 3, having intermediate strength between JLS 1 and 2 has very few points in cluster 1 at the initial stages of loading. However, events in cluster 2 can be found as early as 0.35 s duration. Thus, major damage as in JLS 2 did not occur in JLS 3 specimens at an early stage, nonetheless, the material suffered signiﬁcant damage. Thus, the clustered peak amplitude data of the AE clearly differentiate the damage modes among the three specimens. 3.3
Wavelet Packet Transform Results
Different damage modes in a CFRP emit acoustic signals in different frequency spectra. In that regard, three wavelets each from JLS 1, 2 and 3 specimens were taken for the WPT analysis. One wavelet in each cluster of the three specimens has been taken randomly for the analysis. Under loading, an adhesively bonded CFRP transfers the load entirely through the adhesive region. The thickness of the adherend does not affect the load in a displacementcontrolled condition [4]. Thus, the ﬁber breakage or ﬁber pullout is not
30
C. Barile et al.
expected in the fractured specimens. This can be proved evidently also by the WPT results. In the ﬁrst WPT results of JLS 1 specimens (Fig. 2(a)), the signal has a very low energy and is centered around 200 kHz and 300 kHz frequency bands. However, in the second and third wavelet, it is centered around 300 kHz and 375 kHz (Fig. 2(b) and (c)). Particularly in the third wavelet, the frequency band remains the same, but it is shifted to the right in time domain (Fig. 2(c)).
Fig. 2. WPT results of JLS 1, 2 and 3 specimens
In the WPT results of specimen JLS 2, the ﬁrst wavelet (Fig. 2(d)) has high energy and the frequency band is at 200 kHz to 300 kHz. Unlike Fig. 2(a), this wavelet has higher energy in that region, while comparing the density of the wavelet. In Fig. 2(e), the frequency band has a low energy and is centered around 250 kHz and 375 kHz. The last wavelet is entirely different from the others with two distinct frequency spectrum the time domain (Fig. 2(f)). The ﬁrst spectrum is at 450 kHz to 500 kHz frequency and the second is shifted in the time domain to the right at 250 kHz and 375 kHz. The WPT results of JLS 3 specimens are all centered at 250 kHz to 375 kHz, the only difference is being the shift in the time domain (Fig. 2(g), (h) and (i)). The frequency band between 200 kHz and 300 kHz represents the interfacial debonding. Th frequency band 250 kHz to 375 kHz is mostly misinterpreted as ﬁber
Evaluating Bonding Characteristics of Joggled Lap CFRP
31
breakage. However, recent studies prove that these bands could represent the interlaminar crack growth [5]. JLS 1 suffered a very slight interfacial debonding under the loading and most of the damage suffered is due to the high frequency signals (250 kHz to 375 kHz). This is why the energy of the 200 kHz to 300 kHz signal in Fig. 2(a) is very low. However, the specimen JLS 2 suffered severe damage at a very early stage. This is indicated by the Fig. 2(d) where the energy is high for the 200 kHz to 300 kHz signal. This means that the specimen suffered the interfacial debonding at a very early stage and failed to carry enough load before rupture. This is the reason why it has higher energies in the frequency bands representing debonding and lower energies in the other frequency domains. In all the specimens, most of the signals are centered around the frequency band of 250 kHz to 375 kHz. This signiﬁes that the load was carried through the adhesive layer and the interfacial crack growth in the adhesive area are responsible for most of the acoustic activities. Thus, it is safe to conclude that the major damage modes in JLS specimens are interfacial debonding and crack growth.
4 Conclusions The Joggled Lap Shear specimens are tested under tensile loading. The damage characteristics are studied using AE technique. The kmeans++ clustering technique is used to cluster the peak amplitude data of AE to differentiate the damage modes in the specimens. A wavelet from each cluster was taken for WPT analysis to identify the major damage modes in the specimens. The frequency bands indicate that the major damage modes are interfacial debonding and crack growth. The AE proves to be a powerful tool in characterizing the damage modes in the CFRP specimens.
References 1. Grosse, C.: Acoustic Emission Testing, 1st edn. Springer, Heidelberg (2008) 2. Roundi, W., El Mahi, A., El Gharad, A., Rebiere, J.: Acoustic emission monitoring of damage progression in glass/epoxy composites during static and fatigue tensile tests. Appl. Acoust. 132, 124–134 (2018) 3. Barile, C., Casavola, C., Pappalettera, G., Vimalathithan, P.K.: Damage characterization in composite materials using acoustic emission signalbased and parameterbased data. Compos. B 178, 107469 (2019) 4. Barile, C., Casavola, C., Pappalettera, G., Vimalathithan, P.K.: Characterization of adhesive bonded CFRP laminates using fullﬁeld digital image stereocorrelation and ﬁnite element analysis. Compos. Sci. Technol. 169, 16–25 (2019) 5. Oz, F.E., Ersoy, N., Lomov, S.V.: Do high frequency acoustic emission events always represent ﬁbre failure in CFRP laminates? Compos. A 103, 230–235 (2017)
Experimental Study of Low Concentration Diffusible Hydrogen Effect on Mechanical Behaviour of Carbon Steel I. M. Dmytrakh(&), R. L. Leshchak, and A. M. Syrotyuk Karpenko PhysicoMechanical Institute of NASU, 5 Naukova Street, Lviv 79060, Ukraine [email protected]
Abstract. The presented work is dedicated to the evaluation of the mechanical behaviour of the ferritepearlite carbon steel under a low concentration of diffusible hydrogen in the bulk of the metal. Received standard stressstrain diagrams under different hydrogen concentration CH in the specimens have shown on the existence of some speciﬁc value of the hydrogen concentration CH at which the mechanism of hydrogen influence changes, namely: below this value the enhanced plasticity (decreasing of the yield stress) takes places and above – the hydrogen embrittlement occurs. This phenomenon was explained based on the special tests of tensile specimens, which were preliminary charged by hydrogen to concentration CH and then discharged to the concentration CH 0. It has been found that increasing the number of cycles of chargingdischarging leads to decreasing the value of yield stress. Thus, even a shortterm presence of the hydrogen in the material leads to irreversible changes in the structure of the material, namely: the appearance of defects at the microlevel. This facilitates the deforming ability of steel and reduces the value of the plasticity limit. Keywords: Carbon steel
Hydrogen concentration Enhanced plasticity
1 Introduction Nowadays, this is an indisputable fact that hydrogen can demonstrate various effects on the mechanical properties of structural metallic materials. Although, there is no complete understanding of these effects and the concepts and approaches to the solution of the most important problems of hydrogen materials science are quite contradictory [1]. Furthermore, prevail numbers of investigations in this ﬁeld have a substantial disadvantage: the true level of hydrogen concentration in the metal was unknown and, hence, the degree of its hydrogenation is taken into account indirectly. However, the volume concentration of hydrogen in the metal and its local concentration in the zones of high mechanical stresses are the critical parameters that deﬁne the strength and fracture resistance of materials in given conditions [2, 3]. The presented work removes this disadvantage because the tests were carried out under the known values of the volume concentration of hydrogen in the specimens. The study is dedicated to the evaluation of the mechanical behaviour of the ferritepearlitic © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 32–37, 2020. https://doi.org/10.1007/9783030478834_6
Experimental Study of Low Concentration Diffusible Hydrogen Effect
33
carbon steel under a low concentration of diffusible hydrogen in the bulk of the metal. Here, received dependencies were analyzed as the functions of hydrogen concentration.
2 Experimental Procedure The object of study was low alloyed pipeline steel (rY = 260 MPa and rU = 440 MPa) with nominal chemical composition (in weight %): C = 0.17–0.24; Si = 0.17–0.37; Mn = 0.35–0.65; S < 0.04; remainder Fe. This material consists of grains of ferritepearlite, typical for all steel of this class. The standard cylindrical tensile specimens with a diameter of 5 mm were manufactured from the real pipe. The hydrogen charging of the specimens was made by the electrochemical method under cathodic polarisation at some constant potential Ecath ¼ const:. With the aim to simulate the hydrogen entry at real operating conditions of the buried pipeline, the following procedure has been applied [4]. The special deoxygenated, nearneutral pH NS4 solution, which is the model of underground water, was chosen as the electrolyte for hydrogen charging of steel. The chemical composition of the NS4 solution is given in Table 1. Taking into account the situation of a freely corroding system that exists for the real pipeline, the potential of polarisation Ecath was slightly more negative than the free corrosion potential Ecorr for given steel. Table 1. Chemical composition of NS4 solution (gram/litre). NaHCO3 KCl CaCl2 MgCl2.H2O 0.483 0.120 0.137 0.131
The hydrogen concentration in bulk of steel has been determined on the base of the hydrogen discharging process under anodic polarisation with using modiﬁed hydrogen electrochemical oxidation method proposed [4, 5]. For the realisation of experimental studies on the hydrogen charging of specimens and determination of the hydrogen concentration in bulk of steel, the special testing stand was developed [6]. This facility is based on the dynamic electrochemical laboratory VoltaLab40 (Radiometer Analytical). As the preliminary stage of the study the experimental dependence “hydrogen concentration CH in specimen – time of exposure s” was received. These experimental data were described by power relation: CH ¼ 0:128 A 106 sm ½ppm;
ð1Þ
where A and m are some constants that depend on system “material – environment” and testing conditions. Based on the formula (1) the specimens were hydrogen charged to the assigned level of CH, before testing.
34
I. M. Dmytrakh et al.
3 Results and Discussion Based on the received experimental curves ‘applied load – elongation of specimen’, the dependencies ‘stress r – strain e’ were constructed for different values of the hydrogen concentration CH in the specimens. Here it should be noted that calculation of stresses r was made with taking into account the real values of crosssection area of specimens, i.e. socalled ‘true’ stressstrain diagrams of were received. These diagrams served as the basis for the determination of the true values of the yield stress rY as the function of the hydrogen concentrations CH (Fig. 1).
σY, MPa
350
300
250 CH = 0,227 ppm 200 0
0.2
0.4
0.6
0.8 CH,1ppm
Fig. 1. Dependence of the yield stress rY on the volume concentration of hydrogen CH in the specimens.
As can be seen in Fig. 1, under increasing of the hydrogen concentration in metal, the decreasing of the yield stress value rY was observed up to CH ﬃ 0:227 ppm. This shows the facilitation of a plastic deforming of steel under a given range of CH in the specimens. After exceeding the value CH ﬃ 0:227 ppm, the increase of the yield stress values rY occurs that points to the decrease of plastic deformation under the tensile loading of specimens. After the tensile test, the fracture surfaces of specimens were examined by the scanning electronic microscopy. The following speciﬁc features of the carbon steel fracture on the dependence of the hydrogen concentrations CH in bulk of material were observed. For nonhydrogenated specimens (CH ¼ 0) fracture surface has the signs of the mixed mechanism of failure. Here, along with ‘dimple’ relief that showed on the ductile mechanism of fracture, the relief of typical quasicleavage brittle fracture can be found. With increasing of the hydrogen concentrations CH in material, the increasing of the dimples density and disappearing of quasicleavage elements were found. It points to the increase of the plastic deformation under the fracture process of steel. Such a picture was observed up to the value of hydrogen concentration equal CH ﬃ 0:227 ppm. After that, the further increase of the hydrogen concentration in specimen leads to the appearance of some trace of quasicleavage relief on the fracture surface, i.e. the fracture mechanism of steel becomes gradually mixed again. These data give the basis for the following statement. For this carbon steel, there is some characteristic value of the hydrogen concentration CH ¼ CH ﬃ 0:227 ppm in
Experimental Study of Low Concentration Diffusible Hydrogen Effect
35
bulk of material under which the mechanism of hydrogen influences changes, namely: the strengthening (hydrogen embrittlement) occurs at CH CH and the enhanced plasticity (decreasing of the yield stress value) takes places at CH CH . For a possible explanation of such phenomenon, a special series of the tests were conducted. Before the tensile test, the specimens were preliminary hydrogen charged to the level CH ¼ CH and then fully hydrogen discharged (CH 0). This procedure was repeated to obtain the specimens with the different number of cycles of hydrogen chargingdischarging NH , namely: 0, 2 and 5. Such specimens were tested under tensile loading and the nominal and true stressstrain diagrams were constructed for the specimens with the different values of NH (Fig. 2). It can be seen that the deformation e, which corresponds to the fracture of the specimen, increases with increasing of NH . This fact indicates the facilitation of material deforming depending on the value of the parameter NH . 1000
σ, MPa
800
NH=0
2
5
True diagrams
600
400
200
0 0,00
5
Nominal diagrams
0,10
0,20
NH=0
0,30
2
ε
Fig. 2. Nominal and true stressstrain diagrams for specimens with the different number of cycles of hydrogen chargingdischarging NH.
The stressstrain diagrams (Fig. 2) served as a base for determining the yield stress values rY as the function of the parameter NH (Fig. 3). These results show the monotonic decrease of a yield stress value rY with increasing the chargingdischarging cycles NH . Here, it also may be pointed out on the full coincidence between the data received under conditions of the hydrogen chargingdischarging of the specimens and the case of presence of the hydrogen in the specimens (Fig. 1). Thus, it can be suggested that even a shortterm presence of the hydrogen in the steel leads to the irreversible changes in the material structure that causes the changes in the mechanical behaviour of the material. The fractographs of the specimens tested after the different number of cycles of hydrogen chargingdischarging NH showed (Fig. 4) the appearance of defects at the microstructural level. At that, the defectiveness of material increases with increasing of the number of hydrogen chargingdischarging cycles NH (Fig. 5). This facilitates the deforming ability of steel and reduces the value of the plasticity limit.
36
I. M. Dmytrakh et al. 300
σY, MPa
250
200
150 0
1
2
3
4
5
6
NH, cycles
Fig. 3. Dependence of the true values of yield stress rY on the number of cycles of hydrogen chargingdischarging NH. The solid triangle refers to the data presented in Fig. 1.
60
250
50
200
2
40
S, μm
Number of defects
Fig. 4. Fractographs of the specimens tested after the different number of cycles of hydrogen chargingdischarging NH: a – 0; b – 2; c – 5 (x 500). The area of observation was equal to 41300 lm2.
30
150 100
20 50
10
b)
a)
0
0 0
1
2
3 4 NH, cycles
5
6
0
1
2
3
4
5
6
NH, cycles
Fig. 5. Number defects (a) and their total square (b) in steel after the tensile test as the function of the number of cycles of hydrogen chargingdischarging NH. The area of observation was equal to 41300 lm2.
Experimental Study of Low Concentration Diffusible Hydrogen Effect
37
If it may be assumed that the defectiveness of material is strongly related to the dislocations activity, then the received tendencies can be explained by the interaction between hydrogen and dislocations [7]. The hydrogen affects on the dislocations in two ways: promotes their pinning (or dragging) or enhances of their mobility. Competition between these two roles deﬁnes whether the resulting phenomenon is positive or negative with the point of view of the fracture resistance of the material.
4 Conclusions The fact of the yield stress reduction of carbon steel under the presence of the diffusible hydrogen of low concentration has been found. Hydrogenation and dehydrogenation of the steel do not pass without a trace concerning its microstructure. Even a shortterm presence of the diffusible hydrogen of low concentration in the steel leads to the irreversible changes in the material structure that causes the changes in the mechanical behaviour of the material. The obtained results may be useful under the development of technologies for processing steels of this class for the optimization of their service characteristics.
References 1. Somerday, B., Sofronis, P.: HydrogenMaterials Interaction. ASME Press, New York (2014) 2. Capelle, J., Dmytrakh, I., Gilgert, J., Pluvinage, G.: The effect of hydrogen concentration on fracture of pipeline steels in presence of a notch. Eng. Fract. Mech. 78, 364–373 (2011) 3. Dmytrakh, I.M., Smiyan, O.D., Syrotyuk, A.M., Bilyy, O.L.: Relationship between fatigue crack growth behaviour and local hydrogen concentration near crack tip in pipeline steel. Int. J. Fatigue 50, 26–32 (2013) 4. Capelle, J., Dmytrakh, I., Pluvinage, G.: Comparative assessment of electrochemical hydrogen absorption by pipeline steels with different strength. Corros. Sci. 52, 1554–1559 (2010) 5. Capelle, J., Dmytrakh, I., Gilgert, J., Pluvinage, G.: Sensitivity of pipelines with steel API X52 to hydrogen embrittlement. Int. J. Hydrogen Energy 33, 7630–7641 (2008) 6. Dmytrakh, I.M., Leshchak, R.L., Syrotyuk, A.M.: Effect of hydrogen concentration on strain behaviour of pipeline steel. Int. J. Hydrogen Energy 40, 4011–4018 (2015) 7. Murakami, Y., Kanezaki, T., Mine, Y.: Hydrogen effect against hydrogen embrittlement. Metall. Mater. Trans. A 41, 2548–2562 (2010)
Effects of Temperature on Tensile and Fracture Behavior of Dissimilar Metal Welded Joint for Nuclear SafeEnd Lei Wang(&), Yang Liu, Xiu Song, and Jiahua Liu Key Laboratory for Anisotropy and Texture of Materials, Northeastern University, Shenyang 110819, People’s Republic of China [email protected]
Abstract. The effects of temperature on tensile and the fracture behavior of dissimilar metal welded joint for nuclear safeend were studied. The results show that the strength, elongation and fracture toughness of DMWJ signiﬁcantly decrease with increasing temperature. At room temperature, more deformation twins can make the deflection of the crack propagation direction, so the crack propagation path is extended, and the alloy can absorb more energy during the fracture process, so as to the toughness of the joint is enhanced. While at the evaluated temperature, the second phase particles are more likely to be a crack initiation, which makes the crack propagation easier. In addition, the dislocation density is reduced, resulting in the decreased strength. Keywords: Dissimilar metal welded joint Twining
Temperature Deformation
1 Introduction The nuclear safety end is located in primary water systems pressure boundary of pressurized water reactors (PWRs) and it is usually connected by dissimilar metal welded joints (DMWJs) so it has been regarded as the key part. The DMWJ is exposed to high temperature and high pressure, as well as complex stress, so that it is the most vulnerable components [1–5]. The safety of the joint can be influenced by the signiﬁcant microstructure heterogeneity of DMWJ, residual stress [6, 7], weld composition dilution [8], C diffusion [9–13] and others. It is necessary to study the tensile and fracture behavior of the joint, in order to provide a theoretical basis for the safe operation of nuclear power plants. Some literatures have reported the deformation twins had important effect on the toughness of the alloy [14, 15]. However, little attention has been paid to reveal the mechanism of the temperature effect on the tensile deformation of DMWJ. Therefore, in the present study, tensile deformation behavior of a DMWJ was investigated in a temperature range from room RT to 320 °C.
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 38–43, 2020. https://doi.org/10.1007/9783030478834_7
Effects of Temperature on Tensile and Fracture Behavior
39
2 Experimental Procedures SA508III309L/308L316L DMWJ for the PWRs was used as the experimental material. The tensile and fracture toughness JQ (with a prefatigue crack) tests were conducted from RT (about 23.5 °C) to 320 °C using a SANS CMT5105 universal tensile testing system at a strain rate of 10−3 s−1, and the 25 mm extensometer was employed. For optical microscopy (OM) and scanning electron microscopy (SEM) examinations, the specimens were mechanically polished and etched. Thin foils for transmission electron microscopy (TEM) were prepared from the deformed specimen, polished by twinjet electro polishing machine using an electrolyte consisting of 9% HClO4 and 91% ethanol at a temperature of −30 °C. TEM observation were carried out by a JEOL JEM2100F operating at 200 kV.
3 Results and Discussions Table 1 shows the tensile properties of the joints. The yielding strength (YS), ultimate strength (UTS) and the elongation (El) of the joint signiﬁcantly decrease with increasing tensile deformation temperature. Compared to the joint tested at RT, the YS, UTS and El of that at 320 °C decreased by 63.60%, 28.60% and 49.40%, respectively. Figure 1 shows the JR curves of the joints at different temperatures, which the specimen was bended with a cross head speed of 0.2 mm/min and the JQ is determined by offline of J = 8rY(Da). From Fig. 1, it can be seen that the JQ value of the joint decreases with the increasing of temperature, 246.12 kJ/m2 at RT, 155.96 kJ/m2 at
Table 1. Tensile properties of DMWJ at different temperatures Temp (°C) YS (MPa) RT 332 150 306 240 251 320 121
UTS (MPa) EI (%) 561 27 460 17 427 15 400 13
320 °C, the JQ loss ratio reaches 36.63%. The microstructures of the tested joints (near the fracture position) at RT and 320 ° C are shown in Fig. 2(a) and (b), respectively. It can be noticed that the grain has been
L. Wang et al.
J, /(kJ/m2)
40
Δa, /(mm)
Fig. 1. JR curves of DMWJ at different temperatures
(b)
Loading direction
(a)
Fig. 2. SEM micrographs of longitudinal section of specimens tensile tested at (a) RT, (b) 320 °C
elongated along the tensile direction, which means the fracture positions of the joints are consistent at different temperatures. The fracture surface morphologies of the joints tested at different temperatures are shown in Fig. 3. The fracture surfaces illustrate typical ductile fracture characteristics (a)
(c)
(b)
10μm
10 μm
(d)
10 μm
10 μ m
Fig. 3. Fracture surface morphologies of joint tensile tested at: (a) RT, (b) 150 °C, (c) 240 °C, (d) 320 °C
Effects of Temperature on Tensile and Fracture Behavior
41
with dimples at different temperatures. However, with increasing temperature, the dimple size decreases, and the toughness of the joint decreases. Figure 4 shows the back scattering morphologies of the fracture surface after fracture toughness test at different temperatures. The main cracks expand from the left to right. The gray porphyritic in backscattering is ferrite. It is clear that the secondary cracks can be observed from the specimens at different temperatures except RT. It can be seen that crack propagated with transcrystalline fracture, and sometimes propagated with second phase particle to another (Fig. 4(d)). That means the second phase particles is the main crack source at high temperature. As well known, the dislocations will start to move under a low stress, and then pile up around the second phase particles, when the stress is large enough, the microvoids will form along the interface between the
(a)
Crack propagation 10 μm
(b)
(d)
(c)
10μm
10μm
10μ m
Fig. 4. Crosssection surface morphologies of joint fracture toughness tested at: (a) RT, (b) 150 °C, (c) 240 °C, (d) 320 °C
second phase particles and matrix by the stress concentration with dislocation pole up. And ﬁnally the combination of microvoids became a cracking and lead fracture. Figure 5 shows the dislocation conﬁguration of the tensile tested joints from RT to 320 °C. After tensile testing at RT, the number of twins is higher, and a lot of dislocation tangles can be observed in twins. While, both number of twins and dislocations decrease obviously for the joint tested at 320 °C. Since the thermal vibration of atoms increases with the increasing of testing temperature, more slip systems can be activated at higher temperature, so that the dislocation density will be decreased. The joints can also be coordinately deformed by twins because of relatively low stacking fault. But with the increasing temperature, the number of twins decreases, so the elongation of the joint will decrease. It is well known that fracture toughness of a material is depended on the ability of coordinated deformation at crack tip. If the plasticity of a material is very good, more absorbed energy is needed for the crack tip enlarging, resulting in higher fracture toughness. In addition, when deformation twining occurs, the stress concentration can be released, so the plasticity of the joint increases. It has been reported that crack growth direction is easy deflected by the deformation twining [16, 17]. On the other hand, the dislocation slip can be hindered with the deformation twining during
42
L. Wang et al.
(a)
(b)
(c)
(d)
Fig. 5. Dislocation conﬁguration of joint tensile tested at: (a) RT, (b)150 °C, (c) 240 °C, (d) 320 °C
deformation, then dislocations pile up on the twin boundaries, and this leads to the stress concentration. When a crack propagates to a deformation twin, the stress concentration occurs at the twin boundary. When the stress concentration is difﬁcult to release by the slip of dislocations at the twin boundaries at crack tip, crack will propagate along the twin boundary, therefore the direction of crack propagation will be changed. With such direction changing, the crack propagation route will become longer and longer. So that, more absorb energy is needed for the fracture processing of a joint at RT, comparing with those at elevated temperatures.
4 Conclusions (1) The main crack source of a joint is the second phase particles. With the increasing of testing temperature, the atom vibration increases, and more slip system can be started to motion. It makes the decreasing of dislocation density, as well as the strength of the joint. Because the stacking fault energy is low, the deformation can be coordinated by twinning during tensile deformation at the lower temperatures. With increasing of testing temperature, while a number of deformation twining decreases, the elongation of the joint decreases. (2) Cracks easy propagate along the twin boundary, thus the crack propagation direction will be changed and the crack propagation route becomes longer. The
Effects of Temperature on Tensile and Fracture Behavior
43
fracture toughness of the joint is higher at RT than those at elevated temperatures, because the longer the route is, the more the absorbed energy needs.
References 1. Seifert, H.P., Ritter, S., Shoji, T., et al.: Environmentallyassisted cracking behavior in the transition region of an Alloy182/SA 508 Cl.2 dissimilar metal weld joint in simulated boiling water reactor normal water chemistry environment. J. Nucl. Mater. 378(2), 197–210 (2008) 2. Jang, C., Lee, J., Kim, J.S., et al.: Mechanical property variation within Inconel 82/182 dissimilar metal weld between low alloy steel and 316 stainless steel. Inter. J. Press. Vessels Pip. 85(9), 635–646 (2008) 3. Kim, J.W., Lee, K., Kim, J.S., et al.: Local mechanical properties of Alloy 82/182 dissimilar weld joint between SA508 Gr.1a and F316 SS at RT and 320 °C. J. Nucl. Mater. 384(3), 212–221 (2009) 4. Qin, R.Y., Duan, Z.L., He, G.: Microstructure and ductilitydip cracking susceptibility of circumferential multipass dissimilar weld between 20MND5 and Z2CND1812NS with Nibase ﬁller metal 52. Metall. Mater. Trans. 44A(10), 4661–4670 (2013) 5. Wang, H.T., Wang, G.Z., Xuan, F.Z., et al.: Local mechanical properties of a dissimilar metal welded joint in nuclear power systems. Mater. Sci. Eng., A 568, 108–117 (2013) 6. Qiao, D., Zhang, W., Pan, T.Y., et al.: Evaluation of residual plastic strain distribution in dissimilar metal weld by hardness mapping. Sci. Tech. Weld. Joining 18(7), 624–630 (2013) 7. Joseph, A., Rai, S.K., Jayakumar, T., et al.: Evaluation of residual stresses in dissimilar weld joints. Inter. J. Press. Vessels Pip. 82(9), 700–705 (2005) 8. Chen, Z.B.: Failure analysis of dissimilar steel joints of A/P. Central China power (4), 26– 30 (1996) 9. Pan, C.: Microstructure and transformation mechanism of dissimilar metal welded joints of composite parts. Wuhan Trans. Tech. Univ. (1998) 10. Pavlinov, L.V.: Iron and carbon diffusion in tetra component iron Chromium Nickel Molybdenum alloys in region of gamma solid solutions. Fiz. Met. Metalloved. 41(2), 344– 350 (1976) 11. Yang, H., Shi, G., Zhang, Y., et al.: Finite difference of carbon transfer at high temperature for dissimilar steel welded joints. Weld. J. 4, 77–80 (2001) 12. Zhang, Y., Yang, H., Cao, S., et al.: Analysis on the phenomenon of carbon transfer in dissimilar steel welded joints. J. Weld. 02, 89–92 (2001) 13. Breedis, J.F.: Influence of dislocation substructure on the martensitic transformation in stainless steel. Acta Metal. 13(3), 239–250 (1965) 14. Murr, L.E.: Stackingfault anomalies and the measurement of stackingfault free energy in f. c.c. thin ﬁlms. Thin Solid Films 4(6), 389–412 (1969) 15. Michiuchi, M., Kokawa, H., Wang, Z.J., et al.: Twininduced grain boundary engineering for 316 austenitic stainless steel. Acta Mater. 54(19), 5179–5184 (2006) 16. Chuaiphan, W., ChandraAmbhorn, S., Sornil, B., et al.: Microstructure, mechanical and corrosion behaviour of dissimilar weldments. Sheet Metal 410–411, 533–541 (2009) 17. Chung, W.C., Huang, J.Y., Tsay, L.W., et al.: Microstructure and stress corrosion cracking behavior of the weld metal in Alloy 52A508 dissimilar welds. Mater. Trans. 52(1), 12–19 (2011)
A Multiattribute Information Based Method of Material Strength Distribution Fitting Liyang Xie(&), Bo Qin, and Ningxiang Wu Laboratory of Vibration and Control of AeroPropulsion System, Northeastern University, Shenyang, China {lyxie,bqin,nxwu}@me.neu.edu.cn
Abstract. Information fusion technique has been widely applied to a variety of subjects such as fault diagnosis and image identiﬁcation. Bayes estimation is a special type of information fusion technique applied to parameter estimation for probability distribution of random variable. The present paper presents a new type of information fusion technique for material strength distribution estimation in the situation of small size sample. To precisely describe material strength, threeparameter Weibull distribution is used. To ﬁnd out a reasonable location parameter in the situation that only a few experimental observations are available, the knowledge and information from different aspects are utilized. First, an empirical shape parameter is chosen with reference to the strength distribution of similar material. Then, a location parameter is assigned to make the estimated material strength variation at a realistic level, by judging the rationality of the location parameter through the strength probability distribution thus estimated. At last, big data technique is applied to further verify the rationality of the estimated material strength distribution by testing the relation between location parameter and the minimum observation in a sample of particular size for a special threeparameter Weibull distribution. Keywords: Material strength simulation
Weibull distribution Big data Monte Carlo
1 Introduction To estimate material strength by means of experiment data, a large size sample of strength data are usually required [1–4]. In the situation of small size of sample, especially very small size of sample containing only a few observations, both distribution type identiﬁcation and distribution parameter estimation are difﬁcult. Generally, threeparameter Weibull distribution is suitable to describe material strength since its flexibility, especially the robustness of its shape parameter to the same type of products. Lots of experiences have demonstrated that the shape parameter of the Weibull material strength of a particular type of material will not be much different. Weibull distribution has been applied to a wide range of problems [5]. It has also been employed for smaller sample sizes than any other statistical distribution [6]. However, the mostly applied is the twoparameter Weibull distribution [7–11].
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 44–51, 2020. https://doi.org/10.1007/9783030478834_8
A Multiattribute Information Based Method
45
Contrasting to twoparameter Weibull distribution, threeparameter Weibull distribution has evident advantages. However, a relatively large size of sample is required for threeparameter Weibull distribution ﬁtting. As a typical example of small size of sample, Nagatsuka proposed a least squares procedure for parameter estimation with sample size from 7 to 20 [12]. Another study to describe material fatigue strength is based on 14 observations [13]. To estimate material strength distribution in the situation of small size sample, Yang et al. proposed a new Bayesian method based on the characteristics of the product, using a modiﬁed Weibull distribution to describe the failure rate over entire lifetime [14]. Abbasi et al. presented an approach of Artiﬁcial Neural Networks (ANN) [15]. This paper focuses on new way to estimate the parameters of threeparameter Weibull distributed material strength based on a few experiment data.
2 On the Shape Parameter of Material Strength Distribution For a Weibull distributed material strength, the shape parameter can be determined empirically, i.e. it can be taken from similar material. For the Weibull distribution of metallic materials, a great amount of test data indicate a roughly range between 2.0 and 4.0. In the following ball bearing material strength estimation, the shape parameter is taken as 3.0.
3 On the Location Parameter A popular expression for the threeparameter Weibull probability density function is 8 > bðt cÞb1 tc b < Þ exp½ð tc f ðtÞ ¼ ð1Þ g gb > : 0 t\c where, b, η and c stand for the shape parameter, scale parameter and location parameter, respectively. Threeparameter Weibull probability density function has excellent flexibility to ﬁt the material strengths. As to the classical statistics method, a difﬁculty is to estimate the location parameter in the situation of small sample of observations. Alternatively, big data technique and information fusion concept can help to ﬁnd an appropriate probability density function including all its parameters to describe a random variable for engineering application. For engineering material, the possible minimum strength must be much greater than zero, though the strength random variable may scatter on a quite large scale. If enough experiment data are available about the strength of some kind of material, its probability density function, including all the parameters, can be estimated by classical statistics method. When only a few observations, such as ﬁve, is available, relevant knowledge and information have to be applied. Included are the probability density function of similar material, especially the shape parameter of Weibull distribution, the
46
L. Xie et al.
degree of strength dispersion of similar material, etc. According to these knowledge and information, some distribution parameter can be referred, or its reasonable range can be ﬁgure out, at least. For a Weibull distributed strength random variable, if s(1,n), s(2,n), …, s(n,n) are its n observations arranged in ascending order, the location parameter will be close to s(1,n) if n is large, especially in condition that the shape parameter is not very big. ^ i Þ, a By means of the median rank estimator of cumulative distribution function Fðs sample size np can be ﬁgured out with which the minimal observation can be taken as the estimator of the p 100th percentile for a speciﬁc Weibull distribution. This estimator is usually approximated as ^ i Þ i 0:3 Fðs n þ 0:4
ði ¼ 1; 2; . . .; nÞ
ð2Þ
where, i is the ordinal number of the individual observations in ascending order; n is the size of the sample. To estimate the 0.00135 percentile directly from the observations (equivalent to the lower bound of an interval of 6r for a Gauss distribution), the necessary sample size n0.00135 can be resolved from Eq. 2 as n0.00135 = 518. It means that if there are 518 observations, then the s(1,n) can be approximately taken as the location parameter. For the situation that the sample size is much less than 518, the observation s(1,n) should be modiﬁed as the location parameter. To ﬁnd a reasonable function to modify the minimal observation, Monte Carlo simulation is applied. The principle is that, for a given Weibull distribution, the possible differences between the location parameter c and the minimal observation s(1,n) in an arbitrary sample of size n can be observed by Monte Carlo sampling. Based on the Monte Carlo simulation, the upper envelope curve of the simulated date points can be used to describe the relationship between the possible maximal difference between s(1,n) and the location parameter. When this difference is known, the minimum observation s(1,n) can be modiﬁed to be taken as the location parameter. To perform the simulation to a given Weibull distribution W(c, η, b), the location parameter and scale parameter have to be determined ﬁrst. However, it can only be roughly chosen at this moment if the observations available are quite limited (e.g. there are only ﬁve observations). For a Weibull distribution with location parameter c and scale parameter η, the value of the cumulative probability associated with s = c + η equals to 1e−1 = 0.632, i.e. F(c + η) = 0.632. For the situation of ﬁve strength observations for a material, it is easy to know by Eq. 2 that F(s(4,5)) = 0.685, i.e. s(4,5) will be greater than c + η (corresponding to a percentile of 0.632), while s(3,5) will be less than c + η since F(s(3,5)) = 0.5. Meanwhile, F(s(5,5) − F(s(1,5)) = 0.741, which is greater than the 2r interval of 0.683 for a Gauss distribution. Therefore, s(1,5) − (s(5,5) − s(1,5)) can be approximately taken as the location parameter c, and s(4,5) − c can be used as an approximate value of the scale parameter η. The relationship between these variates and parameters are shown in Fig. 1.
Probability density
A Multiattribute Information Based Method
47
3.E03 2.E03 2.E03 1.E03 5.E04 0.E+00
s1
0
s4 s5
2000 Strength
Fig. 1. The characteristic variates/parameters and their relations
Providing the ﬁve observations for a material strength are 1202, 1014, 773.3, 958.4 and 649, respectively, s(1,5) − (s(5,5) − s(1,5)) = 649 − (1202 − 649) = 96 can be taken as the location parameter, and s(4) − c = 1014 − 96, i.e. 918 can be taken as the scale parameter, i.e. a Weibull distribution W(96,918,3) is estimated. From the procedure mentioned above, it is known that this is a conservative estimation. On the other hand, the Weibull parameters can be solved in cumulation probability equations. For a Weibull distribution, sc b
PðsÞ ¼ 1 eð l Þ
ð3Þ
lnð1 P1 Þ s1 c ¼ lnð1 P5 Þ s5 c
ð4Þ
Therefore,
According to Eq. 2, P1 = 0.130, P5 = 0.870 for the situation of a sample of 5 observation. For the ﬁve observations listed above, a Weibull distribution W(267.9, 735.6, 3) is estimated. This result is not so conservative as W(96,918,3).
4 Weibull Scale Parameter Estimation by ML Method The scale parameter of a Weibull distribution can be estimated by means of maximum likelihood method. When the shape parameter and location parameter are known, the scale parameter can be easily estimated as g¼ð
n X ðsi cÞb =nÞ1=b
ð5Þ
i¼1
For the situation of the ﬁve observations 1202, 1014, 773.3, 958.4 and 649, if the location parameter equals to 96.0 and the shape parameter equals to 3.0, then the scale parameter is estimated as 860.2; if the location parameter equals to 267.9, then the scale
48
L. Xie et al.
Probability density
parameter is estimated as 699.3. If twoparameter Weibull distribution is assumed, the scale parameter is estimated as 951.4. Actually, the ﬁve observations are a sample of the Weibull distribution W(500, 500, 3) (Fig. 2).
2.E03 2.E03 1.E03 1.E03 1.E03 8.E04 6.E04 4.E04 2.E04 0.E+00
Parameter: 267.9,3,735.6 Parameter: 96,3,860.2 Parameter: 267.9,3,699.3
0
500
1000 1500 2000 2500 3000 Strength
Fig. 2. The true Weibull distribution and ﬁtting results
The rationality of the estimation results can be veriﬁed by the dispersion of the estimated distribution. Dispersion can be characterized by deviation, standard deviation or variation coefﬁcient. The mean, deviation and variation coefﬁcient are, respectively 1 l ¼ cþg C 1þ b 2 1 r2 ¼ g2 C 1 þ C2 1 þ b b m ¼ r=l
ð6Þ ð7Þ ð8Þ
Experiments show that for majority of metallic materials, the variation coefﬁcient will not be greater 0.1. For instance, if a Gaussian distributed random variable has a 6r range of tmin*tmax, and tmax = 2tmin, then m¼
ðtmax tmin Þ=6 ð2tmin tmin Þ=6 ¼ 0:111 ðtmin þ tmax Þ=2 ðtmin þ 2tmin Þ=2
Meanwhile, according to Weibull cumulative distribution function, the strength associated with failure probability is sP ¼ gð lnð1 PÞÞ1=b þ c
ð9Þ
A Multiattribute Information Based Method
49
The lower and upper bounds of the 6r range (probability of 99.73%) are respectively t0:00135 ¼ gð lnð0:99865ÞÞ1=b þ c t0:99865 ¼ gð lnð0:00135ÞÞ1=b þ c The ratio of the upper bound to the lower bound, i.e. t0.00135/t0.99865 can also be applied to judge the rationality of the estimation: s0:99865 =s0:00135 ¼
gð lnð0:00135ÞÞ1=b þ c gð lnð0:99865ÞÞ1=b þ c
ð10Þ
Probability density
For the above estimation results, the true situation is l = 946.49, r = 162.28, m = 0.171, and the ratio = 2.59. The threeparameter Weibull estimation results are l = 864.14, r = 279.18, m = 0.323, and the ratio = 8.93. The twoparameter Weibull estimation results are l = 849.58, r = 308.78, m = 0.363, and the ratio = 16.93. To get a reasonable estimation, let c = 400, and η is estimated as 578.93, then l = 916.98, r = 187.98, m = 0.205, and the ratio = 3.20 (Fig. 3). 3.E03
Parameter: 500,3,500
2.E03
Parameter: 400,3,578.9 Parameter: 0,3,951.4
2.E03 1.E03 5.E04 0.E+00 0
500
1000 1500 2000 2500 3000 Strength
Fig. 3. The true Weibull distribution and modiﬁed ﬁtting results
5 Monte Carlo Veriﬁcation In the following, the Weibull distributed life random variable with c = 400, η = 578.9, and b = 3.0 is observed by Monte Carlo simulation. According to the simulation result, for the Weibull probability density function with the only information available is n observations with the minimum sð1;nÞ , the location parameter should be estimated as
50
L. Xie et al.
c ¼ sð1;nÞ þ 0:67g lgð
n 1=2 Þ 518
ð11Þ
Thus, for the situation of ﬁve observation 1202, 1014, 773.3, 958.4 and 649, the location parameter can be estimated as 388.1 with the scale parameter of 578.9. It is not far from the multiattribution estimation result of 400.
6 Conclusions Information fusion technique is applied to material strength probability distribution estimation in the situation of small size of sample. Threeparameter Weibull distribution is used to describe material strength. To estimate a reasonable location parameter and thus a reasonable scale parameter, the knowledge and information from similar materials are utilized, included are an empirical shape parameter, a possibly large dispersion degree, as well as the experiment data. At last, the location parameter assigned is to make the estimated material strength variation at a realistic level. Besides, big data technique is applied to further verify the rationality of the estimated material strength distribution by testing the relation between location parameter and the minimum observation in a sample of particular size. Acknowledgement. This research is subsidized by NSFC (Grant No. U1708255).
References 1. Shen, Y., Xie, M.: Nonparametric estimation of decreasing mean residual life with type II censored data. IEEE Trans. Reliab. 59(1), 111–116 (2010) 2. McLain, A.C., Ghosh, S.K.: Nonparametric estimation of the conditional mean residual life function with censored data. Lifetime Data Anal. 17, 514–532 (2011) 3. Soliman, A.A.: Estimation of the parameters of life for Gompertz distribution using progressive ﬁrstfailure censored data. Comput. Stat. Data Anal. 56, 2471–2485 (2012) 4. Zhao, M., Jiang, H., Liu, X.: A note on estimation of the mean residual life function with lefttruncated and rightcensored data. Stat. Probab. Lett. 83, 2332–2336 (2013) 5. Elmahdy, E.E.: A new approach for Weibull modeling for reliability life data analysis. Appl. Math. Comput. 250, 708–720 (2015) 6. Abernethy, R.B.: The New Weibull Handbook: Reliability & Statistical Analysis for Predicting Life, Safety, Survivability, Risk, Cost, and Warranty Claims, 5th edn. Gulf Publishing Company, Florida (2010) 7. Jia, X., Wang, D., Jiang, P., et al.: Inference on the reliability of Weibull distribution with multiply typeI censored data. Reliab. Eng. Syst. Saf. 150, 171–181 (2016) 8. Mazhar, M.I.: Remaining life estimation of used components in consumer products. J. Oper. Manag. 25, 1184–1193 (2007) 9. Ducros, F., Pamphile, P.: Bayesian estimation of Weibull mixture in heavily censored data setting. Reliab. Eng. Syst. Saf. 180, 453–462 (2018) 10. Ahmed, M.: Bayesian. Estimator for Weibull distribution with censored data using extension of Jeffrey prior information. Procedia Soc. Behav. Sci. 8, 663–669 (2010)
A Multiattribute Information Based Method
51
11. Sobhi, A.A.: Soliman. Estimation for the exponentiated Weibull model with adaptive typeII progressive censored schemes. Appl. Math. Model. 40, 1180–1192 (2016) 12. Nagatsuka, H.: A study of estimation for threeparameter Weitull distribution based on doubly typeII censored data using a least square method. In: 2nd International Conference on Secure System Integration and Reliability Improvement, Yokohama, Japan, pp. 58–165. IEEE Conference Publications (2008) 13. Zhao, Y.X., Liu, H.B.: Weibull modeling of the probabilistic SN curves for rolling contact, fatigue. Int. J. Fatigue 66, 47–54 (2014) 14. Yang, J.W., Wang, J.H., Huang, Q.: Reliability assessment for the solenoid valve of a highspeed train braking system under small sample size. Chin. J. Mech. Eng. 31, 47 (2018) 15. Abbasi, B.: Estimating parameters of the threeparameter Weibull distribution using a neural network. Eur. J. Ind. Eng. 2(4), 428–445 (2008)
Performance of a Carburizing Bearing Steel After Surface Nanosized Yanhui Wang1,2, Fucheng Zhang1(&), Zhinan Yang1, Hezong Li2, and Qian Yang2 1
2
Yanshan University, Qinhuangdao 066004, China [email protected] Hebei University of Engineering, Handan 056038, China
Abstract. Nanobainite and dispersed carbides were gained on surface layer of a modiﬁed carburizing 23Cr2Ni2Si1Mo bainitic bearing steel based on carburization, tempering at high temperature, and succedent lowtemperature isothermal quenching. As compared with the conventional carburizing 20Cr2Ni4 martensitic bearing steel, the novel carburizing 23Cr2Ni2Si1Mo nanobainitic bearing steel showed a much higher wearresisting performance and rolling contact fatigue performance. The excellent properties suggest that the novel carburizing 23Cr2Ni2Si1Mo nanostructured bainitic steel is very promising to manufacture heavyduty bearing, especially for bearings that bear impact load and need high wearresisting performance and high rolling contact fatigue performance during their service life. Keywords: Performance
Carburization Nanobainite Bearing steel
1 Introduction The high carbon martensitic microstructure of the traditional carburizing 20Cr2Ni4 bearing steel possesses high hardness, outstanding wearresisting performance (WRP) and rolling contact fatigue (RCF) resistibility. However, it has poor toughness, high hydrogen embrittlement sensitivity and temper brittleness. The service life of high carbon martensite bearing steel will be greatly reduced when the service condition is bad or there is a big sudden impact load. The nanobainite has much better toughness than the high carbon martensite [1, 2]. Meanwhile, the hardness and strength of nanobainite can match the high carbon martensite [3, 4]. The WRP of a highSiAl nanobainite [5] was increased by 21–51% over the tempered martensite, though the nanobainite had a lower hardness value than the tempered martensite. The RCF life of a C1.26wt% steel sample [6] with 21 vol.% nanobainite was about 3.3 times longer than martensite sample. The prolonged RCF life should owe to the nanobainite and the carbonrich retained austenite. In the present work, we have studied the microstructure and property of new designed 23Cr2Ni2Si1Mo nanobainitic carburizing bearing steel, which are compared with those of the conventional 20Cr2Ni4 martensitic carburizing bearing steel.
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 52–57, 2020. https://doi.org/10.1007/9783030478834_9
Performance of a Carburizing Bearing Steel After Surface Nanosized
53
2 Experimental Procedure The experimental steels were named as 23Cr2Ni2Si1Mo and 20Cr2Ni4 in the paper. The platelike samples with dimensions of U43 mm 6 mm and U52 mm 8 mm were ﬁrst machined, and then carburized. The carburizing process is the same as that in [7]. After hightemperature tempering, the 23Cr2Ni2Si1Mo steel was held at 860 °C for 1 h and austempered at 200 °C for 8 h. And the 20Cr2Ni4 steel was held at 810 °C for 1 h and then quenched in oil at once. In the end, the two steels were moved into a 200 °C furnace to temper. The microstructure pictures were taken by a HitachiSU5000 SEM and a JEM2010 TEM. The surfaces of samples were tested by a D/max2500/PC XRD. The WRP of the experimental steels after carburizing was tested by a MMU5G wear test machine. The test condition is dry sliding friction without lubrication at ambient temperature. The load was 1000 N, while the rotation rate was 200 rpm. The surfaces of all samples were ground and polished before the RCF test. The experiment was performed by using a TLP1 point contact testing machine. The Hertz stress of 4500 MPa and the spin rate of 2040 rpm were chosen.
3 Results and Discussions The carbon contents of the surfaces are *0.83 wt% for 23Cr2Ni2Si1Mo steel and *0.81 wt% for 20Cr2Ni4 steel. And the same carburizing depth is about *2.8 mm. Figure 1 shows the hardness distributions in carburized layer of the experimental steels after heat treatments. Evidently, the hardness declines continuously from surface to center for both steels, because of the carbon content keeps falling from surface to center. The surface of the 23Cr2Ni2Si1Mo steel with nanobainite achieves a hardness of 690 ± 8 HV, and its center with a lowcarbon martensitic microstructure is 492 ± 6 HV. In contrast, the 20Cr2Ni4 steel has a hardness of 680 ± 10 HV in the surface with a highcarbon martensitic microstructure and 431 ± 7 HV in the center with a lowcarbon martensitic microstructure. The hardness in surface of the two carburized steels have little difference in spite of different microstructures are obtained in the surfaces. The high hardness value obtained in the surface layer is helpful to improve the WRP and RCF resistance.
Fig. 1. Hardness distribution in carburized layer after heat treatments.
54
3.1
Y. Wang et al.
Microstructures of the Surfaces of the Experimental Steels After Carburizing
The SEM pictures of the surface are shown in Fig. 2. One can see that the tiny carbides were uniform distribution in matrix of the two steels. Figure 2(a) show that a dominant needlelike bainite was acquired on surface of the 23Cr2Ni2Si1Mo steel. The obvious network carbides, which located at the red arrows, were observed on the surface of the 20Cr2Ni4 steel from Fig. 2(b). The network carbides will increase the brittleness and drop fatigue life. After a lot of observation and measurement statistics, the average area fractions of the carbides in surfaces of the 23Cr2Ni2Si1Mo and the 20Cr2Ni4 were evaluated to be 6.3% and 6.7% for each.
Fig. 2. SEM images in surface of carburized 23Cr2Ni2Si1Mo (a) and 20Cr2Ni4 steel (b).
The mean diameters of carbides for 23Cr2Ni2Si1Mo and 20Cr2Ni4 were evaluated to be 0.19 and 0.22 µm for each. The ﬁne carbides embedded in matrix not only are helpful to increase the WRP [8], but also could restrain the austenite grain coarsening.
Fig. 3. TEM micrographs of the carburized surface: (a) 23Cr2Ni2Si1Mo (b) 20Cr2Ni4. Notes: RAretained austenite, Ccarbides, BFbainitic ferrite, and TMtwinning martensite.
Performance of a Carburizing Bearing Steel After Surface Nanosized
55
The typical TEM pictures are displayed in Fig. 3. The multiphase microstructures composed of bainite plate, carbides, and retained austenite were acquired in the carburized 23Cr2Ni2Si1Mo steel. Twinning martensitie is distinct in surface of the carburized 20Cr2Ni4 steel, whose presence can not only aggravate the stress concentration effect, but also decline the toughness and plasticity. According to a large number of TEM pictures, the measured average thickness of bainite plate (tBF) in the surface of carburized 23Cr2Ni2Si1Mo steel was about 71 ± 12 nm. This is a typical nanobainite. From the XRD patterns, the volume fractions of retained austenite (Vc) in surface of the 23Cr2Ni2Si1Mo and the 20Cr2Ni4 were conﬁrmed to be *18.9% and *17.1%, respectively. Retained austenite in surface is crucial for fatigue life of carburized steels. On one hand, a part of the retained austenite of surface will occur martensitic transformation by strain during RCF testing, which causes the surface hardness to be increased further [9, 10]. On the other hand, volume expansion is inescapable when retained austenite occurs martensitic transformation, thus, a compressive stress is formed in surface [11]. Both the increased hardness and the compressive stress are beneﬁcial to improve the RCF resistance. 3.2
WRP and RCF Performance of the Surfaces After Carburizing
Figure 4 shows weight loss with wearing time on surface of the experimental steels. Obviously, the weight loss of 20Cr2Ni4 steel after 120 min is greater than that of 23Cr2Ni2Si1Mo steel. The weight losses of the 20Cr2Ni4 steel show a linearly increasing trend with the increasing wearing time. The difference values in accumulative weight loss between the 20Cr2Ni4 steel and the 23Cr2Ni2Si1Mo steel become bigger and bigger with the increasing wearing time, which reveals that the wear rate of the 23Cr2Ni2Si1Mo steel is less marked than that of the 20Cr2Ni4 steel. We can consider the relative WRP of the 20Cr2Ni4 steel as one unit, thus the relative WRP of the 23Cr2Ni2Si1Mo steel could be denoted by using the ratio of weight loss for 20Cr2Ni4 steel to 23Cr2Ni2Si1Mo steel. From Fig. 4 the relative WRP of the 23Cr2Ni2Si1Mo steel is calculated to be 1.61, implying that the WRP of 23Cr2Ni2Si1Mo is greater than 20Cr2Ni4 by 61%.
Fig. 4. Weight loss with wearing time on surface of the experimental steels.
56
Y. Wang et al.
The wearing results show that although the initial hardness values of different microstructures are almost the same, they show different WRP. The initial hardness of the microstructure is only one factor affecting the WRP. Microstructure also has an important effect on the WRP. The average thickness of bainite plate (tBF) in carburized 23Cr2Ni2Si1Mo surface was about 71 ± 12 nm, which was much thinner than the martensite plate in carburized surface of 20Cr2Ni4. The surface microstructure reﬁnement of 23Cr2Ni2Si1Mo could directly enhance the plasticity, hardness and strength and indirectly increase the WRP. In addition, the nanocrystals were easily to produce on the nanobainite surface in the process of severe friction and wear [5, 12], which can enhance the WRP further. Figure 5 shows Weibull distribution curves of RCF life of the 23Cr2Ni2Si1Mo steel and the 20Cr2Ni4 steel. Table 1 generalizes the Weibull fatigue lives. Apparently, the RCF life of 23Cr2Ni2Si1Mo is much longer than that of 20Cr2Ni4 steel in spite of the Vc and the hardness value of surface are nearly parallel for the two steels. The L10, L50, and characteristic life of 23Cr2Ni2Si1Mo are 3.10, 3.47, and 3.54 times longer than those of 20Cr2Ni4, respectively. The remarkable RCF performance of 23Cr2Ni2Si1Mo owes to the development of nanobainite in surface. Nanobainite could prolong the RCF life by restraining the nucleation and propagation of micro crack [6]. Stress concentration effect on hard phase in the process of RCF could be relieved by the nanobainite, which is relatively soft. Therefore, the micro crack nucleation becomes difﬁcult. Furthermore, the stress on micro crack tip could be relieved by nanobainite, as a consequence it will demand more energy for the propagation of micro crack.
Table 1. RCF lives of 23Cr2Ni2Si1Mo and 20Cr2Ni4 steel. Steel L10/( 107) 23Cr2Ni2Si1Mo 1.3751 20Cr2Ni4 0.4439 L10 : rated life, L50 : median Weibull slope.
L50/( 107) Vs/( 107) B 4.5339 5.7143 1.58 1.3076 1.6136 1.74 life, Vs : characteristic life, b :
Fig. 5. Weibull distribution curves of RCF life of 23Cr2Ni2Si1Mo and 20Cr2Ni4 steel.
Performance of a Carburizing Bearing Steel After Surface Nanosized
57
4 Conclusions 1. The microstructure, consisting of nanobainite with 71 ± 12 nm thickness bainitic ferrite plates and dispersed carbides, with a hardness of 690 ± 8 HV was obtained on surface layer of the modiﬁed carburizing 23Cr2Ni2Si1Mo bainitic bearing steel based on carburization, tempering at high temperature, and succedent lowtemperature isothermal quenching. 2. The WRP and the characteristic life of RCF of the modiﬁed carburized 23Cr2Ni2Si1Mo nanobainitic bearing steel are about 61% and 254% greater than those of the conventional carburized 20Cr2Ni4 martensitic bearing steel. The excellent WRP and RCF performance of the nanobainitic steel owe to the ultraﬁne microstructure. Acknowledgement. The work in this paper thanks the support of the Natural Science Foundation of Hebei Province (E2019402433), and the University Science and Technology Research Project of Hebei Province (QN2018078), P.R. China.
References 1. Bhadeshia, H.K.D.H.: Nanostructured bainite. Proc. R. Soc. A 466, 3–18 (2010) 2. Yoozbashi, M.N., Yazdani, S., Wang, T.S.: Design of a new nanostructured, highSi bainitic steel with lower cost production. Mater. Des. 32, 3248–3253 (2011) 3. Hasan, H.S., Peet, M.J., AvettandFènoël, M.N., et al.: Effect of tempering upon the tensile properties of a nanostructured bainitic steel. Mater. Sci. Eng. A 615, 340–347 (2014) 4. AmelFarzad, H., Faridi, H.R., Rajabpour, F., et al.: Developing very hard nanostructured bainitic steel. Mater. Sci. Eng. A 559, 68–73 (2013) 5. Yang, J., Wang, T.S., Zhang, B., et al.: Sliding wear resistance and worn surface microstructure of nanostructured bainitic steel. Wear 282–283, 81–84 (2012) 6. Liu, H.J., Sun, J.J., Jiang, T., et al.: Improved rolling contact fatigue life for an ultrahighcarbon steel with nanobainitic microstructure. Scr. Mater. 90–91, 17–20 (2014) 7. Wang, Y.H., Yang, Z.N., Zhang, F.C., et al.: Microstructures and mechanical properties of surface and center of carburizing 23Cr2Ni2Si1Mo steel subjected to lowtemperature austempering. Mater. Sci. Eng. A 670, 166–177 (2016) 8. Chakraborty, J., Bhattacharjee, D., Manna, I.: Development of ultraﬁne bainite + martensite duplex microstructure in SAE 52100 bearing steel by prior cold deformation. Scr. Mater. 61, 604–607 (2009) 9. Zheng, C.L., Dan, R., Zhang, F.C., et al.: Effects of retained austenite and hydrogen on the rolling contact fatigue behaviours of carbidefree bainitic steel. Mater. Sci. Eng. A 594, 364– 371 (2014) 10. Wang, Y.H., Zhang, F.C., Yang, Z.N., et al.: Rolling contact fatigue performances of carburized and highC nanostructured bainitic steels. Materials 9, 960 (2016) 11. Bhadeshia, H.K.D.H.: Steels for bearings. Prog. Mater. Sci. 57, 268–435 (2012) 12. Wang, T.S., Yang, J., Shang, C.J., et al.: Sliding friction surface microstructure and wear resistance of 9SiCr steel with lowtemperature austempering treatment. Surf. Coat. Technol. 202, 4036–4040 (2008)
Residual Strength and Toughness of Nano and Micro Scale Fiber Reinforced Cementitious Composites Panagiotis A. Danoglidis1(&), Maria S. KonstaGdoutos1, and Emmanuel E. Gdoutos2 1
Center for Advanced Construction Materials, The University of Texas at Arlington, Arlington, TX 76019, USA [email protected] 2 Academy of Athens, 106 79 Athens, GR, Greece
Abstract. This study reports a signiﬁcant synergistic effect of using combined networks of nanoscale ﬁbers (CNTs) and micro scale ﬁbers (PPs) on the key mechanical properties of OPC mortars that deﬁne a uniquely tough and energyabsorbing material. The flexural strength at the ﬁrst crack, d, were ﬁrstly investigated by conducting three point close loop bending tests on prismatic specimens of mortars reinforced with 0.1 wt% CNTs and/or 0.73 wt% PPs. To further assess the mechanical performance of the proposed nanocomposites after the formation of the ﬁrstcrack, the residual strength and the energy absorption capability of the nanocomposite mortars are also investigated at three postcrack stages, 3d, 5.5d and 10.5d, according to the ASTM C1018. The experimental results showed that a combination of nano and micro scale ﬁber reinforcement yields a composite with a signiﬁcantly enhanced loadcarrying capacity at the elastic stage, as deﬁned by the approximately 100% higher ﬁrst crack strength. The multi scale ﬁber reinforcement has also an exceptional impact on improving the tensile straincapacity of resultant composite after the formation of the ﬁrst crack. The observed 90% increased residual strength and postcrack toughness of CNTPP reinforced mortars indicate an improved ductility over the mortars reinforced with microscale PP ﬁbers alone. Keywords: Mortar Carbon nanotubes Postcrack toughness
Polypropylene Residual strength
1 Introduction Fiber reinforced concrete presents enhanced ductility overcoming the limited strain capacity of the quasi brittle cementitious materials. The introduction of ﬁbers at the micro scale, such as polypropylene ﬁbers, PPs, polyvinyl alcohol ﬁbers, PVAs, and polyethylene ﬁbers, PEs, into the cementitious matrix results in postelastic mechanical property changes [1, 2]. Although, the micro scale ﬁber reinforcement’s ability to bridge the microcracks and delay the formation of a throughspecimen macrocrack, the initiation of cracks at the nanoscale, which affects the fundamental mechanical response of concrete cannot be prevented. The use of ﬁbers at the nanoscale, such as carbon © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 58–63, 2020. https://doi.org/10.1007/9783030478834_10
Residual Strength and Toughness of Nano and Micro Scale Fiber
59
nanotubes CNTs, in cementitious matrices offers unprecedented improvements in the mechanical properties of cement based materials and concrete [3, 4]. The effective incorporation of individual CNTs and the formation of a complete nanoscale ﬁber network into the cementitious matrix signiﬁcantly improves the nanocomposite’s flexural load carrying capacity; hence the proportionality of stress to strain before the formation of the “ﬁrst crack” [5]. As a result, nanoscale ﬁber reinforced composites were successfully developed, exhibiting 100% increases in their “ﬁrst crack” strength and toughness, modulus of elasticity, energy absorption capability and fracture characteristics [6]. While the effect of micro or nano scale ﬁber addition on the mechanical performance of cementitious materials and concrete is thoroughly reported, there is a lack of information about the synergistic effect of the simultaneous addition of nano and micro scale on the load carrying capacity and energy absorption capability of hybrid cement based composites at the “ﬁrst crack” and the postcrack stages. The purpose of the present study is to investigate the mechanical performance including (i) the “ﬁrst crack” strength and toughness; (ii) the residual strength; and (iii) the postcrack energy absorption capability of mortars reinforced with an optimum network of CNTs and PPs. Prismatic mortar specimens, reinforced with 0.1 wt% CNTs and/or 0.73 wt% PPs, were subjected to a three point close loop bending test. The combination of CNTs and PPs provide signiﬁcantly enhanced mechanical performance at both the ﬁrstcracking and postcracking over the mortars reinforced with polypropylene ﬁbers alone. The hybrid CNT and PP reinforcement increases the ﬁrst crack strength, +98%, and improves the residual strength, +88%, and toughness, +55%, of micro scale ﬁber mortar composites.
2 Experimental Work 2.1
Materials and Specimens
Mortar composites were produced by using OPC Type I (w/c = 0.485), standard sand (s/c = 2.75), multiwalled carbon nanotubes (CNTs) and polypropylene staple ﬁbers (PPs). The nano and micro scale ﬁbers present aspect ratios of 307 and 480, respectively. The uniform dispersion of CNTs in aqueous suspensions was achieved by applying ultrasonication energy and using a polycarboxylate based surfactant [7]. Mortar mixes containing (a) 0.73 wt% PPs; and (b) 0.1 wt% CNTs and 0.73 wt% PPs were prepared following the ASTM C305, and was cast in 4 4 16 cm oiled molds for three point bending experiments. Following demolding, the samples were cured in limesaturated water for 28 days. 2.2
Experimental Determination of First Crack Strength, Residual Strength and Postcrack Toughness
Threepoint bending tests were conducted on 40 40 160 mm prismatic specimens. The tests were performed using a 25 kN MTS servohydraulic, closedloop testing machine under displacement control. The rate of displacement was kept as
60
P. A. Danoglidis et al.
0.1 mm/min. A typical loaddeflection response of a 28d mortar reinforced with 0.1 wt% CNTs and 0.73 wt% PPs is presented in Fig. 1. The ﬁrstcrack strength and toughness at the deflection d; and the residual strength and toughness at the postcrack deflections 3d, 5.5d and 10.5d were evaluated by following the analysis described by the ASTM C1018 [8] and the ACI report on Fiber Reinforced Concrete [9]. 28d Mortar + CNTs + PPs
3.5 Load (N)
3.0
First crack
2.5 2.0 1.5 0 0.0
δ 0.1
0.1
0.2
0.2
0.3
0.3
0.4
0.4
3δ 5.5δ Deflection (mm)
10.5δ
Fig. 1. Typical loaddeflection curve of 28d mortar reinforced with 0.1 wt% CNTs and 0.73 wt% PPs.
3 Results and Discussion Flexural strength of the 28d mortars reinforced with 0.1 wt% CNTs and/or 0.73 wt% PPs at the “ﬁrst crack” deflection (d) and at deflections of 3.0, 5.5 and 10.5 times the ﬁrstcrack deflection are presented in Fig. 2. The nano and micro scale ﬁber reinforced mortars exhibit 98% higher ﬁrst crack strength over the PP reinforced mortars. From the previous studies, it is already observed that mortars reinforced with 0.1 wt% CNTs exhibit an increase ﬁrstcrack strength, compared to the unreinforced matrix, due to an due to an enhanced crackbridging mechanism, resulting in a higher load transfer efﬁciency between the nanotubes and the matrix. Interestingly, and despite the fact that the geometrical characteristics of CNTs are in the scale of nanometers, their addition has a great impact on the residual strength of nanocomposites compared to the singly micro scale ﬁber reinforced mortars. The mortars reinforced with the nano and micro scale ﬁbers are able to sustain much higher loads after the formation of ﬁrst crack, exhibiting higher residual strengths. The simultaneous incorporation of CNTs and PPs leads to higher flexural strength, up to 88%, at the three postﬁrst crack stages, 3d, 5.5.d and 10.5d. To further examine the synergistic effect of nano and micro scale ﬁbers on the mechanical performance of mortar composites at the ﬁrstcrack and postcrack stages, the energy absorption capability, represented by the flexural toughness, at the deflections d, 3d, 5.5d and 10.5d are presented in Fig. 3. The hybrid mortars exhibit an
Residual Strength and Toughness of Nano and Micro Scale Fiber
Flexural strength (MPa)
12
11.3
61
M+PPs
10
M+PPs+CNTs 8.1
8
7.4 6.8 5.7
6
4.3
4.1
4
3.9
2 0 δ
3δ
5.5δ
First crack strength
10.5δ
Residual strength
Fig. 2. First crack and residual strengths of 28d mortars reinforced with CNTs and/or PPs
M+PPs
600
596.4
Fflexural toughness (N∙mm)
M+PPs+CNTs
500 385.2
400 300 200 100 0 0
δ
2
3δ
4
5.5δ6
8
10 10.5δ
12
Fig. 3. First crack and residual strengths of 28d mortars reinforced with CNTs and/or PPs
62
P. A. Danoglidis et al.
improved energy absorption capability at all the stages after the formation of the ﬁrst crack. The flexural toughness of nanomodiﬁed mortars at the postcrack stages up to a deflection of 3.0, 5.5 and 10.5 times the ﬁrstcrack deflection is 88%, 90% and 93% higher than the postcrack toughness of singly PP reinforced mortar. Recently it was found that the incorporation of CNTs in the PP reinforced polymers leads to a higher interfacial shear strength due to the better adhesion between the micro scale ﬁber and the matrix [10]. The strengthen interfacial bonding between the ﬁber and the matrix increases the demand of energy for crack propagation, improving the energy absorption capacity of hybrid mortars.
4 Conclusions In this study, it is demonstrated that a signiﬁcantly higher load carrying capacity and energy absorption capability, at the ﬁrst and the post cracking area, can be attained by incorporating combined reinforcement of nano and micro scale ﬁbers into the cementitious matrix. From the analysis of the three point bending loaddeflection curves, it is presented that the CNT and PP reinforced mortars exhibit extremely higher ﬁrst crack strength, +98%, compared to the singly PP reinforced mortars. The synergistic CNTPP reinforcing mechanism in mortars also leads to an even greater strength and toughening behavior at the postcrack area. The enhanced bridging mechanism, after the formation of the “ﬁrst crack”, by the simultaneous use of nano and micro scale ﬁbers exceptionally improves the composites’ load carrying capacity and postcrack energy absorption capability as reflected by the 88% and 55% higher residual strength and postcrack flexural toughness, respectively.
References 1. Lawler, J.S., Zampini, D., Shah, S.P.: Permeability of cracked hybrid ﬁber reinforced mortar under load. ACI Mater. J. 99(4), 379–385 (2002) 2. Yu, K.Q., Yu, J.T., Dai, J.G., Lu, Z.D., Shah, S.P.: Development of ultrahigh performance engineered cementitious composites using polyethylene (PE) ﬁbers. Constr. Build. Mater. 158, 217–227 (2018) 3. Danoglidis, P.A., KonstaGdoutos, M.S., Shah, S.P.: Relationship between the carbon nanotube dispersion state, electrochemical impedance and capacitance and mechanical properties of percolative nanoreinforced OPC mortars. Carbon 145, 218–228 (2019) 4. KonstaGdoutos, M.S., Danoglidis, P.A., Shah, S.P.: High modulus concrete: effects of low carbon nanotube and nanoﬁber additions. Theor. Appl. Fract. Mech. 103, 102295 (2019). https://doi.org/10.1016/j.tafmec.2019.102295 5. Danoglidis, P.A., KonstaGdoutos, M.S., Gdoutos, E.E., Shah, S.P.: Strength, energy absorption capability and selfsensing properties of multifunctional carbon nanotube reinforced mortars. Constr. Build. Mater. 120, 265–274 (2016) 6. Gdoutos, E.E., KonstaGdoutos, M.S., Danoglidis, P.A.: Portland cement mortar nanocomposites at low carbon nanotube and carbon nanoﬁber content: a fracture mechanics experimental study. Cem. Concr. Compos. 70, 110–118 (2016)
Residual Strength and Toughness of Nano and Micro Scale Fiber
63
7. Shah, S.P., KonstaGdoutos, M.S., Metaxa, Z.S.: Highly dispersed carbon nanotube reinforced cement based materials. United States Patent US9,365,456 (B2), 14 June 2016 8. ASTM C101897: Standard Test Method for Flexural Toughness and FirstCrack Strength of FiberReinforced Concrete (Using Beam With ThirdPoint Loading) (1997) 9. American Concrete Institute: Report on Fiber Reinforced Concrete, ACI 544.1R96 (1996) 10. Yumitoril, S., Araoz, Y., Tanakaz, T., Naito, K., Tanaka, K., Katayama, T.: Increasing the interfacial strength in carbon ﬁber/polypropylene composites by growing CNTs on the ﬁbers. In: Computational Methods and Experimental Measurements XVI, vol. 55, p. 275 (2013)
Experimental and Numerical Strategy for the Determination of Mechanical Properties Related to Human Cortical Bone Fracture J.L. Tailhan1(&), Y. GodioRaboutet2, and C. Boulay3 1
2
MASTEMGCU, Université Gustave Eiffel, IFSTTAR, 77447 MarnelaVallée, France [email protected] AixMarseille Université, Université Gustave Eiffel, IFSTTAR, LBA, 13016 Marseille, France 3 CME, Faverelles, France
Abstract. The paper presents an experimental test of macrocrack propagation in bones associated with a numerical strategy to determine from this test some mechanical properties by inverse identiﬁcation. A 3 point bending test is performed on a notched segment of long human bone, and the load vs notch opening displacement is measured. The compliance method is applied in the context of a realistic FE simulation of the test. A ﬁrst application of this methodology is described and shows its feasibility and capabilities. The ultimate objective of this research project is to develop a probabilistic modelling of the macrocracking processes in human long bone tissues based on an experimental database of mechanical parameters fed up by this methodology. Keywords: Bone cracking method
Experiment Numerical model Compliance
1 Introduction Fracture modes of bone structures prediction is essential for both the comprehension and the prevention of injuries and their surgical treatment. While many works on bone properties and model developments are proposed in the literature [1], the ability to predict more accurately their cracking behaviour remains a major scientiﬁc challenge. The ultimate objective of this research project is to develop a probabilistic modelling of the cracking processes in human long bone tissues, taking into account the effect of the material structural heterogeneity on these processes. In that sense, the present work is deeply inspired by other works originally developed for concrete structures [2–4]. Many natural or humanmade materials exhibit hierarchical innerstructure on one or more length scales [5]. This structure plays an essential role in their physical or mechanical properties. It also has an essential part to play in their cracking processes, especially for quasibrittle materials. It is precisely the case for concrete or bone tissue [6], which have particularly complex and heterogeneous innerstructures. Stress concentrations drive cracking processes. If one excepts potential geometrical singularities on the shape of a considered object of study, subjected to uniform loading © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 64–69, 2020. https://doi.org/10.1007/9783030478834_11
Experimental and Numerical Strategy
65
conditions, the phenomenon of stress concentration can appear in its constitutive material for two different reasons: because of material heterogeneity (in the sense of differences in elastic properties – moduli – of the inner components of the material itself), or because of internal discontinuities (flaws or initial microcracks) [3, 7]. Cracking processes can be conceptually separated into two distinct phenomena: crack creation and crack propagation. Flaws and heterogeneity have a real impact on both phenomena because they directly affect the strength and the toughness of the material. Establishing a (statistical) link between heterogeneity/defects and material mechanical properties to be used for the numerical modelling of cracking processes in human bone requires the elaboration of a substantial database of experimental results involving both mechanisms of crack initiation and propagation. The global strategy proposed for establishing this link consists briefly in (1) the design of an experimental test involving cracking processes in bones, (2) realistic numerical simulations of the test for the inverse determination of model parameters, (3) the characterisation of the level of heterogeneity of the material in the specimen. Given the high complexity of this strategy, and as a ﬁrst step of this research program, the paper focuses mainly on the two ﬁrst points. It presents, in a ﬁrst section, an experimental test of crack propagation in a notched piece of human femur subjected to a threepoint bending. In this test, only the cortical tissue is considered. The second section presents the main steps of the inverse determination of both elastic modulus and fracture energy (the most often used properties in modelling) from realistic numerical simulations of the test. The ﬁnal section will then be devoted to results, comments and conclusions.
2 Experimental Test Long human bones are considered here as “structural elements”. This point sets the scale of study. Considering full bones leads to consider both cortical and trabecular tissues. For simplicity, this study focuses only on the cortical bone. Cracking behaviour of cancellous bone will be studied in future works. In the sake of producing enough samples at this scale, mainly to feed statistical posttreatment results, several samples (generally three) of about 6 cm length are extracted from the diaphysis of femurs from human cadavers. Note that, if present on the sample, the remaining cancellous bone is systematically removed. At ﬁrst, the work will mainly focus on pure mode I cracking, favouring thus local tensile failures. Direct tension is particularly difﬁcult to be applied experimentally (even if the geometry of the specimen is perfectly regular), mostly because of the control of the boundary conditions. Nevertheless, indirect tension can be obtained with a bending test, more comfortable to perform, although it remains delicate because of the geometrical irregularity of the specimens. As the ratio height (about 6 cm) over length (about 3 cm) of the specimens is too small, and to overcome the critical effect of the shear force, it is necessary to extend the sample by adding two prismatic extensions, made of steel, at each end. The bone segment is then sandwiched between the two extensions, and the bond is ensured by glueing. A particular procedure to prepare and
66
J.L. Tailhan et al.
assemble the sandwiched components has been elaborated to guaranty their quite perfect alignment and minimize any geometrical defects. This solution has the advantage of better control of the boundary conditions on the machine. The purpose of the test shown in Fig. 1(a) is to follow the evolution under loading of a localized “structural” macrocrack. A notch (of 500 µm width) is made in the central crosssection of the sample, right under the loading point. Its purpose is to localize the crack initiation in this section of the specimen. The presence of the notch that induces a stress concentration at its tip also leads to a stress level reduction at the boneextension bonds. Note, that this last point can facilitate the glueing solution. A predimensioning numerical simulation of the test (considering the bone as a perfect cylinder of 3 cm of external diameter and 3 mm of thickness) has been carried out to estimate the stress level at the boneextension bonds according to the notch length: as a result, the longer the notch is, the lower the tensile stress level is. An estimation of the maximum tensile stress level of about 20–25 MPa was obtained for a notch length equal to half the diameter of the bone. The glue has been chosen taking into account this level of stress. Two types of glue have been eventually selected: a methacrylate and an epoxy resin. Their respective characteristics ensure to bear the estimated stress level. Glueing components is usually a complicated matter, and a particular attention has also been paid to the defatting pretreatment of the bone itself to avoid any incompatibility with the glue.
Fig. 1. Experimental setup (a) and an example of test results (b). On the curve, P1, P2 are applied loads corresponding to the macrocrack propagations. P3 is an unloading point.
The bending test, Fig. 1(a), is performed on a Landmark 370.10 hydraulic press (MTS Systems corporation, MN, USA). The notch opening is measured with a noncontacting linear proximity measuring system (Kaman KD2300). The sensor and its target are maintained by two aluminium supports to avoid any electromagnetic interferences on the measurements. The supports are directly glued on the bone surface, on each side of the notch allowing the sensor to bridge it. The load applied by the jack is monitored by the notchopening displacement measured. This solution has the advantage to better control the test monitoring and to assess at each time the opening of
Experimental and Numerical Strategy
67
the macrocrack. The test result is given in terms of loadnotch opening displacement curves. Figure 1(b) shows an example of result obtained on a piece of femur taken from a cadaver of an 83 years old woman.
3 Numerical Simulations of the Experiment The longitudinal modulus of elasticity and the fracture energy can be determined from this test by an indirect determination procedure, and a “realistic” numerical simulation of the test is performed for this purpose. The methodology is described as follow: the 3Dgeometry of the tested bone is reconstructed from scans (obtained with a medical scanner before the glueing operation) using specialized pieces of software (slicer3D version 4.8.1, Rhinoceros® Version 5.5.3, McNeel & Assoc. Edt.). The spatial position of the bone relative to its metallic extensions is reproduced identically in Rhino3D by using different tracking techniques based on photographic shots of the sample. Thus oriented in space, the geometry of the bone can then be imported into a ﬁnite element mesh generator. By adding the geometries representing the extensions, the sensor supports and other additional parts used in the test as well as the notch itself, the complete mesh of the test specimen can be generated (Fig. 2(a)). Boundary and loading conditions can also be added. 3.1
Determination of the Longitudinal Modulus of Elasticity
The principle of the methodology is elementary. A simulation of the test is performed in elasticity considering the value of the modulus as the unknown and searching it so that the numerical response ﬁts the experimental one. 3.2
Determination of the Fracture Energy
The methodology is here more complex, but its bases remain relatively classical [8, 9]. The compliance method is based on the Irwin–Kies relation: GI ¼
P2 dCd 2B da
ð1Þ
Where GI represents the fracture energy in mode I, P is the applied load, B is the width of the cracked section, Cd ¼ d=P is the compliance (d being the displacement of the loading point), and a is the crack length. Equation (1) requires the determination of the width B and the compliance Cd as functions of the crack length a. For the considered tested bone, whose geometry is purely irregular, the relationship BðaÞ is determined with a special feature of Rhinoceros®. The relationship Cd ðaÞ is obtained numerically with a series of elastic simulations of the bending test taking into account the presence of an idealized crack of varying length in the central section of the bone as depicted on Fig. 2(b). Note that the displacement of the loading point d is not measured experimentally, and as a consequence, the experimental compliance Cdexp cannot be determined. This difﬁculty is
68
J.L. Tailhan et al.
overcome by considering besides the quantity Cx ¼ x=P (x being the notch opening), which can be assessed experimentally. Numerically, this quantity can also be calculated and expressed as a function of a, i.e. Cx ðaÞ.
Fig. 2. Meshes for the application of the compliance method, and compliance curves
Finally, knowing the experimental value of the quantity Cx , for a given load level corresponding to the propagation of the crack in the material, the point corresponding to Cxexp on the numerical curve Cx ðaÞ gives the length a of the crack. The value of the d derivative da Cd ðaÞ and the one of B are then given by the numerical curves Cd ðaÞ and BðaÞ respectively (Fig. 2(c)). The corresponding value of GI is, therefore, calculated.
4 Results, Discussions and Conclusion An experimental result is given in Fig. 1(a). The test led to the creation of a macro crack starting from the notch and propagating quickly and vertically towards the loading point. The curve gives the evolution of the applied load versus the notch opening. This result clearly shows a relatively linear prepeak behaviour with a slight nonlinearity of the curve in the peak vicinity. This nonlinearity appears between approximately 85% and 90% of the maximum load, corresponding to a microcracking process established at the notch tip. However, remaining relatively small at the scale of the overall curve this phenomenon must be indicative of a limited process. The postpeak part of the curve has a sawtooth shape indicating successive propagations and blockages mechanisms of the macrocrack. The different reloading branches consist of a linear part and a nonlinear part near the local peak, signiﬁcant of a limited evolution of the microcracking at the macrocrack tip before propagation. Besides the tangents to the linear parts of the curve pass almost through the origin of the reference system. This latter point shows that there appears to be little or no permanent deformation. The postpeak brittle failure of the specimen can be explained by two possible hypotheses. The ﬁrst is that of age because due to the evolution of the internal structure of the material (osteoporosis, bone remodelling, …) toughness decreases with age [10, 11]. The second hypothesis is that of the conservation conditions imposed to the specimen before the test, which here probably led to an excessive drying of the specimen.
Experimental and Numerical Strategy
69
The elastic modulus of the bone is assessed following the described methodology and considering the material isotropic. This seemingly rough hypothesis has a minimal consequence on the value obtained since the longitudinal behaviour is mainly mobilized in the test. The value obtained is 11.2 GPa, and remains reasonable compared to values found in the literature. Due to the high brittleness of the test, the fracture energy can be determined by the compliance method for only two points (marked as P1 and P2 on Fig. 1). Values obtained are 0.25 N/mm2 and 1.06 N/mm2. These values, again consistent with the literature on the subject, correspond to equivalent crack lengths of 0.86 mm and 13.6 mm, respectively. Even if the quantity of postpeak information obtained remains modest, this ﬁrst test shows a possible methodology for determining mechanical properties relating to the propagation of a macrocrack in a human cortical bone. Possible leads for improvement are linked to (1) mastering bonding and (2) maintaining an acceptable level of the bone humidity. Repeating these testing and posttreating procedures will produce statistical data essential for the development of a probabilistic cracking model.
References 1. Schwarcz, H.P., Abudeia, D., Jasiuk, I.: The ultrastructure of bone and its relevance to mechanical properties. Front. Phys. 5, 39 (2017). https://doi.org/10.3389/fphy.2017.00039 2. Rossi, P., Richer, S.: Numerical modelling of concrete cracking based on a stochastic approach. Mater. Struct. 20, 334–337 (1987) 3. Rossi, P., Wu, X., Le Maou, F., Belloc, A.: Scale effects on concrete in tension. Mater. Struct. 27, 437–444 (1994) 4. Tailhan, J.L., Dal Pont, S., Rossi, P.: From local to global probabilistic modelling of concrete cracking. Ann. Solid Struct. Mech. 1(2), 103–115 (2010) 5. Lakes, R.: Materials with structural hierarchy. Nature 361, 511–515 (1993) 6. Rho, J.Y., KuhnSpearing, L., Zioupos, P.: Mechanical properties and the hierarchical structure of bone. Med. Eng. Phys. 20, 92–102 (1997) 7. Currey, J.D.: Stress concentration in bones. J. Cell Sci. 3(61), 111–133 (1962) 8. Rossi, P.: Fissuration du béton: du matériau à la structure. Application de la mécanique linéaire de la rupture. PhD thesis, ENPC, December 1986 9. Morais, J.J.L., de Moura, M.F.S.F., Pereira, F.A.M., Xavier, J., Dourado, N., Dias, M.I.R., Azevedo, J.M.T.: The double cantilever beam test applied to mode I fracture characterization of cortical bone tissue. J. Mech. Behav. Biomed. Mater. 3, 446–453 (2010) 10. Koester, K.J., Barth, H.D., Richie, R.O.: Effect of aging on the transverse toughness of human cortical bone: evaluation by rcurves. J. Mech. Behav. Biomed. Mater. 4, 1504–1513 (2011) 11. Phelps, J.B., Hubbard, G.B., Wang, X., Agrawal, C.M.: Microstructural heterogeneity and the fracture toughness of bone. J. Biomed. Mater. Res. 51(4), 735–741 (2000)
Effect of External Field Treatment on the Microstructure and Deformation Behavior of NickelBase Superalloy Yang Liu(&), Lei Wang, Xiu Song, and Yao Wang Key Laboratory for Anisotropy and Texture of Materials, Northeastern University, Shenyang 110819, People’s Republic of China [email protected] Abstract. The electrostatic ﬁeld and electropulsing were applied to the nickelbase superalloy and the effect and mechanism of the external ﬁeld on the microstructure were investigated in the present study. The results showed that the electrostatic ﬁeld has signiﬁcant effect on the vacancy movement and atomic diffusion. As a consequence, a lot of twins can be obtained in the alloy by electrostatic ﬁeld treatment and both the precipitation and growth of the strengthening phase changed. The plastic deformation resistance of the nickelbased superalloy can be effectively reduced by the adding of pulse current as well as the improvement of the plastic deformation ability. At the same time, the activation energy of the recrystallization can also be reduced by the adding of the pulse current, and the promotion of the nucleation and growth of the recrystallization of the alloy. Keywords: External ﬁeld treatment Deformation behavior
Superalloy Microstructure
1 Introduction Recently, the combination of materials science and electromagnetism have been developed into a new ﬁeld, named Electromagnetic Processing of Materials (EPM) [1– 3]. The Electric ﬁeld treatment (EFT) and electropulsing treatment (EPT), as a powerful and controllable external ﬁeld, have been paid highly attention in recent years [4–7]. Electric ﬁeld is another important energy ﬁeld except the temperature ﬁeld and stress ﬁeld, and it shows many special coupling effects when it is combined with the other ﬁelds. Properties of a material are said to be related with the microstructure and defects (including vacancy, dislocation, grain boundary and so on) of the material. Therefore, the improving properties of the material can be achieved by controlling the microstructure and defects. In the present study, the microstructure evolution of the nickelbase wrought superalloys after EFT and EPT were investigated. The mechanisms of the effects were also discussed. The aim of present study is to provide the bases for further application of electromagnetic technology on superalloys.
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 70–75, 2020. https://doi.org/10.1007/9783030478834_12
Effect of External Field Treatment
71
2 Experimental Procedures The chemical compositions of GH4169 and GH4199 alloys used in the present study are listed in Table 1. Table 1. Chemical compositions of GH4169 and GH4199 alloy (wt%) GH4169 Fe 19.25 GH4199 Fe 3.95
Cr 18.78 Cr 25.60
Nb 4.96 W 14.50
Mo 3.09 Mo 1.45
Ti 1.00 Ti 0.65
Al 0.65 Al 0.40
Si 0.082 Si 0.65
C 0.04 C 0.10
S 0.003 S 0.01
Ni Bal. Ni Bal.
The plate type specimen for EFT with a dimension of 120 mm 20 mm 1 mm was machined along the rolling direction of the bar by spark cutting. The specimens were solution treated at 1200 °C for 8 min, followed by air cooling (AC), and then, the aged at 500 °C to 900 °C in the speciﬁc electric ﬁeld, respectively. The specimen was connected to the anode of a direct current voltage power supply, and a stainless steel plate was connected to the cathode. The normal aging treatment was also carried out for comparing to EFT. The EPT of the alloy was carried out on MTS 810 material testing system at 800 °C. The electrode of HPC5 pulsed power was connected with the specimens by the selfmade insulation clamping. The temperature was controlled by the high temperature testing chamber system to keep the specimen at 800 °C. The microstructures were examined by an optical microscope (OLYMPUS GX71), a laser scanning confocal microscope (OLYMPUS LEXT 3100) and a ﬁeld emission scanning electron microscope (JEOL 7001). The morphology of precipitation was observed by a JEOL JEM2100F transmission electron microscope. Positron annihilation lifetime (PAL) and vacancy intensity percentage of specimens were measured by positron annihilation spectroscopy. Radioactive 22NaCl source was adopted, and the measurement was conducted for 4 h at room temperature.
3 Results and Discussions Figure 1 shows microstructure evolution of GH4199 alloy with and without EFT. With EFT, the annealing twins occurred, and with the increasing of treating time, the number of annealing twins increased [8]. While the variation of the grain size and morphology of precipitation with and without EFT was not obvious. Figure 2 shows the grain boundary character distributions of the alloy with EFT for different time [9]. It is clear that there are lots of annealing twins inside the grains in the alloy with EFT. With the increasing of treatment time, the number of annealing twin increases and the interface spacing of annealing twins decreases obviously. It has been reported that the formation of twins during the growth of the grain boundary can decrease the grain boundary energy and increase the fraction of coherent interfaces [9]. While the interfaces with low energy such as twin boundary can inhibit
72
Y. Liu et al.
Fig. 1. Microstructure of specimens aged at 820 °C for 5 h: (a) without EFT, (b) with EFT (4 kV/cm), (c) with EFT (4 kV/cm): TEM image and the corresponding SAED
Fig. 2. OIMreconstructed grain boundaries of the alloy with EFT for: (a) 0 h, (b) 10 h, (c) 20 h
the depletion of alloying elements at high angle grain boundary and improve the corrosion resistance of the alloys effectively [8]. During the formation and growth of the annealing twins in the alloy with EFT, the redistribution of elements at the crossing of the original high angle grain boundaries and annealing twin occurred. The exhaustion of alloying elements can be locally improved and the number of such kind of interface increases with the treatment time of EFT. The original high angle grain boundaries will be replaced and some of continuously distributed original grain boundaries will be partitioned [10]. And also, it has been found [11] that the direction of dislocation slip has been changed by the boundaries of annealing twins during deformation. The direction of microcrack propagation has also been changed on crossing the boundaries of the annealing twins. It causes the increasing plastic deformation work and delays fracture, these are considered as the reasons of the increasing ductility of the alloy by EFT. Figure 3 shows the stressstrain curves of GH4169 alloy tested at 800 °C with different EPT current density. It can be noticed that there is a remarkable change in the flow stress with the increasing of current density. The deformation resistance in the elastic deformation range has no obvious change under the pulse current comparing with that without the pulse current. However, both the elastic limit and the deformation resistance in the plastic deformation range decreases signiﬁcantly, thus the plastic deformation ability increases. The strength decreases more than 20% and the plasticity increases more than 100% under the pulse current with the current density of 1 kA/mm2 comparing with that without the pulse current. And the strength decreases more than 75%, and the plasticity increases 700%, with the current density of 4 kA/mm2 [11–13].
Effect of External Field Treatment
73
Fig. 3. Stressstrain curves of GH4169 alloy tensile test at 800 °C with different EPT current densities
In order to investigate the effect of the nonthermal effects on the recrystallization behavior of GH4169 alloy, the temperature compensation and nitrogen cooling were employed in the present study to ensure the same temperature of 650 °C of the alloy under different EPT conditions.
Fig. 4. Microstructures of GH4169 alloy: (a) at 650 °C for 0.5 h, (b) EPT (4 kA/mm2, 20 Hz, 30 ls), (c) EPT(4 kA/mm2, 30 Hz, 30 ls), (d) EPT(4 kA/mm2, 40 Hz, 30 ls)
Figure 4 shows the microstructure of the GH4169 alloy with different treat processes. It can be seen that the microstructure of the alloy treated at 650 °C for 0.5 h (a) is still the cold rolled microstructure. While under the EPT of 4 kA/mm2, 20 Hz and 30 ls at 650 °C for 0.5 h (b), the recrystallization characteristics and the precipitation of d phase at the original high angle grain boundary can be found, the twin grain boundary and the deformation band although the microstructure is still cold rolling
74
Y. Liu et al.
deformed microstructure. And as the EPT frequency increases, this trend gradually increases. It can be seen that most of the deformed grains in the matrix had been swallowed by a great deal of ﬁne and uniform recrystallization grains when the pulse frequency increases to 40 Hz. Because the distribution of solute atoms in the alloy aged at different temperatures is roughly similar, the distribution of solute atoms in the specimen with EFT is shown as an example in Fig. 5. It is clear that the distribution of Nb, Ti, Al, and Mo atoms is homogeneous in the matrix, but the obvious inhomogeneous distribution of Fe and Cr atoms can be found, and the concentration peak, as shown in Fig. 5(b).
Fig. 5. The distribution of main atoms at various layers in GH4169 alloy with EFT at 800°C.
The vacancy formation energy, diffusion activation energy, or radius of Mo atom is much higher than those of Fe and Cr atoms, so that it is difﬁcult to diffuse even though EFT is applied. The vacancy formation energy of Al atom is much lower than that of Fe or Cr atom, and the diffusion activation energy of Al or Nb atom is within the data range of Fe and Cr atoms.
4 Conclusions (1) Under the EPT, the deformation resistance decreased and the elongation increased signiﬁcantly during tensile test at 800 °C. And this effect increased with the increasing of EPT energy. Since the dislocation motion can be promoted by the electroplastic effect of the EPT. The initial temperature of recrystallization can be reduced by the electric effect of the pulse current and the dynamic recrystalllization nucleation is promoted. Therefore the dynamic recrystallization would occur at lower temperature. This is the main reason for the decreasing of deformation resistance and the increasing of plasticity of the alloy under the EPT. (2) EFT enhances the atomic vibration in the superalloy, and it leads to the increasing of both quantity and average size of vacancies. The vacancy flow consisting of monovacancies generates induced, and monovacancies transform to vacancy clusters under the EFT during aging, which causes the coarsening of precipitins in
Effect of External Field Treatment
75
superallpy. Meanwhile, the shortdistance diffusion of Al and Nb atoms is accelerated with EFT, resulting in the increasing of the diffusion coefﬁcients of these atoms, and which are about 1.6–5.0 times larger than those without EFT.
References 1. Hsieh, C.H., Lo, S.L., Hu, C.Y., et al.: Thermal detoxiﬁcation of hazardous metal sludge by applied electromagnetic energy. Chemosphere 71, 1693–1700 (2008) 2. Tournier, R.F., Beaugnon, E., Noudem, J., et al.: Materials processing in a magnetic force opposed to the gravity. J. Magn. Magn. Mater. 226–230, 2094–2100 (2001) 3. Karaca, H.E., Karaman, I., Basaran, B., et al.: On the stressassisted magneticﬁeld induced phase transformation in Ni2MnGa ferromagnetic shape memory alloys. Acta Mater. 55, 4253–4269 (2007) 4. Ho, P.S., Kwok, T.: Electromigration in metals. Report Progress Phys. 52, 301–348 (1989) 5. Conrad, H., Yang, D.: Effect of an electric ﬁeld on the plastic deformation kinetics of electrodeposited Cu at low and intermediate temperatures. Acta Mater. 50, 2851–2866 (2002) 6. Baranov, Y.V.: Effect of electrostatic ﬁelds on mechanical characteristics and structure of metals and alloys. Mater. Sci. Eng., A 287, 288–300 (2000) 7. Conrad, H.: Influence of an electric or magnetic ﬁeld on the liquidsolid transformation in materials and on the microstructure of the solid. Mater. Sci. Eng., A 287, 205–212 (2000) 8. Wang, L., Liu, Y., Wang, S., et al.: Effects of electric ﬁeld treatment on corrosion behavior of a NiCrWMo superalloy. Mater. Trans. 50, 1644–1648 (2009) 9. Krupp, U., Kane, W.M., Liu, X.Y., et al.: The effect of grainboundary engineeringtype processing on oxygeninduced cracking of IN718. Mater. Sci. Eng., A 349, 213–217 (2003) 10. Schuh, C.A., Kumar, M., King, W.E.: Analysis of grain boundary networks and their evolution during grain boundary engineering. Acta Mater. 51, 687–700 (2003) 11. Liu, Y., Wang, L., Liu, H.H., et al.: Effects of pulse current on dynamic recrystallization behavior of GH4169 superalloy. Mater. Trans. 53, 1400–1404 (2012) 12. Zhou, Y.Z., Qin, R.S., Xiao, S.H., et al.: Reversing effect of electropulsing on damage of 1045 steel. J. Mater. Res. 15, 1056–1061 (2000) 13. Tang, D.W., Zhou, B.L., Cao, H., et al.: Thermal stress relaxation behavior in thin ﬁlms under transient laserpulse heating. J. Appl. Phys. 73, 3749–3752 (1993)
Dynamic Speckle Contrast Imaging for Surface Defect Detection Rishikesh Kulkarni1(&), Shanta Patil1, and Pramod Rastogi2 1
Department of Electronics and Electrical Engineering, Indian Institute of Technology Guwahati, Guwahati, India [email protected] 2 Applied Computing and Mechanics Laboratory, Ecole Polytechnique Federale de Lausanne, Lausanne, Switzerland
Abstract. We propose to explore the dynamic speckle contrast imaging (DSCI) modality for noncontact surface defect detection. In this approach, the object under investigation is subjected to a continuous and monotonic loading. A number of speckle images are recorded during the continuous deformation of object surface. Speckle contrast analysis algorithm is applied to the stack of images which utilizes the fact that the variations on the object surface is reflected in signiﬁcant changes in the speckle intensity variations. A simulation study was performed with the speckle images and with specklegrams recorded in the speckle interferometry and Shearographic setup. The results motivate the applicability of the DSCI technique in surface defect detection. Keywords: Noncontact defect detection Dynamic speckle contrast imaging Correlation measure Singular value decomposition
1 Introduction Optical interferometric techniques such as electronic speckle pattern interferometry (ESPI), holographic interferometry and shearography are commonly used for submicron level deformation analysis applications [1, 2]. In these techniques, intensity of an interference pattern, specklegram, is recorded which is generated due to the superposition of a light beam scattered from the object surface and an undisturbed reference light beam. Both the light beams are derived from the same coherent laser source. A sinusoidally varying intensity pattern, usually termed as fringe image, is obtained from the subtraction of two specklegrams corresponding to the undeformed and deformed state of the object. The deformation of the object surface mainly changes the phase of the scattered light beam. Consequently, fringe analysis for phase estimation plays crucial role in the optical measurement techniques. Apart from quantitative deformation analysis, shearography has found a wide range of applications in industry due to its robustness against environment disturbances for defect detection. Although these techniques have found to be useful in quantitative assessment of deformation process, the major bottleneck of these techniques is the experimental stability requirement which is difﬁcult to meet outside laboratory environment. © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 76–81, 2020. https://doi.org/10.1007/9783030478834_13
Dynamic Speckle Contrast Imaging for Surface Defect Detection
77
Dynamic speckle contrast imaging (DSCI) has been widely used in bioimaging applications mainly due to the simplicity involved in the experimental setup which allows its use outside laboratory conditions [3]. In this technique, the object under investigation is illuminated with a coherent laser light source. The speckle pattern generated by the optically rough object surface is recorded using a CCD or CMOS camera. In bioimaging applications, the bioactivity within the object is the main source of speckle intensity variations. Analysis of these dynamic speckle patterns allows to obtain speckle contrast images. A number of numerical and graphic speckle analysis techniques have been reported in the literature [4]. Speckle correlation technique has also been applied in material characterization [5, 6]. In this work, we propose to explore speckle correlation for noncontact surface defect detection.
2 Dynamic Speckle Contrast Imaging In the context of deformation analysis, when the object surface is subjected to external loading, defective surface points undergo larger deformation compared to the nondefective points. In ESPI and shearography, this fact results into the variation in the fringe density which becomes a signature for the presence of defect. Note that only two specklegrams are recorded one for the undeformed and one for the ﬁnal deformed state of the object. In the paper, we propose a scheme wherein a number speckle images are recorded while the object under investigation is subjected to continuously and monotonically changing load. In this case, variations in the speckle intensities are caused due to the object surface deformation. We propose to utilize these variations in the speckle intensity for locating the surface defects. Consider that K number of speckle images of size M N are recorded during the continuous loading of the object surface. Thus, we have an image stack I of size M N K. In the present study, since we are interested in identiﬁcation of defect location, three graphical speckle contrast analysis techniques are discussed. Fujii [7] and generalized difference (GD) [8] are two commonly used measures for segmentation of object surfaces based on some local activity variations. These are computed as Fujiiðm; nÞ ¼
K X jIk ðm; nÞ Ik þ 1 ðm; nÞj k¼1
GDðm; nÞ ¼
jIk ðm; nÞ þ Ik þ 1 ðm; nÞj
XX k
jIk ðm; nÞ Ik þ l ðm; nÞj
l
We propose a new algorithm for speckle contrast analysis using the singular value decomposition (SVD). Each speckle image in the stack is divided into a number of image patches each of size Mp Np . The patch is converted into a vector of size Mp Np 1. All the vectors associated with same patches in different speckle images are appended together to obtain a matrix Ip of size Mp Np K. The SVD of Ip is computed as
78
R. Kulkarni et al.
Ip ¼ Up Kp VpT ; where, Up and Vp are left and right singular matrices of size Mp Np Mp Np and K K, respectively. Kp is the diagonal matrix of singular values arranged in an ascending order. Depending on the surface activity in a given image patch, the speckle intensity variations change and so does the distribution of singular values in the SVD of Ip . We deﬁne this change in singular values distribution over patches as spatiotemporal speckle correlation (STC) measure as follows K1 STC ¼ 1 P i Ki P where, K1 is the ﬁrst (and highest) singular value and i Ki represents sum of all singular values. Speckles are more decorrelated at the location of defect as the deformation will be higher compared to nondefective location. Accordingly, the ﬁrst singular value K1 corresponding to the image patch at defect will have lower magnitude compared to the same at nondefective location. The STC is computed at each patch and the two dimensional correlation map of the size same as that of the speckle image is computed using interpolation.
3 Results A simulation study was performed to demonstrate the applicability of the DSCI technique for defect detection. The speckle simulation was performed based on the technique proposed in [9] with adjustable speckle size. We considered K ¼ 50 speckle images generated with the phases corresponding to continuous object surface deformation. One such speckle image is shown in Fig. 1(a). Apart from these speckle images, the DSCI technique is also applied to simulated specklegrams corresponding to ESPI and Shearography setup. For the purpose of illustration, the ESPI and Shearographic fringe images corresponding to the ﬁnal surface deformation are shown in Figs. 1(b) and (c), respectively. The speckle contrast images obtained using Fujii, GD and STC methods are shown in second, third and fourth columns, respectively, in Fig. (1). For the purpose of comparison, the speckle contrast images have been normalized. It can be observed that the STC method provides high contrast images compared to Fujii and GD methods with which the defect locations can be clearly identiﬁed.
Dynamic Speckle Contrast Imaging for Surface Defect Detection
79
Fig. 1. (a) Speckle image in DSCI setup. Fringe images corresponding to surface deformation in (b) ESPI and (c) Shearography setup. The speckle contrast images obtained using Fujii, GD and STC methods are shown in second, third and fourth columns, respectively.
A study on the effect of number of speckle images and speckle sizes on the speckle contrast images is performed and the results are shown in Fig. 2. The ﬁrst row shows the speckle contrast images obtained using the proposed STC for increasing number of speckle images (K) from left to right. It can be noted that the speckle contrast does not vary signiﬁcantly with K. The second row shows the speckle contrast images obtained using the proposed STC with increasing speckle sizes from left to right. Expectedly, the speckle contrast decreases with the increase in speckle size.
80
R. Kulkarni et al.
Fig. 2. The speckle contrast images are obtained using the STC method. First row: (a) K = 10 (b) K = 25 and (c) K = 75. Second row corresponds to speckle images with increasing speckle sizes from left to right.
4 Conclusion The simulation results clearly indicate the applicability of DSCI technique for the surface defect detection. The experimental setup in this technique is much easier simpler compared to the interferometric techniques. The proposed STC algorithm based on the singular value decomposition is found to provide higher contrast images compared to the Fujii and GD methods. In fact, other speckle contrast algorithms have also been compared with STC method. The STC seem to provide better contrast images compared to most of them.
References 1. Jacquot, P.: Speckle interferometry: a review of the principal methods in use for experimental mechanics applications. Strain 44, 57–69 (2008) 2. Kulkarni, R.D., Rastogi, P.: Single and Multicomponent Digital Optical Signal Analysis: Estimation of Phase and Its Derivatives. Institute of Physics publishing (2017) 3. Rabal, H.J., Braga, R.A. (eds.): Dynamic Laser Speckle and Applications. CRC Press, Boca Raton (2019)
Dynamic Speckle Contrast Imaging for Surface Defect Detection
81
4. Braga, R.A., Rivera, F.P., Moreira, J.: A Practical Guide to Biospeckle Laser Analysis, Theory and Software (2016) 5. Thomas, F.G., Gerd, G., Klaus, D.H., Karen, W.: Corrosion monitoring with speckle correlation. Appl. Opt. 38, 5948–5955 (1998) 6. Yamaguchi, I., Yokota, M., Ida, T., Sunaga, M., Kobayashi, K.: Monitoring of paint drying process by digital speckle correlation. Opt. Rev. 14, 362–364 (2007) 7. Fujii, H., Nohira, K., Yamamoto, Y., Ikawa, H., Ohura, T.: Evaluation of blood flow by laser speckle image sensing: part 1. Appl. Opt. 26, 5321–5325 (1987) 8. Arizaga, R., Cap, N.L., Rabal, H.J., Trivi, M.: Display of local activity using dynamical speckle patterns. Opt. Eng. 41, 287–294 (2002) 9. Guillermo, H.F., Gustavo, E.G.: Speckle noise reduction in television holography fringes using wavelet thresholding. Opt. Eng. 35(1), 9–14 (1996)
Experimental Investigation of the Elastic Modulus of Timber by Using Density and Fiber Orientation WeiChung Wang(&) and TzuYu Kuo National Tsing Hua University, No. 101, Sec. 2, Kuang Fu Rd, Hsinchu 30013, Taiwan, Republic of China [email protected], [email protected]
Abstract. Wood is a material found in nature with distinct applications in construction engineering. For the sake of greenhouse gas emissions, wood has been widely used. Two essential factors, i.e. ﬁber orientation and density, of the timber were adopted in the prediction model proposed in this paper to obtain the modulus of elasticity (MOE) of the timber. Besides, a bending test was used to verify the accuracy of the prediction model. Good agreement was found between the results obtained from the prediction model and static bending test along the longitudinal direction. Therefore, the proposed model presented in this paper has an excellent feasibility of predicting the MOE of the timber to ensure the reliability and safety of wood construction. Keywords: Timber Modulus of Elasticity Tracheid effect Fiber orientation
1 Introduction Wood is one of the essential natural materials as a composite material found in nature with diverse applications in civil, architectural, and constructional engineering [1]. However, modulus of elasticity (MOE) of the timber is dependent on the density, ﬁber orientations, and position of knots, etc. Hence the values of MOE vary at each location of the timber [2, 3]. Wood research in the Photomechanics Laboratory of National Tsing Hua University (NTHU), Taiwan, Republic of China, started with an international collaboration with Prof. YingHei Chui, University of New Brunswick, Canada, in 2010. In that collaboration, three dimensional (3D) digital image correlation (DIC) technique was ﬁrst used to measure the shrinkage of the timber in three directions on Jack pine [4]. From 2012 to 2019, a series of foundational research work from micro to macroscale were performed to investigate the surface characteristics and mechanical behavior of timber [5–13]. Based on the previous research outcomes, this paper is focused on the establishment of a model to predict MOE of the timber by using the density and ﬁber orientation.
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 82–85, 2020. https://doi.org/10.1007/9783030478834_14
Experimental Investigation of the Elastic Modulus of Timber
83
2 Material Species and the Specimen The specimen of Japanese cedar (Cryptomeria Japonica) was obtained in Hsinchu County of northern Taiwan. For the dimensional stability and moisture content adjustment, the specimen was placed in the lab with temperature controlled at 25°C and relative humidity controlled at 55% for more than one year before the experiment. The dimension of the specimen with a knot is 558 46 17 mm3.
3 Prediction Model for the Modulus of Elasticity A leastsquares ﬁt linear relationship with the coefﬁcient of determination, i.e. R2 = 0.9, between MOE and density of Japanese cedar was reported [12]. By following ASTM D2395 [14], the density of the specimen was measured as 435 kg/m3. As listed in Table 1, material properties, i.e. Young’s modulus (E), shear modulus (G) and Poisson’s ratio (m), of Japanese cedar were measured at density of 435 kg/m3. Table 1. Material properties of Japanese cedar at density of 435 kg/m3. Density El Er Et Glr Grt Gtl vlr vrt vtl 435 kg/m3 10.2 0.31 0.39 0.78 0.23 0.73 0.41 0.84 0.61 1. Unit: GPa. 2. Subscripts: l: longitudinal, r: radial, t: transverse.
By using the tracheid effect, a selfdeveloped optical ﬁber orientation measurement system was used to determine ﬁber orientations from the elliptic shape formed by the laser scattering pattern projected to the surface of the timber [15]. The inplane ﬁber direction was measured by the angle between the major axis of the elliptic shape and the global longitudinal axis of the specimen. The diving angle was determined by the ratio of the minor to major axes of the laser scattering pattern. Measurement of ﬁber orientations on four surfaces of the timber are needed to investigate the variation of MOE at each location of the timber. The proposed prediction model of MOE for the timber was based on the orthotropic elasticity relating strains to stresses. The compliance matrix Sij (i, j = 1, …, 6) was obtained by the ﬁber orientations transformed to the global longitudinal direction. The effective local MOE in the longitudinal direction was obtained from the parameter S11 of the compliance matrix. By using the rule of mixtures, the global MOE was obtained from all ﬁber orientations in four surfaces of each position along the longitudinal direction. By considering both density and ﬁber orientations, a prediction model was proposed to obtain the MOE. A static bending test was used to verify the correctness of the MOE calculated from the prediction model.
84
W.C. Wang and T.Y. Kuo
4 Results and Discussions It should be pointed out here that the linear relationship between MOE and density of Japanese cedar reported in [12] was based on measurement results of the clear wood with ﬁber orientations parallel to the longitudinal direction. However, the specimen used in this paper has a knot in the middle, in addition, the ﬁber orientation is not perfectly parallel to the longitudinal direction. Furthermore, ﬁber orientations in the vicinity of the knot are random. Hence, the MOE value obtained from the relationship between MOE and density reported in [12] is higher than that obtained from the static bending test. By using the optical scanning system developed in this paper, real ﬁber orientation can be obtained so that the position and the size of the knot can be determined. The density value obtained from the linear relationship between MOE and density of Japanese cedar reported in [12] can then be modiﬁed. Therefore, all parameters of the compliance matrix will be recalculated by using the modiﬁed density. The modiﬁed S11 will be used to calculate the modiﬁed MOE in the longitudinal direction.
5 Conclusions A relationship between MOE and density was ﬁrst adopted to calculate material properties in the compliance matrix. With the consideration of the effect of knot on the density and ﬁber orientation, an optical ﬁber scanning system was developed and used in this paper to measure ﬁber orientations on surfaces of the timber. Parameters of the compliance matrix were then modiﬁed to obtain the modiﬁed MOE. Results obtained from the prediction model proposed in this paper and static bending test along longitudinal direction are well matched. Based on the results obtained from this paper, it is clear that the global MOE is strongly related to the density, ﬁber orientation, and position as well as size of the knot. By using the proposed prediction model and the optical scanning system, the value of MOE can be obtained nondestructively. The reliability and safety of wooden structures can be ensured and greenhouse gas emissions can be reduced.
References 1. Matthews, F.L., Rawlings, R.D.: Composite Materials: Engineering and Science. CRC Press, Boca Rathon (1999) 2. Briggert, A., Olsson, A., Oscarsson, J.: Threedimensional modelling of knots and pith location in norway spruce boards using tracheideffect scanning. Eur. J. Wood Wood Prod. 74(5), 725–739 (2016) 3. Kandler G., Lukacevic M., Füssl J.: From the knot morphology of individual timber boards to the mechanical properties of glued laminated timber. In: World Conference on Timber Engineering, WCTE 2016, 22–25 August 2016, Vienna, Austria (2016)
Experimental Investigation of the Elastic Modulus of Timber
85
4. Peng, M., Ho, Y.C., Wang, W.C., Chui, Y.H., Gong, M.: Measurement of wood shrinkage in jack pine using three dimensional digital image correlation (DIC). Holzforschung 66(5), 639–643 (2012) 5. Kuo T.Y., Wang W.C., Chu C.I., Chen J.H., Hung T.H., and Chang J. Y.: Buckling measurement of cylindrical shells by digital image correlation method. In: ASME 2013 International Mechanical Engineering Congress and Exposition, San Diego, California, 15– 21 November 2013 6. Kuo, T.Y., Wang, W.C.: Experimental and numerical investigation of effects of ﬁber orientation of wood stiffness. In: Emerging Challenges for Experimental Mechanics in Energy and Environmental Applications, Proceedings of the 5th International Symposium on Experimental Mechanics and 9th Symposium on Optics in Industry, ISEMSOI, 17–21 August 2015, Guanajuato, Mexico, pp. 249–254 (2015) 7. Kuo, T.Y., Cheng, I.F., Wang, W.C.: Experimental Investigation on Macroscopic Fracture Behavior of Wood Plates under Tensile Load Using Digital Image Correlation Method. In: International Digital Imaging Correlation Society  Proceedings of the First Annual Conference, Philadelphia, PA, 2017, pp. 247–250, 7–10 November 2016 8. Kuo, T.Y., Wang, W.C.: Determination of effective modulus of elasticity of wood from proportion of latewood. In: World Conference on Timber Engineering, WCTE 2016, 22–25 August 2016, Vienna, Austria (2016) 9. Kuo, T.Y., Wang, W.C.: Experimental and numerical investigation of grain orientation of timber with knot by using digital image analysis. In: ECCOMAS Thematic Conference on Computational Methods in Wood Mechanics  from Material Properties to Timber Structures, CompWood 2019, Vienna, Austria, 17–19 June 2017 10. Kuo, T.Y., Wang, W.C., Lin, C.H., Yang, T.H.: Experimental investigation of crosslaminated timber shear wall under shear force by using digital image correlation method. In: Proceedings of the First International Conference on Theoretical, Applied and Experimental Mechanics, Paphos, Cyprus, pp. 95–97, 17–20 June 2018 11. Cheng Y.J., Kuo T.Y., Wang W.C.: Determination of global modulus of elasticity of timber by using ﬁber orientation and proportion of latewood. In: International Conference on Computational Methods in Wood Mechanics  from Material Properties to Timber Structures. ECCOMAS Thematic Conference, CompWood 2019, Växjö, Sweden, 17–19 June 2019 12. Kuo, T.Y., Wang, W.C.: Determination of elastic properties of latewood and earlywood by digital image analysis technique. Wood Sci. Technol. 53(3), 559–577 (2019) 13. Kuo, T.Y., Wang, W.C., Huang, H.S., Wang, J.S.: Determination of moduli of elasticity of latewood and transition latewood of Japanese cedar by using digital image analysis. In: International Conference on Computational Methods in Wood Mechanics  from Material Properties to Timber Structures. ECCOMAS Thematic Conference, CompWood 2019, Växjö, Sweden, 17–19 June 2019 14. ASTM D239517: Standard Test methods for density and speciﬁc gravity (relative density) of wood and woodbased materials. In: ASTM International, West Conshohocken, PA (2017) 15. Nyström, J.: Automatic measurement of ﬁber orientation in softwoods by using the tracheid effect. Comput. Electron. Agri. 41(1), 91–99 (2003)
Effect of pH on Microstructure and Properties of UltrasonicAssisted Electroless NiP Coatings Jingjing Cao(&), Xiaoyu Wang, Yifan Zhao, and Guofang Kong Hebei University of Engineering, Handan 056038, China [email protected]
Abstract. NiP coatings with various pH values (4.5*5.4) were fabricated on Ti6Al4V titanium alloy by ultrasonicassisted electroless deposition. The effect of pH on the deposition rate and phosphorus content was studied, as well as pH on the surface morphology, phase structure and microhardness of the deposited NiP coatings. The results showed that the increasing pH enhanced the deposition reaction, and ultrasonic cavitation and mass transfer effect improved the catalytic activity of the substrate surface and the reaction system. So the deposition rate was increased. But the higher pH decreased the stability of the bath and precipitated NiHPO3, resulting in the decrease of deposition rate. With the increase of pH, the phosphorus content decreased at ﬁrst and then kept stable (17 ± 0.45wt%),while the microhardness enhanced at ﬁrst and then kept stable (605 ± 2HV). The ultrasonicassisted electroless NiP coatings had the typical cauliflowerlike morphology and microcrystalline structure characteristics. Keywords: NiP coating
Ultrasonicassisted pH value
1 Introduction The electroless coatings possess good corrosion resistance, high hardness, good electrical conductivity and high tribological properties [1]. These excellent properties make it popular in many engineering community, such as electronic components, aerospace, petrochemical and others [2]. However, the autocatalytic electroless plating is a relatively slower process. The stability of the plating solution will decreases and the solution generate evaporation in the long time plating. So, it is vital to seek some method to promoting the autocatalytic action or the deposition rate and decreasing the deposition temperature. Many researchers studied the effect of ultrasonic assistance on the microstructure and properties of electroless plating [3, 4]. They found the ultrasonic assistance was beneﬁcial to the increase of deposition rate and the improvement of properties. But the ultrasonic can decrease the plating bath stability and even cause the selfdecomposition of plating solution [5]. During the electroless, various factors can affect the autocatalytic reaction, including the main salt, reducing agents, complex agents, temperature and pH value [6]. But the most important is pH that controls the rate and direction of the deposition reaction. Thus, we proposed to fabricate NiP coatings by ultrasonicassisted electroless on titanium alloy substrate, and performed © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 86–87, 2020. https://doi.org/10.1007/9783030478834_15
Effect of pH on Microstructure and Properties
87
zinc double immersion and alkaline preplating NiP ﬁlm to avoid the oxidation of titanium substrate causing the decrease of adhesion strength between coatings and substrate. And this work aims to study the effect of pH on the microstructure and properties of electroless NiP coatings in case of the ultrasonic ﬁeld.
2 Experimental Details 2.1
Specimen Preparation
The titanium alloy (Ti6Al4V) was used as the substrate, in the shape of sheet with 20 mm 20 mm 2 mm size. A /1.5 mm hole was cut at the center of the edge with laser beam machining machine to make it easy to be hanged. The specimen was grinded using SiC paper followed by ultrasonic cleaning in alcohol. The specimen was ﬁrst cleaned in alkaline solution to degrease. Then the specimen was etched to remove oxide layers. Next, the zincating was conducted to obtain Zn ﬁlms. The zincated titanium alloy plate was dipped into alkaline NiP solution for preplating. And it was worth noting that sufﬁcient water washing was required after each step. After preplating process, ultrasonicassisted electroless plating was performed and the pH was adjusted in the range of 4.5*5.4 ± 0.02. The schematic diagram of ultrasonicassisted electroless plating was shown in Fig. 1).
Fig. 1. Schematic diagram of ultrasonicassisted electroless NiP coatings.
References 1. Hari Krishnan, K., John, S., Srinivasan, K.N.: An overall aspect of electroless NiP depositions  a review article. Metall. Mater. Trans. A 37A, 1917–1926 (2006) 2. Loto, C.A.: Electroless nickel plating  a review. Silicon 8, 177–186 (2016) 3. Jiang, J.B., Chen, H.T., Wang, Y.H.: Effect of ultrasonication and Na2MoO4 content on properties of electroless NiMoP coatings. Surf. Eng. 35(10), 873–882 (2019) 4. Vitry, V., Bonin, L.: Effect of temperature on ultrasoundassisted electroless nickelboron plating. Ultrason. Sonochem. 56, 327–336 (2019) 5. Kobayashi, K., Chiba, A.A., Minami, N.: Effects of ultrasound on both electrolytic and electroless nickel depositions. Ultrasonics 38(1/8), 676–681 (2000) 6. Guo, L., Zhao, X.J., Xiao, L.R.: Kinetic study of electroless cobalt deposition on WC particles. J. Alloy. Compd. 750, 774–780 (2018)
Tailoring the Toughness and Electrochemical Capacitance of CNT Reinforced Mortars Maria S. KonstaGdoutos, Panagiotis A. Danoglidis(&), and Myrsini E. Maglogianni Center for Advanced Construction Materials, The University of Texas at Arlington, Arlington, TX 76019, USA [email protected]
Abstract. To unlock the contribution of carbon nanotubes in potential applications it is necessary to take into consideration the degree of their dispersion. In this work, a simple technique has been used for characterizing the degree of CNT dispersion in mortar based on values of the capacitive reactance measured using AC impedance spectroscopy. The relationship between capacitance values and fracture toughness provides valuable information on the actual CNT distribution in the matrix. Keywords: Fracture toughness
Capacitance Carbon nanotubes Mortars
1 Introduction CNT distribution in a cementitious matrix is a key parameter affecting the mechanical and electrical properties of the nanoreinforced cementitious materials and concrete [1, 2]. Besides the resistive phase, a nanotubemortar composite contains capacitive characteristics, mainly due to the localized nanotube/mortar/nanotube, similar to that of an electrical capacitor [3]. This study characterizes CNT dispersion using AC impedance spectroscopy and fracture mechanics tests [3, 4]. It was observed that the capacitive reactance of the nanoreinforced mortars can accurately evaluate the degree of CNTs dispersion. The relationship among the capacitance measurements and fracture toughness provides information on the actual CNT distribution in the matrix.
2 Results CNTs were added in mortar mixtures at amounts of 0.08%, 0.1%, 0.2%, 0.3% and 0.5 wt% of cement. CNT dispersion was achieved by applying ultrasonic energy with the use of a surfactant [4]. Figure 1 illustrates the capacitance and fracture toughness of mortars as a function of the CNT amount. When the CNTs are added in the mixture at amounts of 0.08% and 0.1 wt% an effective nanotube network is established in the matrix and the capacitance is decreased. This indicates a continuous nanotubenanotube structure, in which the electrical charge cannot be stored. At the same time, 0.08% and 0.1 wt% CNT/mortars exhibit the highest improvements in fracture toughness, 70% and 89%, respectively. The addition of CNTs at amounts higher than 0.1 wt% results in © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 88–89, 2020. https://doi.org/10.1007/9783030478834_16
Tailoring the Toughness and Electrochemical Capacitance of CNT
89
lower increases of the toughness and at the same time higher capacitance. This is indicative of poor CNT dispersion, which consequently leads to a lower toughening mechanism and a higher amount of energy stored in the nanoreinforced structure.
Fig. 1. Fracture toughness and Capacitance of 28d mortars reinforced with CNTs at amounts of 0.08%, 0.1%, 0.2%, 0.3% and 0.5 wt%
3 Conclusions The degree of CNT dispersion was successfully evaluated through electrochemical spectroscopy and fracture mechanics tests. The relation between the capacitive reactance and fracture toughness of the nanoreinforced mortars provides accurate information about the degree of nanotube dispersion. The addition of highly dispersed CNTs leads in an effectively connected carbon nanotube network in the matrix. Mortars reinforced with up to 0.1 wt% exhibit high fracture toughness values and decreasing resistance and capacitance values. Addition of CNTs at higher amounts result in lower toughness values and a relative increase in the ability of the nanotube network to store electrical energy.
References 1. KonstaGdoutos, M.S., Danoglidis, P.A., Shah, S.P.: High modulus concrete: effects of low carbon nanotube and nanoﬁber additions. Theoret. Appl. Fract. Mech. 103, 102295 (2019). https://doi.org/10.1016/j.tafmec.2019.102295 2. KonstaGdoutos, M.S., Danoglidis, P.A., Shah, S.P.: Tailoring the piezoresistive sensing of CNT reinforced mortar sensors. ACI Spec. Publ. 335, 12–26 (2019) 3. Danoglidis, P.A., KonstaGdoutos, M.S., Shah, S.P.: Relationship between the carbon nanotube dispersion state, electrochemical impedance and capacitance and mechanical properties of percolative nanoreinforced OPC mortars. Carbon 145, 218–228 (2019) 4. Danoglidis, P.A., KonstaGdoutos, M.S., Gdoutos, E.E., Shah, S.P.: Strength, energy absorption capability and selfsensing properties of multifunctional carbon nanotube reinforced mortars. Constr. Build. Mater. 120, 265–274 (2016)
Fracture
The Creep Resistance of ShortFibre Reinforced Metal Matrix Composites Vaclav Sklenicka1,2(&), Kveta Kucharova1, Milan Svoboda1,2, Petr Kral1,2, Marie Kvapilova1,2, and Jiri Dvorak1,2 1
Institute of Physics of Materials, Academy of Sciences of the Czech Republic, Zizkova 22, 616 62 Brno, Czech Republic [email protected] 2 CEITEC – IPM, Institute of Physics of Materials AS CR, Zizkova 22, 616 62 Brno, Czech Republic
Abstract. The creep resistance of two discontinuously reinforced with 20 vol.% alumina shortﬁbres magnesium composites were examined by performing a comparison between the creep properties of these composites and their magnesium matrix alloys AZ 91 and QE 22. It was found that the magnesium AZ 91 composite exhibits an improved creep resistance arising mainly from an efﬁcient load transfer effect and the existence of a threshold stress, respectively. By contrast, the beneﬁcial effect of reinforcement and the improved creep resistance of the QE 22 composite is signiﬁcantly influenced by the creep loading conditions. Keywords: Magnesium composites
Creep resistance Reinforcement
1 Introduction The creep resistance of magnesium alloys is rather limited at elevated temperatures. However, a marked improvement in the creep properties of magnesium monolithic alloys can potentially be achieved through the production of composite materials, where the matrices consist of conventional magnesium alloys which are strengthened through the introduction of nonmetallic ﬁbres or particulates to form metal matrix composites (MMCs) [1]. The most fundamental issue of the creep behaviour of these composites is the determination of the mechanism(s) by which the creep life of the composite is increased by reinforcing the creep matrix with lesscreeping nonmetallic shortﬁbres or particulates. Once the mechanism is clariﬁed, one can design new MMC with higher creep resistance by tailoring constituent parameters of the matrix alloy and short ﬁbre phases. This work reports the experimental results obtained in an investigation of the high temperature creep behaviour of shortﬁbre reinforced AZ 91 and QE 22 matrixbased composites and their monolithic alloys. The objective of the present research is a further attempt to clarify the creep strengthening and creep resistance in shortﬁbre reinforced magnesium alloys.
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 93–99, 2020. https://doi.org/10.1007/9783030478834_17
94
V. Sklenicka et al.
2 Experimental All the experimental materials used in this work were fabricated at the Technical University of Clausthal, Germany. Shortﬁbre reinforced and unreinforced blocks of the common AZ 91 alloy (Mg9 wt%Al1 wt%Zn0.3 wt%Mn) and the high strength silvercontaining QE 22 alloy (Mg2.5 wt%Ag2.0 wt%Nd rich rare earths0.6 wt%Zr) were processed by squeeze casting [2]. The ﬁbre preform consisted of planar randomly distributed dalumina short ﬁbres (Safﬁl Al2O3 ﬁbres *5 lm in diameter with varying lengths up to an estimated maximum of *150 lm). The ﬁnal ﬁbre fraction after squeeze casting in both composites was about 20vol.%. For convenience, the composites are henceforth designated AZ 91 + Safﬁl and QE 22 + Safﬁl. All materials were subjected to a T6 heat treatment [2]. Flat creep specimens with a 25 mm gauge length and 3 3.2 mm2 crosssection were machined from the blocks so that the longitudinal specimen axes parallel to the plane in which the long axes of the ﬁbres were situated. Constant stress tensile creep tests were carried out at temperatures from 423 K to 523 K and at applied stresses from 20 to 200 MPa. The creep elongations were measured using a linear variable differential transducer (W2K from HottingerBaldwin Co., Germany) and continuously recorded digitally and computerprocessed. Metallographic and fractographic investigations were conducted after creep testing using scanning electron microscope Lyra 3 TESCAN.
3 Creep Strengthening of the Composite At present it is generally accepted that creep deformation in metal matrix composites is controlled by flow in the matrix materials [2]. Creep strengthening of the magnesium composites may occur by either direct or indirect mechanisms [1] as it is illustrated in Fig. 1. Direct strengthening is due to a load transfer from the matrix to the reinforcements. Thus, load transfer is accompanied by a redistribution of stresses in the matrix and this reduces the effective stress for creep. Indirect strengthening occurs when the presence of the reinforcements or the process used to manufacture the composite influence the matrix microstructure which could modify the creep resistance. Potential microstructural effects include changes in the dislocation arrangements, accelerated ageing, microstructural decomposition, a matrix chemical compositional variation, and/or a reinforcement transformation. As a result, the microstructural changes in the matrix of the composite can retard and/or inhibit dislocation motion and lead to a threshold for creep that increases the creep resistance.
The Creep Resistance of ShortFibre Reinforced Metal Matrix Composites
95
1
10
MATRIX COMPOSITE (WITH THRESHOLD STRESS AND LOAD TRANSFER)
2
STRAIN RATE [a.u.]
10
n
10 3 4
10
1
THRESHOLD EFFECT
10 5 6
10
σ
LOAD TRANSFER EFFECT TH
10 7 0.1
1.0
10.0
STRESS [a.u.] Fig. 1. A schematic illustration of the power law creep in conjunction with the effects of the threshold stress and load transfer.
4 Results and Discussion 4.1
Creep in Monolithic and FibreReinforced AZ 91 and QE 22 Alloys
The most important creep data for the AZ 91 and QE 22 alloys and their composites at a testing temperature of 473 K are shown in Fig. 2, where the minimum creep e_ m rate e_ m and the time to fracture tf are plotted against the applied tensile stress r on a double logarithmic scale. Inspection of the creep data in Fig. 2(a) leads to two observations. First, the AZ 91 + Safﬁl composite exhibits an improved creep resistance (that means a substantial decrease of the minimum creep rate e_ m ), typically by >2 orders of magnitude in comparison with the monolithic alloy and, therefore, the trends of these plots are different because the unreinforced alloy exhibits a decreasing value of the true stress exponent of the creep rate n = (∂ln_em /∂lnr)T at the lower stresses, whereas the composite exhibits a higher value of n with decreasing stress. Second, the creep resistance of the QE 22 + Safﬁl composites is also somewhat better than that the unreinforced alloy but at the low stresses (r 100 MPa) only. Figure 2(b) shows the variation of the time to fracture with the stress for the same specimens tested in Fig. 2(a). The results for AZ 91 alloy and its composite demonstrate the creep lifetimes of the composite are up to one order of magnitude longer than that for the monolithic alloy at low stresses, although this difference decreases with increasing applied stress so that ultimately there is very little difference at stresses r > 100 MPa. By contrast, the creep life of the QE 22 + Safﬁl composite is markedly shorter than that of the unreinforced alloy at stresses > 100 MPa.
96
V. Sklenicka et al.
Mg QE 22 QE 22+Saffil AZ 91 AZ 91+Saffil
3
10
4
10
5
T = 473 K
TIME TO FRACTURE t f [s]
. MINIMUM CREEP RATE ε m [s1]
2
10
10
6
10 10
7
8
10
9
10
10
10
10
100
STRESS σ [MPa]
200
10
8
10
7
10
6
10
5
10
4
10
3
10
2
10
1
10
0
(a)
T = 473 K
Mg QE 22 QE 22+Saffil AZ 91 AZ 91+Saffil
10
100
200
STRESS σ [MPa]
(b)
Fig. 2. Stress dependences of (a) minimum creep rate and (b) time to fracture for the monolithic magnesium alloys and their shortﬁbre composites.
In conclusion, it was found that the presence of reinforcement leads to a substantial decrease in the overall ductility of the monolithic alloys. Thus, the values of the strain to fracture ef in both composites were only 1–2%. By contrast, the strains to fracture in the monolithic alloys were signiﬁcantly higher, typically up to 15% in the AZ 91 alloy and up to 30% in the QE 22 alloy. Despite the general similarity of the creep behaviour of both composites, the presence of the same composition and amount of a shortﬁbre reinforcement in the unreinforced AZ 91 and QE 22 alloys results in a signiﬁcantly different improvement of the creep resistance of composite by comparison with the matrix alloy. Thus, it will only be appropriate here to analyse differences that can be inferred from a comparison between the creep strengthening mechanisms of both composites and the unreinforced alloys (Fig. 1). 4.2
Direct Strengthening Due to a Load Transfer
As already shown in Fig. 2(a), the presence of short ﬁbre reinforcement could lead to a reduced creep rate in both composites. Such effect can arise when signiﬁcant load transfer partitions the external load between the matrix and the reinforcement. In the presence of load transfer, the creep data may be successfully reconciled by putting the ratios of the minimum creep rates of the composite and the rates of the matrix alloy at the same loading conditions, equal to a factor given by (1 – a)n, where a is a load transfer coefﬁcient having values lying within the range from 0 (no load transfer) to 1 (fullload transfer). Thus, the values of a inferred from the data for the unreinforced AZ 91 and its composite in Fig. 2(a) using n = 3 are within the range of 0.8 to 0.9. The predicted values a are in reasonable agreement with the theoretical prediction according to an analytical treatment based on a modiﬁed shearlag model. Unfortunately, values of the load transfer coefﬁcient a, for the QE 22 composite cannot be rigorously obtained due to insufﬁcient creep data inferred from this study. The indicative
The Creep Resistance of ShortFibre Reinforced Metal Matrix Composites
97
experimentally estimated values of a, for which the rate of the composite e_ c \_em were found to be 0.11 and 0.26 for 423 and 523 K, respectively. 4.3
Indirect Strengthening Due to a Threshold Stress r0
Having only a small number of experimental points it was appropriate to make use of the procedure in which it is possible to estimate the magnitude of r0 by plotting the data on linear axes as ð_eÞ1=n against r and linearly extrapolating the data to give the threshold stresses at a zero strain rate. A plot of this type requires, a priori, a judicious selection of the appropriate value of the true stress exponent, n. Figure 3 shows the determination of the threshold stress for the unreinforced AZ 91 alloy (Fig. 3(a)) and its composite (Fig. 3(b)) in double linear coordinates. Detailed inspection of the individual plots shows that a true stress exponent of 3 yields the best linear ﬁt – Fig. 3(b). The ﬁnding of n = 3 provides support for adopting the suggestion that the AZ 91 composite exhibits creep behaviour which is consistent with the behaviour anticipated for magnesium solid solution alloys. Similar results for QE 22 alloy and its composite show that, while no threshold stress was found in the case of monolithic QE 22 alloy, the values of the threshold stress of the composite at 473 K and 523 K were estimated as 22 MPa and 18 MPa, respectively.
0.10
0.010 0.008
0.04 0.02 0.00
0
50
100
0.006
σo= 59 MPa
0.004
3 K σ = 74 MPa o 42
0.002
150
STRESS σ [MPa]
(a)
n=3
473 K
423 K
0.06
. 1/ n  1/ n [s ] εm
n=3
47 3K
. 1/ n  1/ n εm [s ]
AZ 91+Saffil
AZ 91
0.08
200
0.000
0
50
100
150
200
STRESS σ [MPa]
(b)
Fig. 3. Procedure for determining the threshold stress r0 with its estimated values: (a) AZ 91 alloy (no threshold stress), (b) AZ 91 composite.
It was mentioned earlier, that indirect strengthening may be caused by the microstructural changes in the material. In our previous studies [2] we found that the threshold stress values are closely connected with the development of a continuous precipitate morphology of Mg17(Al, Zn)12 particles. Further, it was observed that the ﬁbres in the QE 22 composite can act as nucleation centre in the precipitation process, promoting precipitation of Al2Nd, Mg(Al)12Nd and Mg3Ag phases.
98
4.4
V. Sklenicka et al.
Matrix/Reinforcement Bonding
The creep behaviour of the composites may be substantially influenced by the matrix/ﬁbre interfaces. Weak matrix/reinforcement bonding may lead to inferior creep properties of the composite. Thorough fractographic investigations of the AZ 91 composite did not reveal either substantial creep ﬁbre cracking and breaking or any substantial debonding at the interfaces between the ﬁbres and the matrix due to creep. By contrast, and intensive debonding was revealed at the fracture surfaces at the QE 22 composite. Thus, in the limit of zero interface strength, where no stress can be transmitted to the ﬁbres, the composite may be weaker than the matrix alone. Detailed fractographic investigation revealed enhanced precipitation of secondary phases at the interfaces in the AZ 91 composite, which can favourably affect the strength of the matrix/ﬁbre interface and thus the creep behaviour of the composite (Fig. 4).
Fig. 4. Creep fracture surface: (a) good interface bonding due to an occurrence of precipitates at the ﬁbre surface (AZ 91 composite), (b) weak cohesion of the interface due to clean ﬁbre surface (QE 22 composite).
5 Conclusions Creep strengthening in the composite arises mainly from the load transfer and the existence of a threshold stress. The load transfer occurs by plastic deformation of the matrix being limited by the intact bond of the ﬁbre and enhanced precipitation of secondary phases. Acknowledgement. This research was carried out under the project CEITEC 2020 (LQ1601) with ﬁnancial support from the Ministry of Education, Youth and Sports of the Czech Republic under the National Sustainability Programme II.
The Creep Resistance of ShortFibre Reinforced Metal Matrix Composites
99
References 1. Mileiko, S.T.: Metal and Ceramic Based Composites. Elsevier, Amsterdam (1997) 2. Sklenicka, V., Pahutova, M., Kucharova, M., Svoboda, M., Langdon, T.G.: Creep processes in magnesium alloys and their composites. Metall. Mater. Trans. 33, 883–889 (2002)
Adhesive Joint Fracture Under Combined Pulsed and Vibrational Loading Yuri Petrov1,2, Andrey Logachev1(&), Nickolay Granichin1, and Grigory Volkov1 1
Saint Petersburg State University, Universitetskaya nab. 79, Saint Petersburg 199034, Russia [email protected] 2 Institute of Problems of Mechanical Engineering, Russian Academy of Sciences, Bolshoj pr. 61, V. O, Saint Petersburg 199178, Russia
Abstract. The strength of the adhesion joint under the combined vibrationalpulsed loading is considered. Beam and membrane models on elastic foundation is applied to simulate behavior of adhesion zone. The incubation time criterion is used to determine the threshold parameters of a load required to adhesive zone fracture. The solution of the differential equation describing the behavior of the adhesive zone is obtained by the Fourier method. Different types of combination of pulsed loading with highfrequency external ﬁelds are considered. It demonstrates that background vibration ﬁelds of even low intensity at certain frequencies can signiﬁcantly reduce these critical values. The dependence of the threshold value of the external pulse on the model parameters is shown. The possible way to control to adhesive joint strength by background vibrational ﬁelds is suggested. Keywords: Adhesion zone Vibrational ﬁeld
Incubation time criterion Elastic foundation
1 Introduction Highfrequency harmonic ﬁelds has a signiﬁcant impact on the strength properties of materials. Microelectromechanical Systems (MEMS) is a promising area for applying this effect. Previously, this effect has already been investigated on the model of the adhesion zone based on the string approximation [1]. Winkler base and its modiﬁcations are the most widely used approach for describing the adhesion joint [2–4]. The simplest onedimensional model of beam and 2Dmodel of membrane on the elastic foundation are considered. The influence of external harmonic ﬁelds on the strength of these models is subject of the study.
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 100–105, 2020. https://doi.org/10.1007/9783030478834_18
Adhesive Joint Fracture Under Combined Pulsed
101
2 Incubation Time Criterion The fracture criterion based on the concept of incubation time is used. This criterion is originally formulated in terms of stress. On the contrary, equations describing the behavior of the adhesive zone and boundary conditions are written using displacements. The assumption about elastic behavior is therefore accepted. It makes possible to rewrite the criterion in terms of displacements: 1 Zt uðgÞdg uc ; t2½0;tc s ts
ð1Þ
max
where uðtÞ is displacement, uc is a limit elongation of the link under quasistatic loading, s is fracture incubation time, tc is upper border of considered time period.
3 Adhesive Zone Models 3.1
Membrane Approximation
The adhesive zone of a circular membrane on an elastic base is considered. Only resistance to tensile forces is taken into account. The model is described by the following equation: @2u 1 @u 1 @ 2 u x2 þ u ¼ f ðr; tÞ; @r 2 r @r c2 @t2 c2
ð2Þ
where r is distance from the center of the membrane, c is the wave velocity, x is the characteristic of the elastic foundation of rigidity, f is the external force. Boundary conditions correspond to ﬁxed edge of the membrane and zero initial conditions is considered: uðr; 0Þ ¼
@u ðr; 0Þ ¼ 0; @t
uðR; tÞ ¼ 0:
ð3Þ
The solution of the problem (2, 3) is obtained by Fourier method [5]: n P uðr; tÞ ¼ fk ðr Þgk ðtÞ: k¼1
n J0 a0kRr 2c2 X Zt uðr; tÞ ¼ 2 0 2 R k¼1 Xðk Þ J ða0m Þ 0 0
sinðXðk Þðt gÞÞdg;
ZR
0
f ðe; gÞ e J0
a
om
R
e de
!
ð4Þ
where J0 – is the zeroorder Bessel function, a0m – are the zeroes of the zero Bessel qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ function, Xðk Þ ¼ c2 k2k þ x2 , kk ¼ R aok .
102
Y. Petrov et al.
Constant and Pulse Loading Concentrated constant force P and a background vibration ﬁeld of frequency m is considered: dðr Þ f ðr; tÞ ¼ P H ðtÞ 2 þ c sinðmtÞ ; R r where d(r) is the Dirac delta function, H(t) is the Heaviside function, c is a relative intensity of the background vibration ﬁeld. Fracture is considered at center point. Threshold force amplitude at which delamination of the adhesion zone occurs founded by Eq. (4) and fracture criterion (1). The dependence of the threshold amplitude P versus the background ﬁeld frequency m at various relative intensities c for this type of loading is shown in Fig. 1. Based on these results a signiﬁcant decrease of the threshold amplitude is observed at certain frequencies.
Fig. 1. Dependence of the load threshold amplitude on the background ﬁeld frequency, where load function is the combination of constant force and inﬁnite vibrational ﬁeld
Another considered type of loading is combination of impulse of ﬁnite duration T and background vibration ﬁeld: dð r Þ f ðr; tÞ ¼ P ðH ðtÞ H ðt T ÞÞ 2 þ c sinðmtÞ : R r The critical force change with increasing pulse duration is also investigated at a certain frequency of the background ﬁeld m ¼ Xð1Þ þ2 Xð2Þ. The results are presented on Fig. 2. The plot demonstrates a decrease of the threshold amplitude with the increasing of the pulse duration until T ¼ 0:1. Almost constant dependence is observed after this value.
Adhesive Joint Fracture Under Combined Pulsed
103
Fig. 2. Dependence of the pulse load critical amplitude on its duration in the continuous background vibrational ﬁeld
3.2
Beam Approximation
Similar results are obtained for the model based on beam approximation. BernoulliEuler beam on elastic foundation is considered. Tensile forces are neglected. In this case, the adhesion zone will be described by following equation [6]: @4w 1 @2w x2 þ þ w ¼ f ðx; tÞ; @x4 c2 @t2 c2
ð5Þ
where x is the coordinate along axis of the beam, w is vertical deflection. Zero initial conditions: wðx; 0Þ ¼
@w ðx; 0Þ ¼ 0: @t
ð6Þ
Boundary conditions of 3 types are considered • Hinged ends of the beam wð0; tÞ ¼ wðl; tÞ ¼ 0;
@2w @2w ð 0; t Þ ¼ ðl; tÞ ¼ 0; @x2 @x2
ð7Þ
@w @w ð0; tÞ ¼ ðl; tÞ ¼ 0; @x @x
ð8Þ
• Clamped ends of the beam wð0; tÞ ¼ wðl; tÞ ¼ 0;
104
Y. Petrov et al.
• Beam with free ends @2w @2w ð 0; t Þ ¼ ðl; tÞ ¼ 0; @x2 @x2
@3w @3w ð 0; t Þ ¼ ðl; tÞ ¼ 0: @x3 @x3
ð9Þ
Fig. 3. Dependence of the loading threshold amplitude on the background ﬁeld frequency for the clamped beam
The solution of the problem (5–9) is obtained as follows: 0 1 Zt Zl n X U ð x Þ k @ f ðn; gÞUk ðnÞdnÞÞAsinðXk ðt gÞÞdg; wðx; tÞ ¼ c2 2 U X k k k k k¼1 0
where Xk ¼
ð10Þ
0
qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Rl x2 þ c2 k4k ; kUk k2 ¼ ðUk ð xÞÞ2 dx, Uk and kk is solution of spectral 0
problem U IV k4 U ¼ 0 and expressions of these auxiliary parameters are given in the Table 1.
Table 1. Auxiliary parameters for different types of boundary conditions. Uk kk Hinged beam pk=l sin kk x Clamped beam Roots of chðklÞ cosðklÞ ¼ 1 K4 ðkk xÞ K4 ðkk lÞ K3 ðkk xÞ K3 ðkk lÞ Free ends
Roots of chðklÞ cosðklÞ ¼ 1 K2 ðkk xÞ K4 ðkk lÞ K1 ðkk xÞ K3 ðkk lÞ
Adhesive Joint Fracture Under Combined Pulsed
105
where Ki are the functions of Krylov: K1 ðzÞ ¼ ðch z þ cos zÞ=2 K2 ðzÞ ¼ ðsh z þ sin zÞ=2; K3 ðzÞ ¼ ðch z cos zÞ=2 K4 ðzÞ ¼ ðsh z sin zÞ=2: Constant Load External load of the following form is considered: l f ðx; tÞ ¼ P H ðtÞd x þ rsinðmtÞ : 2
ð11Þ
The loading is similar to the previous one. Solution is obtained in the same way as in the case of membrane. Figure 3 shows the dependence of vibrational frequency and critical force amplitude at point x ¼ l=2: The graph demonstrates the same effect of the threshold amplitude decrease as for membrane approximation.
4 Conclusion The observed effect of reducing the threshold load at certain frequencies appears even for harmonic ﬁelds of relatively small amplitude. In addition, the effect appeared for both models considered (membrane and beam approximation). This phenomena could be used in MEMS application with ultrasound as a control factor to shift volatile regimes of nano electromechanical switches.
References 1. Gorbushin, N., Petrov, Y., Zhao, Y.P., Zhang, Y.: Threshold characteristics of shortpulsed loads combined with the ultrasound ﬁeld causing dynamic delamination of adhesive joints. Theor. Appl. Mech. Lett. 8(1), 28–31 (2018) 2. Dillard, D.A., Mukherjee, B., Karnal, P., Batra, R.C., Frechette, J.: A review of Winkler’s foundation and its profound influence on adhesion and soft matter applications. Soft Matter 14(19), 3669–3683 (2018) 3. Godara, R.K., Joglekar, M.M.: Suppression of contact bounce in beamtype microelectromechanical switches using a feedforward control scheme. JVC/J. Vib. Control 24(23), 5502–5513 (2018) 4. Farokhi, H., Ghayesh, M.H., Gholipour, A., Tavallaeinejad, M.: Stability and nonlinear dynamical analysis of functionally graded microplates. Microsyst. Technol. 24(5), 2109–2121 (2018). https://doi.org/10.1007/s0054201838497 5. Polyanin, A.D., Zaitsev, V.F.: Handbook of Nonlinear Partial Differential Equations. Chapman and Hall/CRC (2016) 6. Zhang, Y., Zhao, Y.P.: Determining both adhesion energy and residual stress by measuring the stiction shape of a microbeam. Microsyst. Technol. 21(4), 919–929 (2015)
Study on the Fracture Mechanism of the P91 Steel During Small Punch Tensile Testing Hezong Li1,4(&), Hao Chen2, H. K. AlAbedy3,4, and Wei Sun4 1
2
Hebei University of Engineering, Handan 056038, China [email protected] University of Nottingham Ningbo China, Ningbo 315100, China 3 Wasit University, Wasit, Iraq 4 University of Nottingham, Nottingham NG7 2RD, UK
Abstract. This paper investigates the fracture generation processing of the P91 steel during a small punch tensile test. P91 disc specimens, 8 mm in diameter and 0.5 mm in thickness, were tested in a small punch test rig at 600 °C using a constant displacement rate of 2 µm/s. Interrupted tests were performed to investigate the crack generation and evolution of P91 in small punch tensile tests. The discshaped specimens were deformed into domes of different depths during the tests. Crosssectional microstructure analysis revealed that thinning and circumferential necking started to occur at the edge of contact before the maximum load was reached, and then signiﬁcant point necking occurred in the circumferential necking area after the maximum load. The crack formed during the tests aligns with the plastic flow of the specimen. Alignment of crack propagation occurred in the plastic deformation direction, before achieving the maximum small punch load. Keywords: Small punch tensile test P91 steel Deformation regimes Crack generation Fracture mechanism
1 Introduction In the last decade, testing techniques using miniature samples have received everincreasing attention from the electricity generation industry for situations where the amount of material used in the test is limited [1, 2]. The Small Punch Tensile Test (SPTT) is widely used as a miniature specimen test method to characterise the tensile mechanical properties for ductile metallic materials, with the specimen being a disc of *8 mm diameter and *0.5 mm thickness [3]. The punch was applied to the disc at a given constant displacement rate. The very small specimen size denotes that the SPTT can be considered as a limited volume and nondestructive methodology to provide a real evaluation of mechanical behaviours when compared with the conventional tensile test [4–7]. Moreover, the SPTT specimen can be taken directly from inservice components without signiﬁcantly affecting their structural integrity [8], allowing the mechanical behaviour to be examined using SPTT [9, 10]. In particular, the SPTT exhibits unique advantages in characterising power plant steels, of which the high temperature mechanical behaviour is crucial to the durability of pressure vessels. © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 106–111, 2020. https://doi.org/10.1007/9783030478834_19
Study on the Fracture Mechanism of the P91 Steel During Small Punch Tensile Testing
107
One of the power plant steels which is of great interest is the 9Cr1Mo steel (commercially known as P91). It is widely recognised that fracture in P91 steels occurs through progressive nucleation, growth and eventual coalescence of voids. Meanwhile, most studies are based on uniaxial tests, using standard specimens where necking appears in a location that cannot be controlled. The understanding and prediction of strain and damage interactions in P91 steels remain a challenging topic. At present, the biaxial loading state of SPTT appears to have the potential to examine the above physical phenomena to reveal the deformation and fracture mechanisms. However, work concerned on this aspect, especially in addressing the microscopic evidence with the deformation and fracture mechanisms of SPTT, does not appear to have been detailed until now. Therefore, considering the signiﬁcance of microstructure characteristics on the degradation of P91 during SPTT, the aim of the work reported in this paper is to investigate speciﬁcally the microstructural evolution of P91 during the SPTT, in an attempt to reveal the deformation mechanisms in different regimes of the SPTT. The results of a physical characterisation of the hightemperature deformation and fracture process of the P91 steel via SPTT at 600 °C are presented and the deformation and fracture mechanisms in different SPTT regimes are discussed.
2 Material and Experimental Procedure The asreceived P91 steel was machined into a cylinder shape with 8 mm in diameter and was then sliced into disc SPTT specimens with a thickness slightly larger than 0.5 mm using wire electrodischarge machining. The specimens were then ground down to a ﬁnal thickness of 0.5 mm using 1200grade silicon carbide papers. A Tinius Olsen H5KS single column material testing machine was used to perform the SPTTs. A 1.0 kN load cell, which has a loading accuracy of ±0.5% of the applied load, is installed to measure the load transmitted to the specimen through a hemispherical punch head. The displacement of the punch was recorded as the average reading of two linear variable differential transformers, which have an accuracy of ±0.01 mm, a resolution of 1 µm and a speed resolution of 1 µm/min. A constant displacement rate of 2 µm/s was applied to the punch when the specimen has failed or when the displacement of the punch has reached the setting values (for interrupted tests) and a backoff speed of 4 mm/s was applied.
3 Mechanical Behaviour 3.1
LoadDisplacement Curves
A schematic diagram of the applied force, F, and displacement, u, of SPTT for a ductile material is shown in Fig. 1a. According to Abendroth and Dymacek [11, 12], the Fu curve obtained from the present tests can be divided into six stages, representing different deformation regimes during SPTT. Thus, to investigate the physical nature of the above deformation process and the fracture behaviour of the P91 steel at 600 °C, a
108
H. Li et al.
series of interrupted SPTTs have been carried out. Firstly, two specimens are used to perform the repeated SPTTs for the whole stroke until fracture. The loaddisplacement curves obtained are shown in Fig. 1b. To investigate the deformation mechanisms of P91 in SPTT, the key interrupted displacements were determined based on Fig. 1a. The main objective of interrupted SPTTs is to provide “In Situ” investigations into the evolution of deformation at each stage of the SPTT until fracture. Seven interrupted SPTTs were conducted on the P91 steel at 600 °C in Fig. 1b. The interrupted displacements are set as 0.26, 0.60, 1.00, 1.25, 1.50, 1.65 and 1.74 mm respectively to represent the different deformation regimes in Fig. 1a.
Fig. 1. The schematic diagram of the SPTT loaddisplacement curve (a), the loaddisplacement curves at interrupted displacements and whole stroke (b).
3.2
Physical Characterization of the Deformation Process
The crosssectional microstructure of the above deformed P91 specimen is shown in Fig. 2. The small deformation after a displacement of 0.26 mm in Fig. 2a exhibits the dome shape is about to form due to the punch movement. It can be seen that the thickness of the specimen remains the same without obvious material thinning in Fig. 2a. The primary phase that can be seen is the prior austenitic phase in Fig. 2b. No large voids have formed yet for a displacement of 0.26 mm. The dome shape becomes more evident when the deformation of specimen increases. The alignment of the grains is not found in Fig. 2b and 2d, but such evidence is seen at large punch displacements in Fig. 2f and 2h. This indicates that the grain alignment will tend to occur when the plastic deformation becomes dominant. The beginning of necking occurs, as shown in Fig. 2e and g, due to the bending and stretching stress at the edge of contact between the punch and specimen. Figure 3 shows the crosssectional microstructure of the P91 after achieving the maximum load. The dome shape has developed further due to the increased punch displacements. It is noticed that the necking and thinning at the edge of contact progress in these specimens, where the thickness of the specimen has been further reduced, as shown in Fig. 3c due to the ongoing bending and stretching stresses under the biaxial loading state. Meanwhile, void nucleation and elongation are found to exist in Fig. 3b. Due to the large plastic deformation in these punch displacements, the voids
Study on the Fracture Mechanism of the P91 Steel During Small Punch Tensile Testing
109
have been deformed into elongated shapes of which the long axis is pointing in the direction of the plastic flow. The phases also align with the plastic flow in Fig. 3b and 3d. Moreover, it is found from Fig. 3d that the austentic and martensitic phases have been elongated along the plastic flow direction due to the extensive plastic deformation at the edge of contact. A number of voids, approximately 35 µm across, are found in Fig. 3d. The morphology of the voids has been further stretched and elongated. Figure 3e and 3f depict the microstructure of the fracture point at the edge of contact. It can be seen that the phases have also been elongated due to the large plastic
Fig. 2. The crosssectional microstructure of the P91 specimen at interrupted displacements of 0.26 mm (a & b), 0.6 mm (c & d), 1.0 mm (e & f) and 1.25 mm (g & h).
Fig. 3. The crosssectional microstructure of the P91 specimen at interrupted displacements of 1.5 mm (a & b), 1.65 mm (c & d) and 1.74 mm (e & f).
110
H. Li et al.
deformation in Fig. 3f. Some discrete and ellipsoidal voids are found in this region, especially close to the fracture site. Noting that signiﬁcant material necking and thinning have occurred during this stage, it is possible that the thinning of the specimen at the edge of contact allows the coalescence of voids to occur, resulting in the fracture of the specimen. Eventually, the tearing of the material occurs, producing the rough fracture surface.
4 Deformation and Facture Mechanisms Figure 4 gives the schematic diagram of deformation of P91 in SPTT at 600 °C at different stages. The ﬁrst stage, I, is related to the elastic deformation, which is not shown in Fig. 4. Stage II represents the transition zone from elastic to plastic deformation, in which at the beginning, the plastic deformation occurs in the local area outside of the contact zone of punch and specimens. And then it will expand to the materials in the gap between the punch and the die along the circle. Stage III represents the homogeneous plastic deformation and the specimen thickness will reduce relatively uniformly in the deformation zone (as shown Fig. 2a, c, e from punch displacement approximately 0.26 mm to 1.0 mm). In stage III, the energy consumed is more than 40% of the total energy. The thickness of specimen will reduce at local circle band near the punch contact area in stage IV (as shown in Fig. 2g), in which a circumferential necking will occur and the energy consumed rate is 20.2%, in which a circumferential necking will occur and the energy consumed rate is 20.2%. In stage V, the plastic deformation will focus on a point until crack occurring in the local circle band happened in stage IV (as shown in Fig. 3a, c), in which the voids will have a nucleation, growth, coalescence and creates a macroscale crack in the point necking area and the energy consumed 29.4% or so. Finally, the crack will extend and the material will be teared ductility until failure in state VI (as shown in Fig. 3e), in which the energy consumed is only 4.1% of the total energy due to the connect area reducing down to immediate failure.
Fig. 4. The schematic diagram of deformation regimes of P91 in SPTT at different stages.
Study on the Fracture Mechanism of the P91 Steel During Small Punch Tensile Testing
111
5 Conclusions The interrupted small punch tensile tests of P91 were performed at 600 °C to investigate the deformation and fracture mechanisms of P91. The dome shape of the SPTT specimen gradually develops when the punch displacements increase from 0.26 to 1.74 mm. It is found that the voids are likely to form after the maximum load is achieved, which indicates that the fracture of the P91 specimen is starting to occur. From the microstructure evolution, it is shown that signiﬁcant necking and thinning occur after the maximum load.
References 1. Morris, A., Cacciapuoti, B., Sun, W.: The role of small specimen creep testing within a life assessment framework for high temperature power plant. Int. Mater. Rev. 63, 102–137 (2018) 2. Hyde, T.H., Sun, W., Williams, J.A.: Requirements for and use of miniature test specimens to provide mechanical and creep properties of materials: a review. Int. Mater. Rev. 52, 213– 55 (2007) 3. Blagoeva, D., Hurst, R.: Application of the CEN (European Committee for Standardization) small punch creep testing code of practice to a representative repair welded P91 pipe. Mater. Sci. Eng., A 510, 219–223 (2009) 4. Panayotou, N., Puigh, R., Opperman, E.: Miniature specimen tensile data for high energy neutron source experiments. J. Nucl. Mater. 104, 1523–1526 (1981) 5. Madia, M., Foletti, S., Torsello, G., Cammi, A.: On the applicability of the small punch test to the characterization of the 1CrMoV aged steel: mechanical testing and numerical analysis. Eng. Fail. Anal. 34, 189–203 (2013) 6. Lucas, G.: The development of small specimen mechanical test techniques. J. Nucl. Mater. 117, 327–339 (1983) 7. Ha, J.S., Fleury, E.: Small punch tests on steels for steam power plant (I). KSME Int. J. 12, 818 (1998) 8. Rodríguez, C., Fernández, M., Cabezas, J., García, T., Belzunce, F.: The use of the small punch test to solve practical engineering problems. Theoret. Appl. Fract. Mech. 86, 109–116 (2016) 9. Rodríguez, C., García, J., Cárdenas, E., Belzunce, F., Betegón, C.: Mechanical properties characterization of heataffected zone using the small punch test. Weld Jt. 88, 188–192 (2009) 10. Fernández, M., Rodríguez, C., Belzunce, F., García, T.: Use of small punch test to estimate the mechanical properties of powder metallurgy products employed in the automotive industry. Powder Metall. 58, 171–177 (2015) 11. Dymáček, P.: Recent developments in small punch testing: applications at elevated temperatures. Theoret. Appl. Fract. Mech. 86, 25–33 (2016) 12. Abendroth, M.: FEM analysis of small punch tests. Key Eng. Matet. 734, 23–36 (2017)
Damage Accumulation and Growth Models for the CreepFatigue Interaction A. V. Tumanov(&) and V. N. Shlyannikov Institute of Power Engineering and Advanced Technologies, FRC Kazan Scientiﬁc Center, Russian Academy of Sciences, Kazan, Russia [email protected]
Abstract. The residual life prediction based on damage accumulation models for the BT31 titanium alloy are present. Mechanical properties were obtained at temperature 370 °C. Life prediction was based on the Kachanov–Rabotnov damage model for creep and the DuyiZhenlin model for fatigue. The contribution of each type of loading to the generalized damage parameter was calculated according to the law proposed by Skelton and Grandy. Damage accumulation laws were integrated into ANSYS software. Cyclic loading with a trapezoidal form cycle was simulated. The integrated model of damage accumulation under creepfatigue interaction allows obtaining a fatigue life of structural elements. The model is recommended to be used for cases when the scalar damage parameter is justiﬁed. Keywords: Creepfatigue interaction Damage accumulation Life prediction
1 Introduction It is well known that the creep damage accumulation is different from damage caused by cyclic loading. At the moment, there are many models allow to take into account the damage accumulation, both during creep and cyclic loading independently. The Hayhurst model [1] one of the most generalized models for the creep damage accumulation. In order to describe the damage accumulation according to this model, it is necessary to use six material constants. Moreover, the methods for determining these constants are mainly indirect. In this regard, the RabotnovKachanov model one of the most popular due to the direct method of material constants. One of the most perspective model for the fatigue damage accumulation prediction is the Lemaitre model [2]. Using the tensor damage parameter in similar phenomenological models leads to considerable difﬁculties for material constants determination. In the identical creep laws if the stress state is unchanged and scalar, vector, and tensor parameters give almost identical results. It is correct not only for a “pure” complex stress state, but for solving some boundary value problems In this regard, models with scalar damage parameters can be considered as a simpliﬁed alternative [3–6]. The main problem of the residual life prediction under the creepfatigue interaction is the complex nature of their interaction [7–10]. In this direction the most common approach is the statistical approximation of the experimental results by any functions. The basic procedure for taking into account the creepfatigue interaction isn’t © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 112–116, 2020. https://doi.org/10.1007/9783030478834_20
Damage Accumulation and Growth Models
113
introduced in any ﬁnite element software. Simple summation is used at most cases. In this regard, there is a need to develop damage accumulation models taking into account a complex nature of creepfatigue interaction.
2 Damage Accumulation Model According to [7] it is recommended to use the following expression to calculate the total level of accumulated damage under creepfatigue interaction: Dx ¼
Dxcr Dxf þ ; 1 Dxf 1 Dxcr
ð1Þ
where Dxcr  creep damage increment, Dxf  fatigue damage increment. At the beginning of each iteration, the level of accumulated damage from fatigue and creep is determined independently. General integration is carried thru taking into account the both contribution. The creep damage is proposed to be established by the classical KachanovRabotnov power law. According to this model, the strain rate, taking into account the accumulation of damage, is written as follows: e_ e ¼ B
re 1 xcr
n
:
ð2Þ
where the creep damage accumulation rate is: m dxcr re ¼D : dt 1 xcr
ð3Þ
B, n, D, m – material properties. The creep damage increment can be obtained by integrating the expression (3): Dxcr ¼ 1 ½ðDrm Dt C3 Þðm þ 1Þm þ 1 : 1
ð4Þ
where C3  integration constant which can be determined from the previous iteration. C3 ¼
ð1 x0 Þm þ 1 Drm e t0 : mþ1
ð5Þ
It is well known that the creep damage accumulation is different from damage caused by fatigue. Usually, the one of the main characteristic in models with a scalar damage parameter is the number of cycles before fracture Nf at the stress amplitude ra . In the simplest case of uniaxial tensioncompression, the relationship between them is follow:
114
A. V. Tumanov and V. N. Shlyannikov
2Nf ¼
ra r0f
!1b ;
ð6Þ
where r0f and b are fatigue constants. The damage parameter at constant stress amplitude is determined from [3] xfN1 N xf ¼ ln 1 : Nf ln Nf
ð7Þ
where xfN1  the critical value of the damage parameter in the penultimate cycle and it is associated with static toughness UT0 by the following relationship: xfN1 ¼ 1
r2a : 2EUT0
ð9Þ
where E  Young’s modulus.
3 Mechanical Properties and Finite Element Modeling Mechanical properties were obtained during static, cyclic and creep tests (Table 1). Table 1. Mechanical properties of BT31 for 370 °C E, MPa m B, (MPan.h)−1 n r02, MPa C, (MPan.h)−1 M 97553 0.3 1e−15 1.934 699 1e−10 3
In order to predict the residual life at creepfatigue interaction, the above models were integrated into the ANSYS ﬁnite element method software as user programmable features. The ﬁnite element model of the specimen geometry recommended by ASTM E466 was used. The threedimensional model of the specimen consists of two hundred thousand of second order ﬁnite elements. In numerical simulation, the loading was applied in the form of a trapezoidal loading cycle with different holding time (6, 60, 600 and 3600 s).
4 Results and Discussion The stressstrain ﬁelds in cylindrical specimen were obtained by ﬁnite element method with taking into account the accumulated damage on each loading cycle. It is assumed that the failure is occur if the value of the generalized damage parameter exceeded 0.9 at any point in specimen volume.
Damage Accumulation and Growth Models
115
Fig. 1. Relationship between the fatigue life and the time to failure
Figure 1 shows the numerical results of the fatigue life prediction at various combinations of applied load levels and holding time within each loading cycle. It is shown that the integrated damage accumulation model allows to cover the wide spectrum of load parameters for creepfatigue interaction. The relative damage accumulation rate in each loading cycle can be considered as a parameter characterizing the contribution of load type to the total damage. The dependences of relative damage rate on the holding time for the penultimate loading cycle are shown in Fig. 2. It is clear that the increasing load level leads to situation when fatigue makes a greater contribution to the overall damage of the material. Accordingly, the nominal stresses decreasing leads to increasing of creep contribution to the damage.
Fig. 2. Relationship between the holding time and the relative damage accumulation rate
116
A. V. Tumanov and V. N. Shlyannikov
5 Conclusions The model allows to take into account the nonlinear contribution of damage accumulation caused by creepfatigue interaction is integrated into the ANSYS software as user programmable features. Integrated model of damage accumulation allow, to predict the macro damage initiation during the creepfatigue interaction.
References 1. Hayhurst, D.R.: Creep rupture under multiaxial states of stress. J. Mech. Phys. Solids 20, 381–390 (1972). https://doi.org/10.1007/9783642844553_43 2. Lemaitre, J.: Coupled elastoplasticity and damage constitutive equations. Comput. Methods Appl. Mech. Eng. 51, 31–49 (1985). https://doi.org/10.1016/00457825(85)90026X 3. Ye, D.Y., Wang, Z.L.: A new approach to lowcycle fatigue damage based on exhaustion of static toughness and dissipation of cyclic plastic strain energy during fatigue. Int. J. Fatigue 23, 679–687 (2001). https://doi.org/10.1177/1056789512456030 4. Lv, Z., Huang, H.Z., Zhu, S.P., Gao, H., Zuo, F.: A modiﬁed nonlinear fatigue damage accumulation model. Int. J. Damage Mech 24, 168–181 (2015). https://doi.org/10.1177/ 1056789514524075 5. Zhang, J., Xi, F., Lin, J., Liu, Z., Liu, N., Bin, W.: Study on damage accumulation and life prediction with loads below fatigue limit based on a modiﬁed nonlinear model. Materials 11, 1–16 (2018). https://doi.org/10.3390/ma11112298 6. Huang, T., Ding, R.C., Li, Y.F., Zhou, J., Huang, H.Z.: A modiﬁed model for nonlinear fatigue damage accumulation of turbine disc considering the load interaction effect. Metals 9 (919), 1–10 (2019). https://doi.org/10.3390/met9090919 7. Skelton, R.P., Gandy, D.: Creep – fatigue damage accumulation and interaction diagram based on metallographic interpretation of mechanisms. Mater. High Temp. 25, 27–54 (2008). https://doi.org/10.3184/096034007X300494 8. Esztergar, E.P.: Creepfatigue interaction and cumulative damage evaluations for type 304 stainless steel. OAK Ridge National Laboratory, Oak Ridge, Tennessee, p. 131 (1972) 9. Barbera, D., Chen, H., Liu, Y.: On creep fatigue interaction of components at elevated temperature. J. Press. Vessel Technol. Trans. ASME 138, 28 (2015). https://doi.org/10.1115/ 1.4032278 10. Wright, J.K., Carroll, L.J., Sham, T.L., Lybeck, N.J., Wright, R.N.: Determination of the creep–fatigue interaction diagram for alloy 617. In: Proceedings of the ASME 2016 Pressure Vessels and Piping Conference. PVP201663704, pp. 110 (2016). https://doi.org/10.1115/ PVP201663704
Crack Growth and Plastic, Fracture Process and Damage Zones Behavior Under Mixed Mode Loading Valery Shlyannikov(&) and Daria Fedotova FRC Kazan Scientiﬁc Center of Russian Academy of Sciences, Kazan 420111, Russia [email protected]
Abstract. Fatigue crack paths for inclined cracks are studied through experiments and computations under different mixedmode loading. The experimental study of fatigue crack growth in the aluminum and titanium alloys and two types of the steels is performed on compact tension shear specimens. The cyclic fracture process and damage zone concepts are introduced and used for numerical analysis of the crack tip ﬁelds. The elastic K1, K2 and plastic KP stress intensity factors are calculated by ﬁnite element method to characterize the fracture resistance along the curvilinear trajectories in compact tension shear specimens. The influence of modemixity and elasticplastic material properties on the behavior of three crack tip regions as a function of cyclic loading is demonstrated. Keywords: Crack path
Fracture process and damage zones Mixed mode
1 Introduction To date, several of models have been presented in the literature for the purpose of analyzing the process of fatigue crack growth from the viewpoints of micromechanics, fracture and damage mechanics. Many fracture mechanics models are based on a critical distance local to the crack tip. It is considered a fundamental characteristic parameter that distinguishes damage at the microscopic and macroscopic scale levels. This characteristic distance is often identiﬁed with a fracture process zone or fracture damage zone. A general assumption regarding the distance criterion under elastic– plastic cyclic loading conditions is that a crack increment occurs when the fracture resistance parameter (stress, strain, or energy) reaches a critical value at a characteristic distance from the crack tip. It is well known that mixedmode conditions appear when the direction of the applied loading does not coincide with the orthogonal KIKIIKIII space. The main feature of the mixedmode fracture is that the crack growth no longer takes place in a selfsimilar manner and does not follow a universal trajectory. Various fracture criteria and phenomenological approaches can predict the behavior of cracks in
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 117–123, 2020. https://doi.org/10.1007/9783030478834_21
118
V. Shlyannikov and D. Fedotova
brittle and ductile materials loaded in combined modes. Even though many studies have been carried out in the literature to determine fracture characteristics of ductile materials under cyclic loading, it is important to investigate the local crack tip zones behavior due to low cycle fatigue for quasibrittle and moderate ductile materials under mixed mode conditions.
2 Material Properties and Loading Conditions Compact tension shear specimens (CTS, Fig. 1a) are made from P2M and 34X steels as well as aluminum Al7050 and titanium Ti6Al4 V alloys and used for cyclic mixedmode fracture test with the loading direction variation from 90° (pure Mode I) to 0° (pure Mode II) with respect to the initial crack plane. Main static and lowcyclic mechanical properties of the tested materials are listed in Tables 1 and 2. The mixedmode parameters expressed through the elastic and plastic stress intensity factors (SIFs) were varied by changing the load direction. Both Mode I and Mode II elastic SIFs K1 and K2 as well as general plastic SIF KP are evaluated along experimental crack path of each tested material based on the series of numerical calculations. On the CTS was realized the full range of mixedmode cyclic fracture from tensile to shear loading. Figure 1b represents experimental fatigue crack growth trajectories with initial pure Mode II loading for tested steels, aluminum and titanium alloys.
Table 1. The static properties of materials. Material P2M steel 34X steel Al7050 Ti6Al4 V
E (GPa) 226.9 216.21 70.57 118.0
r0 (MPa) rb (MPa) 362.4 636.0 714.4 1040.0 471.6 524.4 118.0 963.8
ru (MPa) N 1190.0 4.13 1260.4 7.89 701.0 10.85 1289.6 12.59
Table 2. The cyclic properties of materials. Material
r0f
B
e0 f
c
Kʹ
nʹ
P2M steel 34X steel Al7050 Ti6Al4V
1785.0 1890.6 1170.7 2153.6
−0.087 −0.087 −0.095 −0.095
0.424 0.381 0.35 0.35
−0.58 −0.58 −0.69 −0.69
1963.5 2079.6 1128.6 2076.2
0.15 0.15 0.11 0.11
a 4.141 0.529 1.570 1.225
Crack Growth and Plastic, Fracture Process and Damage Zones Behavior
119
Fig. 1. Experimental crack paths in CTS specimens at pure mode II.
Crack growth in the CTS specimen with the applied load angle b = 0° has its own characteristics. Initially, the deformation mode corresponds to the pure shear with ME = MP = 0. With an increase in the number of loading cycles N, the contribution of mixed modes of deformation and fracture gradually increases. As follows from Fig. 1, the crack path in an aluminum alloy Al7050 differs signiﬁcantly from the experimental trajectories for other materials under the same loading conditions.
3 Plastic, Cyclic Fracture Process and Damage Zones Behavior In front of a stable growing crack, we may distinguish three regions. The ﬁrst outer contour represents the reversed plastic zone where the current values of stresses and deformations exceed the yield stress or strain of the material. The second region is fatigue fracture process zone. The third small area exists immediately ahead of the crack tip which is called the damage zone. For a strainhardening material the elasticplastic boundary around the crack tip can be obtained using the equivalent von Mises stress as a function of principal stress ratio k = r2/r1 re ¼ r1 gi pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
ð1Þ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 k þ k2 þ mðm 1Þð1 þ kÞ2 .
where for plane stress gi ¼ 1 k þ k2 and plane strain gi ¼ Fullﬁeld 3D FEanalyses are carried out to determine stressstrain ﬁelds, elastic and plastic SIFs along the curvilinear crack path in the CTS subjected to different mixed mode loadings. Figure 2 shows that, for pure mode I (Fig. 2a) and pure mode II (Fig. 2b) the plastic zones have a symmetrical shape while for mixed mode (Fig. 2c) they is nonsymmetrical with respect to the initial crack plane. The dimensions of the plastic zones in Fig. 2 for titanium alloy are satisﬁed to the conditions of smallscale yielding. Similar shapes of plasticity zones are observed for other tested materials.
120
V. Shlyannikov and D. Fedotova
Fig. 2. Plastic zone under different mode mixity in CTS specimen for Ti6Al4 V.
The variable critical distance is one of important parameter in modern fracture mechanics, denoted to as the fracture process zone (FPZ) size. A general assumption regarding the distance criterion under elastic–plastic cyclic loading is that a crack increment occurs when the fracture resistance parameter (stress, strain, or energy) reaches a critical value at a characteristic distance from the crack tip. The following expression was proposed by Shlyannikov [1] for normalized fracture process zone size based on the nonlinear cracktip stress ﬁeld and the main low cycle fatigue material properties rf ¼
2 0 0 ð b þ cÞ rf ef E rn ðS1 þ SP Þ= 4 2 2Nf r0 r0
0 0 Keqv 2 ren þ 1 S1 ¼ ð1 þ mÞ a11 Y 2 þ a12 Y1 Y2 þ a22 Y 2 ; SP ¼ an p~ pﬃﬃﬃﬃﬃﬃ 1 2 2 ð n0 þ 1Þ I n rn pa
ð2Þ
ð3Þ
where n′ is low cycle fatigue hardening exponent, e0f and r0f are the fatigue ductility and strength coefﬁcients, respectively, a is the crack length, ru is the ultimate true tensile ~e ðhÞ is dimensionless strength, r0 is the yield stress, rn is the nominal stress, r equivalent stress angular function, In is the governing parameter of the nonlinear crack tip ﬁeld [1], Nf is the number of cycles to failure, Y1 and Y2 are geometry dependent for SIF correction factors. The equivalent elastic stress intensity factor (SIF) for mixed mode fracture can be determined by using energy release rate criterion [2] Keqv ¼ cos
h 2
qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ K12 ð1 þ cos h Þ 4K1 K2 sin h þ K22 ð5 3 cos h Þ
pﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃ K1 ¼ rn pa Y1 ða=wÞ; K2 ¼ rn pa Y2 ða=wÞ
ð4Þ ð5Þ
where, h* is the crack deviation angle, w is the cracked body width. The most general criterion of mixed mode crack growth direction is obtained [3] on the basis of the limiting state theory under multiaxial loading.
Crack Growth and Plastic, Fracture Process and Damage Zones Behavior
121
During lowcycle fatigue, the accumulation and growth of damage occurs in the local fracture process zone that covers the crack tip. The size of the fracture process zone is typically regarded as a distancedependent parameter that physically represents the increase in crack size during the basic cyclic fracture process. Figure 3 shows the dependence of the both size and shape of the fracture process zone, according to Eqs. (2–5), on the accumulated number of loading cycles for the pure mode (Fig. 3a), pure mode II (Fig. 3b) and mixed mode (Fig. 3c, d) loading. It can be clearly observed that the FPZ contour behavior is not constantsize and were dependent on the accumulated loading cycles, mode mixity and both the static and lowcycle fatigue material properties. Figure 3c presents the process of changing the FPZ in the 7050 aluminum alloy according to the stages of cyclic loading, which are accompanied by corresponding changes in the mixed modes of fracture. Figure 3d give a comparison of the dimensions of the mixedmode fatigue fracture process zone in the CTS specimen for all tested materials having different crack paths at ﬁnal the number of cycles of loading, N/Nf = 1, as shown in Fig. 1b. Initially, owing to the same pure mode II plastic deformation in the crack tip region in several ﬁrst cycles, the size of the lowcycle fatigue fracture process zone due to mode mixities is changed in different degree as a function of the tested material main mechanical properties.
Fig. 3. Fracture process zone contour under (a) pure mode I, (b) pure mode II and (c, d) mixed modes cyclic fracture.
122
V. Shlyannikov and D. Fedotova
A fatigue damage evolution equation was proposed by the authors [4] through connecting the damage variable with the static toughness exhausting during cyclic loading. This equation has the following form xN ¼
xN1 N ln 1 ; Nf ln Nf
ð6Þ
where xN−1 denotes the critical value of the damage variable, that is expressed by xN1 ¼ 1
Dr2 2Eru
ð7Þ
An amplitude of cyclic stress at the crack tip can be determined by applying the singular HRRtype stress ﬁeld 1 0
Prcn þ 1 r ~ ð hÞ Dr ¼ K
ð8Þ
where KP is the plastic stress intensity factor and rc is the critical distance. The damage variable xN indicate in Eq. (6) the measure of fatigue damage with xN = 0 denoting the undamaged state and xn = 1 the fully damaged state.
Fig. 4. Damage distributions as a function of accumulated number of loading cycles (apure mode I, bmixed mode).
Figure 4 presents a comparison of the predicted values of the fatigue fracture damage evolution for pure mode I (Fig. 4a) and mixed modes (Fig. 4b) according to Eqs. (6–8) for all considered structural metallic materials. It may be seen that the mode mixity changed signiﬁcantly the processes of fatigue damage accumulation only in the range N/Nf < 0.5. In this work, an expression for the low cycle fatigue fracture process is derived; this includes static and cyclic material properties, as well as mixed mode fracture parameters. The elastic–plastic crack tip singularity ﬁelds are employed. The main ﬁnding,
Crack Growth and Plastic, Fracture Process and Damage Zones Behavior
123
based on the numerical and experimental results, is that the effect of mixed mode fracture during lowcycle fatigue crack growth in considered steels, aluminum and titanium alloys leads to the conclusion that under pure mode I, pure mode II and mixed mode loading conditions and shape and size of the plastic, fracture process and damage zones do not coincide with each other and have a hierarchical structure.
References 1. Shlyannikov, V.N.: Creep–fatigue crack growth rate prediction based on fracture damage zone models. Eng. Fract. Mech. 214, 449–463 (2019) 2. Citarella, R., Cricri, G.: Comparison of DBEM and FEM crack path predictions in a notched shaft under torsion. Eng. Fract. Mech. 77, 1730–1749 (2010) 3. Shlyannikov, V.N.: Mixedmode static and fatigue crack growth in central notched and compact tension shear specimens. ASTM STP 1359, 279–294 (1999) 4. Duyi, Y., Zhenlin, W.: A new approach to lowcycle fatigue damage based on exhaustion of static toughness and dissipation of cyclic plastic strain energy during fatigue. Int. J. Fatigue 23, 679–687 (2001)
Miscellaneous (Computational Mechanics, Dynamics, Nanomaterials, Plasticity, Wave Propagation)
Parametric Resonance of a Microbeam with Flexible Support Under Fringing Field Excitation Zhichong Wang(&) Hebei University of Engineering, Handan, China [email protected] Abstract. A new resonance structure with flexible support under electrostatic fringing ﬁeld excitation is designed. This structure can be used in sensor. In this paper, the nonlinear frequency responses of the movable beam in resonance structure are analyzed by the Method of Multiple Scales. The effects of electrode thickness, slit gap and initial displacement on the vibration of the movable beam are investigated in detail. The key results are as follows. A smaller electrode thickness and slit gap can lead to a larger change of the actuated frequency, and they can also lead to a larger vibration amplitude. The initial displacement has an influence on the frequency response, but this influence is not obvious, since the electrostatic force is small when the initial displacement is not large. This resonance structure can avoid superposition of input signal and output signal. Thus, the signaltonoise ratio and the accuracy of the sensor can be improved. Keywords: Electrostatic MEMS Parametric resonance excitation Flexible support Nonlinear response
Fringing ﬁeld
1 Introduction The sensing mechanisms or actuation mechanisms for Micro Electro Mechanical Systems (MEMS) mainly include electrothermal mechanism [1, 2], piezoelectric mechanism [3, 4] and electrostatic mechanism [5–10]. Among them, the last one is the most popular because of its fast speed, low power consumption, ease of fabrication and small size. In electrostatic MEMS, the gap between movable structure and stationary electrodes can be changed, once the electric ﬁeld is applied on the surface of the movable structure. The electrical stiffness acts in conjunction with the mechanical stiffness. By modulating the applied voltage, the overall stiffness of the structure can be controlled. The electric force is nonlinearly related to the gap distance between movable structure and stationary electrodes. Thus, it can drive the system into parametric resonance if the voltage is large enough to overcome nonconservative forces and the driving frequency is inside an instability tongue (usually at twice the natural frequency). This parametric excitation system is excited by changing the parameters of the system instead of applying a direct force in the direction of desired motion [11].
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 127–132, 2020. https://doi.org/10.1007/9783030478834_22
128
Z. Wang
More attractive than other nonlinear system, parametric excitation system, in which resonance occurs at twice the natural frequency, can avoid superposition of input signal and output signal. In this paper, a new resonance structure with flexible support is designed; an analytical investigation of the parametric vibration actuated by fringing electrostatic ﬁelds is provided; the nonlinear behaviors are analyzed.
2 Problem Formulation A new resonance structure with flexible support is designed. This structure includes movable beam, support beam and electrode, as shown in Fig. 1. In Fig. 1, lb wb and tb denote the length, width and thickness of the movable beam respectively; lb0 wb0 and tb0 denote the length, width and thickness of the support beam respectively; ws and ts denote the width and thickness of the stationary electrode respectively; dg is the slit gap between the movable beam and stationary electrode in the width direction; dg0 is the slit gap between the support beam and stationary electrode in the width direction; d is the initial displacement of the movable beam measured from the stationary electrode in the thickness direction. In order to study the vibration behaviors of the beam, the geometric parameters of the structure are taken as lb = 5 mm, wb = 0.4 mm, tb = 0.01 mm, lb0 = 1 mm, wb0 = 0.4 mm, tb0 = 0.01 mm, ws = 0.5 mm, ts = 0.3 mm, dg = 0.1 mm and dg0 = 0.5 mm. The range of the initial displacement is less than half of the electrode thickness in this structure.
Fig. 1. Schematic illustration of resonance structure (a) 3D view (b) section view
Make u(x, t) denote the deflection of the movable beam. According to the elastic beam theory, the governing equation and the boundary conditions of the beam are EI EI
@ 4 uðx; tÞ @ 2 uðx; tÞ þ qwb tb ¼ qa þ qe 4 @x @t2
ð1Þ
@ 2 uð0; tÞ @uð0; tÞ @ 3 uð0; tÞ @ 2 uðlb ; tÞ @ 3 uðlb ; tÞ ; EI ¼ k ¼ k u ð 0; t Þ; ¼ 0; ¼ 0: r t @x2 @x @x3 @x2 @x3
ð2Þ
Parametric Resonance of a Microbeam with Flexible Support
129
In this paper, the coefﬁcients in the above equations are as following. The Young’s modulus is E = 108GPa. The inertial moment of the movable beam cross section is I ¼ wb tb3 =12. The mass density of the beam is q = 8500 kg/m3. qa represents the aerodynamic force per unit length, which is qa = − 0.5 qa wb ca (∂u/∂t) ∂u/∂t, and the drag coefﬁcient is set as ca = 5, qa is the density of the air. qe represents the excitation force per unit length. The electrostatic force is generated on the basis of the fringing ﬁelds. The distributed electrostatic force is qe ¼ fe v2e . fe is electrostatic force on the movable beam per unit length per square voltage, which is set as fe = r1 d r3 d3, and r1, r3 are ﬁtting parameters. Thus, the relationship between electrostatic force and deflection is fe = ep (1 + ep1 u + ep2 u2 + ep3 u3), in which ep = r1 d + r3 d3, ep1 = (r1 + 3r3 d2)/ep, ep2 = 3 r3 d/ep, ep3 = r3/ep. ve is a combined DC/AC voltage actuating the microbeam, i.e., ve (t) = vDC + vAC cos(xe t). In the boundary conditions, kr = 2 EI0/lb0 and kt = −2 3 E I0/l3b0 are the rotational and translational stiffness of the flexible boundary respectively, in which I0 = wb0 t3b0/12 is the inertial moment of the support beam cross section. The Galerkin discretization method is used, and the steadystate solution of the nondimensional governing equation is written by U(X, T) = U(X) H(T), and the mode function U(X) for movable beam is U(X) = n1 cos(kr X) + n2 sin(kr X) + n3 ch(kr X) + n4 sh(kr X), Substituting this mode function into the nondimensional boundary conditions yields 2
kr 6 KT 6 4 coskr sin kr
KR k3r sinkr coskr
kr KT chkr shkr
32 3 n1 KR 6 n2 7 k3r 7 76 7 ¼ 0 shkr 54 n3 5 chkr n4
ð3Þ
For a nontrivial solution, the determinant of the matrix on the left side must be zero, thus the value kr is given. Then, the equation of the boundary condition is solved to ﬁnd n1, n2, n3 and n4. Thus, the mode function can be obtained. Multiplying the nondimensional governing equation by the mode function, and integrating the resultant equation from X = 0 to 1. The displacement splits into a static displacement and a dynamic displacement, i.e. H(T) = H0p + #p (T), and we obtain static equation and dynamic equation. S0 þ S1 H0p þ S2 H20p þ S3 H30p ¼0 #00p þ K1 #p þ K2 #2p þ K3 #3p þ aa #0p #0p ¼ 2 3 ðFE1 cos We T þ FE2 cos 2We T Þ 6 7 6 þ KE1P1 #p þ KE1P2 #2p þ KE1P3 #3p cos We T 7 6 7 4 5 2 3 þ KE2P1 #p þ KE2P2 #p þ KE2P3 #p cos 2We T
ð4Þ
ð5Þ
130
Z. Wang
The Method of Multiple Scales is used to investigate the response of the resonator with small vibration amplitude. We obtain steadystate response as following 2 2 2 W e aa 3K3 2 We2 2K1 15K32 4 a0 2 þ 2 a20 KEP21 þ a KEP22 ¼ KEP22 KEP21 p 2e 2e e 16We2 0 2 We aa 3K3 2 We2 2K1 15K32 4 a tan 2b0 ¼ þ 2 a KEP2 a0 KEP1 = p 2e 0 2e2 e 16We2 0
ð6Þ ð7Þ
3 Dynamic Analysis Based on the steadystate response equation, the thickness of electrode is set as ts = 0.20 mm and ts = 0.30 mm, the slit gap between the movable beam and stationary electrode in the width direction is set as dg = 0.06 mm, dg = 0.08 mm and dg = 0.10 mm, the frequency response curves are shown in Fig. 2 to analyze the effect of electrode thickness and slit gap. As shown in Fig. 2, a smaller electrode thickness and slit gap can lead to a larger change of the actuated frequency, and they can also lead to a larger vibration amplitude. What’s more, as shown in Fig. 2, the resonance occurs at twice the natural frequency, which can avoid superposition of input signal and output signal; the range of the actuated frequency is related small, which can serve and improve the signaltonoise ratio. These advantages can improve the accuracy of the sensor.
Fig. 2. Frequency response curves showing the effect of electrode thickness and slit gap (a) ts = 0.20 mm (b) ts = 0.30 mm
The system parameters are set as ts = 0.30 mm and dg = 0.10 mm. The dynamic equation is solved by using the MMS and the Fourth  Order Runge  Kutta Method (RK4). Figure 3 shows the effects of the initial displacement on the frequency response when lb0 = 0.01 mm. As shown in the ﬁgure, the results of the MMS and the RK4 are in a good agreement when the amplitude is small; the error between the results of the
Parametric Resonance of a Microbeam with Flexible Support
131
MMS and the RK4 increases, when the vibration amplitude increases. The initial displacement has an influence on the frequency response, but this influence is not obvious, since the electrostatic force is small when the initial displacement is not large.
Fig. 3. Frequency response curves of the MMS and the RK4 showing the effect of initial displacement
4 Conclusions This paper investigates a new resonance structure with flexible support. This resonator is a parametric excitation system, which resonance occurs at twice the natural frequency. The nonlinear behaviors of the movable beam are analyzed by using the MMS to get the frequency response equation. The effects of electrode thickness, slit gap and initial displacement on the vibration of the movable beam are focused. A smaller electrode thickness and slit gap can lead to a larger change of the actuated frequency, and they can also lead to a larger vibration amplitude. The initial displacement has an influence on the frequency response, but this influence is not obvious, since the electrostatic force is small when the initial displacement is not large. This resonance structure can avoid superposition of input signal and output signal. Thus, the signaltonoise ratio and the accuracy of the sensor can be improved.
References 1. Shi, H., Fan, S., Zhang, Y., Sun, J.: Nonlinear dynamics study based on uncertainty analysis in electrothermal excited MEMS resonant sensor. Sens. Actuators A 232, 103–114 (2015) 2. Ramini, A.H., Hajjaj, A.Z., Younis, M.I.: Tunable resonators for nonlinear modal interactions. Sci. Rep. 6, 9 (2016) 3. Ahmed, S., Ounaies, Z., Arrojado, E.A.F.: Electric ﬁeldinduced bending and folding of polymer sheets. Sens. Actuators A 260, 68–80 (2017) 4. Wang, C., Zhang, Q., Wang, W., Feng, J.: A lowfrequency, wideband quadstable energy harvester using combined nonlinearity and frequency upconversion by cantileversurface contact. Mech. Syst. Signal Process. 112, 305–318 (2018) 5. Ilyas, S., Arevalo, A., Bayes, E., Foulds, I.G., Younis, M.I.: Torsion based universal MEMS logic device. Sens. Actuators A 236, 150–158 (2015)
132
Z. Wang
6. Alqasimi, J.E., Ouakad, H.M.: Vibrational response of initially deformed bistable microbeams under the combined effect of mechanical shock loads and electrostatic forces. J. Vib. Acoust. 140 (2017). 021013021013021012 7. Wu, G.Q., Chua, G.L., Gu, Y.D.: A dualmass fully decoupled MEMS gyroscope with wide bandwidth and high linearity. Sens. Actuators A 259, 50–56 (2017) 8. Feng, J., Liu, C., Zhang, W., Hao, S.: Static and dynamic mechanical behaviors of electrostatic MEMS resonator with surface processing error. Micromachines 9, 34 (2018) 9. Han, J., Li, L., Jin, G., Feng, J., Li, B., Jia, H., Ma, W.: Vibration identiﬁcation of foldedMEMS comb drive resonators. Micromachines 9, 381 (2018) 10. Uhlig, S., Gaudet, M., Langa, S., Schimmanz, K., Conrad, H., Kaiser, B., Schenk, H.: Electrostatically driven inplane silicon micropump for modular conﬁguration. Micromachines 9, 190 (2018) 11. Pallay, M., Towﬁghian, S.: A parametric electrostatic resonator using repulsive force. Sens. Actuators A 277, 134–141 (2018)
Measurement of Elastic Nonlinearities Using the Fundamental Edge Wave Mode James Martin Hughes1(&) , Andrei Kotousov1 and ChingTai Ng2 1
,
School of Mechanical Engineering, The University of Adelaide, Adelaide, SA 5005, Australia [email protected] 2 School of Civil, Environmental, and Mining Engineering, The University of Adelaide, Adelaide, SA 5005, Australia
Abstract. Measurement of the nonlinear elastic properties of materials represents a great interest in engineering and materials science. Changes of these properties are often related to mechanical damage and applied stresses, which are paramount for maintaining integrity and safety of structures. Current ultrasonic techniques typically utilise bulk, Lamb, or Rayleigh waves to measure material nonlinearities, however, spatial and velocity dispersion make this a very difﬁcult task, and the use of several (empirical) correction factors is usually required. In this work we suggest using the fundamental edge wave mode – a natural analogue of the classical Rayleigh wave propagating in a ﬁnite thickness plate – for the purpose of measuring elastic nonlinearities. Edge waves naturally avoid spatial dispersion as they are guided by the apex of a plate, thus avoiding the need for correction factors. Additionally, the fundamental edge wave mode can propagate long distances without signiﬁcant attenuation under certain conditions. The outcomes of this study demonstrate that the measurement of material nonlinearities is achievable using the fundamental edge wave mode. A linear trend between the nonlinearity parameter and propagation distance is experimentally observed, which is predicated by theoretical studies. Therefore, potential applications of the fundamental edge wave mode are very promising for the evaluation of mechanical damage and measurement of applied or residual stresses. Keywords: Harmonic generation
Edge waves Feature guided waves
1 Introduction Material nonlinearities can be acquired through mechanical processes such as fatigue, creep, thermal stress, and physical damage [1]. Measurement of the nonlinear properties can therefore provide an insight into the health of the material and structure [2], which explains the growing interest in incorporating nonlinear methods for Structural Health Monitoring (SHM). Typically, bulk, Lamb, or Rayleigh waves are used to measure material nonlinearity through the growth of higherorder harmonics [3, 4], however, these wave modes are subject to spatial dispersion, multimodal generation, © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 133–139, 2020. https://doi.org/10.1007/9783030478834_23
134
J. M. Hughes et al.
and velocity dispersion, meaning the matching conditions required for cumulative second harmonic generation are only achievable for certain frequencythickness products [5]. Using such wave modes therefore requires the application of numerous correction factors [6]. Consequently, there is a growing interest in alternative methods or wave modes which may be used to measure material nonlinearity more directly. One promising candidate is the fundamental edge wave mode, ES0, which is a natural analogue of the Rayleigh wave propagating in a ﬁnite thickness plate [7]. Similarly to Rayleigh waves, edge waves are surface waves, but are guided by the apex of a platestructure. From a mathematical standpoint, the main difference between Rayleigh and edge waves is the latter must additionally satisfy tractionfree boundary conditions on the side surfaces of the plate, whereas the former propagates under either plane stress or plane strain conditions. The inclusion of the plate side faces in the mathematical formulation naturally results in the absence of spatial dispersion, which presents a major problem facing measurements conducted using Lamb and Rayleigh waves. In addition, edge waves are weakly velocity dispersive, which allows approximate internal resonance conditions to be satisﬁed over a wide frequency range – a requirement for cumulative harmonic growth and measurement of material nonlinearity. Although edge waves are not spatially dispersive, they are energy dispersive, and gradually decay through conversion to other wave modes, namely the S0 Lamb wave mode. This amplitude decay is negligible for low frequencythickness values (x2h=c2 \6), however, theoretical studies indicate that at higher frequencies and Poisson’s ratios the decay is more signiﬁcant [8]. The problem of multimodal generation can also be reduced by exciting at a relatively low frequencythickness product, see Fig. 1, and by utilising the wedge excitation method, which has been used in a previous study to excite the fundamental edge wave mode [9]. 12
Re(κ) 2 h
Working Frequency Range
Multimodal Generation
8 SH0
4
ES0 S0
0 0
4
8
12
ω 2 h / c2 Fig. 1. Dispersion curves showing edge, shear, and Lamb wave modes. Solid lines depict the fundamental modes (ES0, S0, and SH0) and dotted lines represent higherorder modes.
Measurement of Elastic Nonlinearities
135
Edge waves were ﬁrst documented by Shaw in 1956 [10], and later described by Gazis and Mindlin in 1960 [11]. In the following decades several theoretical studies were published which focused on the mathematical formulation of edge waves, higherorder modes, and the velocity dispersion characteristics [7, 8]. However, there have been relatively few studies which experimentally investigate the properties of edge waves for practical purposes. One recent study conducted by Wilde et al. [7] showed that edge waves may be generated using a bonded piezoelectric transducer, although this produced a complicated wave ﬁeld due to generation of other wave modes such as the fundamental shearhorizontal and fundamental Lamb. This work was extended by the current authors who demonstrated edge wave excitation using the wedge method, which is more commonly applied to Lamb and Rayleigh waves, and produces a cleaner edge wave packet [9]. The purpose of this paper is therefore to demonstrate the excitation of ES0 mode using the wedge method, and to investigate cumulative harmonic generation at low frequencythickness values. It is believed that the results of this study will be of interest for researchers and engineers working in SHM and NDT ﬁelds.
2 Mechanics of HigherHarmonic Generation The excitation of harmonics in an ultrasonic signal occurs as a result of the adoption of nonlinear equations of elasticity. A perturbation technique can be applied to solve these equations, where the resultant relationship for a weakly nonlinear onedimensional wave is: A2 j2 0 bx ¼ b x ¼ 8 A21
ð1Þ
where A1 and A2 are the amplitudes of the fundamental and second harmonic respectively, x is the distance from the excitation source, j is the wavenumber, b0 is the relative nonlinearity parameter, and b is the acoustic nonlinearity parameter, which is a material property related to the second and thirdorder elastic constants. Similar relationships can be derived for higherorder harmonics [12]. It is widely accepted that Eq. (1) holds true for other types of waves when some correction factor is applied [6]. Therefore, through measurement of the fundamental and second harmonic of a propagating elastic wave, it is possible to determine the relative or acoustic nonlinearity parameters, which are an indicator of damage as mentioned in the Introduction. Measurement of the harmonic amplitudes is typically achieved using a fast Fourier transform (FFT) to decompose the displacement signal produced by the wave into its frequency components. The amplitudes of the fundamental and higherharmonic components are then extracted, and the relative nonlinearity parameter can be determined if the displacement signal is recorded at a number of propagation distances, x. Typically, corrections related to the source, spatial dispersion, and attenuation must be applied to
136
J. M. Hughes et al.
reveal the linear relationship between A2 =A21 and b0 , however, the favourable characteristics of edge waves (no spatial dispersion and minimal attenuation at low frequencythicknesses) allows direct measurements without requiring correction factors. This represents a signiﬁcant advantage over current ultrasonic techniques which use bulk, Lamb, and Rayleigh waves.
3 Experimental Methodology Excitation of the ES0 mode was achieved using the wedge method, which has been well documented for the generation of many types of guided waves [13, 14]. The wedge was constructed from an ultrahigh molecular weight polyethylene plastic called ‘Polystone’ by manufacturer ‘Dotmar’. The wedge angle of 52 was chosen to facilitate conversion of the longitudinal wave to the edge wave mode due to Snell’s law. The wedge assembly was coupled to a 5083H116 aluminium plate with dimensions 700 mm 500 mm and thickness 5 mm using motor oil.
PC & DAQ
Function Generator
Laser Vibrometer
Amplifier Edge Wave
Measurements
Wedge & Transducer
Aluminium
Fig. 2. Signal flow schematic of experimental setup.
A longitudinal wave of frequency f = 300 kHz was excited using an Ultran GC350D13 contact transducer. The 15 cycle squarewindowed excitation signal was generated using an AFG3012B arbitrary function generator and ampliﬁed to approximately 150Vpp using a KhronHite 7500 ampliﬁer. Measurement of the outofplane displacement was achieved using a Polytec PSV400M220 scanning laser vibrometer in 1D mode, which was directed perpendicularly along the centre line of the aluminium plate. The outofplane displacement was recorded at 7 locations equispaced between 350 mm and 500 mm from the front of the wedge, and 10 trials were recorded at each point. A schematic of the experimental setup is shown above in Fig. 2.
Measurement of Elastic Nonlinearities
137
10
Edge wave
5 0 5 a)
10 0
Reflection
80 160 240 320 Time (μs)
Norm. Amplitude
Displacement (nm)
4 Results
1.2 1 0.8 0.6 0.4 0.2 0
f
2f 3f
4f
b)
0 3 6 9 12 15 Frequency (kHz × 102)
Fig. 3. a) Typical time domain signal showing the edge wave and a reflection from the plate end, and b) FFT of the edge wave signal after applying a Hannwindow.
A typical outofplane displacement signal recorded by the laser vibrometer is shown above in Fig. 3(a). The region of the signal corresponding to the edge wave is clearly identiﬁed, and veriﬁcation that the signal corresponds to the fundamental edge wave mode was achieved through measurement of the wave speed. A reflection from the plate end is also visible. A Hannwindow is applied to the portion of the signal corresponding to the edge wave before performing an FFT, the results of which are presented in Fig. 3(b). There is a clear peak at the second harmonic frequency (600 kHz), as well as peaks which correspond to the third and fourth harmonics, indicating that harmonic generation does indeed occur for edge waves under approximate internal resonance conditions. Although beyond the scope of this paper, the presence of the two higherorder harmonics is promising for future research and could allow measurement of nonlinearities with the third or fourthorder harmonics. Figure 4 shows the relationship between the relative nonlinearity parameter, b0 , and propagation distance, x. The data gathered is well represented by a linear trendline, which is supported by the high Rsquared value of 0.87 and theoretically predicted by Eq. (1). Although the fundamental edge wave mode is weakly dispersive, the linearisation error for the current experiment amounts to approximately 10% at the furthest measurement point, and therefore Eq. (1) can be applied. It is difﬁcult to compare the rate of accumulation of the second harmonic found in this study against other studies which were based on Rayleigh or Lamb waves due to various correction and conversion factors, however, the corresponding experimental values of b0 are of the same order of magnitude.
138
J. M. Hughes et al. 3.5
β'x (×103)
2
= 0.87
3 2 2 1
2.5
=
′
2 1.5 0.3
0.35 0.4 0.45 0.5 Distance from Wedge (m)
0.55
Fig. 4. Growth of the relative nonlinearity parameter using the fundamental edge wave mode, where error bars show the standard deviation. The linear trend seen is supported by both theoretical predictions (Eq. (1)) and previous studies which utilised Rayleigh and Lamb waves.
5 Conclusion The outcomes of this study demonstrate the potential of the ES0 mode for measurement of material nonlinearities. A linear growth of the relative nonlinearity parameter with propagation distance was observed as predicated by both theoretical and experimental studies. Though it is difﬁcult to compare the current results to those which use Rayleigh and Lamb waves, the experimental values of b0 are of the same order. It is important to highlight that the measurements using the ES0 mode can be achieved without applying empirical or numerically obtained correction factors. Finally, it is believed that the fundamental edge wave mode is the most promising candidate for ultrasonic measurements of elastic nonlinearities. The applications of this work therefore have great potential for use in the evaluation of mechanical damage and applied or residual stresses. Acknowledgment. This work was supported by the Australian Research Council through DP160102233, LE170100079, DP200102300 and the Australian Research Training Program Scholarship. Their support is greatly appreciated.
References 1. Matlack, K.H., Kim, J.Y., Jacobs, L.J., Qu, J.: Experimental characterization of efﬁcient second harmonic generation of Lamb wave modes in a nonlinear elastic isotropic plate. J. Appl. Phys. 109, 014905 (2011) 2. Matlack, K.H., Kim, J.Y., Jacobs, L.J., Qu, J.: Review of second harmonic generation measurement techniques for material state determination in metals. J. Nondestr. Eval. 34, 273 (2014) 3. Zuo, P., Zhou, Y., Fan, Z.: Numerical and experimental investigation of nonlinear ultrasonic Lamb waves at low frequency. Appl. Phys. Lett. 109(2), 021902 (2016) 4. Pruell, C., Kim, J.Y., Qu, J., Jacobs, L.J.: Evaluation of plasticity driven material damage using Lamb waves. Appl. Phys. Lett. 92(23), 231911 (2007)
Measurement of Elastic Nonlinearities
139
5. Li, W., Cho, Y., Achenbach, J.D.: Detection of thermal fatigue in composites by second harmonic Lamb waves. Smart Mater. Struct. 21(8), 085019 (2012) 6. de Lima, W.J.N., Hamilton, M.F.: Finiteamplitude waves in isotropic elastic plates. J. Sound Vib. 265(4), 819–839 (2003) 7. Wilde, M.V., Golub, M.V., Eremin, A.A.: Experimental and theoretical investigation of transient edge waves excited by a piezoelectric transducer bonded to the edge of a thick elastic plate. J. Sound Vib. 441, 26–49 (2019) 8. Zvernov, V., Kaplunov, J.: Threedimensional edge waves in plates. Proc. R. Soc. A 464, 301–318 (2008) 9. Hughes, J.M., Kotousov, A., Ng, C.T.: Generation of higher harmonics with the fundamental edge wave mode. Appl. Phys. Lett. 116, 101904 (2020) 10. Shaw, E.A.G.: On the resonant vibrations of thick barium titanate disks. J. Acoust. Soc. Am. 28(1), 38–50 (1956) 11. Gazis, D.G., Mindlin, R.D.: Extensional vibrations and waves in a circular disk and a semiinﬁnite plate. J. Appl. Mech. 27(3), 541–547 (1960) 12. Kube, C.M., Arguelles, A.P.: Ultrasonic harmonic generation from materials with up to cubic nonlinearity. J. Acoust. Soc. Am. 142(2), 224–230 (2017) 13. Hughes, J.M., Vidler, J., Ng, C.T., Khanna, A., Mohabuth, M., Rose, L.F.R., Kotousov, A.: Comparative evaluation of in situ stress monitoring with Rayleigh waves. Struct. Health Monit. 18(1), 205–215 (2019) 14. Hughes, J.M., Vidler, J., Khanna, A., Mohabuth, M., Kotousov, A., Ng, C.T.: Measurement of residual stresses in rails using Rayleigh waves. In: SIF18 Conference, Perth (2019)
Unsteady Axisymmetric ElectroMagnetoElastic Oscillations of a Continuous Cylinder Under the External Displacement Field Vladimir Vestyak(&) and Vasily Scherbakov Moscow Aviation Institute (National Research University), Volokolamskoe shosse, 4, 125993 Moscow, Russian Federation [email protected], [email protected]
Abstract. In the present work is considered an axisymmetric timedependent waves of an inﬁnite cylindrical body. The body material is taken to be isotropic and electro magneto elastic. Piezoelectric effects are not taken into account. The deformation process is described by a system of equation with respect to radial and angular components of deformation of the body points in cylindrical coordinate system. In additional, it takes into account the effect of current density, surface charges, electric and magnetic ﬁelds. All parameters and ratios are reduced to dimensionless form. To solve the problem, are used the Fourier transformation of angles and the Laplace transformation of time. Then, the resulting expressions expansion in series in terms of a small parameter. The small parameter characterizes the relationship between mechanic and electromagnetic ﬁelds. To move into the space of the originals using the inverse Laplace transformation via residue theorem. Keywords: Electromagnetoelasticity Axisymmetric waves Residue theorem Coupled problems Timedependent axisymmetric problems Green’s functions
1 Problem Statement 1.1
Basic Equations
Consider the unsteady oscillations of a continuous cylinder of inﬁnite length with a radius R. The material of a cylindrical body is considered electro magneto elastic and isotropic. Piezoelectric effects will not be taken into account. The flat deformed state of the continuous medium will be investigated, therefore all the required functions of the problem will depend on three parameters: s – time, r – radial coordinate and h – angular coordinate. The interaction of mechanical and electromagnetic ﬁelds is described by the following system of equations [1–7]:
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 140–144, 2020. https://doi.org/10.1007/9783030478834_24
Unsteady Axisymmetric ElectroMagnetoElastic Oscillations of a Continuous Cylinder
141
– equations of motion respect to displacement @I1 g2 @uh €ur ¼ 1 g2 þ g2 Dur 2 2 þ ur þ aFer ; @r r @h ð1 g2 Þ @I1 g2 @ur €uh ¼ þ g2 Duh þ 2 2 uh þ aFeh ; r @h r @h where I1 ¼ 1r
h
@ ðrur Þ @r
þ
@uh @h
i @ @ r @r þ ; D ¼ 1r @r
1 @2 r2 @h2
ð1Þ ð2Þ
;
– Maxwell’s equations 1 @ ðrEh Þ @Er _ @H ¼ g2e cjh þ E_ h ; ¼ H; r @r @r @h 1 @H 1 @ ð rEr Þ @Eh 2 _ ¼ ge cjr þ Er ; þ ¼ qe ; r @h r @r @h
ð3Þ
jr ¼ Er þ H0 u_ h þ qe0 u_ r =c; jh ¼ Eh H0 u_ r þ qe0 u_ h =c;
ð4Þ
– Ohm’s law
– Lorentz force Fer ¼ qe0 Er þ qe E0r þ cðj0h H þ jh H0 Þ; Feh ¼ qe0 Eh þ qe E0h cðj0r H þ jr H0 Þ;
ð5Þ
– Physical relationships of electromagnetism Dr ¼ Er ; D# ¼ E# ; B ¼ H:
ð6Þ
Here ur ; uh – components of the displacement vector; Fer ; Feh – components of the Lorentz force; Er ; Eh – components of electric ﬁeld; H; B – components of magnetic ﬁeld; jr ; jh – components of current density; qe – volume charge density; Dr ; Dh – components of electric displacement ﬁeld. All of these parameters are unknown and depend on three variables: s, r and h. H0 , qe0 , E0r , E0h , j0r and j0h are the parameters of the initial electromagnetic ﬁeld and do not depend on time. The above equations are dimensionless. In order to make these equations dimensionless, the following substitutions were applied (the “” sign indicates a dimensional parameter):
142
V. Vestyak and V. Scherbakov
4p qe R Bc1 e c1 r ¼ Rr ; s ¼ cR1 t ; uk ¼ uRk ; H ¼ Hl cE ; B ¼ cE ; qe ¼ eE ;
R Dk ; jk ¼ rEjk ; Fek ¼ kFþek2l ; ge ¼ cc1e ; Ek ¼ EEk ; Dk ¼ eE eE 2
k þ 2l l 2 2 a ¼ 4pðk þ 2lÞ ; c ¼ cce1R ¼ 4prR ec1 ; c1 ¼ q ; c2 ¼ q ; 2 c g ¼ cc21 ; ce ¼ 4pr e ; ce ¼ l e ; 2
e
where c1 and c2  propagation velocities of tensioncompression waves and shear waves; E  characteristic level of electric ﬁeld; k and l – Lame’s parameters; e and le dielectric and magnetic permeability coefﬁcients; k ¼ r; h; c  light speed in vacuum; r  conductivity coefﬁcients. 1.2
Initial and Boundary Conditions
It is assumed that at the initial moment of time, there are no perturbation in the solid body. As conditions on the boundary of a cylindrical body, the following are assumed: ur ðs; r; hÞjr¼1 ¼ Ur ðs; hÞ; uh ðs; r; hÞjr¼1 ¼ 0: At the point at r ¼ 0, disturbances in a cylindrical body are considered limited: ur ðs; r; hÞjr¼0 ¼ Oð1Þ; uh ðs; r; hÞjr¼0 ¼ Oð1Þ: The system of Eqs. (3)–(6) can be reduced to a system of equations of two equations: € r þ cE_ r ¼ N11 ðEr Þ þ N12 ðE# Þ g2e ðqe0 € g2e E ur þ cH0 € uh Þ; € # þ cE_ # ¼ N21 ðEr Þ þ N22 ðE# Þ þ g2e ðcH0 € g2e E ur qe0 € uh Þ; 1 @2 1 @ @ 1 N11 ¼ r2 @#2 ; N12 ¼ r @# @r þ r ; h i @ @ 1 @ 1 @ ðrÞ ; N N21 ¼ 1r @# ¼ 22 @r r @r r @r :
ð7Þ
2 Solution Methods To solve the problem of the ﬁeld of displacement and the electric ﬁeld are expressed through the vector and scalar potentials: u ¼ gradu þ rotw; E ¼ gradue þ rotwe ; divw ¼ 0; divwe ¼ 0;
ð8Þ
Unsteady Axisymmetric ElectroMagnetoElastic Oscillations of a Continuous Cylinder
143
where u and ue  scalar potentials, w and we  vector potentials. The Lorentz force vector can also be represented via scalar and vector potentials: Fe ¼ gradU þ rotW;
ð9Þ
where DU ¼ divFe ¼
1 @ ðrFer Þ 1 @Feh 1 @ ðrFeh Þ 1 @Fer þ þ ; DW ¼ rotFe ¼ : r @r r @h r @r r @h
In order to fulﬁll the axisymmetric conditions, it is necessary that the deﬁning parameters of the problem, as well as the vector and scalar potentials correspond to the following equations: ur ¼ ur ðs; r; hÞ; uh ¼ uh ðs; r; hÞ; uz 0; Fez 0; Er ¼ Er ðr; h; tÞ; Eh ¼ Eh ðr; h; tÞ; Ez ¼ E0z 0; E0r ¼ E0r ðr; hÞ; E0h ¼ E0h ðr; #Þ; u ¼ uðr; h; tÞ; ue ¼ ue ðr; h; tÞ; Fer ¼ Fer ðr; h; tÞ; Eh ¼ Eh ðr; h; tÞ; wr ¼ wh 0; wer ¼ weh 0; wz ¼ w ¼ wðr; h; tÞ; wez ¼ we ¼ we ðr; h; tÞ; Hr ¼ H0r ¼ Hh ¼ H0h 0; Hz ¼ H ðr; h; tÞ; H0z ¼ H0 ðr; #Þ: By substituting (8) and (9) into systems (1), (2) and (7), we obtain a system of equations for u; w and ue ; we . First, the unknown functions are decomposed into a complex Fourier series: uðs; r; hÞ ¼ ue ðs; r; hÞ ¼
þ1 X
n¼1 þ1 X n¼1
uFn ðs; r Þeih ; wðs; r; hÞ ¼
uFen ðs; r Þeih ; we ðs; r; hÞ ¼
þ1 X n¼1 þ1 X n¼1
wFn ðs; r Þeih ;
wFen ðs; r Þeih ;
then, the Laplace transforms in time are applied to the obtained coefﬁcients … wFen ðs; r Þ (s  conversion parameter):
uFn ðs; r Þ
L
uFn ðs; r Þ ! uFL n ðs; r Þ; : : L wFen ðs; r Þ ! wFL en ðs; r Þ: FL The resulting coefﬁcients uFL n ðs; r Þ. . . wen ðs; r Þ are expanded in a power series for a small parameter a:
144
V. Vestyak and V. Scherbakov
uFL n ¼
1 X m¼0
FL m uFL nm a ; . . .; wen ¼
1 X m¼0
m wFL enm a :
After that we get a new recurrent system of differential equations for the coefﬁcient FL of expansion uFL nm … wnm . FL And ﬁnally in order to move obtained uFL nm … wnm parameters into the space of the originals it is using the inverse Laplace transformation via residue theorem.
References 1. He, T., Tian, X., Shen, Y.: A generalized electromagnetothermoelastic problem for an inﬁnitely long solid cylinder. Eur. J. Mech. A. 24(2), 349–359 (2005) 2. Wang, X., Dong, K.: Magnetothermodynamic stress and perturbation of magnetic ﬁeld vector in a nonhomogeneous thermoelastic cylinder. Eur. J. Mech. A. 25(1), 98–109 (2006) 3. Vestyak, V.A., Lemeshev, V.A.: Rasprostranenie nestatsionarnykh radialnykh vozmushcheniy ot tsilindricheskoy polosti v elektromagnitouprugoy srede. In: Mater. XIV Intern. Symp. “Dynamic and technoloronmental problems of mechanics of structures and continua” named A.G. Gorshkov. Moscow, vol. 1, pp. 59–60 (2008) 4. Tarlakovskii, D.V., Vestyak, V.A., Zemskov, A.V.: Dynamic processes in thermoelectromagnetoelastic and thermoelastodiffusive media. In: Encyclopedia of Thermal Stresses, vol. 2, pp. 1064–1071. Springer, Dordrecht (2014) 5. Gorshkov, A.G., Medvedsky, A.L., Rabinsky, L.N., Tarlakovsky, D.V.: Waves in Continuous Mediums Textbook for Higher Education Institutions, p. 472. FIZMATLIT, Moscow (2004). (in Russian) 6. Vestyak, V.A., Lemeshev, V.A., Tarlakovsky, D.V.: Onedimensional timedependent waves in an electromagnetoelastic halfspace or in a layer. Doklady Phys. 54(6), 262–264 (2009) 7. Vestyak, V.A., Lemeshev, V.A., Tarlakovskii, D.V.: The propagation of timedependent radial perturbations from a spherical cavity in an electromagnetoelastic space. Doklady Phys. 55(9), 468–470 (2010)
Development of Micromechanical Models of Fatigue Damage James Vidler1(&) 1
, Andrei Kotousov1
, and ChingTai Ng2
School of Mechanical Engineering, The University of Adelaide, Adelaide SA 5005, Australia [email protected] 2 School of Civil, Environmental, and Mining Engineering, The University of Adelaide, Adelaide SA 5005, Australia
Abstract. Accumulation of fatigue damage in high and low cycle regimes is largely associated with nucleation and development of irreversible plastic deformations and voids. The effect of these microstructural changes on conventional (secondorder) elastic constants is typically very small, which makes experimental evaluation of the progressive fatigue damage accumulation difﬁcult and the classical damage theories inapplicable. It was demonstrated in the past that the thirdorder elastic constants are sensitive to fatigue damage and these material constants can be evaluated using various ultrasonic techniques. The ultimate aim of this study is to develop micromechanical models, which link the microporosity and microplastic deformations, to the effective thirdorder elastic constants of the material. These models could provide a foundation for the evaluation of early fatigue damage, i.e. the damage prior formation of a microdefect (crack), as well as the remaining fatigue life of structures. Keywords: Fatigue damage
ThirdOrder Elastic Constants Finite elasticity
1 Introduction Inspired by Eshelby, micromechanics literature abounds with studies of dilatations, inhomogeneities, and inclusions, which are relevant to analysis of many problems of mechanics and material science involving plasticity, thermal expansion and phase transformations [1]. Unfortunately, in the case of ﬁnite deformations the analysis is usually prohibitively difﬁcult. The ﬁnite deformation analysis requires solutions to the nonlinear equations of equilibrium, which are scarce. The lowest order of nonlinear response of an elastic body is represented by the third order elastic constants (TOECs), which can be formally obtained from the series expansion of strain energy density with respect to the strain components [2]. The TOECs of a material have both an intrinsic and an acquired nature. The intrinsic TOECs, which are related to the anharmonic forces in crystals, play an important role in predictions of mechanical behaviour, the ideal strength and ductility in metals and in the explanation of anharmonic properties of solids such as the thermal expansion. The acquired TOECs are often related to various dislocation, microplasticity and phase
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 145–150, 2020. https://doi.org/10.1007/9783030478834_25
146
J. Vidler et al.
transformation phenomena as well as to accumulation of mechanical damage such as fatigue and radiation damage [3]. Material nonlinearities and TOECs were investigated extensively with ultrasonic techniques in the early 1960s. Over the past two decades, however, the focus has shifted to ultrasonic guided waves, which can be used in nondestructive techniques as well as in online damage monitoring systems. Monitoring of accumulated mechanical damage is currently considered as a signiﬁcant engineering problem, speciﬁcally for structures subjected to fatigue. In the absence of manufacturing defects the accumulation of microdamage (or the early damage stage) normally precedes the crack nucleation and propagation stages. Depending on the material, its microstructure and the presence of preexisting defects, the early damage stage can occupy from 10% to up to 90% of the total fatigue life in highcycle fatigue (HCF) regime, and it fully dominates in the ultrahigh cycle fatigue (UHCF) regime (up to 109 cycles and beyond) [4]. Previous studies have found that fatigue damage in metals and advanced engineering alloys in LCF and HCF regimes increases with applied cycles in a cumulative manner, and material degradation is largely associated with the accumulation of irreversible microplastic deformations and nucleation and growth of voids, respectively. Classical damage mechanics links the conventional (or secondorder) elastic constants to fatigue damage [5]. However, the conventional elastic constants (e.g. shear and bulk moduli) and the damage parameter(s)/function(s) are not very sensitive to microstructural damage until the ﬁnal stages of the fatigue life, particularly in the HCF and UHCF regimes. This has been well documented in past experimental studies, e.g. [6, 7] and has recently been conﬁrmed by direct numerical computations using grainsize models [8]. Therefore, it is difﬁcult to validate the damage mechanics models in the early stages of the fatigue life, or quantify the cumulative microstructural damage experimentally based on measurements of the conventional (secondorder) elastic constants. At the same time, many recent studies have demonstrated that the change of nonlinear (or thirdorder) elastic constants is usually much stronger than the change of conventional elastic constants, particularly at the initial (or early) stages of the fatigue life. As discussed above these changes can be detected using various ultrasonic techniques, which are under development since 1960s. The ultimate aim of this work is to develop micromechanical models, which describe the change of the effective thirdorder elastic constants (TOECs) with accumulation of microplastic deformations, as well as nucleation and growth of microvoids. Previous analytical studies [9–11] have investigated the effective properties of nonlinear elastic material in the theory of micromechanics, but have not combined their research with a model of damage accumulation. The development of such models could provide a theoretical foundation for the development of new earlydamage assessment techniques as well as mode adequate fatigue life evaluation procedures.
2 Theoretical Framework Consider a material body undergoing deformation with material points X mapped to spatial points x, so that x ¼ vðXÞ. The deformation gradient is
Development of Micromechanical Models of Fatigue Damage
F ¼ Grad v:
147
ð1Þ
For a hyperelastic and isotropic material, a strain energy density function exists, and may be represented as a function of the principal invariants of the material strain tensor. In Murnaghan’s form [2], the strain energy density function including terms up to thirdorder is 1 1 W ðI1 ; I2 ; I3 Þ ¼ ðk þ 2lÞI12 2lI2 þ ðl þ 2mÞI13 2mI1 I2 þ nI3 2 3
ð2Þ
where I1 , I2 , I3 are the principal invariants of the material strain tensor, E¼
1 T F FI 2
the secondorder elastic constants are k and l, and the TOECs of the material are l, m, and n. The nominal stress tensor for compressible materials is S ¼ @W=@F
ð3Þ
and the equilibrium condition expressed in the referential coordinates, neglecting body forces, is Div S ¼ 0:
ð4Þ
The governing equations of elasticity presented above are nonlinear, and most often solved using numerical methods. Exact, closed form solutions have been derived only under highly restrictive boundary conditions, or using speciﬁc forms of the strain energy density function. However, provided that the displacements and rotations be sufﬁciently small, secondorder corrections to the linear elasticity solution may be derived using a perturbation approach [12]. Consider the expansion of the deformation vðXÞ X ¼ ku1 þ k2 u2 where k is a small parameter, the vector u1 corresponds to the solution for the displacement vector in the linear theory of elasticity, and the vector u2 is the secondorder correction to the linear solution. Substitution of the above expansion into the governing equations of elasticity and the boundary conditions yields a hierarchy of systems of equations, each corresponding to a linear elasticity problem. Each system of equations features a body force and surface tractions dependent on the solution to the lowerorder systems of equations. Applying the perturbation approach to the problem of a medium containing voids allows the derivation of the effective elastic constants of the material. If the medium is assumed to consist of a dilute distribution of spherical voids at a volume concertation of c 1, the relevant problem for prediction of effective properties is a spherical shell
148
J. Vidler et al.
containing an isolated void at the centre, with outer radius such that the volume concentration of voids is c. Three loading cases are considered: pure dilatation, simple extension, and simple tension. In each loading case, the linear solution u1 is constructed in the standard manner using spherical harmonic functions; the secondorder correction is constructed using spherical harmonic functions, a displacement potential, and a Galerkin vector. After solving the secondorder elasticity problem for each of the three loading conditions, the total strain energy stored in the medium with voids is calculated and equated to the strain energy stored in an equivalent, homogeneous medium [11, 13], Z
Z
W ðI1 ; I2 ; I3 ÞdV ¼ WH ðI1 ; I2 ; I3 ÞdVH
ð5Þ
where WH is the strain energy function of the effective homogeneous medium, and I1;H , I2;H , I3;H are the principal invariants of the material strain tensor for the homogeneous medium. The equivalent homogeneous medium has elastic properties which coincide with the effective properties of the porous medium, and is subjected to identical surface loading conditions. By considering three separate loading cases, all three TOEC of an isotropic hyperelastic material may be calculated and related to the volume concentration of voids.
3 Selected Results
Effective elastic constant (GPa)
The derivations and ﬁnal expressions for the effective third order elastic constants of a medium containing a dilute distribution of microvoids are extremely lengthy and cumbersome, which prevents the presentation of explicit expressions in this short
100 0 100 200 300 400 500
0
0.1
0.2 0.3 Volume concentration of voids
0.4
0.5
Fig. 1. Change in effective elastic constants for 6061T6 aluminium due to a dilute distribution of microvoids.
Development of Micromechanical Models of Fatigue Damage
149
paper. For the purposes of illustration, the change in the effective elastic constants as the volume concentration of microvoids increases is presented in Fig. 1, for the elastic constants of 6061T6 aluminium reported in [14], k ¼ 54:308 GPa, l ¼ 27:174 GPa, l ¼ 281:5 GPa, m ¼ 339:0 GPa, n ¼ 416:0 GPa. The ﬁve (two secondorder and three thirdorder) effective elastic constants are shown in Fig. 1. The plots are truncated at c ¼ 0:5, due to the assumption of a dilute distribution of voids. It is seen that, for 6061T6 aluminium, the TOECs feature a much higher sensitivity to the volume fraction of microvoids. These constants have been derived from consideration of three different load cases: pure dilatation, simple extension, and simple tension.
4 Conclusion A micromechanical model for the evaluation of effective conventional and thirdorder constants has been developed for an isotropic material with a dilute distribution of voids, which can be related to early lowcycle fatigue damage. The numerical calculations for aluminum support previously published experimental results claiming that the nonlinear elastic constants (TOECs) are more sensitive to fatigue damage than the conventional (secondorder) constants. Future work will be focused on the validation of theoretical results by conducting ultrasonic measurements of the change of TOECs in LCF regime. Similar models will be developed for microplastic deformations to describe the similar changes in HCF regime. Acknowledgement. This work was supported by the Australian Research Council through DP160102233, LE170100079, DP200102300 and the Australian Research Training Program Scholarship. Their support is greatly appreciated.
References 1. Eshelby, J.D.: The determination of the elastic ﬁeld of an ellipsoidal inclusion, and related problems. Proc. R. Soc. Lond. A 241, 376–396 (1957) 2. Destrade, M., Ogden, R.W.: On stressdependent elastic moduli and wave speeds. IMA J. Appl. Math. 78, 965–997 (2012) 3. Matlack, K.H., Kim, J.Y., Jacobs, L.J., Qu, J.: Review of second harmonic generation measurement techniques for material state determination in metals. J. Nondestruct. Eval 34, 273 (2014) 4. Chan, K.S.: Roles of microstructure in fatigue crack initiation. Int. J. Fatigue 32(9), 1428– 1447 (2010) 5. Lemaitre, J.: A continuous damage mechanics model for ductile fracture. ASME J. Eng. Mat. Technol. 107, 83–89 (1985) 6. Chaboche, J.L., Lesne, P.M.: A nonlinear continuous fatigue damage model. Fatigue Fracture Eng. Mater. Struct. 2, 1–17 (1988) 7. Lissenden, C., Liu, Y., Rose, J.: Use of nonlinear ultrasonic guided waves for early damage detection. Insight NonDestr. Test. Cond. Monitoring 57, 206–211 (2015)
150
J. Vidler et al.
8. Benedetti, I., Gulizzi, V.: A grainscale model for highcycle fatigue degradation in polycrystalline materials. Int. J. of Fatigue 116, 90–105 (2018) 9. Ogden, R.W.: On the overall moduli of nonlinear elastic composite materials. J. Mech. Phys. Solids 22, 541–553 (1974) 10. Chen, Y., Jiang, X.: Nonlinear elastic properties of particulate composites. J. Mech. Phys. Solids 41(7), 1177–1190 (1993) 11. Imam, A., Johnson, G.C.: Ferrari, M,: Determination of the overall moduli in second order incompressible elasticity. J. Mech. Phys. Solids 43(7), 1087–1104 (1995) 12. Clayton, J.D.: Defects in nonlinear elastic crystals: differential geometry, ﬁnite kinematics, and secondorder analytical solutions. Z. Angew. Math. Mech. 95(5), 476–510 (2015) 13. Hill, R.: On constitutive macrovariables for heterogeneous solids at ﬁnite strain. Proc. R. Soc. Long. A. 326, 131–147 (1972) 14. Mohabuth, M.: Effect of uniaxial stress on the propagation of higherorder Lamb wave modes. Int. J. NonLinear Mech. 86, 104–111 (2016)
Research on Springback of 5A02 Aluminum Alloy Considering Thickness Normal Stress in Hydroforming Peicheng Jiang, Lihui Lang(&), and Sergei Alexandrov Beihang University, No. 37 Xueyuan Road, Haidian District Beijing, People’s Republic of China {jiangpc,lang}@buaa.edu.cn https://ev.buaa.edu.cn/
Abstract. Springback is an unavoidable problem in sheet metal forming. When the amount of sheet springback exceeds the allowable range, it becomes a forming defect. In the process of hydraulic bulging, the fluid medium acts on the surface of the sheet uniformly instead of the rigid mold, so that the material is simultaneously stressed, which makes the deformation law of the material different from that of the sheet in the traditional rigid bulging. In this paper, the research on the springback of 5A02 aluminum alloy is carried out by taking the active hydroforming process of a typical shallow drawn rotatory body arc surface part as the research object. The theoretical analysis method is used to take the thickness normal stress into the theoretical calculation of the springback amount, and a theoretical springback amount calculation model of the threedimensional state of stress. Numerical simulations are carried out under different loading paths with hydraulic pressure of 1, 2, 3, 10, 20 and 30 MPa. The influence and law of springback of the parts under different loading paths and different hydraulic conditions are also obtained. Keywords: Springback Hydraulic bulging Theoretical analysis Threedimensional state of stress Numerical simulation
1 Introduction Springback has been a focus of attention in the ﬁeld of sheet metal forming manufacturing. Scholars have carried out a large number of fruitful studies on sheet springback since the last century [1–4]. Research on the springback of ordinary steels such as carbon steel, stainless steel, and automotive steel has accumulated a wealth of experimental data and mature research methods. As for the springback research of aluminum alloys and other light alloy materials, it is just in its infancy, especially aluminum alloy materials for advanced manufacturing. The prediction accuracy of the springback numerical simulation depends largely on the mechanical properties of the aluminum alloy sheet. Among them, anisotropy and Bauschinger effect are two important aspects, which directly affect the accuracy of springback prediction. The anisotropy of the material is closely related to the selected yield criterion, while the Bauschinger effect is directly related to the plastic hardening model. Therefore, the © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 151–157, 2020. https://doi.org/10.1007/9783030478834_26
152
P. Jiang et al.
coupling relationship between the yield criterion and the plastic hardening model is of great signiﬁcance for springback prediction. In this paper, the springback research is carried out with the active hydroforming process of a typical shallow drawn rotatory body arc surface part. Considering the influence of key process parameters on the springback during hydroforming, such as the hydraulic pressure loading path, two types of highpressure and lowpressure loading have been performed. Among them, numerical simulation of hydraulic bulging in 6 cases of high pressure of 10, 20, 30 MPa and low pressure of 1, 2, 3 MPa respectively. Finally, the results of the numerical simulation can be used to verify the accuracy of the springback theoretical analysis Equation for the hydraulic bulging process to predict the springback trend of sheet metal under different hydraulic pressure paths.
2 Theoretical Analysis of Springback in Hydraulic Bulging Process Taking the contour of the meridian passing through the rotating body as the research object, the deformation of the metal sheet during the hydraulic bulging process can be regarded as the traditional bending deformation. In order to facilitate the study of springback in the process of hydraulic bulging, the model is simpliﬁed. Based on the calculation process of the classic bending springback theory, the thickness normal stress is introduced into it. The simpliﬁed sheet bending model with thickness normal stress is shown in Fig. 1.
Fig. 1. The theoretical diagram of sheet metal bending process
Here Ri —Inner edge radius of the sheet, Ro —Outer edge radius of the sheet, q— Neutral layer radius, r—Microunit radius.
Research on Springback of 5A02 Aluminum Alloy
153
During the bending deformation of the sheet, the bending moment effect occurs inside the sheet under the action of external force, which causes the sheet to change from elastic deformation to plastic deformation. When the external force is unloaded, a part of the sheet recovers elastically [5]. We choose a microunit and name it ABCD, assuming the material has ideal plasticity, according to the Mises yield criterion [6, 7] Outside the neutral layer: rq [ rh [ rt , the rq and rt have opposite signs, we can know that rq þ rt ¼ brs
ð1Þ
And inside the neutral layer: rt [ rh [ rq , the rq and rt have the same signs, so we can get rq rt = brs
ð2Þ
The width of the microunit ABCD is a unit length. At any moment of bending deformation, the microunit should be in a state of force equilibrium. The stress rh in the width direction has no effect on the equilibrium of the microunit in this plane. In addition, in order to maintain its tangential balance, the tangential stress rq on both sides of the microunit should be equal. Because the microunit must satisfy the equilibrium condition of the force, the algebraic sum of the forces on the microunit in the radial direction must be zero. Therefore, we can list the equilibrium equation of the microunit ABCD according to the equilibrium conditions: rt r da ðrt þ drt Þ ðr þ dr Þ da rq dr da ¼ 0
ð3Þ
Among them, rt r da is the force on the AB arc surface, ðrt þ drt Þ ðr þ dr Þ da is the force on the AB arc surface, and rq dr da is the resultant force on the AC and BD surfaces. Further simpliﬁcation and derivation rt ¼ brs ln r þ c
ð4Þ
Outside the neutral layer, when r ¼ Ro , rt ¼ rN . Among them, rN is the reaction force of the die to the sheet. So we can get the value of the constant c: c ¼ rN þ brs ln Ro . From (1) and (4) we can know: rq ¼ brs ln r þ brs rN brs ln Ro
ð5Þ
As for the inner side of the neutral layer, when r ¼ Ri , rt ¼ P. P is the hydraulic pressure. So we can get the value of the constant c: c ¼ P brs ln Ri .
154
P. Jiang et al.
Then rq = brs ln r þ brs þ P brs ln Ri
ð6Þ
The radius of the neutral layer before unloading is q, which increases to q0 after unloading. If we use Dk to represent the amount of curvature reduction, then Dk ¼ q1  q1 . 0 It is assumed that the load bending moment of the sheet in plastic bending deformation is M, and the moment of inertia of the section is J. Using the formula about elastic bending in “Materials Mechanics”, it can be known that after the bending moment is removed, the springback Dk of the sheet is: Dk ¼
M EJ
ð7Þ
Here J ¼ Bt12 . B is the sheet width, and we take its size as 1. The sheet is compacted in the middle of the mold, and there is no external force, so the load bending moment M is generated by the tangential stress rq inside the sheet. With the neutral layer as the boundary, it can be divided into the bending moment caused by the inner tangential stress and the outer tangential stress, that is: 3
M ¼ Mi þ Mo
ð8Þ
Here Mi is the bending moment caused by the inner tangential stress, and Mo is the bending moment caused by the outer tangential stress. Z Mi ¼ Z Mo ¼
Ro
q
q
Ri
Z rq r b dr ¼ Z
rq r b dr ¼
q
q
ðbrs ln r þ brs þ P brs ln Ri Þ r dr
ð9Þ
ðbrs ln r þ brs rN brs ln Ro Þ r dr
ð10Þ
Ri Ro
Finally, the equation of sheet springback amount in the hydraulic bulging process considering the thickness normal stress is obtained, as shown in Eq. (11). 12 Dk ¼ 3 Et
Z
q Ri
ðbrs ln r þ brs þ P brs ln Ri Þ r dr
Z
þ
Ro q
ðbrs ln r þ brs rN brs ln Ro Þ r dr
ð11Þ
Research on Springback of 5A02 Aluminum Alloy
155
3 Finite Element Simulation Analysis of Hydraulic Bulging The software Dynaform is used to simulate the hydraulic bulging process. In the process of hydraulic bulging, the pressure value and loading rate of the fluid medium affect the deformation behavior of the sheet forming process. Therefore, in this section, the simulation scheme studies of the hydraulic pressure of 1, 2, 3, 10, 20, and 30 MPa are performed. The loading path of the hydraulic pressure is shown in Fig. 2.
Fig. 2. Hydraulic pressure loading path
In the process of sheet hydraulic bulging, the central area is the ﬁrst to undergo plastic deformation due to the bending moment effect and then expands to other areas. With the increase of the hydraulic pressure, the deformation of the vertex area gradually increases until the mold is fully ﬁtted (20 MPa has been fully ﬁtted), and the reaction force of die on the sheet is also greater. The maximum bulging height H, the curvature radius q, and the wall thickness d of the bulging apex are measured and calculated, as shown in Table 1.
Table 1. Relevant data obtained from numerical simulation of hydraulic bulging P (MPa) 1 2 3 10 20 30
H (mm) 10.2 13.4 16.8 19.2 20.0 20.0
d (mm) 0.983 0.970 0.944 0.938 0.937 0.940
q (mm) rN (MPa) 194.116 5.5 146.500 9.5 112.986 13.3 98.725 40.0 98.820 80.0 98.817 120.0
156
P. Jiang et al.
The wall thickness data of the parts under different hydraulic loading paths are measured. The 13 measurement points are located on the symmetry plane of the center of the part and are evenly distributed. The simulation curve of the wall thickness distribution is shown in Fig. 3.
Fig. 3. The distribution of wall thickness
4 Conclusion Based on 5A02 aluminum alloy, this paper uses the theoretical analysis method to derive the theoretical calculation model of springback amount considering thickness normal stress. In the later stage, q value and rN value obtained by numerical simulation and experiment can be substituted into Eq. (11) for comparison and veriﬁcation. Numerical simulations are carried out under hydraulic loading paths with hydraulic pressures of 1, 2, 3, 10, 20, 30 Mpa. Studies have shown that due to strain strengthening or strain rate strengthening, the increase in deformation resistance in the region with the largest amount of deformation is also the largest, thereby making the deformation more dispersed. Macroscopically, the deformation is more uniform, so the wall thickness distribution will be more uniform.
References 1. Lingbeek, R., Huétink, J., Ohnimus, S., et al.: The development of a ﬁnite elements based springback compensation tool for sheet metal products. J. Mater. Process. Technol. 169(1), 115–125 (2005) 2. Kinzel, G.L.: A new model for springback prediction for aluminum sheet forming. J. Eng. Mater. Technol. 127(3), 279–288 (2005) 3. Vrh, M., Halilovič, M., Starman, B., et al.: Modelling of springback in sheet metal forming. Int. J. Mater. Form. 2(1), 825–828 (2009)
Research on Springback of 5A02 Aluminum Alloy
157
4. Tamura, S., Sumikawa, S., Uemori, T., et al.: Experimental observation of elastoplasticity behavior of type 5000 and 6000 aluminum alloy sheets. Mater. Trans. 61(6), 255–261 (2011) 5. Shiguang, H.: Engineering Analysis of Sheet Metal Cold Stamping. Beijing University of Aeronautics and Astronautics Press, Beijing (2004) 6. Yu, H.Q., Chen, J.D.: Principles of Metal Forming. China Machine Press, Beijing (2010) 7. Zhang, Q.: Research on Composite Hydroforming Process and Key Technology of Aluminum Alloy Sheet. Beihang University, Beijing (2018)
On the Friction Test for Metal Forming Applications Sergei Alexandrov1,2(&), Marko Vilotic3, and Dragisa Vilotic3 1
2
School of Mechanical Engineering and Automation, Beihang University, 37 Xue Yuan Lu, Haidian Qu, Beijing Shi, China [email protected] Ishlinsky Institute for Problems in Mechanics, Russian Academy of Sciences, 1011 Prospect Vernadskogo, 119526 Moscow, Russia 3 Faculty of Technical Sciences, University of Novi Sad, Trg Dositeja Obradovica 6, 21000 Novi Sad, Serbia
Abstract. The ring compression test is a conventional test for identifying the friction law for metal forming applications. This test is very widely used but has a signiﬁcant disadvantage. In particular, if the friction stress is high, then a sticking region occurs over a part of the friction surface. In this case, the interpretation of experimental results is difﬁcult because the friction law at sliding is not valid over the sticking region. If the friction stress is very high, then this region occupies the entire friction surface. In this case, the process becomes insensitive to the friction factor at sliding at all. In order to overcome this difﬁculty and keep the conventional procedure for identifying the friction law, it is proposed to carry out the compression test between fat and conical dies. The geometry of the conical die should be chosen such that no sticking region occurs on the friction surface. Keywords: Friction
Sticking Metal forming
1 Introduction The most popular friction law in metal forming applications is Tresca’s law, which postulates that the friction stress is equal to a portion of the local shear yield stress. The friction factor involved in this law should be found from experiment. A typical test for this purpose is the ring compression test. The test must be supplemented with a theoretical analysis. The latter is often based on upper bound solutions. Several upper bound solutions for axisymmetric ring forging have been found in [1]. Solutions based on the velocity ﬁeld proposed in [2] have been derived in [3, 4]. Other upper bound solutions for axisymmetric ring forging have been given in [5–8]. The solutions above are based on kinematically admissible velocity ﬁelds with no rigid regions. On the other hand, conventional friction laws used in conjunction with rigid perfectly plastic models demand the existence of such a region in certain cases. For example, in the case of axisymmetric ring forging a rigid region must appear if the friction stress changes its direction. The existence of a rigid zone can affect the interpretation of theoretical
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 158–161, 2020. https://doi.org/10.1007/9783030478834_27
On the Friction Test for Metal Forming Applications
159
solutions. For example, the deﬁnition for the neutral radius accepted in [2] is not valid in this case. To overcome the difﬁculty above, it is proposed to use the compression test between flat and conical dies. In this case, the geometry of the conical die can be chosen such that no sticking region occurs independently of the friction stress.
2 Conventional Ring Compression Test A schematic diagram of the conventional ring compression test is shown in Fig. 1.
Fig. 1. Schematic diagram of the conventional ring compression test.
The interpretation of this test requires a theoretical solution. It is usually assumed that the regime of sliding occurs over the entire friction surface. This means that the friction law in the form sf ¼ mk
ð1Þ
is valid over the entire friction surface. In (1) sf is the friction stress, m is the friction factor and k is the shear yield stress. However, in reality, a sticking region usually occurs over a portion of the friction surface (Fig. 1). In this case, the friction law (1) is valid over region AB whereas the friction stress is not controlled by the friction law at sliding over region AC. Therefore, the interpretation above is not valid. Moreover, the region of sticking may occupy the entire friction surface. In this case, the solution becomes insensitive to the value of m at all. In the case of constraint forging, it has been found in [9] that the upper bound solution is not affected by the friction law if m [ mcr . The value of mcr depends on geometric parameters.
160
S. Alexandrov et al.
3 New Ring Compression Test In the present paper, it is proposed to use the ring compression test between flat and conical dies (Fig. 2).
Fig. 2. Schematic diagram of the new ring compression test.
In general, the geometric parameters can be chosen such that no sticking region occurs on the friction surface between the conical die and specimen. Then, the procedure similar to that used in conjunction with the conventional ring compression test can be applied to evaluate the friction factor involved in (1). Several tests have been carried out to show the efﬁciency of the method proposed (Fig. 3).
Fig. 3. Conical dies used in the new ring compression test (cone angle: 8° 30′, 15° and 30°)
On the Friction Test for Metal Forming Applications
161
4 Conclusions A disadvantage of the conventional ring compression test for identifying the friction law (1) is that a rigid region usually occurs over a part of the friction surface. This region may occupy the entire friction surface if the friction stress is high enough. It is proposed to use the compression between flat and conical dies (Fig. 2) to overcome the difﬁculty above. Several tests have been carried out to conﬁrm the efﬁciency of the new test. Acknowledgments. This work was carried out within the framework of the international project supported by grants RFBR185176001 (Russia) and BULKSURFACE – 359 (Ministry of education, science and technological development, Serbia).
References 1. Liu, J.Y.: Upperbound solutions of some axisymmetric cold forging problems. ASME J. Eng. Ind. 93, 1134–1144 (1971) 2. Avitzur, B., Van Tyne, C.J.: Ring formation: an upper bound approach. Part 1: flow pattern and calculation of power. ASME J. Eng. Ind. 104, 231–237 (1982) 3. Avitzur, B., Van Tyne, C.J.: Ring formation: an upper bound approach. Part 2: process analysis and characteristics. ASME J. Eng. Ind. 104, 238–247 (1982) 4. Avitzur, B., Van Tyne, C.J.: Ring formation: an upper bound approach. Part 3: constrained forging and deep drawing applications. ASME J. Eng. Ind. 104, 248–252 (1982) 5. Avitzur, B., Sauerwine, F.: Limit analysis of hollow disk forging. Part 1: upper bound. ASME J. Eng. Ind. 100, 340–344 (1978) 6. Lee, J.H.: Upper bound analysis of the upsetting of pressure – sensitive polymeric rings. J. Mater. Process. Technol. 30, 601–612 (1988) 7. Alexandrov, S.: An analysis of the axisymmetric compression of viscous materials. J. Mater. Process. Technol. 105, 278–283 (2000) 8. Wu, M.C., Yeh, W.C.: Effect of natural boundary conditions on the upperbound analysis of upset forging of ring and disks. Mater. Des. 28, 1245–1256 (2007) 9. Alexandrov, S., Lyamina, E., Jeng, J.R.: A general kinematically admissible velocity ﬁeld for axisymmetric forging and its application to hollow disk forging. Int. J. Adv. Manuf. Technol. 88, 3113–3122 (2017)
From the Linear Theory of Elasticity to Bending Equations for Beams with Variable CrossSection Boris Gusev1 1 2
and Vasily Saurin2(&)
RUT – MIIT, Obrazcova Str. 9b9, 127994 Moscow, Russia IPM RAS, Vernadskogo Prt 1011, 119626 Moscow, Russia [email protected]
Abstract. A formulation of a boundary value problem to ﬁnd natural frequencies of an inhomogeneous beam in the framework of the linear theory of elasticity is represented. The main attention in the article is paid to the analysis of transverse vibrations of beams with a variable crosssection. A system of two connected ordinary differential equations with variable coefﬁcients is obtained in the framework of the linear theory of elasticity, by using semidiscrete approximations and a projection approach. Various bilateral energy quality estimates for approximate solutions that follow from the method of integrodifferential relations are proposed. In the ﬁnal part of the paper the advantages of the variational technique in problems of free vibrations of inhomogeneous beams are discussed based on a numerical example. Keywords: Dynamics
Beams Variable crosssection
1 Statement of the Problem Consider an isotropic plate occupied in the plane Ox1 x2 some area symmetric with the axis Ox1 : V ¼ fx : L=2\x1 \L=2;
hðx1 Þ\x2 \hðx1 Þg
with
x ¼ ðx1 ; x2 Þ:
It is considered that the stressstrain state of the plate is described by twodimensional equations of the linear theory of elasticity and, also external plate boundaries are free of loading. Similar problems are considered in [1] and [2]. By using symmetry properties of the plate shape the low dimensional polynomial approximations of the unknown displacements u and stress r functions with respect to one of the coordinates x2 describing the lateral vibrations can be given as r11 ¼
M X _2j þ 1 2j þ 1 x r11 ðx1 Þ; j¼0
M X _2j þ 1 2j þ 1 u1 ¼ x u1 ðx1 Þ; j¼0
r12 ¼
M X _2j 2j x r12 ðx1 Þ; j¼0
M X _2j 2j u2 ¼ x u2 ðx1 Þ;
r22 ¼
M X _2j þ 1 2j þ 1 x r22 ðx1 Þ; j¼0
_
x ¼ x2 =hðx1 Þ:
j¼0
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 162–163, 2020. https://doi.org/10.1007/9783030478834_28
From the Linear Theory of Elasticity to Bending Equations for Beams
163
In a projection approach, it is required that the displacements and stresses provide zero values to the integral projections of the constitutive vector and tensor on the selected tensor ﬁelds. These conditions give the possibility to construct different systems of ordinary differential equations with variable coefﬁcients to study spectral properties of the beam.
Fig. 1. Convergence of the eigenfrequencies.
Figure 1 shows the behavior of the ﬁrst three eigenfrequencies versus the number of degrees of freedom Nd for two different mathematical models, describing the natural motion of a beam with variable cross section. The solid lines correspond to the eigenfrequencies that are obtained from the proposed equations with M ¼ 1 and the dashed lines show the frequencies obtained from the classical beam equation qðxÞ
@2v @2 @2v þ EJðxÞ ¼ 0: @t2 @x2 @t2
Here v is the transverse displacements of the beam center line points, q is the linear density of the material. This work is ﬁnancially supported in part by the State Program № AAAAA171170213103801 and Russian Foundation for Basic Research, projects no. 180100812, 180801346, 182903228, 190100173.
References 1. Saurin, V.: Analysis of dynamic behavior of beams with variable crosssection. Lobachevskii J. Math. 40, 364–374 (2019) 2. Kostin, G., Saurin, V.: Dynamics of Solid Structures. Method Using Integrodifferential Relations. De Gruyter, Berlin (2017)
On Different Representations of Equations for Beam with Variable CrossSection Vladimir Poliakov1 1 2
and Vasily Saurin2(&)
RUT – MIIT, Obrazcova Str. 9b9, 127994 Moscow, Russia IPM RAS, Vernadskogo Prt 1011, 119626 Moscow, Russia [email protected]
Abstract. The main part of the paper is devoted to the formulations of the boundary value problem to ﬁnding natural frequencies of an inhomogeneous beam in the framework of the EulerBernoulli hypotheses. Three different formulations of the beam equation in displacements, momentums, and bending moments are discussed. Next, the possibilities to constructing various bilateral energy quality estimates for approximate solutions that follow from the method of integrodifferential relations are investigated. In the ﬁnal part, based on a numerical model example, the advantages of the variational technique in problems of free vibrations of inhomogeneous beams are discussed. Keywords: Dynamics
Beams Variable crosssection
1 Beam Equations Consider a thin beam with a length L, which is described by an equation under the EulerBernoulli hypotheses. It is supposed that the cross section of the beam is a rectangle with the width b ¼ const and the height h ¼ hðxÞ, which can be varied along its length. The beam lateral motions in the framework of this model can be represented by a linear partial differential equation qðxÞytt þ ðEJðxÞyxx Þxx ¼ qðxÞ
x 2 ð0; LÞ:
ð1Þ
Here, y is the function described lateral displacements of the beam midline, qðxÞ is a linear density of the beam material, E is Young’s modulus, qðxÞ is the external distributed load, JðxÞ is a cross sectional moment of inertia. Similar problems are considered in [1] and [2]. Let us introduce new variables pðt; xÞ and mðt; xÞ that characterize the beam dynamics and, at the same time, have a clear physical meaning. The function pðt; xÞ is the linear momentum density and mðt; xÞ is the bending moment in a cross section of the beam. Introduce miscellaneous functions g and n g ¼ qy p ¼ 0;
n ¼ EJyxx m ¼ 0
ð2Þ
By using relations (2) Eq. (1) can be respectively expressed through momentum and moment functions © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 164–165, 2020. https://doi.org/10.1007/9783030478834_29
On Different Representations of Equations for Beam
p ptt þ EJ ¼ 0; q xx xx
mxx q mtt þ EJ ¼ 0: q xx
165
ð3Þ
It can be seen that these equations differ from each other and this is primarily due to the fact that the variable functions of bending stiffness EJðxÞ and linear density qðxÞ enter differentiation with respect to time t and spatial coordinate x in different way, respectively. However, one should not assume that these equations lead to different results, since they are obtained from a unique generating system of equations. But they can have different convergence rates when a numerical solution is ﬁnding.
Fig. 1. Dependence the value of accuracy lgðImðx1 Þ= lgðReðx1 Þ with respect to the parameter h0 .
Figure 1 shows the behavior of the accuracy of the ﬁrst eigenfrequencies x1 versus the to the parameter h0 , hðxÞ ¼ ð12h0 þ 1:2Þx2 þ h0 Þ obtained for three beam formulations discussed in this paper (black curve correspond to the statement in displacements, red – momentums, blue – moments). The value h0 ¼ 0:1 reflects the beam with constant height. It is seen that better accuracy is obtained for moment formulation and difference in accuracies reach several orders. Acknowledgments. This work is ﬁnancially supported in part by the State Program № AAAAA171170213103801 and Russian Foundation for Basic Research, projects no. 180100812, 180801346, 182903228, 190100173.
References 1. Saurin, V.: Analysis of dynamic behavior of beams with variable crosssection. Lobachevskii J. Math. 40, 364–374 (2019) 2. Kostin, G., Saurin, V.: Dynamics of Solid Structures. Method Using Integrodifferential Relations. De Gruyter, Berlin (2017)
Shear Residual Stresses Induced by Torsional Loading D. Pérez Gallego(&), J. Ruiz Hervías, and D. A. Cendón Franco Departamento de Ciencia de Materiales, Universidad Politécnica de Madrid, ETSI Caminos, Canales y Puertos, c/Profesor Aranguren, 3, 28040 Madrid, Spain [email protected]
Abstract. Residual stresses can be induced by fabrication processes and service conditions that lead to nonuniform deformations. In the standard test method for residual stress analysis by xray diffraction (EN 15305), the validation is done by using reference specimens with known normal residual stress. However, the method also stablishes restrictions to the values of both normal and shear stresses, although the latter can be negligible with respect to the former. Consequently, it would be interesting to have a reference specimen with known shear residual stresses for independent validation. In the present work, torsion tests have been performed in a steel sample with the aim of producing shear residual stresses. Residual stresses were simulated by FEM modelling and measured by Xray diffraction. Keywords: Residual shear stresses Xray diffraction Finite element method
1 Motivation The analysis of residual stresses has an important role in the study of materials science or manufacturing processes. There are several methods to calculate the residual stresses, one of the most extended techniques being the Xray diffraction. The standard EN 15305 [1] establishes certain criteria for reference specimens to validate the method. Most reference specimens are prepared by shoot peening [2], which produces residual compressive stresses at the surface. These kind of reference specimens have bee qualiﬁed by means of round robin tests [3]. With shot peening, a homogenous compressive residual stress can be generated in metallic materials in a controlled way, where shear stresses are negligible. However, the standard imposes restrictions for both normal and shear stresses which could be difﬁcult to fulﬁll a reference specimen with known normal residual stresses. In summary, the standard limits the value of shear stresses in reference specimens although there are no such specimens with known residual shear stresses. The main idea of the present work is to develop an experimental procedure to create reference specimens with known shear residual stresses. Torsional loads have been applied to pearlitic steel sample to induce this kind of stresses The residual stresses will to be measured by Xray diffraction and the results will be compared with numerical simulations to study the residual stress distribution in the sample. © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 166–167, 2020. https://doi.org/10.1007/9783030478834_30
Shear Residual Stresses Induced by Torsional Loading
167
2 Experimental and Numerical Methods Round bars of pearlitic steel have been loaded under torsion up to a given value of shear strain (see Fig. 1a). After unloading the bars, their surface shear residual stresses will be measured by Xray diffraction, and compared with the numerical predictions obtained with the commercial FEM code ABAQUS (see Fig. 1b).
Fig. 1. a) Torsion test; b) Shear residual stresses obtained by FEM simulation.
References 1. European Standards: Nondestructive testing. Test method for residual stress analysis by Xray diffraction (EN 15305) (2008) 2. Kobayashi, M., Matsui, T., Murakami, Y.: Mechanism of creation of compressive residual stress by shot peening. Int. J. Fatigue 20(5), 351–357 (1998). https://doi.org/10.1016/S01421123(98)000024 3. Lefebvre, F., Wasniewski, E., François, M., Cacot, J., LeBec, P., Baumhauer, E., Bouscaud, D., Bergey, T., Blaize, D., Gloaguen, D., Cosson, A., Jégou, S., Cheynet, Y., Leray, S., Meheux, M., Monvoisin, J., Allain, P., Vidal, J.C., Sprauel, J., Hamdi, H.: External reference samples for residual stress analysis by xray diffraction. Adv. Mater. Res. 996, 221–227 (2014). https://doi. org/10.4028/www.scientiﬁc.net/AMR.996.221
Elastoplastic Analysis of Reentrant Cell Formation in Auxetic Foams Under Compression and Heat Treatment YunChe Wang(&)
, TsaiWen Ko, and HsiangWei Lai
National Cheng Kung University, Tainan 70101, Taiwan, Republic of China [email protected]
Abstract. Negative Poisson’s ratio of polymeric foam can be obtained by using the thermal transformation method to convert cell shape from convex to reentrant ones. In this work, the largedeformation ﬁnite element analysis is performed to quantify the magnitudes of compression and temperature for subsequent heat treatment to reduce elastic recovery, such that the reentrant shape can be maintained when the compression is removed. The amount of compression and temperature for heat treatment that can produce NPR foam can be used as a guide for experimental investigations, instead of trialanderror methods to determine manufacturing parameters. Keywords: Elastoplastic analysis Negative Poisson’s ratio
Finite element method Auxetic foam
1 Introduction Classical elasticity allows the Poisson’s ratio (PR) of materials in three dimensions be in the range between 1 and 0.5. Through design of material microstructures, effective Poisson’s ratio of polymeric foam can be negative when its cell shape is reentrant [1]. Recently, numerical investigations of the negative Poisson’s ratio (NPR) properties in the 2D starshaped lattice have been reported [2–4]. A method to convert the initially convex cell shape, which gives rise to positive Poisson’s ratio, to the concave, i.e. reentrant, one is through the thermal transformation technique [1]. The thermal transformation method requires triaxial compression of the foam ﬁrst and subsequent heat treatment while the compression is maintained. Permanent deformation due to plasticity and release of stress under heat treatment are responsible for minimizing elastic recovery when the compression load is removed. For metallic foam, sequential compression along three orthogonal directions on a cube is sufﬁcient. In this work, we numerically model the deformation processes of the foam changing from positive to negative PR by ﬁnite element analysis with the elasticperfectlyplastic material model and of the Mises flow rule.
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 168–169, 2020. https://doi.org/10.1007/9783030478834_31
Elastoplastic Analysis of ReEntrant Cell Formation in Auxetic Foams
169
2 Results and Discussion Starting from the conventional cell shape, as shown in Fig. 1 at time t = 0, we adopt largedeformation plasticity theory to model the deformation of the unit cell under hydrostatic compression in two dimensions. The color bar indicates the Mises stress in units of MPa. The boundary conditions of the left and bottom edges are of the roller type. Uniform compressive stress is applied on the top and right edges. As time progresses, the snapshots of deformation at time t = 1, 1.5, 2 s are shown in Fig. 1. The reentrant cell shape can be clearly observed. The stress in the skeleton is removed by heat treatment, so that the reentrant shape is maintained. Elastic analysis of the reentrant unit cell reveals the effective Poisson’s ratio is about 0.3.
Fig. 1. Snapshots of the deformation processes of the reentrant unit cell at time t = 0, 1, 1.5, 2 s under biaxial compression.
References 1. Lakes, R.: Foam structures with a negative Poisson’s ratio. Science 235(4792), 1038–1040 (1987) 2. Wang, Y.C., Shen, M.W., Liao, S.M.: Microstructural effects on the Poisson’s ratio of starshaped twodimensional systems. Phys. Status Solidi B 254, 1700024 (2017) 3. Wang, Y.C., Lai, H.W., Ren, X.J.: Enhanced auxetic and viscoelastic properties of ﬁlled reentrant honeycomb. Phys. Status Solidi B, 1900184 (2019) 4. Wang, Y.C.: Negative Poisson’s ratio in plane elasticity. In: Altenbach, H., Öchsner, A. (eds.) Encyclopedia of Continuum Mechanics. Springer, Heidelberg (2019)
Analytical Modeling of the ThermoMechanical Behavior of a FrictionPendulum Seismic Isolator Todor Zhelyazov(&) Technical University of Soﬁa, 1000 Soﬁa, Bulgaria [email protected]
Abstract. The contribution outlines the modeling of the thermomechanical behavior of a curved surface slider employed as a device for passive seismic isolation of buildings and structures. The Lagrange formalism is employed to derive the equation of motion of the slider on the spherical surface of the lower sliding pad. Besides the equations of motion, accurate modeling requires the formulation of the response of the friction interface. Previous studies have shown the dependence of the friction coefﬁcient on the sliding velocity. Reportedly, the rise in temperature during sliding also affects the magnitude of the friction coefﬁcient. The model is being developed in order to be further integrated into a ﬁnite element model of a baseisolated structure. Keywords: Seismic isolation
FrictionPendulum system Analytical model
1 Introduction Bearing devices for passive seismic isolation are increasingly used for buildings, bridges, and other types of structures. By dissipating energy, seismic isolation reduces the demands of the superstructure in terms of ductility and loadcarrying capacity. Among other types of devices, the most frequently used are highdamping rubber bearings, leadcore rubber bearings, and frictionpendulum systems. The latter type is the object of the research. The simplest version of the frictionpendulum isolator (sometimes also referred to as a curved surface slider) consists of a slider and two sliding pads upper and lower. Generally, contact surfaces have a spherical form.
2 Equations of Motion The equations of motion are derived from the Lagrangian of the slider constrained to move on the spherical surface of the inferior sliding pad of the bearing device [1]. The resulting system of differential equations of motion is solved numerically. Mechanical behavior of the bearing device, subjected to strong ground motion, is investigated (see Fig. 1). The analysis assumes a constant value of the friction coefﬁcient and an effective unilateral response of the sliding interface. © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 170–171, 2020. https://doi.org/10.1007/9783030478834_32
Analytical Modeling of the ThermoMechanical Behavior of a FrictionPendulum
171
Fig. 1. Trajectory of the slider’s motion (on the spherical surface of the lower sliding pad) in response to strong ground motion.
3 Response of the Sliding Interface A model proposed by [2] is used to model the frictional behavior at the slider/spherical surface interface. The analytical model includes empirical relationships deﬁned to take into account the influence of the normal pressure acting on the interface [3], as well as of the temperature rise during sliding [4, 5]. The outlined model is developed in order to be implemented into a ﬁnite element analysis of a baseisolated structure. Thus, in a more general context, the analytical model is employed in the assessment of the robustness of baseisolated structures.
References 1. Monti, G., Petrone, F.: Analytical thermomechanics 3D model of friction pendulum bearings. Earthquake Eng. Struct. Dyn. 45, 957–977 (2016) 2. Park, Y.J., Wen, Y.K., Ang, A.H.S.: Random vibration of hysteretic system under a bidirectional ground motions. Earthquake Eng. Struct. Dyn. 14(4), 543–557 (1985) 3. Mokha, A.S., Amin, N., Constantinou, M.C., Zayas, V.: Seismic isolation retroﬁt of large historic building. J. Struct. Eng. 122(3), 298–308 (1996) 4. Kumar, M., Whittaker, A.S., Constantinou, M.C.: Characterizing friction in sliding isolation bearings. Earthquake Eng. Struct. Dynam. 44, 1409–1425 (2015) 5. Quaglini, V., Bocciarelli, M., Gandelli, E., Dubini, P.: Numerical assessment of frictional heating in sliding bearings for seismic isolation. J. Earthquake Eng. 18, 1198–1216 (2014)
Symposium on Theoretical and Experimental Approaches in Mechanics of Solids with Nonhomogeneities and Defects, by Roman Kushnir
Damage Accumulation and Limit State of Welded Pipelines with CorrosionErosion Metal Loss Due to UltraLowCycle Fatigue Alexey Milenin(&), Elena Velikoivanenko, Galina Rozynka, and Nina Pivtorak E.O. Paton Electric Welding Institute of NAS of Ukraine, 11, K. Malevich Street, Kiev 03150, Ukraine [email protected]
Abstract. Analytical prediction of the reliability of pipelines under ultralowcycle loading demands the consideration of the several interrelated damaging factors, those determine the limit state of speciﬁc structure. For that in this work it was developed the complex numerical technique for ﬁniteelement assessment of damage accumulation and limit state of welded pipelines with corrosionerosion metal loss. The ductile mechanism of subcritical damage was considered as the main one that assumes certain material softening due to voids nucleation and accumulation up to limit state. Additionally, it was necessary to take into account the material hardening and softening in plastic strain that was described by isotropic and kinematic mixed hardening laws. This complex approach allowed revealing the major physicalmechanical mechanisms of structure failure depending on the type of external loading, size of the local metal loss and the features of welding on the limit state of typical pipeline element. Keywords: Pipeline Corrosionerosion metal loss Limit state Isotropic hardening Kinematic hardening Ductile fracture
Welding
1 Introduction Numerical assessment of residual strength of pipeline elements (PE) with revealed corrosionerosion metal losses is the typical problem for expert analysis of reliability of various industrial systems. The common approach for solving this problem is the determination of the limit state of speciﬁc structure under rated loading. As the most of pipelines are welded ones the influence of residual state of stresses and strains should be taken into account if the metal loss belongs to welding area. This problem is studied well for static loading (e.g. by internal pressure) whereas for cyclic loading complexity of physicalmechanical processes, those cause the subcritical damage and failure, demands sufﬁcient conservativeness of corresponding analytical techniques. Ultralowcycle fatigue is notable for the sufﬁcient plastic flow of material which demands taking into account the material hardening and softening as well as nucleation and accumulation of distributed voids of ductile fracture of certain volume concentration f. Presence of welded joint and local geometry anomalies of structure (operational defects of © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 175–180, 2020. https://doi.org/10.1007/9783030478834_33
176
A. Milenin et al.
corrosionerosion metal loss) leads to peculiar state of stresses and strains of PE under internal pressure and/or bending moment that influences on the susceptibility of speciﬁc welded structure to fracture. Within the limits of this work it is proposed the complex numerical technique for ﬁniteelement prediction of damage accumulation and limit state of welded pipelines with corrosionerosion metal losses under ultralowcycle loading.
2 Numerical Procedure for Prediction of Limit State of Welded Pipeline with CorrosionErosion Metal Loss Under UltraLowCycle Loading 2.1
Main Assumptions and Material Model
Ultimate limit state of corroded (eroded) PE depends on a number of physicalmechanical processes initiated by operational and technological influence. In case of large cyclic strain loading (e.g. earthquake, landslide, inaccurate overloading, buckling, etc.) limit state of pipeline is determined by the evolution of plastic strains and corresponding accumulation of subcritical damage up to nucleation of macroflaw. Local corrosionerosion metal losses and corresponding stress concentrations lead to a certain decrease of bearing capacity of pressurized PE. Their admissibility is determined by relevant standard speciﬁcations for design operational loads, but ultralowcycle loading considers exceptional conditions of pipeline operation that complicates expert analysis of their compliance with design demands. The main complexity consists in nonlinear response of material to cyclic plastic deformation and evolution of its properties. Thus, along with characteristic strain hardening, two possible mechanisms of material softening could be assigned [1]: Bauschinger effect due to change of the direction of plastic deformation, and the accumulation of porosity ductile damage which is caused by plastic strain and lead to the reduction of true crosssection of the structure. As the typical technological and main pipelines are the welded ones, the presence of assembly girth welds causes the spatial inhomogeneity of stressstrain state and complex interaction of operational and residual stresses. This also should be taken into account, especially in case of close location of the metal loss and weld. 2.2
FiniteElement Description of PhysicalMechanical Processes in UltraLowCycle Loading of Welded Pipeline with Local CorrosionErosion Metal Loss
The physical phenomena, those determine the ultimate limit state of typical welded PE with local geometry anomaly, are spatially nonuniform and the conventional approach for their description is the ﬁniteelement (FE) modeling. For considered problem the defective pipeline of diameter D and wall thickness t was modeled within the limits of the cylindrical set of coordinates (r, b, z), local metal loss was approximated as semielliptical wall thinning of the size of 2 s, 2u and a (see Fig. 1). In welding and further lowcycle loading of PE by internal pressure P and bending moment M the current and limit state of stresses and strains is determined by several mechanisms of deformation,
Damage Accumulation and Limit State of Welded Pipelines
177
those corresponds to respective summand of total strain tensor eij (i, j = r, b, z) namely: elastic eeij , plastic epij , thermal dijeT and ductile damage dij(f/3).
Fig. 1. Scheme of welded pipeline element with defect of semielliptic shape in cylindrical coordinate system (r, b, z).
Elastic strains correlate with current stresses as follows: eeij ¼
rij dij rm þ dij ðKrm þ uÞ 2G
ð1Þ
where rm= (rrr+ rbb+ rzz)/3; K ¼ ð1 2mÞ=E, G ¼ 0:5E=ð1 þ mÞ, E is Young modulus, m is Poison’s ratio, u is volumetric changes (thermal or caused by structural changes). The increment of plastic strains for a speciﬁc FE linearly depends on the scalar function K and deviator component of the stress tensor, namely: depij ¼ dKðrij dij rm Þ
ð2Þ
In turn, the speciﬁc value of the function K depends on the stress state in the considered area of the structure, as well as on the shape of the yield surface U [2]. For numerical prediction of porosity nucleation in material of welded pipeline with local metal loss the strainbased criterion was used [3], further growth of voids depends on stress triaxiality (ratio of the hydrostatic rm to equivalent req stress) and the intensity of the plastic strain epi according to RiceTracey law [4]. Thus, the increment of strain tensor components could be presented as follows [5]: deij ¼ deeij þ depij þ dij ðdeT þ df =3Þ
ð3Þ
Equation (3) in differential form has the next expression: 1 rij dij rm þ ðKrm Þ Deij ¼ W rij dij rm þ dij ðKrm þ DeT þ Df =3Þ 2G
ð4Þ
178
A. Milenin et al.
where symbol “*” refers to the variable of the previous tracing step, W is the state function of the material, which is determined by plastic flow surface U, that was considered according to GursonTvergaardNeedleman model [6]: 2 req 3rm 0 2 0 U¼ ðq3 f Þ þ 2q1 f cosh q2 rY 2rY
ð5Þ
where q1, q2, q3 are constants, f’ is equivalent concentration of voids, rY is yield stress. The solvable system of equations in the variables of the vector of displacement increments DUi in FE nodes at each step of tracing and Witerations was determined by the minimization of the functional L (Lagrangian variational principle), i.e. [2] @L ¼ 0; ð6Þ @DUi P P P where L ¼ 12 rij þ Jij Deij Vm;n;r þ Fi DUi DSm;n;r , is the sum operator by P V SP PV internal FEs, is the sum operator on surface FEs on which the components of the SP
force vector Fi are speciﬁed. It was considered that limit state of speciﬁc structure is reached in case of fulﬁlling the one of three conditions of numerical criterion of brittleductile fracture [2]: 1 W 2G 0
f
1 q1 r1 12f =3
ef ðepi Þ
ð
Þ
1:5rY epi ;f 0
;
exp 3q2r2 rY m ; [ SK ;
ð7Þ
where SK is the microcleavage stress, ef is the critical strain (Mackenzie rule). The mixed hardening rule was used for prediction of material properties evolution under ultralowcycle fatigue loading. It combines the linear kinematic hardening rule in Von Mises form [7] and isotropic hardening effect for taking into account the of yield surface transformation due to plastic deformation and accumulation of ductile: rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 3 rij dij rm X r0Y ðf 0 Þ½1 þ ðep =e0 Þm 0 rij dij rm X 2
ð8Þ
is shift tensor of kinematic hardening, r0Y ðf 0 Þ is material state according to (5), where X m, e0 are material constants.
3 Results and Discussion Residual state of stresses and strains in the weld region, kinematic hardening and ductile damage have an influence on limit state of eroded PE under ultralowcycle loading with internal pressure and bending moment. One of the fundamental problems,
Damage Accumulation and Limit State of Welded Pipelines
179
that could be solved with the described above FE approach, is the determination of influence of this interrelated phenomena on bearing capacity of speciﬁc welded structure. As a case of study it was considered the PE of D t = 315 10 mm size made of 316L stainless steel (E = 193 GPa, m = 0.3, rY = 170 MPa). Individual erosion metal loss of semielliptical shape on inner surface of the pipe (2s 2u a = 40 20 5 mm). Examples of equivalent stresses distributions over crosssection of the pipe after welding and under operational conditions are given in Fig. 2.
Fig. 2. Numerically assessed distributions of equivalent stresses req in the pipeline (D t = 315 10 mm, 316L stainless steel): (a) – residual state in the region of girth weld; (b) – with internal erosion defect (2s 2u a=40 20 5 mm) under operational pressure 8.0 MPa.
Figure 3a shows the dependencies of local stresses rbb on strains ebb near the internal defect of erosion thinning with and without taking into account the ductile damage of material caused both with internal pressure P = 10 MPa and cycling bending moment M from −85 to 85 kN∙m (that corresponds to the range of maximum axial stress from −120 to 120 MPa). As it could be seen, accumulation of porosity in plastic deformation of pipe steel leads to the total shifting of stressstrain hysteresis loops to higher strains because of porous material softening and decrease of the structure bearing crosssection. Intensity of ductile damage accumulation in ultralowcycle loading (i.e. growth rate of porosity volume concentration f per number of cycles N) has three main stages: plastic deformation before nucleation of ductile damage; nucleation of porosity and redistribution of the ﬁelds of strains and stresses; stable growth plastic strains and porosity volume concentration up to limiting state according (7). First two stages correspond to the static loading and take place on the ﬁrst cycles whereas the third one is connected with fatigue fracture of plastically deformed material. Figure 3b shows the results of numerical assessment of ductile damage accumulation for considered example of eroded PE in stable growth stage. As it could be seen, ductile porosity concentration f increases quasilinearly starting the second cycle of loading with bending moment under the same internal pressure P. That means, that growth rate of f mostly depends on applied range of cycling load, but not the plastic (or total) strain path.
180
A. Milenin et al.
Fig. 3. Dependencies of local stresses rbb on strains ebb near the internal defect of erosion thinning (2s 2u a = 40 20 5 mm) of pipe (D t = 315 10 mm, 316L) with and without taking into account the ductile damage of material (internal pressure P = 10 MPa and bending moment M = −85 85 kN∙m) – (a) and growth rate of porosity volume concentration f per number of cycles N – (b).
References 1. Jia, L.J., Kuwamura, H.: Ductile fracture model for structural steel under cyclic large strain loading. J. Constr. Steel Res. 106, 110–121 (2015). https://doi.org/10.1016/j.jcsr.2014.12.002 2. Makhnenko, V.: Problems of examination of modern critical welded structures. Paton Weld. J. 5, 21–28 (2013) 3. Milenin, A., Velikoivanenko, E., Rozynka, G., Pivtorak, N.: Probabilistic procedure for numerical assessment of corroded pipeline strength and operability. Int. J. Press. Vessels Pip. 171C, 60–68 (2019). https://doi.org/10.1016/j.ijpvp.2019.02.003 4. Chen, Z., Butcher, C.: Micromechanics Modelling of Ductile Fracture. Springer, Dordrecht (2013). https://doi.org/10.1007/9789400760981 5. Velikoivanenko, E.A., Rozynka, G.F., Milenin, A.S., Pivtorak, N.I.: Modelling of processes of nucleation and development of ductile fracture pores in welded structures. Paton Weld. J. 9, 24–29 (2013). https://doi.org/10.1016/j.ijpvp.2019.02.003 6. Xue, L.: A uniﬁed expression for low cycle fatigue and extremely low cycle fatigue and its implication for monotonic loading. Int. J. Fatigue 30, 1691–1698 (2008). https://doi.org/10. 1016/j.ijfatigue.2008.03.004 7. Lemaitre, J., Chaboche, J.L.: Mechanics of Solid Materials. Cambridge University Press, Cambridge (1990)
Unsteady ElasticDiffusion Oscillations of a Simply Supported Kirchhoff Plate Under the Distributed Transverse Load Action O. A. Afanasieva1 and A. V. Zemskov1,2(&) 1
2
Moscow Aviation Institute (National Research University), Moscow, Russia [email protected] Institute of Mechanics, Lomonosov Moscow State University, Moscow, Russia
Abstract. We study unsteady vibrations of a isotropic Kirchhoff plate considering mass transfer. In the general case, the plate is subjected to tensile and shear forces as well as bending moments and torque. Densities of diffusion fluxes are also deﬁned. For the problem formulation, we use the coupled elastic diffusion continuum model in a rectangular Cartesian coordinate system. Further, the unsteady model of an elastodiffusive Kirchhoff plate is obtained using the d’Alembert variational principle. The solution is sought in integral form. To ﬁnd the Green’s functions, we use the Laplace integral transform and Fourier series expansion. Keywords: Elastic diffusion Coupled problem Unsteady problem Integral transformation Multicomponent continuum Kirchhoff plate Green’s function
1 Problem Formulation We consider the unsteady vibrations problem of a rectangular isotropic N  component Kirchhoff plate under action of mechanical and diffusion perturbations. Figure 1 shows the orientation of Cartesian axes as well as how the forces and the moments are applied. When moment density and transverse load density are absent, the transverse vibrations equation of the plate has the form (the dots denote the time derivative) [1]: D€ w
N X 12 € aq DHq ; w ¼ DDw þ h2 q¼1
H_ q ¼ Dq DHq þ Kq DDw:
All quantities in (1) are dimensionless. We accepted the following notation: xi ¼ aq ¼
xi w Ct k k lm ; w¼ ; s¼ ; k¼ ; ; l ¼ ; l ¼ m l l l k þ 2l k þ 2l l
aq
k þ 2l
; Dq ¼
Dq Cl
ðqÞ
; Kq ¼
mðqÞ Dq aq n0 q RT0 Cl
; C2 ¼
k þ 2l h ; h¼ ; q l
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 181–186, 2020. https://doi.org/10.1007/9783030478834_34
ð1Þ
182
O. A. Afanasieva and A. V. Zemskov
Fig. 1. Forces and moments acting upon the plate.
where t is time; xi are Cartesian coordinates; w is a plate transversal displacement; l is the characteristic linear size of the problem (in this case, the plate diagonal, which has dimensions l1 l2 and thickness h ); Hq are concentration increments for the qth ðqÞ
medium component of an Ncomponent continuum; n0 are initial concentrations; k and l are Lame coefﬁcients; q is density; aq are coefﬁcients characterizing the medium volumetric changes due to diffusion; Dq are the selfdiffusion coefﬁcients; R is the universal gas constant; T0 is the initial temperature; mðqÞ is the molar mass. The Eq. (1) are supplemented by the boundary conditions. In the case of pure ðlÞ bending under the action of bending moments Mk , boundary conditions has the form: ! þ aq Hq ¼ f111 ðx2 ; sÞ; q¼1 x ¼0 1 ! N P @2w @2 w þ k þ a H ¼ f112 ðx2 ; sÞ; 2 2 q q @x1 @x2 q¼1 x ¼l 1 1 ! N P @2 w @2w k @x2 þ @x2 þ aq Hq ¼ f121 ðx1 ; sÞ; 1 2 q¼1 x ¼0 ! 2 N P @2 w @2w k @x2 þ @x2 þ aq Hq ¼ f122 ðx1 ; sÞ; 1 2 q¼1 @2w @x21
2 þ k @@xw2 2
N P
ð2Þ
x2 ¼l2
wjx1 ¼0 ¼ f211 ðx2 ; sÞ; wjx1 ¼l1 ¼ f212 ðx2 ; sÞ; wjx2 ¼0 ¼ f221 ðx1 ; sÞ; wjx2 ¼l2 ¼ f222 ðx1 ; sÞ; Hq x1 ¼0 ¼ fq þ 2;11 ðx2 ; sÞ; Hq x1 ¼l1 ¼ fq þ 2;12 ðx2 ; sÞ; Hq x2 ¼0 ¼ fq þ 2;21 ðx1 ; sÞ; Hq x2 ¼l2 ¼ fq þ 2;22 ðx1 ; sÞ;
Unsteady ElasticDiffusion Oscillations of a Simply Supported Kirchhoff Plate
12 ð1Þ M ðx2 ; sÞ; h3 1 12 ð2Þ f121 ðx1 ; sÞ ¼ 3 M1 ðx1 ; sÞ; h
f111 ðx2 ; sÞ ¼
183
12 ð1Þ M ðx2 ; sÞ; h3 2 12 ð2Þ f122 ðx1 ; sÞ ¼ 3 M2 ðx1 ; sÞ: h f112 ðx2 ; sÞ ¼
The initial conditions are assumed to be zero.
2 Solution Method The solutions of the problem (1), (2) are sought in integral form wðx1 ; x2 ; sÞ ¼ ¼
l N þ2 Z2 X k¼1
þ
½G1k1 ðx1 ; x2 ; f; sÞ fk11 ðf; sÞ þ G1k1 ðl1 x1 ; x2 ; f; sÞ fk12 ðf; sÞdf
0
l N þ2 Z1 X k¼1
½G1k2 ðx1 ; x2 ; n; sÞ fk21 ðn; sÞ þ G1k2 ðx1 ; l2 x2 ; n; sÞ fk22 ðn; sÞdn;
0
Hq ðx1 ; x2 ; sÞ ¼ ¼
l N þ2 Z2 X k¼1
þ
Gq þ 1;k1 ðx1 ; x2 ; f; sÞ fk11 ðf; sÞ þ Gq þ 1;k1 ðl1 x1 ; x2 ; f; sÞ fk12 ðf; sÞ df
0
l N þ2 Z1 X k¼1
Gq þ 1;k2 ðx1 ; x2 ; n; sÞ fk21 ðn; sÞ þ Gq þ 1;k2 ðx1 ; l2 x2 ; n; sÞ fk22 ðn; sÞ dn;
0
where Gikl are the surface Green’s functions, which satisfy the equations: € 1kl DG
N X 12 € G ¼ DDG þ aq DGq þ 1;kl ; 1kl 1kl h2 q¼1
G_ q þ 1;kl ¼ Dq DGq þ 1;kl þ Kq DDG1kl ; ð3Þ
and the following boundary conditions:
184
O. A. Afanasieva and A. V. Zemskov
@ 2 G1kl @x21
! þ aq Gq þ 1;kl ¼ d1k d1l dðsÞdðx2 fÞ; q¼1 !x1 ¼0 N P @ 2 G1kl þ @x2 þ aq Gq þ 1;kl ¼ d1k d2l dðsÞdðx1 nÞ; 2 q¼1 x2 ¼0 ! N P 2 2 @ G1kl @ G1kl þ k þ a G ¼ 0; 2 2 q q þ 1;kl @x1 @x2 q¼1 !x1 ¼l1 N P 2 2 k @ @xG21kl þ @ @xG21kl þ aq Gq þ 1;kl ¼ 0; 1 2 q¼1
2 þ k @ @xG21kl 2
k @ @xG21kl 2
1
N P
ð4Þ
x2 ¼l2
G1kl jx1 ¼0 ¼ d2k d1l dðsÞdðx2 kÞ; G1kl jx2 ¼0 ¼ d2k d2l dðsÞdðx1 kÞ; Gq þ 1;kl x1 ¼0 ¼ dq þ 2;k d1l dðsÞdðx2 kÞ; Gq þ 1;kl x2 ¼0 ¼ dq þ 2;k d2l dðsÞdðx1 kÞ; G1kl jx1 ¼l1 ¼ 0; G1kl jx2 ¼l2 ¼ 0; Gq þ 1;kl x1 ¼l1 ¼ 0; Gq þ 1;kl x2 ¼l2 ¼ 0: To ﬁnd the Green functions Gikl , the expanding into double trigonometric Fourier series in spatial coordinate and the Laplace transform in time are use. As a result, problem (3), (4) is reduced to the following system of linear algebraic equations (s is Laplace transform parameter): k1 ðmnm ; sÞGLss 1kl ðkn ; lm ; n; f; sÞ
N X
aq m2nm GLss q þ 1;kl ðkn ; lm ; n; f; sÞ
q¼1
¼ F1kl ðkn ; lm ; n; f; sÞ;
ð5Þ
Lss Kq m4nm GLss 1kl ðkn ; lm ; n; f; sÞ þ kq þ 1 ðmnm ; sÞGq þ 1;kl ðkn ; lm ; n; f; sÞ
¼ Fq þ 1;kl ðkn ; lm ; n; f; sÞ; where kn ¼ pn=l1 , lm ¼ p m=l2 . Other quantities are deﬁned as: 12 2 k1 ðmnm ; sÞ ¼ s mnm þ 2 þ m4nm ; kq þ 1 ðmnm ; sÞ ¼ s þ Dq m2nm ; m2nm ¼ k2n þ l2m ; h 4kn ð6Þ d1l d1k d2k k2n þ ð2 kÞl2m þ s2 sin lm f F1kl ðkn ; lm ; n; f; sÞ ¼ l1 l2 4l m d2l d1k d2k l2m þ ð2 kÞk2n þ s2 sin kn n; l1 l2 2
Unsteady ElasticDiffusion Oscillations of a Simply Supported Kirchhoff Plate
4 Fq þ 1;kl ðkn ; lm ; n; f; sÞ ¼ Kq kn d2k d1l k2n þ ð2 kÞl2m sin lm f l1 l2 4 Kq lm d2k d2l ð2 kÞk2n þ l2m sin kn n l1 l2 " # N X 4 þ Kq d1k þ Dq dq þ 2;k Kq aj dj þ 2;k ðlm d2l sin kn n þ kn d1l sin lm fÞ; l1 l2 j¼1 GLss ikl ðkn ; lm ; n; f; sÞ ¼
4 l1 l2
Zl1
ð7Þ
Zl2 GLikl ðx1 ; x2 ; n; f; sÞ sin kn x1 sin lm x2 dx2 dx1 ;
0
GLikl ðx1 ; x2 ; n; f; sÞ ¼
185
1 X 1 X
0
GLss ikl ðkn ; lm ; n; f; sÞ sin kn x1 sin lm x2
n¼1 m¼1
The solution of the system (5) has the form q; p ¼ 1; N;
l ¼ 1; 2
P1kl ðkn ;lm ;n;f;sÞ GLss ; 1kl ðkn ; lm ; n; f; sÞ ¼ Pðmnm ;sÞ
GLs q þ 1;1l ðkn ; lm ; n; f; sÞ ¼
4Kq ðd1l kn sin lm f þ d2l lm sin kn nÞ P ðkn ;lm ;n;f;sÞ þ q þ 2;1l ; Qq ðmnm ;sÞ l1 l2 kq þ 1 ðmnm ;sÞ 2 2 4 Kq kn d1l kn þ ð2 kÞlm sin lm f
GLs q þ 1;2l ðkn ; lm ; n; f; sÞ ¼ l1 l2 kq þ 1 ðmnm ; sÞ 2 2 4 Kq lm d2l ð2 kÞkn þ lm sin kn n Pq þ 2;2l ðkn ; lm ; n; f; sÞ þ kq þ 1 ðmnm ; sÞ l1 l2 Qq ð mnm ; sÞ d k D d K 4K 1l n q qp q ap sin lm f q GLs q þ 1;p þ 2;l ðkn ; lm ; n; f; sÞ ¼ kq þ 1 ðmnm ; sÞ l1 l2
4Kq d2l lm Dq dqp Kq ap sin kn n Pq þ 2;p þ 2;l ðkn ; lm ; n; f; sÞ þ ; þ kq þ 1 ðmnm ; sÞ Qq ðmnm ; sÞ l1 l2
ð8Þ
where Pðmnm ; sÞ ¼ k1 P m6nm
N X
aj Kj Pj ;
Qq ðmnm ; sÞ ¼ kq ðmnm ; sÞPðmnm ; sÞ:
j¼1
4 P11l ðkn ; lm ; n; f; sÞ ¼ l1 l2
P
m2nm
N X
! aj Kj Pj ðkn d1l sin lm f þ lm d2l sin kn nÞ;
j¼1
P12l ðkn ; lm ; n; f; sÞ ( ) N X 2 2 4kn 2 2 2 2 d1l kn þ ð2 kÞlm þ s P mnm aj Kj kn þ ð2 kÞlm Pj sin lm f ¼ l1 l2 j¼1 ( ) N X 2 2 4lm 2 2 2 2 þ d2l lm þ ð2 kÞkn þ s P mnm aj Kj lm þ ð2 kÞkn Pj sin kn n; l1 l2 j¼1
186
O. A. Afanasieva and A. V. Zemskov
P1;q þ 2;l ðkn ; lm ; n; f; sÞ ¼
4aq m2nm l1 l2
D q Pq
N P
! aj Kj Pj ðkn d1l sin lm f þ lm d2l sin kn nÞ;
j¼1
Pq þ 1;kl ðkn ; lm ; n; f; sÞ ¼ Kq m4nm P1kl ðkn ; lm ; n; f; sÞ; N N Q Q Pðmnm ; sÞ ¼ kj þ 1 ðmnm ; sÞ; Pj ðmnm ; sÞ ¼ kr þ 1 ðmnm ; sÞ: j¼1
r¼1;r6¼j
Since Prkl ðkn ; lm ; n; f; sÞ are rational functions of the transformation parameter s, the originals in equalities (8) are calculated on the base of residues and the tables of operational calculus. This work was funded by the subsidy from RFBR (Project №200800589 A).
Reference 1. Zemskov, A.V., Tarlakovskii, D.V.: Model nestatsionarnykh uprugodiffuzionnykh kolebaniy plastiny Kirchhoffa. XII Vserossiyskiy syezd po fundamentalnym problemam teoreticheskoy i prikladnoy mekhaniki: sbornik trudov v 4 tomakh. T. 3: Mekhanika deformiruyemogo tverdogo tela, pp. 906–909, Ufa, RITs BashGU (2019). In Russian). https://doi.org/10.22226/ 241035352019congressv3
A Dynamic Contact Problem of Torsion that Reduces to the Singular Integral Equation with Two Fixed Singularities V. Popov(&)
and O. Kyrylova
National University «Odessa Maritime Academy», Odessa, Ukraine [email protected], [email protected] Abstract. An elastic cylinder of ﬁnite length, one of the ends of which is perfectly coupled to the surface of the elastic halfspace is considered. A round rigid plate of the same radius is coupled to the other end of the cylinder, and is loaded the torsion moment that is harmonic depend of time. The surface of the halfspace outside the contact area with the cylinder and the side surface of the cylinder are been unload. The formulated boundary problem is reduced to a singular integral equation for a function related to stresses in the contact area of the cylinder and halfspace. Since the kernel of this integral equation contains ﬁxed singularities, a numerical method for solving this equation the is main result. After solving the integral equation, approximate formulas for calculating the contact stresses. Keywords: Torsion oscillation Contact problem Singular integral equation
1 Introduction At nowadays, one of the effective methods for solving the boundary value problems of the mechanics of a deformable body is to reduce them to solving integral equations, most often singular ones. Since the exact solution of these equations is rarely possible, the actual problem is the creation of numerical methods for their solution. The presence in the singular part of kernels with ﬁxed singularities makes it difﬁcult to solve r integral equations. In the monograph [1], as well as in articles [2–4] where exact solutions of singular integral equations are found, it is proved that the presence of ﬁxed singularities affects the asymptotic behavior of the solution near the ends of the integration segments. Despite this, in many cases the real asymptotic of the unknown functions is either not taken into account Therefore, the convergence of these numerical methods is quite slow. Articles [5–8] show that the methods based on the use of special quadrature formulas for singular integrals and taking into account the real asymptotic of the solution are most effective in the sense of convergence. Such method for an integral equation with two ﬁxed singularities, to which the contact problem of torsional vibrations of a cylinder on an elastic half space reduces is proposed in this article.
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 187–192, 2020. https://doi.org/10.1007/9783030478834_35
188
V. Popov and O. Kyrylova
2 Statement of the Problem and Its Reduction to a Singular Integral Equation
Fig. 1. The elastic cylinder coupled with half space
Let an elastic cylinder 0 r\r0 ; 0 z\a; 0 u\2p locate on the elastic halfspace 0 r\ þ 1; 1\z 0; 0 u \2 p (Fig. 1) and coupled to it. A round rigid plate of the same radius as the cylinder and the thickness d is connected to the upper end of the cylinder. A torsion moment Mei x t , harmoniously dependent on time, is exerted to the plate. The factor ei x t that determines the dependence on time is omitted farther. Under such conditions, an axisymmetric torsional deformation is realized in the cylinder and halfspace and only angular displacements wj ðr; zÞ; j ¼ 1; 2 is nonzero. They are determined from the equations q2j x2 @ 2 wj 1 @wj w2j @ 2 wj 2 2 þ þ þ j w ¼ 0; j ¼ ; j ¼ 1; 2; j 2j 2j r @r @r 2 r2 @z2 G2j
ð1Þ where w1 ðr; zÞ is displacement in cylinder, w2 ðr; zÞ is displacement in half space, q1 ; G1 are shear modulus and density of the cylinder, q2 ; G2 are shear modulus and density of the half space. In the area of contact between the cylinder and the halfspace, the following equations are satisﬁed: sðu1zÞ ðr; þ0Þ ¼ qðr Þ; sðu2zÞ ðr; 0Þ ¼ qðr Þ; 0 r\r0
ð2Þ
where qðr Þ is unknown stresses in the contact area. Also in the contact area, the condition of continuity of displacements is fulﬁlled w1 ðr; þ0Þ ¼ w2 ðr; 0Þ; 0 r\r0 :
ð3Þ
The surface of the halfspace outside the contact area is considered unloaded sðz2uÞ ðr; 0Þ ¼ 0; r [ r0 :
ð4Þ
On the upper end of the cylinder, the conditions of couple to the plate is satisﬁed w1 ðr; aÞ ¼ h0 r; 0 r r0 :
ð5Þ
where h0 is unknown plate rotation angle, It is determined from the equation x2 j0 h0 ¼ M MR ; j0 ¼ p r04 dq0 =2
ð6Þ
A Dynamic Contact Problem of Torsion that Reduces to the Singular Integral Equation
189
where j0 is the moment of inertia of the plate, MR is the moment of the reaction forces. There q0 is density of the plate. The lateral surface of the cylinder is not loaded: sðru1Þ ðr0 ; zÞ ¼ 0; 0\z\a:
ð7Þ
Angular displacement in a cylinder is the solution of the boundary value problem (1), (2), (5), (7) and it equal Zr0 w1 ðr; zÞ ¼
g 0
qðgÞ cos j21 z F1 ðg; r; zÞdg þ h0 r : G1 cos a j21
ð8Þ
1 2X K2 ðqk1 r0 Þ 1 I1 ðqk1 gÞI1 ðqk1 r Þ cos kk z; g ðg; r Þ þ F1 ðg; r; zÞ ¼ a k¼1 k I2 ðqk1 r0 Þ g1k ðg; r Þ ¼
I1 ðqk1 r ÞK1 ðqk1 gÞ; r\g; I1 ðqk1 gÞK1 ðqk1 r Þ; r [ g;
kk ¼
pð2k 1Þ ; qk1 ¼ 2a
qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ k2k g221 :
Angular displacement in halfspace is the solution of boundary value problem (1), (2) (4), and it equal to Zr0 w2 ðg; r Þ ¼ 0
qðgÞ g G2
Zþ 1 0
b eq2 ðbÞz J1 ðb r ÞJ1 ðb gÞdb dg; q2 ðbÞa ¼ q2 ðbÞ
qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ b2 j222
ð9Þ
Now it is necessary to ﬁnd the unknown contact stresses qðr Þ for the ﬁnal determination of the displacement in the cylinder and the halfspace For this purpose, the integral equation was obtained by substitution (8), (9) in (3). This integral equation can be transformed into a secondkind integral equation [9] for a new unknown function. This function is related to contact stresses by the next formulas Zr0 uð xÞ ¼ x
qðgÞ 2 @ g pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ dg; qðgÞ ¼ 2 2 p @g g x
Zr0 g
uð xÞdx pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ: x2 g2
ð10Þ
As a result of the transformations detailed in [9] and the extraction of the singular component, this equation takes the following form: 1 ð1 þ cÞgðfÞ þ p
Z1
1 1 15 þ lnð2 þ s þ fÞ 2 s f 2þsþf 4 1 15 2h0 f lnð2 þ s þ fÞ þ Rðs; fÞ ds ¼ ; 1\f\1: 4 cosðc j0 Þ gð s Þ
ð11Þ
190
V. Popov and O. Kyrylova
When deriving Eq. (11) the next notation was taken: x ¼ r0 s; y ¼ r0 f , uðr0 sÞ ¼ r0 G1 gðsÞ; c ¼ a=r0 ; j0 ¼ j21 r0 ; c ¼ G1 =G2 .
3 The Numerical Solution of Integral Equation For construction an efﬁcient numerical method of solving Eq. (11), we need to ﬁnd out the asymptotic of the unknown function gðsÞ for s ! 1. This deﬁnes the following form of solution: r 1 1 ; gðsÞ ¼ 1 s2 wðsÞ; r ¼ arcsin p cþ1
ð12Þ
where wðsÞ is a function that satisﬁes the Holder conditions. Quadrature formulas for singular integrals are based on the approximation of the function by the following interpolation polynomial: wðsÞ Wn ðsÞ ¼
n X m¼1
wm
Pr;r n ðsÞ ; 0 r;r ½Pn ðsm Þ ðs sm Þ
ð13Þ
where wm ¼ wðsm Þ, Pr;r n ðsÞ are Jacobi polynomials and sm are roots of these polynomials. As a result, we obtain the quadrature formulas by the method described in detail in the article [5] Z1 1
rr 0 r nþ1 n X Arr Bn 11 ð1 s2 Þ wðsÞ m Pn ðsm Þ þ ð1Þ 2 ds ¼ ; wm rr ðs Þ 0 ð2 s 1Þ 2sf P m m m¼1 n
ð14Þ
" # þ1 þ1 X Cð1 þ r þ nÞ X rþj j Cnj Y Bnj Y ; Bn ðYÞ ¼ þ 22r n! j¼0 j¼0 Cnj ¼
ð1Þ j Cðr nÞCð1 þ r þ n þ jÞ ð1Þ j Cðr jÞCð1 þ n þ jÞ ; Bnj ¼ ; j!Cð1 þ r þ n þ jÞ j!Cð1 þ 2r þ n jÞ
where Arr m are coefﬁcients of the Gauss – Jacobi quadrature formula [10]. Similar formulas for integrals with a logarithmic singularity are obtained by the same method [5]: Z1
2 r
ð1 s Þ wðsÞlnð2 s fÞds: ¼ 1
n X m¼1
Arr m wm
n1 Prr ðs Þ
X 1f m j : j 2 hj 2 j¼0 ð1Þ rj
ð15Þ
The functions hj ðY Þ are represented by series similar to these in formula (17). Then in Eq. (11) the quadrature formulas (15), (17) are applied to the singular integrals, and to the regular ones the Gauss  Jacobi quadrature formulas [12] and as
A Dynamic Contact Problem of Torsion that Reduces to the Singular Integral Equation
191
collocation points are taken f ¼ sk ; k ¼ 1; 2; . . .; n. The result of these actions is a system of linear algebraic equations for wm ; m ¼ 1; 2; . . .; n. To the resulting system it is necessary to add the equation of motion of the plate (6). After solving the system, from formulas (10), (12), (13) we obtain formulas for the approximate calculation of the contact stresses. sðfÞ ¼
n 1 X qðr0 fÞ ¼ fð1 f2 Þr2 Wm Arr m Wm ðfÞ G1 m¼1
ð16Þ
Here functions Wm ðfÞ are represented through hypergeometric functions very cumbersomely.
4 Results of Numerical Analysis and Conclusions The cylinder of radius r0 ¼ 0,2 m of aluminum coupled to a cast iron base is considered, as an example. The plate adhered to the upper end of the cylinder is steel and has a thickness of d ¼ 0,02 m. The plate is loaded by the moment with amplitude of M ¼ 1000 n m. The frequency of oscillation changes so that the dimensionless wave pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ number j0 ¼ j2 r0 ¼ x r0 q1 =G1 is in the range 0 j0 10 (Fig. 2).
a) κ 0 = 0
b) κ 0 = 2
Fig. 2. The contact stresses for other values of frequency and relative height of cylinder
The calculations showed that to obtain the values of contact stresses and the angle of rotation with a relative error of less than for the numerical solution of the integral Eq. (11) in the formula (13), it sufﬁces to use 10–15 interpolation points. Using formula (18), the influence of the frequency and the ratio of the dimensions of the cylinder on the values of contact stresses is studied. The results of these studies are shown in the ﬁgures. The graphs in these ﬁgures correspond to the following values of the ratio of the height of the cylinder to its radius 1−c ¼ 1; 2−c ¼ 2; 3−c ¼ 3; 4−c ¼ 4: The following conclusions can be drawn based on the analysis of the results
192
V. Popov and O. Kyrylova
of the calculations. The proposed method for numerically solving a singular integral equation with a ﬁxed singularity with a small volume of calculations allows us to obtain results with high accuracy. This is explained by the fact that the solution takes into account the real asymptotic of unknown functions, and use special quadrature formulas are derived for singular integrals. At torsion of a cylinder which is coupled with an elastic foundation, the highest values of contact stress are observed under static loading j0 ¼ 0. In the same case, with an increase in the relative length of the cylinder, the absolute values of the contact stress increase. Monotonic increase in the absolute values of contact stresses is observed when approaching the boundary of the contact region in the considered frequency range 0 j0 10.
References 1. Duduchava, R.: Integral Equations of Convolution with Discontinuous Presymbols, Singular Integral Equations with Fixed Singularities, and Their Applications to Problems of Mechanics. Razmadze Institute of Mathematics, Academy of Sciences of Gruz. SSR. Tbilisi (1979). (in Russian) 2. Stullybrass, M.: A crack perpendicular to an elastic halfplane. Int. J. Eng. Sci. 8(5), 351– 362 (1970) 3. Hrapkov, A.: The problems of elastic equilibrium of an inﬁnite wedge with an asymmetric incision at the apex, solved in a closed form. Prikladnaya matematika i mehanika. 36(6), 1062–1069 (1971) 4. Afyan, B.: On the integral equations with ﬁxed singularities in the theory of branched cracks. Dokl. AN Arm. SSR 79(4), 60–65 (1984) 5. Popov, V.: A dynamic contact problem which reduces to a singular integral equation with two ﬁxed singularities. J. Appl. Math. Mech. 76(3), 348–357 (2012) 6. Popov, V.: A crack in the form of a threelink broken line under the action of longitudinal shear waves. J. Math. Sci. 222(2), 143–154 (2017) 7. Popov, V.: Problems of interaction longitudinal shear waves with Vshape tunnels defect. J. Phys: Conf. Ser. 991(1), 012066 (2018) 8. Lytvyn, O., Popov, V.: Interaction of harmonic longitudinal shear waves with vshaped. Incl. J. Math. Sci. 240, 1–16 (2019) 9. Popov, V.: Stress state of ﬁnite elastic cylinder with a circular crack undergoing torsion vibration. Int. Appl. Mech. 48(4), 430–437 (2012) 10. Krylov, V.: Approximate Calculation of Integrals. Dover, New York (2006)
Some Dynamic Problems for Layered Composites Sergey Pshenichnov(&) Institute of Mechanics, Lomonosov Moscow State University, Michurinsky Prospect 1, Moscow 119192, Russia [email protected]
Abstract. The problems of constructing analytical solutions of nonstationary dynamic problems for layered composites in the case when all the layers are linearly viscoelastic, but their hereditary properties are determined by only one kernel, the same for all layers, are considered. In this case, the Poisson’s ratio of the material of each layer becomes timeindependent. A special case is considered when all the layers are linearly elastic. The perturbation propagation region is assumed to be limited. The integral Laplace transform in time is applied, followed by inversion. Sufﬁcient conditions, under which all the poles of the solution in the transforms are simple, are formulated. The question of the location of these poles is considered. An example is given of constructing an analytical solution to a twodimensional nonstationary dynamic problem for a cylindrical body consisting of elastic or viscoelastic layers under the above assumption. The results of a study of twodimensional transient wave processes in a layered cylindrical elastic body, based on the corresponding analytical solution, are presented. Keywords: Dynamics of layered composites bodies Wave processes
Piecewise homogeneous
1 Introduction In the study of transient wave processes in layered solids, one of the important directions is to conduct research based on analytical solutions of the corresponding initialboundaryvalue problems. Known analytical results in this area for the case when the layers are linearly viscoelastic can be found, for example, in [1–7]. At the same time, many unexplored issues remain within the framework of this topic. This primarily concerns the study of the influence of the properties of the material on nononedimensional transient wave processes in bodies with an arbitrary number of interfaces between homogeneous components. Known analytical solutions often turn out to be valid only in a limited range of time changes, or with signiﬁcant restrictions on the material properties of homogeneous components (layers), or the solution is difﬁcult to analyze. Earlier, the author of this paper examined theoretical issues related to the construction of solutions to nonstationary dynamic problems for composites with an arbitrary number of homogeneous linear viscoelastic layers by the Laplace transform method with subsequent inversion [8]. At the interfaces between the layers, it © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 193–197, 2020. https://doi.org/10.1007/9783030478834_36
194
S. Pshenichnov
was assumed that the continuity conditions for the displacement and stress vectors were fulﬁlled, and the disturbance propagation region was considered limited. Statements about important properties of solutions in images were formulated and proved, which facilitate the construction of originals. These statements reveal the connection between the branch points and the poles of the solution of the problem in images with the spectrum of the corresponding problem of free vibrations of the piecewisehomogeneous body under consideration. This work is devoted to nonstationary dynamic problems for layered composites in the case when all the layers are linearly viscoelastic, but their hereditary properties are determined by only one kernel, the same for all the layers. Moreover, the Poisson’s ratio of the material of each layer does not depend on time. A special case when all layers are linearly elastic is considered.
2 Mathematical Formulation of the Problem Let us consider the nonstationary dynamic problem for a layered composite occupying a domain X with a boundary R and consisting of N homogeneous isotropic linearviscoelastic components (layers): X ¼ X1 [ X2 [ . . . [ XN (Xi and Xj do not intersect at internal points if i 6¼ j). On the contact surfaces between these components the conditions of continuity of displacement and stresses vectors are satisﬁed. Consider the case when volumetric and shear relaxations kernels of the material of every component ðnÞ ðnÞ are identical: Tv Ts ðtÞ TðtÞ; n ¼ 1; 2; . . .; N. In this case Poisson’s ratio in ðnÞ every component is timeindependent: mðnÞ m0 ðconstÞ. For each component of the body we write the equations of dynamics (n ¼ 1; 2; . . .; N): ^ L ^ðnÞ uðnÞ ðx; tÞ þ f ðnÞ ðx; tÞ ¼ qn u €ðnÞ ðx; tÞ ð1 TÞ
ð1Þ
and the constitutive relations ^ ^lðnÞ uðnÞ ðx; tÞ; ~ðnÞ ðx; tÞ ¼ ð1 TÞ r
xðx1 ; x2 ; x3 Þ 2 Xn
ð2Þ
For components with numbers 1 m N, having the common points with a boundary R ¼ R1 [ R2 , we present the boundary conditions ~ðmÞ ðx; tÞn ¼ pðmÞ ðx; tÞ; r ðmÞ
u
x 2 R1 ðmÞ
ðx; tÞ ¼ q
ðx; tÞ;
x 2 R2 ;
t[0
ð3Þ
On the contact surface of adjacent components with numbers p and q let us write down the relationships uðpÞ ðx; tÞ ¼ uðqÞ ðx; tÞ;
~ðpÞ ðx; tÞ n ¼ r ~ðqÞ ðx; tÞn; r
x 2 Rpq
ð4Þ
Some Dynamic Problems for Layered Composites
195
For each component, we set the initial conditions ðnÞ
uðnÞ ðx; 0Þ ¼ b1 ðxÞ;
ðnÞ u_ ðnÞ ðx; 0Þ ¼ b2 ðxÞ;
x 2 Xn
ð5Þ
^ðnÞ and ^lðnÞ are differential operators, T^ is integral operator: Here L ^ðnÞ uðnÞ ðx; tÞ ¼ ðkðnÞ þ lðnÞ Þgrad div uðnÞ ðx; tÞ þ lðnÞ D uðnÞ ðx; tÞ; L 0 0 0 ^lðnÞ uðnÞ ðx; tÞ ¼ 2lðnÞ def uðnÞ ðx; tÞ þ kðnÞ div uðnÞ ðx; tÞ ~I; 0 0 Zt ^ ^ TnðtÞ ¼ Tðt sÞnðsÞ dsTnðtÞ;
ð6Þ
ð7Þ
0
~ðnÞ is the stress tensor; uðnÞ , pðmÞ , qðmÞ A dot above a letter means a time derivative; r ðnÞ ðnÞ f , b1 , b2 are the vectors of displacements, the vectors of boundary actions, the volume forces, and the initial displacements and velocities related to the layer with the corresponding number; qn is density; n is the unit outward normal to the corresponding ðnÞ ðnÞ boundary; D is the Laplace operator; ~I is the unit tensor; k0 ; l0 are Lame elastic constants. It is assumed that the area of disturbance is bounded, the displacement of the body as a rigid whole is excluded, and the creep of the material is limited. ðnÞ
3 The Theoretical Results To equations and relations (1)–(4) the Laplace transform in time is applied. Taking into account (6), (7) and the initial conditions (5), we obtain the problem for the transforms. Sufﬁcient conditions under which all the poles of the solution in the transforms UðnÞ ðx; sÞ are simple are formulated (s is the complex parameter of the Laplace transform, UðnÞ ðx; sÞ is the transforms of variables uðnÞ ðx; tÞ). The question of the location of these poles is considered. The case when the initial conditions are zero and the volume forces are absent: ðnÞ
b1 0;
ðnÞ
b2 0;
f ðnÞ ðx; tÞ 0;
ð8Þ
vectors of external influences are represented in the form: ðmÞ
pðmÞ ðx; tÞ ¼ p0 ðxÞ uðtÞ;
ðmÞ
qðmÞ ðx; tÞ ¼ q0 ðxÞ wðtÞ
ð9Þ
and the hereditary properties of the layers are characterized by a kernel: TðtÞ aebt ; is considered separately.
0\a\b=2;
ð10Þ
196
S. Pshenichnov
It is shown that if uðtÞ ¼ h ðtÞ, wðtÞ ¼ h ðtÞ, where h ðtÞ is the Heaviside function, then the poles of the transforms UðnÞ ðx; sÞ will obviously be simple. They are located to the left of the imaginary axis (except s ¼ 0) and are easily found. If, under these conditions, all homogeneous layers of the body are linearly elastic (TðtÞ 0), then all the poles of the transforms UðnÞ ðx; sÞ, being simple, are located on the imaginary axis. Here, it is assumed that the disturbance propagation region is limited, therefore, according to the general statement proved in [8], under the assumptions made, the branch points of the transforms UðnÞ ðx; sÞ are absent. This greatly simpliﬁes the construction of the original uðnÞ ðx; tÞ using the theory of residues, which, under the assumptions made, are not difﬁcult to ﬁnd. We note that, having built a solution for the case uðtÞ ¼ h ðtÞ, wðtÞ ¼ h ðtÞ, it is possible to obtain solutions using other uðtÞ; wðtÞ as well.
4 An Example of Applying Theoretical Results Let us consider the process of twodimensional nonstationary wave propagation in crosssection of a hollow inﬁnite cylinder R0 \R\RN , p\h p (R; h – polar coordinates in the plane of the cross section). The cylinder consists of N homogeneous coaxial layers. On the contact surfaces between these layers R ¼ Rm , m ¼ 1; 2; . . .; N 1 the conditions of continuity of displacement and stresses vectors are satisﬁed. We consider the material ðnÞ ðnÞ of layers to be linearly elastic or viscoelastic with the condition Tv Ts ðtÞ TðtÞ when the hereditary kernel has the form (10). Cylinder surface R ¼ R0 is free. Its external surface R ¼ RN is subjected to the constant along the cylinder element radial load fR ðh; tÞn, fR ðh; tÞ ¼ PðtÞ H ðhÞ (n is the unit outward normal), starting from time point t ¼ 0. Here the function H ðhÞ has such a form that the load is selfbalanced. The solution of this problem for the case of elastic layers was constructed in the work [9]. In this paper, for the case when all layers are elastic, the solution is slightly modiﬁed and made more convenient for numerical implementation. In addition, a solution is constructed for the case when all the layers are viscoelastic. Fourier series expansion in h and time Laplace transform with the following inversion were applied. In the represented work we have carried out research of transient wave processes for an elastic layered cylinder with different initial data. In particular, cases where the physicomechanical properties of the layers differ quite signiﬁcantly are considered. For example, shear moduli differ by two orders of magnitude.
5 Conclusions Nonstationary dynamic problems of class (1)–(7) are considered for layered composites in the case when the region of propagation of perturbations is bounded. At the same time, all the layers are linearly viscoelastic and their hereditary properties are determined by only one kernel, the same for all the layers. It is shown that in the case of a twoparametrical exponential kernel (10) the solution of a nonstationary dynamic problem for viscoelastic layered composite will not be hard to obtain if a solution of the
Some Dynamic Problems for Layered Composites
197
corresponding problem for elastic layered composite is already known. In the above stated example of a twodimensional nonstationary dynamic problem, the solution remains correct for the entire period of time changing.
References 1. Sabodash, P.F.: Propagation of longitudinal viscoelastic waves in a threelayer medium. Polymer Mech. 7(1), 124–128 (1971). [in Russian] 2. Kozlov, V.I., Kucher, N.K.: Dynamic behavior of multilayer cylindrical structures with transient loads. Strength Mater. 12(5), 639–648 (1980). [in Russian] 3. Nuriev, B.R.: Impact on a Viscoelastic Layered Composite. Izv. Akad. Nauk AzSSR. Ser. FizTekh. Mat. Nauk 4, 35–41 (1985). [in Russian] 4. Songnan, L., Ping, G.: Dynamic response of layered viscoelastic halfspace and its application to dynamic foundation problems. Hubnan Daxue Xuebao. J. Hunan Univ. 20(1), 57–64 (1993) 5. Lokshin, A.A.: The head wave at the boundary of two hereditaryelastic halfspaces. The case of a linear source. J. Appl. Math. Mech. 58(1), 171–176 (1994) 6. Suk Lee, H.: Viscowave – a new solution for viscoelastic wave propagation of layered structures subjected to an impact load. Int. J. Pavement Eng. 15(6), 542–557 (2014) 7. Hosseini Hashemi, S., Bakhshi Khaniki, H.: Dynamic behavior of multilayered viscoelastic nanobeam system embedded in a viscoelastic medium with a moving nanoparticle. J. Mech. 33(5), 559–575 (2017) 8. Pshenichnov, S.G.: Dynamic linear viscoelasticity problems for piecewise homogeneous bodies. Mech. Solids 51(1), 65–74 (2016) 9. Bulychev, G.G., Pshenichnov, S.G.: Propagation of elastic waves in layered cylinder. Doklady AN USSR 303(5), 1074–1078 (1988). [in Russian]
The Influence of Geometric Parameters on the Bearing Capacity of TransformableVolume Structure L. M. Lobanov(&), V. S. Volkov, O. V. Makhnenko, S. M. Kandala, and Y. V. Borovyk E.O. Paton Electric Welding Institute of the NAS of Ukraine, Kiev, Ukraine [email protected], [email protected]
Abstract. The metal transformablevolume structure (TVS) for aerospace purposes, which consist of corrugated conical sections, was investigated. The design scheme of the TVS with a minimum mass should provide stability to the action of inertial loads in operating conditions in space orbit. The influence of the main geometric parameters of TVS made of stainless steel on the bearing capacity are determined. The effect of corrugation of the conical sections on natural frequency of TVS was considered. The results of calculating estimation of stressstrain state of the TVS under speciﬁed for space orbital station inertial loads were showed. Keywords: Transformablevolume structures Stainless steel Loadcarrying shells Foldable shells Deployable structures Inflatable structures Surfaces of zero total curvature
Light multicone TVSs with a large transformation coefﬁcient are promising for use in space apparatus engineering as loadbearing elements for the distancing of an equipment to several meters from the base orbital station. The advantages of multicone TVS in comparison with other transformable structures of equal mass and length are, ﬁrst of all, signiﬁcantly higher compactness and the ability to compensate for large load values without loss of stability [1].
1 Features of the Formation of Geometry TVS In the manufacture of multicone TVS the truncated conical section is shaped to a compact state using the proposed in E.O.Paton Electric Welding Institute the method of successive mirror image of surface sections Q1 … Qn with respect to equidistant parallel planes c1 … cn (see Fig. 2a), in which the transformation is close to isometric and occurs with the minimum possible stretching and compression of the middle surface of a thin shell. The sequence of transformed sections of the surface Q1…Qn when using sheet metals takes the form (Fig. 2b), which is explained by restrictions on the minimum allowable bending radius of the material. This restriction is one of the main factors determining the fold step b, the number of annular folds n for a given cone angle a, generatrix length S and the compactness KT of the shell of a multicone TVS: © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 198–203, 2020. https://doi.org/10.1007/9783030478834_37
The Influence of Geometric Parameters
KT ¼ 2 n ¼
2 S sin a ; b
199
ð1Þ
at the same time, n increases with decreasing thickness of the material of the conical section, and sections with a smaller thickness at a constant KT have a lower height HK.
2 Determination of the Influence of TVS Geometric Parameters on the Bearing Capacity TVS consists of a certain number of tapered sections hermetically welded together, the geometric parameters of which are determined by the technical requirements for the design. In the process of investigating the influence of TVS parameters on the bearing capacity, such parameters as the diameter, number of cones, and also the thickness and degree of flatness of the corrugation of the metal shell were varied, while its physical and mechanical characteristics were unchanged. The main characteristic characterizing the rigidity of the structure was the ﬁrst form of natural vibrations, which was determined by numerical calculation methods. The equation for determining the values of the own oscillations has the form [2]: x2 ½M þ ½K fug ¼ 0;
ð2Þ
where [M] is the mass matrix, [K] is the stiffness matrix, {u} is the eigenvector. 2.1
Natural Frequencies of Smooth Conical Sections
The investigation was conducted on ﬁnite element models TVS 3000 mm long, consisting of a different number of smooth conical shell elements (from 25 to 68), a diameter of 426 mm to 1000 mm and a wall thickness in the range of 0.15…0.4 mm Material  AISI321 stainless steel. The model consisted of smooth conical elements, which eliminates the influence of the degree of corrugation of the surface on the results of a investigation of the influence of the main geometric parameters of TVS (Fig. 3). The results obtained (Fig. 4) within the investigated range of TVS parameters showed that the natural frequency of TVS vibrations increases with increasing wall thickness (T) and diameter of conical elements (D), as well as reducing their number (N). Nevertheless, an increase in the wall thickness and the diameter of the conical elements to increase the rigidity of the TVS leads to an increase in the mass of the shell, the limitation of which is critically important in the design of aerospace structures. In addition, an increase in thickness leads to a sharp increase in the force of forming and internal pressure for subsequent disclosure, i.e. to increase the complexity, the required reliability and weight and size characteristics of auxiliary technological equipment. According to results Fig. 4c, we can conclude that the number of conjugation sections of conical sections (especially, smaller diameter) that have the smallest relative rigidity and in which the strains during the oscillations are maximal contributes to the change in the natural frequency of vibrations of the TVS. Thus, one of the solutions to
200
L. M. Lobanov et al.
increase the frequency can be a change in the possible limits of the geometric parameters of the conical sections with their constant thickness, in particular, a slight decrease in the taper angle and an increase in the height of the section. The limits for decreasing the angle a require experimental conﬁrmation, since a concomitant increase in the crease depth a (see Fig. 4) can signiﬁcantly worsen the quality of the TVS disclosure. 2.2
Natural Frequencies of Corrugated Conical Elements
After the TVS is disclosure by internal excess pressure, the conical sections acquire concentric annular features corresponding to the vertices of the folds in which the front surfaces of the metal shell undergo plastic deformation. The initial generatrix of a smooth conical shell after folding and subsequent disclosure has a wavelike proﬁle, which can be approximately described by a sinusoidal function. Each of the proﬁles is described by a function of the form y ¼ c sinðpx tÞ;
ð3Þ
where c = 1..2, p = 0.25 and t = 1.57. The degree of corrugation of the TVS surface is determined primarily by the parameter c, the amplitude of the sinusoidal shape of the corrugation. The surface flatness increases with decreasing parameter c. To take into account the influence of the degree of corrugation of the TVS surface on the results of the investigation, FE models consisting of conical elements whose surface had a wavy proﬁle were used (Fig. 1a). The results of numerical solutions (Fig. 5) have shown a signiﬁcant decrease in the natural frequency (f = 2,8…5,1 Hz) of oscillations of a TVS with a wavelike proﬁle compared with a flat design (f = 7,8 Hz). According to Fig. 5b, with an increase in the depth of the corrugation, a decrease in the frequency of natural vibrations is observed. This is due to an increase in the mass of the structure and a decrease in its stiffness.
Fig. 1. The geometric scheme of TVS in the folded (a) decomposed (b) state.
Reduction the degree of corrugation can reduce the mass of TVS, but requires more internal pressure to disclosure of structure. Thus, a rational way to optimizing the TVS design scheme is to reduce the number of conical sections while reducing their taper in the approaching a more rigid cylindrical structure.
The Influence of Geometric Parameters
201
Fig. 2. Theoretical scheme of transformation of the middle surface of a truncated conical shell (a), a sequence of transformed sections of the surface Q1 … Qn when using sheet metals (b)
Fig. 3. TVS geometric model for numerical analysis
2.3
TVS Stress Strain State Determination
According to [3], one of the main loads acting on equipment installed inside and outside the ISS modules is inertial loads, which are speciﬁed in the form of angular and linear accelerations: aX = 12 m/s2, aY = 12 m/s2, aZ = 9 m/s2, eX = 1.4 rad/s2, eY = 1.4 rad/s2, eZ = 0.4 rad/s2, where the Z axis corresponds to the axial direction of the structure, and the X and Y axes correspond to orthogonal radial directions. [4]. Additionally, as a payload for one of the design cases, a load of 3 kg was secured at the top of the TVS. As a criterion for the strength of TVS, the condition r0:2 reqv
ð4Þ
where r0.2 = 205 MPa is the yield strength of the material; reqv – equivalent stresses. The results of calculating the stressstrain state of the TVS (f = 5,1 Hz) under speciﬁed inertial loads showed that the maximum equivalent stresses do not exceed 148 MPa, stress concentrators are located in the area of welded joints at the junction of small diameters and adjacent corrugated folds with a predominance of axial tensile stresses. For the loading with 3 kg payload rather substantially higher equivalent stresses up to 200 MPa and maximum displacement 27 mm (Fig. 6) were obtained. Besides the optimization of geometric parameters the bearing capacity of TVS would be increased by the introduction of additional structural elements (stiffeners).
202
L. M. Lobanov et al.
Fig. 4. The dependence of the natural frequencies of vibration of the TVS (L = 3000 mm) on the thickness (a) of the structural material, the diameter of the conical section (b), the number of cones (c), the elastic modulus of the material (d)
Fig. 5. Natural frequency of TVS: corrugated and flat surface depending on the thickness of the material (a), corrugated surface depending on the depth of the corrugation (b)
The Influence of Geometric Parameters
203
Fig. 6. Calculation model (a), where 1 – rigid ﬁxing, 2 – inertial loads [2], 3 – payload; Mises stresses, MPa (b); equivalent displacements, mm (c).
3 Conclusions • an increase in the bearing capacity of TVS due to an increase in diameter and wall thickness is advisable but within the massdimension requirements of the structure; • the approximation of TVS to a cylindrical shape by reducing the number of conical elements is an effective way to increase the loadbearing capacity of the structure, but it has strict technological limitations in the manufacturing; • the corrugation of a conical surface greatly reduces rigidity of TVS, thus the loadbearing capacity of the structure can be signiﬁcantly increased by reduction the degree of corrugation of the conical sections.
References 1. Lobanov, L., Volkov, V., Yakimkin, A.: Construction methods and comparative evaluation of metal deployable loadcarrying shell structures. J. Aerosp. Technol. Manag. 10, e3818 (2018). https://doi.org/10.5028/jatm.v10.959 2. Abaqus 6.13 Online Documentation. http://dsk.ippt.pan.pl/docs/abaqus/v6.13/ 3. ISS User Manual (ISS RS Guide). http://knts.tsniimash.ru/ru/src/CenterInfRes/iss_rs_guide. pdf 4. Lobanov, L.M., Volkov, V.S., Yakimkin, A.V., Savitsky, V.V.: Functional characteristics improvement of metal transformablevolume structures for space applications. J. Aerosp. Technol. Manage. 8(1), 55–62 (2016). https://doi.org/10.5028/jatm.v8i1.529
The Influence of Mixed Conditions on the Stress Concentration in the Neighborhood of Interfacial Inclusions in an Inhomogeneous Transversely Isotropic Space Oleksandr Kryvyi1(&) 1
and Yurii Morozov2
National University “Odessa Maritime Academy”, Odessa, Ukraine [email protected] 2 Odessa National Polytechnic University, Odessa, Ukraine
Abstract. Two mixed nonaxisymmetric problems on an absolutely rigid circular interphase inclusion in a piecewisehomogeneous transversalisotropic space are considered. One face of inclusion is in conditions of smooth contact, and on the other, conditions of full adhesion to the medium are realized or there is no contact with the medium. Using exact solutions to these problems, the influence of the boundary conditions on the stress concentration in the neighborhood of the inclusion is analyzed. In particular, it has been established that under mixed conditions the stresses have a powerlaw singularity, the indices of which depend on the elastic constant transversally isotropic halfspaces. In the case of detachment, the powerlaw singularity is ampliﬁed by oscillatory multiplier. Keywords: Interphase circular inclusion Singular integral equations Piecewisehomogeneous transversely isotropic space
1 Formulation of the Problem Let an absolutely rigid interfacial inclusion occupying a circular region X ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ f x2 þ y2 ag; in the plane z ¼ 0 of connection of two different transversally isotropic halfspaces. An arbitrary load is applied to the inclusion, the action of which leads to the resultant force P ¼ ðP1 ; P2 ; P3 Þ and the main moment M ¼ ðM1 ; M2 ; M3 Þ. The positions of the inclusion faces will be described by the functions 0 0 f 6 ¼ f6 þ #0 ðx; yÞ; fk ¼ fk ; k ¼ 4; 5; ðx; yÞ 2 X
f04 ¼ d1 u3 x3 ; f05 ¼ d2 þ u3 x1 ; f06 ¼ d3 þ u2 x2 þ u1 x2 ; 8 fn k gk¼1 ¼ fr3 ðx; y; 0Þ; r4 ðx; y; 0Þ; r5 ðx; y; 0Þ; u1 ðx; y; 0Þ;
u2 ðx1 ; x2 ; 0Þ; u3 ðx1 ; x2 ; 0Þg; r¼
frk g6k¼1
¼ frx ; ry ; rz ; syz ; sxz ; sxy g;
u ¼ fuk g3k¼1 ¼ fu; v; wg;
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 204–209, 2020. https://doi.org/10.1007/9783030478834_38
ð1Þ
The Influence of Mixed Conditions on the Stress Concentration in the Neighborhood
205
# 0 ðx; yÞ functions, that describe the inclusion form, respectively, when z ¼ 0; dk ; uk ; k ¼ 1; 2; 3 translational displacements and turning angles of the inclusion around the corresponding axes. The mixed conditions for the interaction of the inclusion with the medium (task A) is considered: the upper face is linked to the upper halfspace z ¼ þ 0, the lower side is in smooth contact with another halfspace z ¼ 0. The following functions will be known in the area: 0 þ v 6 ðx; yÞ ¼ # ðx; yÞ þ ð1 1Þf6 ; # ¼ #0 #0 ; n4þ ðx; yÞ ¼ f04 ; n5þ ðx; yÞ ¼ f05 ; n 2 ðx; yÞ ¼ n3 ðx; yÞ ¼ 0; ðx; yÞ 2 X
ð2Þ
þ v k ¼ hfk ðx; yÞi ¼ fk ðx; yÞ fk ðx; yÞ; k ¼ 1; 8; ðx; yÞ 2 X
The case of a delaminated inclusion is also considered (task B): one inclusion face is linked to the upper halfspace z ¼ þ 0, and there is no inclusion contact with the lower halfspace z ¼ 0. The following functions will be known in this area: n6þ ðx; yÞ ¼ #0þ ðx; yÞ þ f06 ; n4þ ðx; yÞ ¼ f04 ; n5þ ðx; yÞ ¼ f05 n j ðx; yÞ ¼ f4j ðx; yÞ; j ¼ 1; 2; 3; ðx; yÞ 2 X;
ð3Þ
were fj ðx; yÞ load applied to the lower halfspace z ¼ 0. Using the approach described in [1–8], both problems are reduced to systems of twodimensional singular integral equations. For task A, relatively unknown þ þ þ þ h1 ; s ¼ h3 þ ih2 ; u ¼ h4 þ ih5 ; fhk ðx; yÞg6k¼1 ¼ fv 1 ; n2 ; n3 ; n4 ; n5 g
ð4Þ
this system has the form þ þ 2 ¼ g1 ; ðq22 2Þs þ 2q21 DK½h1 þ q DDK½u þ q s þ q23 22 DK0 ½ 23 D K½u þ þ 2 ½h1 þ q22 DK 0 ½s þ q23 DDK K ½ ½ u þ q23 D ðq22 2Þs þ 2q21 DK u ¼ g1 ; þ þ 0 ½h1 þ q K½s þ q DK½#s q DK0 ½ ðq33 þ 2Þu 2q31 K u ¼ g2 ; 32 32 33 þ þ ðq33 þ 2Þu 2q31 K0 ½h1 þ q32 K½s þ q32 DK½xs q33 DK0 ½ u ¼ g2 ;
were ZZ ZZ h i h i vj ðt; sÞ vj ðt; sÞ 1 1 dtds: K v dtds; K v ¼ ¼ 0 j j 2p 2p r0 # X
r0 ¼
X
qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ðx tÞ2 þ ðy sÞ2 ; # ¼ ðx tÞ þ iðy sÞ:
ð5Þ
206
O. Kryvyi and Y. Morozov
For the task B, relatively unknown functions h1 ; s ¼ h3 þ ih2 ; u ¼ h4 þ ih5 ; h6 ; fhk ðx; yÞgk¼1;6 ¼ fv k ðx; yÞgk¼1;6
ð6Þ
the task is reduced to a system of six twodimensional SIE: q13 uÞ q12 ðD K½s þ D K½sÞ q D D K½h6 ¼ h ; ðD uþD 14 1 2 2 þ þ q22 q q q K½u 23 D2 K½ 1Þs q24 D h6 þ q21 D K½h1 þ 22 D K0 ½s 23 D D ð u ¼ s ; 2 2 2 2 þ þ q q 2 0 ½s q23 D D K½ K½h1 þ q22 DK u 23 D K½u ¼ s ; ð 22 1Þs q24 D h6 þ q21 D 2 2 2 2 þ þ q 0 ½h1 þ q32 K½s þ q32 D K½#s þ q33 D K0 ½ ð 33 1Þu q31 K u þ q34 D K½h6 ¼ u ; 2 2 2 2 þ þ q 0 ½h1 þ q32 K½s þ q32 D K½#s þ q33 D K0 ½ ð 33 1Þu q31 K u þ q34 D K½h6 ¼ u ; 2 2 2 2 ðq11 1Þh1 þ
ð7Þ For determine of unknown functions dx ; dy ; d7 ; ux ; uy ; uz are use force and moment equilibrium equations ZZ
ZZ vk dxdy ¼ P4k ; k ¼ 1; 2; 3;
X
X
x y
!
M2
v1 dxdy ¼
M1
! ZZ ðxv2 yv3 Þdxdy ¼ M3 : ; X
ð8Þ
2 The Solution of the SIE Following the works [1–11], after the transition to polar coordinates ðq; u; zÞ, the solution of problems is constructed in the form v j ðq; uÞ
¼
1 X n¼1
inu Vj; ; Vj; n ðqÞe n ðqÞ
1 ¼ 2p
Zp
inu v du; j ¼ 1; 3; 5; j ðq; uÞe
p
v1 ðr; uÞ ¼ h1 ðq cos u; q sin uÞ; v2 ðr; uÞ ¼ eiu sðq cos u; q sin uÞ;
ð9Þ
v3 ðr; uÞ ¼ eiu uðq cos u; q sin uÞ; v4 ðr; uÞ ¼ h6 ðq cos u; q sin uÞ: Regarding functions Vj; n ðqÞ, we obtain systems of integral equations with WeberSonin kernels, The solution of which [1–11] made it possible to obtain explicit asymptotic representations for stresses, for the task A:
The Influence of Mixed Conditions on the Stress Concentration in the Neighborhood
rz jz¼0 ’ k11 ðq aÞ2a0 þ k12 ðq aÞ2 þ k13 ðq aÞ2 þ a0 ; q ! a þ 0; 1 1 1 sz q z¼0 ’ k21 ðq aÞa0 2 þ k22 ðq aÞ2 þ k23 ðq aÞa0 2 þ ; 1 1 ~ 1 szu z¼0 ’ k31 ðq aÞ~a0 2 þ k32 ðq aÞ2 þ k33 ðq aÞa0 2 : 1
1
207
1
ð10Þ
For the task B: rz sz q
!
( ’
1 ﬃ pﬃﬃﬃﬃﬃﬃ qa
z¼0
P
" ðq aÞ
a0
n
k11
! cosðb0 ln qa 2a Þ þ
k21
k12 k22
#
! sinðb0 ln qa 2a Þ
þ
o
~ a0 1 ﬃ þ k33 ðq aÞ~a0 þ k32 : szu z¼0 ’ pﬃﬃﬃﬃﬃﬃ qa k31 ðq aÞ
k10 k20
!)
ð11Þ The expressions for translational displacements for task A have the form P3 M3 P1 þ iP2 M2 þ iM1 ; uz ¼ sz 3 ; dx þ idy ¼ cx þ cy ; a a a a2 P1 þ iP2 M2 þ iM1 þ sy uy þ iux ¼ sx 2 a a3 dz ¼ c z
ð12Þ
For task B expressions take place.
dx
dy ux uy
!
cxy ¼ a
P1
þ c0xy a
P2 sm sxy M1 xy 2 ¼ a M2 a
P01 P02 P2 P1
! !
cm xy þ 2 a
s0xy
M2
!
M1 ! P01 P02
; dz ¼ c z
P3 c0z aP03 ; a
M3 ; uz ¼ sz 3 : a
ð13Þ
Tables 1 (task A) and 2 (task B) are given the values of bielastic constants a0 and ~a0 for some combinations of materials and opposite combinations: Ceramics A (BaTiO3) (material m1), Ceramics B (BaTiO3+5%CaTiO3) (material m2), Yttrium (material m3), Magnesium (material m4), Beryl (material m5), Cobalt (material m6). From tables it is visible that the replacement of halfspaces signiﬁcantly affects the behavior of stresses in the neighborhood of the inclusion. This effect is especially noticeable if the elastic characteristics of halfspaces are signiﬁcantly different and less noticeable in the opposite case. So, the asymptotic representations for the stresses in the neighborhood of the inclusion have three terms and depend on the bielastic constants a0 and ~ a0 satisfying the conditions 0\a0 \1=2; 0\~a0 \1=2: For a homogeneous space a0 ¼ ~ a0 ¼ 1=4; b ¼ 0: The presence of delamination, which leads to the appearance of oscillations at the neighborhood of the inclusion, q ! a, has a signiﬁcant effect on the concentration of stresses.
208
O. Kryvyi and Y. Morozov Table 1. The values a0 and ~a0 for the combination of some transversely isotropic materials (task A) Кoмбинaция мaтepиaлoв m1 – m2 m3 – m2 m3 – m4 m6 – m2 m6 – m3 m6 – m5 m5 – m2 m5 – m4
a0
~a0
0,25650 0.30914 0.21835 0.20062 0.16679 0,24159 0,20640 0,15173
0,25644 0.30957 0.22259 0.21931 0.18731 0,25374 0,21652 0,17411
Кoмбинaция мaтepиaлoв m2 – m1 m2 – m3 m4 – m3 m2 – m6 m3 – m6 m5 – m6 m2 – m5 m4 – m5
a0
~ a0
0,24367 0,20403 0,28283 0,30662 0,36701 0,25874 0,29729 0,38770
0,24383 0,20655 0,28311 0,28795 0,35202 0,24635 0,29236 0,39060
Table 2. The values a0 and ~a0 for the combination of some transversely isotropic materials (task B) ~ Кoмбинaция мaтepиaлoв a0 Кoмбинaция мaтepиaлoв a0 a~0 a0 m1 – m2 0,2553 0,2626 m2 – m1 0,2446 0,2374 m3 – m2 0,2994 0,3481 m2 – m3 0,2006 0,0434 m3 – m4 0,2250 0,1905 m4 – m3 0,2745 0,3095 m6 – m2 0,2000 0,1829 m2 – m6 0,2990 0,3171 m6 – m3 0,1523 0,1028 m3 – m6 0,3437 0,3972 m6 – m5 0,2367 0,2574 m5 – m6 0,2634 0,2426 m5 – m2 0,2134 0,1762 m2 – m5 0,2857 0,3238 m5 – m4 0,1394 0,0683 m4 – m5 0,3532 0,4317
References 1. Eﬁmov, V.V., Krivoi, A.F., Popov, G.Y.: Problems on the stress concentration near a circular imperfection in a composite elastic medium. Mech. Solids 33(2), 35–49 (1998). Springer ISSN: 00256544 2. Kryvyy, O.: The discontinuous solution for the piecehomogeneous transversal isotropic medium. Oper. Theory Adv. Appl. 191, 387–398 (2009). https://doi.org/10.1007/9783764399214_25 3. Kryvyy, O.F.: Singular integral relations and equations for a piecewise homogeneous transversally isotropic space with interphase defects. J. Math. Sci. 176(4), 515–531 (2011). https://doi.org/10.1007/s1095801104192 4. Kryvyi, O.F.: Interface crack in the inhomogeneous transversely isotropic space. Mater. Sci. 47(6), 726–736 (2012). https://doi.org/10.1007/s1100301294509 5. Kryvy, O.F.: Interface circular inclusion under mixed conditions of interaction with a piecewise homogeneous transversally isotropic space. J. Math. Sci. 184(1), 101–119 (2012). https://doi.org/10.1007/s1095801208566
The Influence of Mixed Conditions on the Stress Concentration in the Neighborhood
209
6. Kryvyi, O.F.: Delaminated interface inclusion in a piecewise homogeneous transversely isotropic space. Mater. Sci. 50(2), 245–253 (2014). https://doi.org/10.1007/s1100301497147 7. Kryvyi, O.F.: Mutual influence of an interface tunnel crack and an interface tunnel inclusion in a piecewise homogeneous anisotropic space. J. Math. Sci. 208(4), 406–416 (2015). https:// doi.org/10.1007/s1095801524559 8. Kryvyi, O.F.: The solution method nonaxisymmetric problems of stress concentration for an inhomogeneous transversal isotropic space with interfacial cracks and inclusions. In: ICF201714th International Conference on Fracture, Conference Paper, pp. 560–561 (2017) 9. Kryvyi, O., Morozov, Yu.: Interphase circular inclusion in a piecewisehomogeneous transversely isotropic space under the action of a heat flux. In: Gdoutos, E. (eds.) Proceedings of the First International Conference on Theoretical, Applied and Experimental Mechanics. ICTAEM 2018. Structural Integrity, vol. 5. Springer, Cham (2019). https://doi. org/10.1007/9783319919898_94 10. Kryvyi, O., Morozov, Yu.: Solution of the problem of heat conduction for the transversely isotropic piecewisehomogeneous space with two circular inclusions. J. Math. Sci. 243(1), 162–182 (2019). https://doi.org/10.1007/s10958019045331 11. Kryvyi, O., Morozov, Yu.: Heatactive circular interphase inclusion in the conditions of smooth contact with halfspaces. In: Gdoutos E. (eds) Proceedings of the Second International Conference on Theoretical, Applied and Experimental Mechanics. ICTAEM 2019. Structural Integrity, vol 8. Springer, Cham (2019). https://doi.org/10.1007/9783030218942_36
On an Approach to the Thermoelastic Analysis of Nonhomogeneous Solids Roman Kushnir(&)
and Yuriy Tokovyy
Pidstryhach Institute for Applied Problems of Mechanics and Mathematics, National Academy of Sciences of Ukraine, Lviv 79060, Ukraine [email protected]
Abstract. A general approach to the analysis of thermoelastic response of solids exhibiting spatial or thermal variation in their material properties is addressed in this study. The approach is based on the idea of the direct integration method, which allows for the construction of analytical solutions to the relevant thermoelasticity problems in explicit functional form satisfying the thermal and force boundary conditions on the entire surface of a solid. Keywords: Nonhomogeneous solids
Thermoelasticity Explicit solutions
1 Introduction Construction and improvement of structural elements of nowadays technique along with the development and implementation of new materials with advanced properties necessitate the fundamental analysis of heat and masstransfer along with the stressstrain state in multiphase materials under the simultaneous action of different physical ﬁelds with account for wide ranges of the operating and constructional features (e.g., the material anisotropy and non homogeneity, the distributions of ﬁbers and capillaries, thermo sensitivity of the phase components, stratiﬁcation, etc.), as well as the interaction of the structural elements of different geometry. The exhaustive analysis of the impact caused by mentioned factors on the thermal and mechanical behavior of the structure members allows for controlling the technological processes for composite materials in order to achieve the required operational performance of the objective work pieces. This is vital, in particular, for the development of technologies involved into the fabrication of functionallygraded materials (FGM), whose phaseproperty proﬁles can be controlled on the design stage so that the composed materials can have predicted thermal conductivity, deformability and durability under extreme operation conditions. This feature makes FGM to be a perfect choice for various implementations when designing elements of electronic and space techniques, hypersonic aviation, protective systems of nuclear and chemical energetic, technical and engineering hardware of widerange application. The foresaid makes it clear that the problem on the establishment of bythetargetvalues optimal criteria for the implementation of FGM in view of achieving required regimes of the operational performance of the nowadays machinery, devices, and structures becomes extremely important.
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 210–215, 2020. https://doi.org/10.1007/9783030478834_39
On an Approach to the Thermoelastic Analysis of Nonhomogeneous Solids
211
This paper briefly introduces a general approach developed for the thermoelastic analysis of nonhomogeneous and thermosensitive (FGM) solids with arbitrary dependence of the material properties on the spatial coordinates or nonuniform distribution of the transient temperature. The approach is based on implementation of the direct integration method developed for the solution of governing equations of the relevant thermoelasticity problems [1], which is adopted for the case of nonhomogeneous solids with concern to the establishing the fundamental relationships between the stresstensor, straintensor, and displacementvector components, as well as the integral equilibrium and compatibility conditions. In the ﬁnal count, this method implies the reduction of the original problems to solution of secondkind integral equations with corresponding boundary and integral conditions [2].
2 Analysis of Thermal Stresses in Nonhomogeneous Solids 2.1
The Idea of the Method
The algorithm of the direct integration method, whose idea was originated from the solution of speciﬁc optimization problems [3], implies the following principal stages [1]: • Select one or several of the stresstensor components (or their combinations, e.g., the total stress, the difference of normal stresses, etc.) to be the key functions; • Basing on integration of the equilibrium equations, derive the relations expressing the stresstensor components through the key functions; • By making use of these relations and the original boundary conditions, derive local boundary conditions and integral equilibrium conditions for the key functions; • By making use of the compatibility equations in terms of stresses along with the relations obtained in the second stage, derive the governing equations for the key functions; • Using the derived integral and boundary conditions for the key stresses, calculate the key stresses from the governing equations; • Finally, calculate all the stresses from the relations obtained in the second stage. In order to illustrate the ability of this method, consider its application to solving one, two, and threedimensional problems of thermoelasticity for a radiallynon homogeneous cylinder. Consider a long cylinder C related to the dimensionless cylindricalpolar coordinate system ðr; h; zÞ with inner and outer radii ri and ro ¼ 1, respectively. If ri ¼ 0, then the cylinder can be regarded as a solid one. Let the material properties of the cylinder be arbitrary functions of the radial coordinate r. The inner and outer surfaces of the cylinder are exposed to steadystate thermal and force loadings. 2.2
A OneDimensional Problem
First, assume the applied loadings to be uniform with respect to the angular and axial coordinates h and z. In this case, the elastic equilibrium of the cylinder is governed by the following equations
212
R. Kushnir and Y. Tokovyy
d 2 ðr rrr Þ ¼ rr; dr
r
dehh ¼ err ehh dr
ð1Þ
where the total stress r is given by the formula r ¼ rrr þ rhh
ð2Þ
and the normal stresstensor, rrr ; rhh , and straintensor, err ; ehh , components are related through the following constitutive equations Eerr ¼ ð1 m2 Þrrr mð1 þ mÞrhh þ að1 þ mÞET;
ð3Þ
Eehh ¼ ð1 m2 Þrhh mð1 þ mÞrrr þ að1 þ mÞET:
Here, E ¼ EðrÞ is the Young modulus, m ¼ mðrÞ is the Poisson ratio, a ¼ aðrÞ is the linear thermal expansion coefﬁcient, and T ¼ TðrÞ is the temperature ﬁeld in the cylinder C due to the applied thermal loadings on the inner and outer lateral surfaces. The Eqs. (1)–(3) are to be solved under the following boundary conditions rrr ðri Þ ¼ pi ;
rrr ð1Þ ¼ p1
ð4Þ
for the radial stresses. In order to solve the boundary value problem (1)–(4), we select the total stress r to be the key function and, by making use of Eqs. (1)1 and (2) in view of the boundary conditions (4), express the normal stresses as r 2 1 Z r i þ 2 grðgÞdg; rrr ðrÞ ¼ pi r r ri
r 2 1 Z r i rhh ðrÞ ¼ rðrÞ þ pi 2 grðgÞdg: r r ri
ð5Þ The ﬁrst formula of (5) along with the second condition (4) yield Z1 rrðrÞdr ¼ pi ri2 p1 :
ð6Þ
ri
Putting Eqs. (2) and (3) into Eq. (1)2 yields the compatibility equation d 1 mðrÞ d 1 ðrðrÞ þ 2aðrÞEðrÞTðrÞÞ ¼ rrr ; dr GðrÞ dr GðqÞ where 2GðrÞ ¼ EðrÞ=ð1 þ mðrÞÞ. In view of formula (5)1, Eq. (7) can be given as
ð7Þ
On an Approach to the Thermoelastic Analysis of Nonhomogeneous Solids
213
Zr rðrÞ ¼ f ðrÞ þ
rðnÞKðr; nÞdn;
ð8Þ
ri
where GðrÞ pi ri2 1mðrÞ f ðrÞ ¼ 2AGðrÞaðrÞEðrÞTðrÞ 1mðrÞ n GðrÞ Kðr; nÞ ¼ 1mðrÞ
Rr n
1 d g2 dg
Rr ri
1 d g2 dg
1 GðgÞ
1 GðgÞ
dg;
dg;
and A is a constant of integration, which can be determined from condition (6). Equation (8) can be solved by making use of an appropriate analytical, semianalytical or numerical method [4] in order to determine the total stress r. After the key function is found, the remaining stresstensor components can be computed by means of the formulae (5). 2.3
A TwoDimensional Problem
Assume the external loadings of the cylinder C to be irrespective of the axial coordinate z. In this case, we arrive at the state of plane strain, which implies the elastic equilibrium to be governed by the following set of equations @rrh @rhh 1 @ 2 1 @ 2 r @r ðr rrr Þ þ @h ¼ r; r @r ðr rrh Þ þ @h 2 2 @ ðrer h Þ @ err @er @ 2 @ehh @r@h ¼ @h2 þ @r r @r r @r
¼ 0;
ð9Þ
under the constitutive equations Eerr ¼ rrr mðrhh þ rzz Þ þ a ET; Eehh ¼ rhh mðrrr þ rzz Þ þ a ET; Eezz ¼ rzz mðrhh þ rrr Þ þ a ET; Gerh ¼ rrh :
ð10Þ
Here, the total stress is given by formula (2). The boundary conditions are imposed in the form rrr ðri ; hÞ ¼ pi ;
rrr ð1; hÞ ¼ p1 ;
rrh ðri ; hÞ ¼ qi ;
rrh ð1; hÞ ¼ q1 :
ð11Þ
In order to solve the problem (9)–(11), we represent Eqs. (9)1 and (9)2, in view of formula (2), in the form D rrr ¼
@ðr 2 rÞ @2r þr 2 ; @r @h
and Eq. (9)3 as
D rhh ¼ r
@ 2 ðr 2 rÞ @ 2 ðrrÞ ; ; D rrh ¼ r 2 @r @r@h
ð12Þ
214
R. Kushnir and Y. Tokovyy
1 mðrÞ d2 1 rhh d 1 D r þ 2aðrÞð1 þ mðrÞÞT ¼ rrr 2 þ ; GðrÞ dr GðrÞ r dr GðrÞ
ð13Þ
@ 2 @ 1 @2 @ @2 1 @ where D ¼ @r r @r r þ r @h . 2 and D ¼ r @r r @r þ r 2 @h2 By determining the normal stresses from Eqs. (12)1,2 and putting the results into Eq. (13), we can arrive at an integral equation similar to Eq. (8), which can be solved in the same manner [1]. 2.4
An Axisymmetric Problem
Assume the external loadings to be irrespective of the angular coordinate h that refers to the case of axial symmetry. The problem is governed by the equilibrium and compatibility equations @ðrrrr Þ @rzz @ rz þ r @r @r ðrrrz Þ þ r @z ¼ 0; @z ¼ rhh ; @r 2 @erz @ezz r@ehh r@ ehh @r ¼ err ehh ; @z2 @z þ @r ¼ 0
ð14Þ
under the constitutive ones given by Eq. (10). For the simplicity sake impose ri ¼ 0 and the thermal loading to be absent. The force loadings are represented by the conditions rrr ð1; zÞ ¼ pðzÞ;
rrz ð1; zÞ ¼ qðzÞ:
ð15Þ
The total stress in this case is to given by the formula r ¼ rrr þ rhh þ rzz :
ð16Þ
Making use of Eqs. (10) and (16) allows for representing Eqs. (14)3,4 in terms of stresses as
@ r @z 2 2
@ r @r
rhh mðrÞðrrr þ rzz Þ EðrÞ
rhh mðrÞðrrr þ rzz Þ EðrÞ
1 @rrz GðrÞ @z
þ
þ
rhh rrrr 2GðrÞ @ @r
¼ 0;
rzz mðrÞðrrr þ rhh Þ EðrÞ
¼ 0:
ð17Þ
Having applied the integral Fourier transform with respect to coordinate z to Eqs. (14)–(17), expressing the shearing stress from Eqs. (14)1,2 and putting them into Eqs. (17)1,2, the latter ones can be given, after some algebra, as rz ðrÞ ¼ AI1 ðsrÞ þ r
Rr
ðK11 ðr; nÞ rrz ðnÞ þ K12 ðr; nÞ rðnÞÞdn;
0 0 ðsrÞ ðrÞ ¼ B EðrÞI r 1mðrÞ þ
Rr
ðK21 ðr; nÞ rrz ðnÞ þ K22 ðr; nÞ rðnÞÞdn;
ð18Þ
0
where the overline denotes a function in the Fourier mapping domain, A and B are constants of integration, which can be determined from the conditions (15), and
On an Approach to the Thermoelastic Analysis of Nonhomogeneous Solids
215
Rr d d 1 d 1 þ s2 n2 v11 ðr;gÞ dg; K11 ðr; nÞ ¼ dn nv11 ðr; nÞ dn ln GðnÞ dg ln GðgÞ g n
K12 ðr; nÞ ¼
2is d EðnÞ dn ðn GðnÞv11 ðr; nÞÞ þ isn
Rr v11 ðr;gÞ g
d dg
1 ln GðgÞ dg;
n n EðrÞ R q v01 ðr;gÞ d 1 K22 ðr; nÞ ¼ s1mðrÞ n g dg 2GðgÞ dg; iEðrÞ d 1 ðsnv00 ðr; nÞ v01 ðr; nÞÞ dn K21 ðr; nÞ ¼ 1mðrÞ 2GðnÞ ! r R 2 2 nþm d 1 s 2n v01 ðr;gÞ Kn ðsrÞIm ðsnÞ: dg GðgÞ dg ; vnm ðr; nÞ ¼ In ðsrÞKm ðsnÞ ð1Þ g n
ðrÞ from Eq. (18), the remaining stresses rz and r Having found the key stresses r can be restored by making use of the relations derived from Eqs. (14)1,2 [5]. Acknowledgement. This research was supported by the budget program of Ukraine “Support for the Development of Priority Research Areas” (CPCEC 6451230)
References 1. Tokovyy, Y.V.: Direct integration method. In: Hetnarski, R.B. (ed.) Encyclopedia of Thermal Stresses, vol. 2, pp. 951–960. Springer, Dordrecht (2014) 2. Tokovyy, Y.V., Kalynyak, B.M., Ma, C.C.: Nonhomogeneous solids: integral equations approach. In: Hetnarski, R.B. (ed.) Encyclopedia of Thermal Stresses, vol. 7, pp. 3350–3356. Springer, Dordrecht (2014) 3. Kushnir, R.M., Yasinskyy, A.V.: Identiﬁcation of the temperature ﬁeld and stresses in a thermosensitive cylinder according to the surface strains. Mater. Sci. 43(6), 814–822 (2007) 4. Tokovyy, Y.V., Chyzh, A.I., Ma, C.C.: An analytical solution to the axisymmetric thermoelasticity problem for a cylinder with arbitrarily varying thermomechanical properties. Acta Mech. 230(4), 1469–1485 (2019) 5. Tokovyy, Y.V., Ma, C.C.: Axisymmetric stresses in an elastic radially inhomogeneous cylinder under lengthvarying loadings. J. Appl. Mech. 83, 1110071–7 (2016)
The Stress State Near the Corner Point of the Interface of Piecewise Homogeneous Plane in the Presence of Interfacial Shear Cracks V. M. Nazarenko and A. L. Kipnis(&) S.P. Timoshenko Institute of Mechanics of the National Academy of Science of Ukraine, Kiev, Ukraine [email protected]
Abstract. In the framework of plane deformation, a piecewise homogeneous isotropic elastic body with interfacial shear cracks near the corner point of the interface is considered. The exact solution of the corresponding problem of the theory of elasticity for a wedgeshaped body is constructed by the WienerHopf method. Based on the constructed solution, the behavior of stresses near the corner point is investigated. Keywords: Interface of media Wiener – Hopf method
Corner point Interfacial shear crack
Modern structures made from composite materials often contain elements in which the surface between the layers of the composite is not smooth. Such elements are modeled by a piecewisehomogeneous body with a media interface in the form of the sides of the angle, the corner point of which can be a stress concentrator and can be dangerous from the point of view of the origin of interfacial cracks in it. Therefore, studies of the stress state of piecewise homogeneous bodies weakened by interfacial cracks. born at a corner point of the interface is a topical problem in the mechanics of a deformable solid. Below, using the Wiener – Hopf method, an exact solution of the plane static problem of the theory of elasticity for a piecewisehomogeneous isotropic elastic body with smallscale interfacial shear cracks at the corner point of the interface is constructed. Based on the constructed solution, the stress state of the body at the corner point is investigated.
1 Formulation of the Problem Under the conditions of plane deformation, within the framework of the static symmetric problem, we consider a piecewise homogeneous body with a media interface in the form of sides of the angle, which is composed of isotropic elastic parts with Young’s moduli E1 ; E2 (E1 [ E2 ) and Poisson’s ratios v1 ; v2 (see Fig. 1). © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 216–221, 2020. https://doi.org/10.1007/9783030478834_40
The Stress State Near the Corner Point of the Interface
Fig. 1. Piecehomogeneous isotropic body with the interface of media in the form the sides of angle
217
Fig. 2. Piecehomogeneous isotropic body with smallscale interior interfacial shear cracks
In accordance with the general provisions on the behavior of stresses at the corner points of elastic bodies, the corner point of the interface is a stress concentrator with a powerlaw singularity. In this case, the following representations take place for stresses in the vicinity of the corner point: srh ðr; 0Þ ¼ Cg1 ða; e0 ; v1 ; v2 Þr k0 þ o r k0 ; E1 rh ðr; 0Þ ¼ Cg2 ða; e0 ; v1 ; v2 Þr k0 þ o r k0 ; e0 ¼ E2 ðr ! 0Þ; where g1 ¼ k0 g11 sin k0 a g12 sinðk0 þ 2Þa; g11 ¼ ð1 eÞk20 sin2 2a cosðk0 þ 2Þa ð1 1 2eÞk0 sin 2a cosðk0 þ 2Þa cos k0 ðp aÞ sin½k0 ðp aÞ 2a þ ½2 ð1 2 Þek0 sin 2a cos k0 a cosðk0 þ 2Þa cos k0 ðp aÞ sin½k0 ðp aÞ 2a þ ð1 þ 1 Þk0 sin 2a sinðk0 þ 2Þa cos k0 ðp aÞ cos½k0 ðp aÞ 2a þ ð1 þ 1 Þð1 2 Þ cos k0 a sin2 ðk0 þ 2Þa cos k0 ðp aÞ cos½k0 ðp aÞ 2a ð1 þ 2 Þk0 sin 2a cos k0 a sinðk0 þ 2Þa cosðk0 þ 2Það1 þ 1 Þð1 2 Þ cos k0 a sinðk0 þ 2Þa cosðk0 þ 2Þa cos k0 ðp aÞ sin½k0 ðp aÞ 2a; g12 ¼ ð1 eÞð1 2 þ k0 Þk20 sin2 2a cos k0 a ð1 1 2eÞk0 ð1 2 þ k0 Þ sin 2a cos k0 a cos k0 ðp aÞ sin½k0 ðp aÞ 2a þ ½2 ð1 2 Þek0 ð1 2 þ k0 Þ sin 2a cos2 k0 a sinðk0 þ 2Þa 2½1 1 ð1 2 Þeð1 2 þ k0 Þ cos2 k0 a sinðk0 þ 2Þa cos k0 ðp aÞ sin½k0 ðp aÞ 2a þ ð1 þ 1 Þk20 sin 2a sin k0 a cos k0 ðp aÞ cos½k0 ðp aÞ 2a
þ ð1 þ 1 Þð1 2 Þk0 sin k0 a cos k0 a sinðk0 þ 2Þa cos k0 ðp aÞ cos½k0 ðp aÞ 2a ð1 þ 2 Þk20 sin 2a sin k0 a cos k0 a cosðk0 þ 2Þa þ ð1 1 Þð1 þ 2 Þk0 sin k0 a cos k0 a cosðk0 þ 2Þa cos k0 ðp aÞ sin½k0 ðp aÞ 2a;
218
V. M. Nazarenko and A. L. Kipnis
e ¼
1 þ v2 e0 ; 1;2 ¼ 3 4v1;2 1 þ v1
The degree of stress singularity is the unique root of the characteristic equation in the interval (−1; 0): Dðk 1Þ ¼ 0; DðzÞ ¼ d0 ðzÞ þ d1 ðzÞe þ d2 ðzÞe2 ; d0 ðzÞ ¼ ðsin 2za þ z sin 2aÞ½1 sin 2zðp aÞ þ z sin 2a; d1 ðzÞ ¼ ð1 þ 1 Þð1 þ 2 Þ sin2 zp ðsin 2za þ z sin 2aÞ½1 sin 2zðp aÞ þ z sin 2a ½sin 2zðp aÞ z sin 2að2 sin 2za z sin 2aÞ;
d2 ðzÞ ¼ ½sin 2zðp aÞ z sin 2að2 sin 2za z sin 2aÞ Constant C, which is included in these representations, is determined by the solution of each speciﬁc problem of the theory of elasticity, which is depicted in Fig. 1. The constant C, which depends on the external load, can be regarded as the stress intensity factor at the corner point of the interface. If C \ 0 (it is shown that this condition must be fulﬁlled) and a 2 ða1 ; p=2Þ [ ða2 ; pÞ then, according to the information about the function and the formula given above, rh ðr; 0Þ ! 1 when r ! 0; therefore, at the interface between the media at the corner point, normal stresses are compressive. In this case, due to the high concentration of stresses at the corner point, it is possible to initiate interfacial shear cracks with completely contacting faces extending from this point, the length of which is much less than the sizes of the body (see Fig. 2). The larger the ratio of Young’s moduli e0 ¼ E1 =E2 [ 1, the wider the range of angle a values at which such cracks should be expected to form. Taking into account the smallness of the cracks, we arrive at the plane static symmetric problem of the theory of elasticity for a piecewise homogeneous isotropic plane with a media interface in the form of sides of an angle containing cuts of ﬁnite length starting from the corner point and located on this boundary (see Fig. 3).
Fig. 3. Piecehomogeneous isotropic plane with interior interfacial shear cracks
The Stress State Near the Corner Point of the Interface
219
At inﬁnity, the asymptotic behavior of the stress ﬁeld is given, which is a solution to a similar problem without cuts (problem K), a homogeneous problem of the theory of elasticity for a piecewise homogeneous plane with a media interface in the form of the sides of the angle, which is generated by the unique root k0 of its characteristic equation on the interval ð1; 0Þ. An arbitrary constant C included in the indicated solution is considered given. It characterizes the intensity of the external ﬁeld and should be determined from the solution of the external problem. Taking into account the symmetry, we write the boundary conditions of the problem (Fig. 3) as follows: h ¼ p a; srh ¼ 0; uh ¼ 0; h ¼ 0; hrh i ¼ hsrh i ¼ 0; hur i ¼ 0;
ð1Þ
h ¼ 0; r \ l; srh ¼ 0; h ¼ 0; r [ l; hur i ¼ 0;
ð2Þ
h ¼ 0; r ! 1; srh ¼ Cg1 r k0 þ oð1=r Þ ða h p aÞ:
ð3Þ
The solution of the formulated problem of the theory of elasticity (Fig. 3) is the sum of the solutions of the following two problems. The ﬁrst (problem 1) differs from it in that instead of the ﬁrst of conditions (2) we have h ¼ 0; r \ l; srh ¼ Cg1 r k0 ;
ð4Þ
and at inﬁnity, the stresses fade as oð1=r Þ (in (3) the ﬁrst term is absent). The second problem is problem K. Since the solution to the second problem is known, it is enough to construct a solution to the ﬁrst. To construct an exact solution to problem 1, we will use the Wiener – Hopf method [1] in combination with the Mellin integral transform apparatus [2].
2 Solution of the Wiener – Hopf Equation Applying the Mellin transforms with the complex parameter p to the equilibrium equations, the compatibility conditions for the strains, Hooke’s law, conditions (1) and taking into account the second of conditions (2) and condition (4), we obtain the Wiener – Hopf functional equation U þ ð pÞ þ A¼
s ¼ ActgppGð pÞU ð pÞ p þ k0 þ 1
ð1 þ 1 Þ½1 þ 1 þ ð1 þ 2 Þe G 1 ð pÞ ; Gð pÞ ¼ 2 2½1 þ ð1 þ 1 2 Þe þ 2 e G 2 ð pÞ
G1 ð pÞ ¼ 1 þ ð1 þ 1 2 Þe þ 2 e2 ½a0 ð pÞ þ a1 ð pÞe sin pp;
ð5Þ
220
V. M. Nazarenko and A. L. Kipnis
G2 ð pÞ ¼ ½1 þ 1 þ ð1 þ 2 Þe b0 ð pÞ þ b1 ð pÞe þ b2 ð pÞe2 cos pp; a0 ðpÞ ¼ ð1 þ 1 Þ½cos 2pðp aÞ cos 2aðsin 2pa þ p sin 2aÞ; a1 ðpÞ ¼ ð1 þ 2 Þðcos 2pa cos 2aÞ½sin 2pðp aÞ p sin 2a; b0 ðpÞ ¼ ðsin 2pa þ p sin 2aÞ½1 sin 2pðp aÞ þ p sin 2a; b1 ðpÞ ¼ ð1 þ 1 Þð1 þ 2 Þ sin2 pp ðsin 2pa þ p sin 2aÞ½1 sin 2pðp aÞ þ p sin 2a ½sin 2pðp aÞ p sin 2að2 sin 2pa p sin 2aÞ;
b2 ðpÞ ¼ ½sin 2pðp aÞ p sin 2að2 sin 2pa p sin 2aÞ; s ¼ Cg1 lk0 ; R1 R1 @ur E1 U þ ðpÞ ¼ srh ðql;0Þqp dq; U ðpÞ¼ h @r ij r ¼ ql qp dq 2 4ð1v Þ 1 1 0 h¼0 ðe1 \ Rep \ e2 Þ: The factorization of the equation coefﬁcient on the imagine axis carried out by its splitting into two functions: the function which factorizes using gammafunctions [3] and the function which factorizes according Gakhov’s formula [4]. The solution of Eq. (5) is the follows. U þ ð pÞ ¼
sK þ ð pÞG þ ð pÞ 1 1 ðRep\0Þ; p þ k0 þ 1 K þ ðk0 1ÞG þ ðk0 1Þ K þ ð pÞG1þ ð pÞ
U ð pÞ ¼ 2 1 exp4 2pi
spG ð pÞ ðRep [ 0Þ AK ðk0 1ÞG þ ðk0 1Þðp þ k0 þ 1ÞK ð pÞ
þ i1 Z
i1
þ
3 ln GðzÞ 5 dz ¼ zp
(
G þ ð pÞ; Rep \ 0 G ð pÞ; Re p [ 0
; K ð pÞ ¼
ð6Þ
Cð1 pÞ Cð1=2 pÞ
3 Investigation of the Behavior of Stresses in the Vicinity of a Corner Point Based on the solution (6) of the Wiener – Hopf Eq. (5), expressions for Mellin stress transformants are obtained. As a result of applying Mellin’s inversion formulas to these expressions, the stress in problem 1 is found. The following formula holds: rh ðr; hÞ ¼ r k1 SðhÞC1 þ o r k1 ;
ð7Þ
The Stress State Near the Corner Point of the Interface
C1 ¼
g1 Cðk0 þ 3=2ÞCðk1 þ 2ÞG1þ ðk1 1Þ Clk0 k1 ; ðk1 k0 ÞsCðk0 þ 2ÞCðk1 þ 3=2ÞG1þ ðk0 1Þ
221
ð8Þ
s ¼ ð1 þ 1 Þf½cos 2ðk1 þ 1Þðp aÞ cos 2a½2a cos 2ðk1 þ 1Þa þ sin 2a 2ðp aÞ½sin 2ðk1 þ 1Þa þ ðk1 þ 1Þ sin 2a sin 2ðk1 þ 1Þðp aÞg þ ð1 þ 2 Þf½2ðp aÞ cos 2ðk1 þ 1Þðp aÞ sin 2a½cos 2ðk1 þ 1Þa cos 2a 2a½sin 2ðk1 þ 1Þðp aÞ ðk1 þ 1Þ sin 2a sin 2ðk1 þ 1Þage; where SðhÞ is known function. Formula (7) gives the main term of the expansion of the normal stress rh ðr; hÞ in the asymptotic series for r ! 0 for material 1 (0\h\p a). Similar representations take place for rh ðr; hÞ when a \ h \ 0, as well as for srh ðr; hÞ and rr ðr; hÞ. In expression (7) k1 is the unique root of the following equation in the interval ð1; 0Þ ð1 þ 1 Þ½cos 2ðk þ 1Þðp aÞ cos 2a½sin 2ðk þ 1Þa þ ðk þ 1Þ sin 2a þ ð1 þ 2 Þ½cos 2ðk þ 1Þa cos 2a½sin 2ðk þ 1Þðp aÞ ðk þ 1Þ sin 2ae ¼ 0: ð8Þ It follows from (7) that the corner point O is a special point of the boundaryvalue problem of the elasticity theory under consideration (Fig. 3). It is a stress concentrator. As the point of the region approaches the point O, stress goes to inﬁnity. The degree of singularity of stresses depends on the angle, the ratio of the Young’s modulus, and the Poisson’s coefﬁcients. This degree r is the unique one in the interval ð1; 0Þ of roots of a certain transcendental equation (Eq. (8)). As the angle a increases from zero to p=2 the stress concentration near the corner point decreases, and with increasing it from p=2 up to p – increases. If the angle a tends to zero or to p, the degree of the singularity of stresses tends to 1. If the angle a tends to p=2, then the degree of the singularity of stresses tends to zero. If the angle a is acute, then as the ratio of Young’s modulus e0 ¼ E1 =E2 [ 1 increases, the stress concentration near the angular point decreases, and if the angle obtuse – increases.
References 1. Nobl, B.: Applying the Wiener – Hopf Method for Solving Partial Derivatives Differential Equations. Inostr. Lit., Moscow (1962). (in Russian) 2. Uflyand, Ya.S.: Integral Transformations in Elasticity Theory Problems. Nauka, Leningrad (1967). (in Russian) 3. Lavrentiev, M.A., Shabat, B.V.: The Theory of Complex Variable Methods. Nauka, Moscow (1973). (in Russian) 4. Gakhov, F.D.: Boundaryvalue problems. Nauka, Moscow (1977). (in Russian)
Coupled Nonstationary Longitudinal Vibrations of an Inﬁnite Electromagnetoelastic Rod Thong D. Pham1, Dmitry V. Tarlakovskii1,2(&), and Vladimir A. Vestyak1 1
2
Moscow Aviation Institute, National Research University, Volokolamskoe Shosse. 4, Moscow 125993, Russia [email protected], [email protected] Institute of Mechanics, Lomonosov Moscow State University, Michurinskii Prospekt. 1, Moscow 119192, Russia
Abstract. We study the associated nonstationary longitudinal vibrations of an inﬁnite electromagnetoelastic rod. It is assumed that the material of the rod is a homogeneous isotropic conductor. In this case, the initial electromagnetic ﬁeld, the Lorentz force, Maxwell’s equations and the generalized Ohm’s law are taken into account. Assuming that the desired functions depend only on the longitudinal coordinate, using the corresponding relations for the shells, a closed system of equations of motion is obtained. The desired functions are assumed to be bounded, and the initial conditions to be zero. The Fourier transform in the coordinate and the Laplace transform in time, as well as the small parameter method characterizing the relationship of mechanical and electromagnetic ﬁelds, are used to solve this problem. The solution is presented in integral form with the cores in the form of Green functions for which images and originals are constructed. An example of calculation is given. Keywords: Nonstationary electromagnetoelasticity Inﬁnite rod Longitudinal vibrations Green’s function Laplace and Fourier transforms
1 Problem Statement In a rectangular Cartesian coordinate system Oxyz we consider nonstationary longitudinal movements of a straightline homogeneous isotropic inﬁnite electromagnetoelastic rod with an Ox axis under zero initial conditions and the absence of an initial electric ﬁeld. The equations of the corresponding process are written in the space of Laplace transforms [2] in time (additional superscript «L» indicates image; s  corresponding parameter) as a special case of the general equations for a thin shell constructed in [1]:
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 222–227, 2020. https://doi.org/10.1007/9783030478834_41
Coupled Nonstationary Longitudinal Vibrations
223
@ 2 uL @wL3 acH0 H0 uL þ eL3 þ qL1 ; þ f 2 @x @x 2 L L @ w @u H02 cs @wL3 L L 2 L 2 2 3 þ w3 þ a sw3 þ mL ; r f s w3 ¼ g s þ c @x @x2 @x
ð1Þ
@eL3 @hL2 cs H0 wL3 : ¼ g2e ðs þ cÞeL3 þ csH0 uL ; ¼ shL2 þ sþc @x @x
ð2Þ
s2 u L ¼
where u  longitudinal movement; w3  compression (deformation in the Oz direction); e3 и h2  changes in electric and magnetic ﬁelds on the axis of the rod, respectively, in the directions Oz and Oy; H0  surface charge, the intensity of the initial magnetic ﬁeld, respectively, in the direction; q1 и m  external linear load and moment in the Oxy plane. Assuming that the required functions are limited. Hereinafter, the following dimensionless quantities are used (for the same style, the dimension parameters are indicated by a prime symbol): x0 c1 t u0 q01 L ; u ¼ ; q1 ¼ ; ;s ¼ L ðk þ 2lÞh L L m0 L2 h3 2 I m ¼ ;I ¼ ;r ¼ 2 ; Lh ðk þ 2lÞI 12 c1 k 2 2 k þ 2l 2 l ¼ 1 2 ; c1 ¼ ; c2 ¼ ; g ¼ ;f ¼ k þ 2l g q q c2 e03 h02 le c1 H00 le c1 c1 e3 ¼ ; h2 ¼ ; H0 ¼ ; ge ¼ ; E cE cE ce 2 2 ee E 4prL 2 c a ¼ ;c ¼ ;c ¼ ; ee c1 e 4pðk þ 2lÞ le e x ¼
here t  time; L и E  some characteristic linear dimension and the electric ﬁeld intensity; k; l  Lame elastic constants; h  cross section height; q  material density; r, ee и le  conductivity, dielectric and magnetic permeability coefﬁcients.
2 The Solution in the Image Space To construct a solution to the system of Eq. (1), (2), we additionally apply the Fourier transform [2] along the x coordinate (additional superscript «F» indicates image; q corresponding parameter):
FL FL k12 þ acH02 s uFL þ iqfwFL 3 þ acH0 e3 ¼ q1 ; 2 2 2 FL ¼ g2 ðs þ cÞmL ; k2 þ g2 r 2 ðs þ cÞ þ aH02 g2 csðiq þ sÞ wFL 3 iqfg r ðs þ cÞu FL FL 2 FL g2e csH0 uFL þ g2e ðs þ cÞeFL ¼ 0; csH0 wFL ¼ 0; 3 þ iqðs þ cÞe3 þ se h 3 þ iqh
224
T. D. Pham et al.
Here k1 ¼
pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃ q2 þ s2 ; k2 ¼ q2 þ g2 s2 ; se ¼ sðs þ cÞ; Re [ 0
FL Eliminating functions eFL from this system of equations, we obtain a 3 and h system of linear algebraic equations 2 FL a11 ðq; sÞuFL þ a12 ðq; sÞwFL 3 ¼ ðs þ cÞke q1 ; 2 FL a21 ðq; sÞuFL þ a22 ðq; sÞwFL 3 ¼ g ðs þ cÞm ;
where a11 ðq; sÞ ¼ a11 ðq; sÞ ¼ ðs þ cÞ k12 ke2 þ acsH02 q2 þ g2e s2e cg2e s ; a12 ðq; sÞ ¼ iq fðs þ cÞke2 þ ac2 H02 s ; a21 ðq; sÞ ¼ ir2 fg2 ðs þ cÞq; a22 ðq; sÞ ¼ ðs þ cÞ k22 þ g2 r 2 þ ag2 H02 csðiq þ sÞ: Its solution is written as follows: FL FL FL uFL ¼ GFL uq ðq; sÞq1 þ Gum ðq; sÞm ;
ð3Þ
FL FL FL FL wFL 3 ¼ Gw3 q ðq; sÞq1 þ Gw3 m ðq; sÞm :
where ðs þ cÞke2 a22 ðq; sÞ g2 ðs ; GFL um ðq; sÞ ¼ Dðq; sÞ ðs þ cÞke2 a21 ðq; sÞ g2 ðs ; GFL GFL w3 q ðq; sÞ ¼ w3 m ðq; sÞ ¼ Dðq; sÞ GFL uq ðq; sÞ ¼
þ cÞa12 ðq; sÞ ; Dðq; sÞ þ cÞa11 ðq; sÞ ; Dðq; sÞ
Dðq; sÞ ¼ a11 ðq; sÞa22 ðq; sÞ a12 ðq; sÞa21 ðq; sÞ: FL FL FL Here GFL uq ðq; sÞ, Gum ðq; sÞ, Gw3 q ðq; sÞ and Gw3 m ðq; sÞ  images of influence functions. FL Similarly, we can represent functions eFL 3 and h2 .
3 Originals of the Influence Functions and Solutions The originals of the Laplace transform are quite simple, since the images of the influence functions are rational functions of the parameter s. However, the analytic inversion of the Fourier transform is impossible. An attempt at numerical inversion does not lead to a satisfactory result due to the presence of rapidly oscillating functions. Therefore, a simpliﬁed model is used in which the compression of the rod is FL neglected. For this, it sufﬁces to set wFL 3 ¼ 0 in (3) and exclude m . We obtain the following result
Coupled Nonstationary Longitudinal Vibrations
FL FL uFL ¼ CFL uq ðq; sÞq1 ; Cuq ðq; sÞ ¼
ke2 ; k12 ke2 þ acsH02 q2 þ g2e s2
225
ð4Þ
where CFL uq ðq; sÞ  image of the influence function for a simpliﬁed model. In this case, the abovementioned difﬁculties remain. Therefore, we use the method of a small parameter, for which we take the coupling coefﬁcient of the mechanical and electromagnetic ﬁelds a. Limiting the linear approximation, we obtain FL FL CFL uq ðq; sÞ ¼ Cuq0 ðq; sÞ þ Cuq1 ðq; sÞa;
where CFL uq0 ðq; sÞ
2 2 2 1 FL 2 q þ ge s s ¼ 2 ; Cuq1 ðq; sÞ ¼ cH0 : k1 k14 ke2
Originals are found using transformation properties and tables [2–4]: Cuq ðx; sÞ ¼ Cuq0 ðx; sÞ þ aCuq1 ðx; sÞ; 1 Cuq0 ðx; sÞ ¼ H ðs j xjÞ; Cuq1 ðx; sÞ ¼ cH02 fuq ðx; sÞ þ fuq3 ðx; sÞ ; 2
ð5Þ
where i
1 1 þ g2e h ce ðsjxjÞ 2ðs j xjÞece ðsjxjÞ fuq ðx; sÞ ¼ e 1 H ðs j xjÞ; ce 4 1 g2e c qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ cs g2e c 2 g2 x2 H ðs g j xjÞ; c ¼ e þ ece s ecs=2 I0 s fuq3 ðx; sÞ ¼ : e e e 2 1 g2e 2ge 1 g2e Here Im ð xÞ  modiﬁed Bessel function of the ﬁrst kind of order m[5], H ðsÞ Heaviside function. Note that the function Cuq0 ðx; sÞ corresponds to a purely elastic solution. The original of movement according to (4) is written as follows (asterisks symbol indicate convolutions in time and coordinate): uðx; sÞ ¼ Cuq ðx; sÞ q1 ðx; sÞ
4 Examples for the Calculation As an example, consider an aluminum rod, the material of which is characterized by the following values [6]:
226
T. D. Pham et al.
g ¼ 2; 04; f ¼ 0; 519; ge ¼ 0; 111 104 ; c ¼ 5; 06; a ¼ 0; 0806: It is accepted here E ¼ 100 B=M and L ¼ 1 M. We also assume that H0 ¼ 1 and the rod has a square cross section with the following geometric parameters: h ¼ 0; 05 M; r 2 ¼
h2 ¼ 0; 208 103 12L2
In Fig. 1 and 2 show the dependences of the Cuq1 ðx; sÞ function obtained using (5) on the coordinate and time, respectively, for different values of s and x.
Fig. 1. The dependences of Cuq1 on x
Fig. 2. The dependences of Cuq1 on s
In Fig. 3 and 4 show similar dependences for the influence function Cuq ðx; sÞ.
Fig. 3. The dependences of Cuq on x
Fig. 4. The dependences of Cuq on s
Coupled Nonstationary Longitudinal Vibrations
227
Note that, as follows from (5), for the material under consideration the fuq3 ðx; sÞ function has the order of a small coefﬁcient ge , then for s [ ge j xj the contribution of this term to the Cuq1 function is insigniﬁcant. Taking into account the connectivity of the process gives a difference from the elastic solution of the order of a, which in these calculations corresponds to approximately eight percent.
5 Conclusion An approach to the study of coupled nonstationary longitudinal vibrations of an electromagnetoelastic rod is proposed. A small correction introduced by taking into account the connectivity is explained by the parameters of the material under consideration. Similarly, the problems of longitudinal vibrations of a semiinﬁnite and ﬁnal rod, as well as transverse vibrations, can be solved.
References 1. Vestyak, V.A., Tarlakovskii, D.V.: The model of thin electromagnetoelastic shells dynamics. In: Proceedings of the Second International Conference on Theoretical, Applied and Experimental Mechanics. Structural Integrity, pp. 254–258. Springer, Switzerland AG (2019) 2. Gorshkov, A.G., Medvedskii, A.L., Rabinskii, L.N., Tarlakovskii, D.V.: Waves in Continuous Media. Physmatlit, Moscow (2004) 3. Prudnikov, A.P., Brychkov, Yu.A., Marichev, O.I.: Integrals and Series. Gordon and Breach Science Publishers, New York (1986) 4. Ditkin, V.A., Prudnikov, A.P.: Handbook of operational calculus. “Higher School”, Moscow (1965) 5. Abramowitz, M., Stegun, I.A.: Handbook of Mathematical Functions with Formulas, Graphs and Mathematical Tables. U.S. Department of Commerce, National Bureau of Standards (1964) 6. Vestyak, V.A., Gachkevich, A.R., Musiy, R.S., Tarlakovskii, D.V., Fedotenkov, G.V.: Twodimensional nonstationary waves in electromagnetoelastic bodies. Physmatlit, Moscow (2019)
The Effect of Cracks Interaction in Materials Under Loading Along Cracks Viacheslav Bogdanov(&) and Vladimir Nazarenko S. P. Timoshenko Institute of Mechanics of the National Academy of Sciences of Ukraine, Kyiv 02053, Ukraine [email protected]
Abstract. The nonclassical problems of the fracture of materials loaded along the cracks they contain are analyzed. Two fracture mechanisms are considered, namely, the fracture of materials with initial (residual) stresses acting in parallel to the surfaces of cracks location and the fracture of the bodies compressed along cracks. In the study of such problems, a new combined approach developed in the framework of the threedimensional linearized mechanics of deformable bodies is used. The results of the investigation of two and threedimensional problems for typical conﬁgurations of parallel coaxial Mode I and Mode II cracks are presented. The effect of residual stresses on stress intensity factors is analyzed for highly elastic materials and composites. The compressive strength for bodies with interacting cracks located in parallel planes under compression is calculated using the approach mentioned. The crack length (diameter), mechanical properties of materials and the mutual position of cracks were found to influence the critical fracture parameters. Keywords: Nonclassical problems of fracture mechanics Residual stresses Compression along cracks Parallel coaxial cracks Highly elastic materials Composites
1 Introduction Initial (or residual, technological) stresses are nearly always present in actual structural materials and elements as a result of technological processes of their production, joining, mechanical and thermal surface treatment, exploitation, producing a considerable effect on the fracture processes in bodies with cracks. The nonclassical nature of the problems on fracture of prestressed materials, when initial (residual) stresses are directed in parallel to the surfaces of cracks location, is accounted for by the fact that the solutions of respective problems of linear elasticity theory show that these initial stresses are not involved in the expressions for stress intensity factors, Jintegral and crack opening displacements. As a result, the stress components directed along cracks cannot be taken into consideration in Grifﬁth–Irwin and Cherepanov–Rice classical models and fracture criteria, critical crack opening displacements or their generalizations [1]. At the same time, this is contrary to the data of numerous experimental studies, which reveal the effect of the load component directed along cracks on fracture parameters under both static and cyclic loads. In [2] an approach based on the three© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 228–234, 2020. https://doi.org/10.1007/9783030478834_42
The Effect of Cracks Interaction in Materials Under Loading Along Cracks
229
dimensional linearized mechanics of deformable bodies to solving the problems of the fracture of bodies with residual stresses was proposed and fracture criteria for the abovementioned problems were formulated. The nonclassical nature of fracture mechanics problems on body compression along cracks is related to the fact that under uniform compression strictly along the planes of cracks location in an isotropic and orthotropic material, a uniform stressstrain state emerges, which leads to the absence of singularities at crack tips in corresponding solutions. Hence, it is also impossible to directly apply the classical criteria of fracture, since in linear fracture mechanics both the stress intensity factors and crack opening displacements are equal to zero in this situation. In the problem at issue the most likely mechanism of the onset (start) of the fracture process, by analogy with the problem on the compression of structural elements along the symmetry axes, is the local loss of equilibrium stability of the material that surrounds cracks. In [3] it was proposed to determine the critical compressive loads that correspond to local buckling of the material near cracks by solving eigenvalue problems in the framework of the threedimensional linearized theory of the stability of deformable bodies. As follows from the above, the common point in investigating these two fracture mechanics problems on loading along cracks is the employment of related mathematical apparatuses within the threedimensional linearized mechanics of deformable bodies. For both classes of problems the linearized equilibrium equations and constitutive stressstrain relations are identical, as are, within corresponding design diagrams, the considered conﬁgurations of bodies and defect location patterns. But a signiﬁcant difference in the formulation and solution of problems on the fracture of the bodies compressed along the arrays of cracks located in parallel planes and problems on the fracture of materials with residual stresses acting along cracks, is that in the former case we end up investigating eigenvalue problems with zero boundary conditions on crack faces, while in the latter we examine boundary problems with nonzero boundary conditions on crack faces. Taking into account those considerations, a combined approach to the investigation of the problems on the fracture mechanics of cracked materials compressed along cracks and the problems on the fracture of bodies with residual stresses was proposed in [4, 5]. In this approach, critical loading parameters in the problems on the bodies compressed along the cracks they contain can be determined via the solution of corresponding nonhomogenous problems of the fracture mechanics of materials with residual stresses, as the values of compressive residual loads which, when achieved, lead to a dramatic “resonancelike” change in stresses and displacements near crack contours. This situation can be interpreted relying on the following physical considerations. Consider a body with initial stresses acting along a single inner crack. When the initial compressive stresses achieve the values that correspond to the surface instability of the halfspace, a neutral equilibrium state emerges in the vicinity of the crack tip. In this situation, a minor increase in the external load is sufﬁcient to break the neutral equilibrium and launch the fracture process characterized with a local loss of material’s stability in the vicinity of the crack. Below we demonstrate the employment of this combined approach by investigating 2D and 3D problems on the fracture of bodies containing interacting cracks (two parallel coaxial cracks or a periodic array of coaxial parallel cracks). In the investigation of composite materials it is assumed that crack sizes are signiﬁcantly larger than
230
V. Bogdanov and V. Nazarenko
those of the structural elements of composites (i.e. macrocracks are considered); besides, we only analyze fracture processes in which the composite does not demonstrate properties of the piecewiseuniform medium (like fracture on the media interface etc.). Under such assumptions, we use the continuum composite model with the abovementioned characteristics of an orthotropic body (in the case of 2D problems) or a transversely isotropic body (in the case of 3D problems).
2 Problems Formulations Let us consider 3D problems (the procedure of solving 2D problems is similar). We use the Cartesian coordinates yj ; j ¼ 1; 3 of the initial state induced by the initial stresses S0ij that are the components of a symmetric stress tensor per unit area of the nondeformed conﬁguration. Let the initial stresses (or compressive forces) act strictly in the crack planes y3 ¼ const resulting in the following homogeneous initial stressstrain state: S033 ¼ 0; S011 ¼ S022 ¼ const 6¼ 0; u0j ¼ k1 kj 1 yj ; k1 ¼ k2 6¼ k3 ; j ¼ 1; 3; j
ð1Þ
where uoj are the components of the displacement vector in the initial conﬁguration and kj ¼ const are coefﬁcients of elongations (or contractions) along the coordinate axes caused by the initial tensile (or compressive) stresses S0ij . We also denote by Q0ij the components of the asymmetric stress tensor per unit area in the initial conﬁguration, and by uj – the associated components of the displacement vector. General solutions of the linearized equilibrium equations expressed in terms of harmonic potential functions have the following form in circular cylindrical coordinates ðr; h; y3 Þ derived from the Cartesian coordinates [6]: @ ðu 1 þ u 2 Þ m1 @u m2 @u ; u3 ¼ pﬃﬃﬃﬃﬃ 1 þ pﬃﬃﬃﬃﬃ 2 ; @r n1 @z1 n2 @z2 2 2 d1 @ u 1 d2 @ u 2 @ 2 u1 @ 2 u2 0 0 þ pﬃﬃﬃﬃﬃ þ d2 l2 Q3r ¼ C44 pﬃﬃﬃﬃﬃ ; Q33 ¼ C44 d1 l1 ; n1 @r@z1 n2 @r@z2 @z21 @z22 ur ¼
ð2Þ
where values C44 , ni , mi , di and li depend on material’s properties and residual stresses. Below we formulate boundary conditions on the faces of cracks and on the body boundary for different types of problems. E.g., in the case of an unbounded body containing a periodic array of parallel coaxial Mode I pennyshaped cracks of the same radii a located in parallel planes, y3 ¼ const: fr\a; 0 h\2p; y3 ¼ 2hn; n ¼ 0; 1; 2; . . .g the boundary conditions take the forms u3 ¼ 0 ðy3 ¼ 0; r [ aÞ; Q033 ¼ rðrÞ ðy3 ¼ 0; r\aÞ; Q03r ¼ 0; ðy3 ¼ 0; 0 r\1Þ; u3 ¼ 0; Q03r ¼ 0; ðy3 ¼ h; 0 r\1Þ:
ð3Þ
The Effect of Cracks Interaction in Materials Under Loading Along Cracks
231
(Note that additional loads on the crack faces must be zero in problems on the fracture of cracked materials compressed along cracks).
3 Fredholm Integral Equations. Stress Intensity Factors By applying Bessel integral transformation (Fourier transformation for plane problems) to the harmonic potential functions in (2), we reduce the above problems ﬁrst to the systems of dual integral equations and then to Fredholm integral equations of the second kind, which can be effectively analyzed numerically. E.g., by solving the problem for the body containing a periodic array of parallel coaxial Mode I cracks we obtain the resolving system of Fredholm integral equation in dimensionless form Z1
Zp=2 2 k1 f ðgÞKðn; gÞdg ¼ n rðn sin hÞ sin hdh; 0 n; g 1; p kC44 d1 l1 0 0 1 k1 iz k2 iz Rew 1 þ K ðn; gÞ ¼ Rðn gÞ Rðn þ gÞ; RðzÞ ¼ Rew 1 þ : k b1 2b1 2b2 b2 1 f ðnÞ p
ð4Þ In (4) the following notation has been introduced: 1=2 n a1 x, g a1 t, k1 ¼ l1 ðn1 Þ1=2 , k2 ¼ l2 ðn1 Þ1=2 , k ¼ k1 k2 bk ¼ nk ha1 , k ¼ 1; 2. As is customary in LEFM [1], we deﬁne stress intensity factors as the coefﬁcients of the singularities in the distributions of the stress components in the neighbourhood of the crack tips. By solving Fredholm integral Eq. (4), we can obtain the representations of potential functions u1 and u2 , and then from (2) we can determine the distribution of the components of the stress tensor Q0ij ðr; y3 Þ. Analyzing the values of these components in the crack plane beyond the crack, we can derive the following expressions for the stress intensity factors (SIFs) KI ¼ C44 d1 l1
k pﬃﬃﬃﬃﬃﬃ paf ð1Þ; KII ¼ 0; KIII ¼ 0; k1
ð5Þ
where function f should be found by solving (4). It can be seen from (5) that the value of KI depends on the initial stresses, cracks radii a and distance h between the cracks because f , as it follows from (4), also depends on these parameters. In the similar way, we can obtain the expressions of SIFs for the periodic array of parallel coaxial Mode II and Mode III cracks in an unbounded body as well as for two parallel coaxial Mode I, Mode II and Mode III cracks in an inﬁnite body [4–6].
232
V. Bogdanov and V. Nazarenko
4 Numerical Results We present the results obtained for the cracks subjected to uniform stresses on their faces. Consider a highly elastic material with Bartenev–Khazanovich potential [6]. For 1 3D problems the dependences of the ratio of SIFs KI =K 1 I (where KI is the SIF for a single isolated Mode I crack in an unbounded body) on dimensionless halfdistance between cracks b ¼ h=a are shown in Fig. 1 for the values of initial stress parameters k1 ¼ 1:2 (tensile initial stresses), k1 ¼ 0:8 (compressive initial stresses), k1 ¼ 1:0 (no initial stresses). These data show that the interaction of cracks in an unbounded body with a periodic array of coaxial Mode I cracks (the solid lines), as in the case of two parallel coaxial Mode I cracks (the dashed lines), leads to a decrease of KI values as compared to KI1 . On the other hand, when the separation distance between cracks increases, their mutual influence quickly weakens and the respective values of SIFs tend to the values obtained for a single isolated crack in an unbounded material. For the distances between cracks which exceed 8 crack radii, the interaction between them can be neglected in practical calculations, since in that case the difference between the values of KI and KI1 is less than 5% for all considered values of parameter k1 .
Fig. 1. Dependence of SIF ratio on dimensionless distance between cracks for elastic material with Bartenev–Khazanovich potential
Fig. 2. Dependence of SIF ratio on the parameter of initial stresses for a laminated (layered) composite material
Figure 2 presents results for a laminated twocomponent composite material with isotropic layers for the values of the ratio of elastic moduli of the layers Eð1Þ Eð2Þ ¼ 3, Poisson’s ratios of the layers mð1Þ ¼ mð2Þ ¼ 0:3, and the volume concentration of the ﬁrst layer c1 ¼ 0:3. This ﬁgure shows the ratio KII KII1 (where KII1 is the SIF for a Mode II crack in an unbounded material) versus parameter of initial stress k1 for the periodic array of parallel coaxial Mode II cracks for different values of b. As can be seen, the curves in Fig. 2 have vertical asymptotes representing the resonant behavior of the SIFs when the initial compressive stresses are so high as to cause local buckling of the material near the cracks. According to the combined approach described in the Introduction, this phenomenon allows us to determine the critical loads for a material compressed along a periodic array of parallel coaxial cracks. Figure 3 shows the critical
The Effect of Cracks Interaction in Materials Under Loading Along Cracks
233
¼ S011 =E (the stress divided by the effective elastic dimensionless compressive stress r modulus of the laminated composite) obtained this way versus the ratio of the elastic moduli of the layers E ð1Þ E ð2Þ for b ¼ 0:5. The results are presented for the periodic array of cracks (solid line), as well as for two parallel cracks (dashed line). For a highly elastic material with Treloar potential [6], Fig. 4 illustrates the effect of the cracks interaction on the values of relative critical contraction parameter e1 ¼ 1 k1 in the 2D problem (the condition of plane strain state is assumed) for an unbounded body containing a periodic array of parallel coaxial cracks under compression along cracks. It can be seen that at small distances between cracks b their mutual influence results in a signiﬁcant reduction of the critical compression parameter e1 . At the same time, with the increased distance between cracks the values of relative critical contraction parameter e1 tend to e1 ¼ 0:456, which for Treloar potential corresponds to the critical contraction parameter for a single crack in an inﬁnite body.
Fig. 3. Dependence of the critical dimensionless compressive stress on the ratio of elastic moduli of layers for the laminated composite
Fig. 4. Dependence of the relative critical contraction parameter on dimensionless distance between cracks for the material with Treloar potential
5 Conclusions The results obtained allow the following conclusions: (1) for all the problems considered the stress intensity factors are substantially dependent on the initial (residual) stresses; (2) the values of the stress intensity factors change abruptly (the “resonancelike” effect) when the initial contraction ratio k1 tends to the value with which there is a local loss of stability in the crack vicinity. According to the combined approach used here this effect enables one to determine critical loading parameters in problems on bodies compressed along cracks; (3) the geometrical parameters of the problems and materials’ properties produce a signiﬁcant effect both on the values of SIFs and on the critical compression parameters.
234
V. Bogdanov and V. Nazarenko
References 1. Gdoutos, E.E.: Fracture Mechanics: An Introduction. Springer, Dordrecht (2005) 2. Guz, A.N.: Brittle Fracture of Materials with Initial Stresses. Naukova Dumka, Kyiv (1991). (in Russian) 3. Guz, A.N., Dyshel, M.S., Nazarenko, V.M.: Fracture and Stability of Materials with Cracks. Naukova Dumka, Kyiv (1992). (in Russian) 4. Guz, A.N., Nazarenko, V.M., Bogdanov, V.L.: Combined analysis of fracture under stresses acting along cracks. Arch. Appl. Mech. 83(9), 1273–1293 (2013) 5. Bogdanov, V.L., Guz, A.N., Nazarenko, V.M.: Spatial problems of the fracture of materials loaded along cracks (Review). Int. Appl. Mech. 51(5), 489–560 (2015) 6. Bogdanov, V.L., Guz, A.N., Nazarenko, V.M.: Uniﬁed Approach in NonClassical Problems of Fracture Mechanics. LAP LAMBERT Acad. Publ, Saarbrücken (2017). (in Russian)
Safe Loading of the Orthotropic Plate with Periodic System of Collinear Cracks Olga Bogdanova(&) S.P.Timoshenko Institute of Mechanics of National Academy of Sciences of Ukraine, Nesterov Str, 3, 02053 Kyiiv, Ukraine [email protected] Abstract. On the basis of a modiﬁed dc model of crack, the safe loading of an orthotropic plate with periodic system of collinear cracks is studied. The plate material is satisfying the strength condition in general form. The relations for the determination of major parameters of the crack model (the size of process zones, stresses in these zones, and the cracktip opening displacements) are deduced. The mechanism of fracture of the plate containing a periodic system of collinear cracks is investigated. The influence of the degree of anisotropy and geometric parameters of the problem on the formation of the process zones and limiting state of the elastic orthotropic plate is revealed. The region of safe loading of an orthotropic viscoelastic plate with cracks is determined. The influence of the rheological parameters of the material on the region of safe loading is analyzed. Keywords: Periodic system of collinear cracks loading Orthotropic materials
Critical loading Safe
1 Limiting State of an Orthotropic Plate with Periodic System of Collinear Cracks Consider a thin orthotropic plate with periodic system of collinear cracks of length 2l located along the axis of orthotropy which coincides with the Oxaxis. The centers of the cracks are located at the points xn ¼ 2nD(xn ¼ 0; 1; 2; . . ., y ¼ 0). The plate is stretched by a homogeneous load applied at inﬁnity ry ¼ p [ 0; rx ¼ 0; sxy ¼ 0; z ! 1; ðz ¼ x þ iyÞ; Replace the process zones formed under the action of the load near the crack tips by additional cuts of length d on the continuations of the cracks whose lips are subjected to the action of stresses r0x ; r0y . Assume that the limiting state of the material in the process zones is described by a strength criterion F ðr1 ; r2 ; Ci Þ ¼ 0;
ð1Þ
where r1 ; r2 are the principal stresses and Ci are constants of the material. For the numerical analysis and conclusions the Mises–Hill condition of strength is used [1]. © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 235–241, 2020. https://doi.org/10.1007/9783030478834_43
236
O. Bogdanova
In view of the symmetry of the problem, the directions x and y are principal. Therefore, the stresses r0x ; r0y satisfy the condition of strength (1) in the process zone. These stresses are found from the solution of the system of two Eqs. [1]: r0x ¼ b r0y p ;
F r0x ; r0y ; Ci ¼ 0
ð2Þ
pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ b ¼ E1 =E2 ; E1 ; E2  are the elasticity moduli of the material in directions 1 and 2. The crack opening displacement dðx; l; LÞ at a point x from the segments jx xn j L; y ¼ 0 is given by the formula [2]: 9 8 > > sec q > > Z = 2T0 r0y l arc sin ~l ðt2 1Þ 1 t2 cos2 q > > > ; :arc sin l ~x=~l ð3Þ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 þ x cos2 r þ 1 x2 cos2 r sin r ðx 1Þ where F ðx; r Þ ¼ ln ; pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 x cos2 r þ 1 x2 cos2 r sin r ðx þ 1Þ 1 T0 ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ E1 E2
sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ rﬃﬃﬃﬃﬃ E1 E1 px ~ pl pp ; l ¼ sin ; q ¼ 0; m12 þ ; ~x ¼ sin 2 2D 2D 2ry E2 G12
It is clear that the integral in relation (3) is computed in the ﬁnite form as D ! 1, which corresponds to the case of a single crack [1]. The size of process zone is determined by the ratio [2] ~
d 2D sin l ¼ arc sin l pl cos q
ð4Þ
In accordance with the dc  criterion, a crack starts when dðlÞ ¼ dc . Then, basing on (3), the ﬁeld of ultimate loads p can be deﬁned by [2] ~ ~ ZL=l ð1Þ ~l dt p p 0 ð1Þ ; ﬃ F ðt; q Þ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ p r0y ðp Þ ln sec ¼ 2r y 2 0 pð1Þ arc sin ~l 2 ~ 2r 1 t l y 1
ð5Þ
ð1Þ
where q ¼ 2rp0 ðpp Þ, p  the limiting load in the case of a plate with a single crack. The y
ð1Þ
change p from 0 to r02 corresponds to a change in the crack length from inﬁnity to zero. It should be noted that the boundary condition of the plane, weakened by the system of cracks, is not always determined by the fracture criteria of type (5). If the
Safe Loading of the Orthotropic Plate
237
external load is such that the condition d ¼ D l is fulﬁlled, then the fusion of the areas for the elimination of neighboring cracks occurs, which can also be considered as a condition of the boundary state. Taking into account equality (4), this condition will be written as: ðd Þ
D p p p ; ¼ ; qð d Þ ¼ ð d Þ ðd Þ l 2 arcsinðcos q Þ 2r0y p
ð6Þ
ðd Þ
The relation (6) determines the load p at which the areas of process zones of neighboring cracks occur. The dependence of this load on the dimensionless distance between cracks D=l is constructed (Fig. 1). Increasing the degree of anisotropy of the material reduces the level of the maximum allowable load at which the merge of process zones occurs, but in general, the effect of the degree of anisotropy on this process is small.
1,0 0,9 0,8
p/
0,7
02
0,6 0,2 0,1 0,0
0
5
10
D/l
15
20
ðd Þ
Fig. 1. Dependence of the load p =r02 on the dimensionless distance between the cracks D=l: solid line  b ¼ 0; 3; dashed line  b ¼ 0; 5; dashdotted line b ¼ 0; 9
Fig. 2. Dependence of the load p =r02 on the dimensionless distance between ð1Þ
the cracks D=l: p =r02 = 0,1 (1); 0,5 (2); 0,7 (3); 4 – load when the process zones are joined
Thus, the boundary condition of the plate with the periodic system of collinear cracks is determined by the set of conditions (5) and (6): p ¼ min pðdÞ ; p ;
ð7Þ
The dependence of the critical load on the dimensionless distance between the cracks D=l obtained on the basis of the relations (5) and (6) for b ¼ 0:3 was constructed (Fig. 2). It is obvious that for arbitrary crack lengths and the distance between them, there is such a “critical” level of load when there is a partial destruction of the entire intersection along the line of location of the cracks. This “critical” load is higher, the smaller the length of the cracks.
238
O. Bogdanova
2 Safe Loading of a Viscoelastic Orthotropic Plate, Weakened by a Periodic System of Collinear Cracks Consider a thin orthotropic plate of viscoelastic material, weakened by a periodic system of collinear cracks, located along one of the orthotropy axes. Assume that the deformation properties of a material are described by linear relationships up to destruction. During the destruction of such materials areas of destruction formed at the tops of cracks, inside which there is a destruction of a less durable binder and a part of highstrength ﬁttings. We will replace these zones with additional cuts of length d ðtÞ on the continuation of cracks, on the banks of which there is a uniformly distributed selfequilibrium stress. Since these stresses are determined on the basis of the condition (1), which is constant in time, they also do not depend on time and can be determined at the time t ¼ 0 from the solution of the corresponding problem of the theory of elasticity, that is, the stresses in the process zones are determined by a system of Eqs. (2). Thus, it is necessary to investigate the stressstrain state of an orthotropic viscoelastic plate with a periodic system of collinear incisions jx xn j LðtÞ; y ¼ 0 along the axis of orthotropy Ox, under the action of a uniformly distributed load independent of time ry ¼ p [ 0; rx ¼ 0; sxy ¼ 0; jx þ iyj ! 1. As is known [3, 4], the Volterra principle can be applied to the problem, according to which the viscoelastic opening of the shore of the crack can be written as: dðx; tÞ ¼ T d0 ðx; tÞ;
ð8Þ
where d0 ðx; tÞ  function of power and geometric parameters, T  the function of integral operators whose form is determined from the solution of the corresponding problem of the theory of elasticity. For this problem we have [3]: vﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ ! u sﬃﬃﬃﬃﬃ u 1 E E 1 t2 m12 þ 1 ; T ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ E2 G12 E1 E2 ~=~lðtÞ L Z ~lðtÞ 2r0y lðtÞ ds d0 ðx; tÞ ¼ F ðs; qÞ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 ~ p arc sin lðtÞ 1 s2 ~lðtÞ ~x=~lðtÞ
ð9Þ
ð10Þ
It has been experimentally shown that for some orthotropic viscoelastic materials it is possible to disregard the creep along the orthotropic axes and take into account only creep at displacement, that is, to put [3]: E1 E10 ¼ const; E2 E20 ¼ const; m12 m012 ¼ const;
1 1 ¼ ½1 þ kR ðcÞ; G12 G012 ð11Þ
Safe Loading of the Orthotropic Plate
239
where E10 ; E20 ; m012 ; G012  instantaneous values of relevant characteristics, R  resovent Rt integral operator of the form R f ¼ Rðt sÞf ðsÞds. 0
Using the method of integral continued fractions, the operator (9) can be represented as a linear combination of resolvent integral operators [3]: "
T ¼ T0 1 þ
N X
#
Ai R ðci Þ
ð12Þ
i¼1
with the kernel T ðt sÞ ¼
N P
Ai Rðt s; ci Þ, Rðt s; ci Þ  kernels of operators R ðci Þ.
i¼1
If the criterion of fracture is to choose a criterion for the critical crack opening, we obtain the equation for determining the moment of the beginning of the slow crack development t (or the duration of the incubation period of the crack development in the viscoelastic body) if the external load is constant over time in the form [3]: Zt T ðhÞdh ¼ 0
dc 1; dðl0 Þ
ð13Þ
where dð xÞ ¼ T0 d0 ð xÞ  elastic opening of the crack at the point x. For bodies with limited creep, there are “safe” loads, for which the value dðl0 ; tÞ can’t reach the critical value dc , and the development of the crack does not happen. In the general case, the safe load ﬁeld is determined from the ratio [3]: dc T1 ¼ ; T1 ¼ T 1jt¼1 ; dðl; pS ; qS Þ T0
ð14Þ
If, as the kernel of an integral operator, we choose the fractionalexponential function of Yu.M. Rabotnov [3], then from (4) we obtain:
T1
vﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ ! u sﬃﬃﬃﬃﬃ 0 0 u 1 t E1 E1 m012 þ 1 ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 0 0 0 G E E1 E2 12 2 vﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ ! u sﬃﬃﬃﬃﬃ 0 0 u 1 t E1 E1 k : m012 þ 1 ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1þ 2 0 0 0 cj G j E2 E1 E2 12
ð15Þ
where, c – the rheological parameters of the material. Then, on the basis of (5), (10) and (14), we obtain an equation for determining a safe load pS :
240
O. Bogdanova
r0y ðpS Þ
~ ~ ZL=l ð1Þ ~l ds T0 0 ð1Þ p p : F ðs; qS Þ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ r p ln sec ¼ 2 y 2 ð1Þ T1 arcsin ~l 2r0 p 1 s2 ~l
ð16Þ
y
1
ð1Þ
The value p uniquely determines the length of the crack l0 and, consequently, Eq. (16) determines the safe load pS for a given initial crack length. Instantaneous fracture of the plate with the system of cracks occurs at a critical load p , which is ðd Þ determined by the relation (5). In addition, there is some load p on which there is an instantaneous partial destruction of the material on the line of location of the cracks. This load is determined from the equation: ðdÞ
cos
p p pl ¼ sin 0 : ðdÞ 2D 2r0y p
ð17Þ
Thus, the development of a crack in a viscoelastic body will occur only in the region of load change, which is limited by curves, which are determined by the relations (5), (16) and (17). Numerical results are obtained for a material with the following characteristics [3] 0 E1 ¼ 1; 553 109 Pa, E20 ¼ 2; 315 109 Pa, G012 ¼ 0; 3086 109 Pa, m012 ¼ 0; 08, a ¼ 0; 85, k ¼ 0; 275 sec1a , c ¼ 0; 181 sec1a . Figure 3 show the dependence of the “safe” load (16) on the dimensionless distance between the cracks D=l for ð1Þ ð1Þ ð1Þ p =r02 = 0,1 (curves 1); p =r02 = 0,5 (curves 2); 3−p =r02 = 0,7 (curves 3); curve 4 show loading when the process zones are joined; dashed line – critical loading p =r02 . The dependence of the safe load on the rheological parameters of the material are shown on Fig. 4 and Fig. 5 for D=l ¼ 3; 0.
Fig. 3. Dependence of the safe load pS =r02 on the dimensionless distance between the cracks D=l
Fig. 4. Dependence of the safe load pS =r02 on the rheological parameter c
Fig. 5. Dependence of the safe load pS =r02 on the rheological parameter k
Safe Loading of the Orthotropic Plate
241
It can be noted that the change in the rheological parameters of the material k and c signiﬁcantly affects the area of safe load: the decrease k or increase jcj in other permanent characteristics leads to an increase in the level of safe loading. The parameter a does not affect the level of safe load, since it is not part of the ratio (15). Thus, by changing the rheological parameters of the material, it is possible to achieve a decrease in the area of loading, in which the development of cracks occurs.
3 Conclusions The proposed modiﬁcation of the LeonovPanasyukDagdale crack model to the case of orthotropic materials allows to effectively solve problems of the destruction of orthotropic bodies with cracks, the material of which satisﬁes the condition of the strength of the general form. With this model, the boundary state of the orthotropic plate, relaxed by the periodic system of collinear cracks, the material of which is elastic or viscoelastic, is investigated. The mechanism of fracture of the plate with cracks and the influence on the boundary and safe loading of the properties of the material have been investigated.
References 1. Kaminsky, A.A., Bogdanova, O.S., Bastun, V.N.: On modeling cracks in orthotropic plates under biaxial loading: synthesis and summary. Fatigue Fract. Eng. Mater. Struct. 5(34), 345– 355 (2011) 2. Bogdanova, O.S.: Limiting state of an elastoplastic orthotropic plate with a periodic system of collinear cracks. Int. Appl. Mech 5(43), 539–546 (2008) 3. Kaminsky, A.A.: Fracture mechanics of viscoelastic bodies with cracks. Nauk. Dumka, Kyiv (1990)
Boundary Element Analysis of Partially Debonded ShellLike Rigid Inclusions in Anisotropic Medium Heorhiy Sulym1
, Nataliia Ilchuk2
, and Iaroslav Pasternak2(&)
1
2
Pidstryhach Institute for Applied Problems of Mechanics and Mathematics of NASU, Naukova Street 3b, 79060 Lviv, Ukraine Lutsk National Technical University, Lvivska Street 75, 43018 Lutsk, Ukraine [email protected]
Abstract. The paper presents boundary element models of anisotropic thermoelastic medium containing partially debonded shelllike rigid inclusions, which possess high rates of heat conduction. Boundary integral equations are derived, which account for partial debonding of a shelllike inclusion at one of its faces. Special attention is paid to full debonding of a rigid shell at two faces simultaneously (bilateral debonding). Obtained equations are implemented in a fast and accurate boundary element approach. Keywords: Boundary element method intensity factor
Anisotropic Thermoelastic Stress
1 Introduction Structural materials, including composite and anisotropic ones, generally contain different natural or artiﬁcial inhomogeneities, which influence ﬁeld distribution and can even initiate fracture processes. In particular, composite materials consisting of ﬁbre, ribbonlike or platelike ﬁlament are widely used in modern mechanical and airspace engineering due to their high performance. However, the nonhomogeneous structure of such materials produces redistribution of mechanical and thermal ﬁeld. In this case partial debonding of a ﬁlament can cause high stress concentration, which influence safety and structural integrity. Another example of stress concentrator are anchors in rock mechanics, which are in general, partially bonded, which signiﬁcantly influences stress distribution. Therefore, these raises interest to the problems for solids with partially debonded inhomogeneities. The problems on debonding of spatial thin rigid inclusions dates back to Selvadurai et al. [1], who considered rigid disc inclusion with circular debonded region. Since then the interest to problems of partially debonded inclusions has only raised. In particular, recently Shahmohamadi et al. [2] considered a frictionless contact of a rigid disk with crack faces, Nategh et al. [3] considered bonded contact of a rigid disk with a pennyshaped crack. Nevertheless, the studies of debonded inclusions are limited to analytic or semianalytic methods, which constrains the shape of inclusion and a debonded region to simple geometries, i.e. planar circular or elliptic domains. © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 242–247, 2020. https://doi.org/10.1007/9783030478834_44
Boundary Element Analysis of Partially Debonded ShellLike Rigid Inclusions
243
Therefore, this study is concerned with the development of numerical boundary element approach, which can hold problems of partially debonded 3D rigid shelllike inclusions of arbitrary smooth shape. It is natural continuation of recent studies on cracks [4] and perfectly bonded inclusions [5] in anisotropic thermoelastic medium.
2 Modelling of Partially Debonded Rigid ShellLike Inclusions 2.1
Boundary Integral Equations of Anisotropic Thermoelasticity
Consider linear thermoelastic anisotropic solid B in the reference coordinate system Ox1 x2 x3 , which contains internal smooth opened surface C of ﬁeld discontinuity. According to [4, 5] the boundary integral equations of steadystate heat conduction and thermoelasticity of anisotropic solids are as follows ZZ ZZ X 1X hðx0 Þ ¼ H ðx; x0 Þ hn ðxÞdSðxÞ CPV H ðx; x0 ÞDhðxÞdSðxÞ 2 S S ZZZ H ðx; x0 Þfh ðxÞdV ðxÞ;
ð1Þ
B 2 ZZ X 1 Dhn ðx0 Þ ¼ nj ðx0 Þ4CPV H hn ðxÞdSðxÞ i ðx; x0 Þ 2
ZZ HFP
@B
Hi ðx; x0 ÞDhðxÞdSðxÞ
@B
ZZZ
3 5 H i ðx; x0 Þfh ðxÞdV ðxÞ ;
B
ZZ ZZ X 1X ui ðx0 Þ ¼ Uij ðx; x0 Þ tj ðxÞdSðxÞ CPV Tij ðx; x0 ÞDuj ðxÞdSðxÞ 2 S S ZZ h i X þ Ri ðx; x0 ÞDhðxÞ þ Vi ðx; x0 Þ hn ðxÞ dSðxÞ S
ZZZ þ
ð2Þ
ð3Þ
ZZZ Uij ðx; x0 Þfj ðxÞdV ðxÞ
B
Vi ðx; x0 Þfh ðxÞdV ðxÞ; B
2 ZZ ZZ X 1 Dti ðx0 Þ ¼ nj ðx0 Þ4CPV Dijk ðx; x0 Þ tk ðxÞdSðxÞ HFP Sijk ðx; x0 ÞDuk ðxÞdSðxÞ 2 @B @B ZZ ZZ X Qij ðx; x0 ÞDhðxÞdSðxÞ þ Wij ðx; x0 Þ hn ðxÞdSðxÞ þ CPV ZZZ þ
@B
ZZZ
Dijk ðx; x0 Þfk ðxÞdV ðxÞ B
@B
3
Wij ðx; x0 Þfh ðxÞdV ðxÞ5;
B
ð4Þ
244
H. Sulym et al.
P P P where x0 2 S; S ¼ C [ @B; and h ¼ Dh ¼ h, hn ¼ Dhn ¼ hn , ui ¼ Dui ¼ ui , P P P f ¼ f þ þ f ; Df ¼ f þ f ; hn ¼ hi ni ; hn ¼ hiþ ti ¼ Dti ¼ ti on @B; þ þ þ niþ þ h i ni ¼ hi hi ni ; n ðxÞ ¼ n ðxÞ are unit outwards normal vectors to þ the faces C and C of the mathematical cut C; ti ¼ rij nj is a stress vector; rij is a stress tensor; fi is a body force vector; hi is a heat flux; hn ¼ hi ni ; fh is a distributed heat source density; ui is a displacement vector; h is a temperature change with respect to the reference temperature. CPV stands for the Cauchy Principal Value of the integral and HFP stands for the Hadamard Finite Part of the integral. The indices vary from 1 to 3. Here and further the Einstein summation convention is used. A comma at subscript denotes differentiation with respect to a coordinate indexed after the comma, i.e. ui;j ¼ @ui @xj . The kernels of Eqs. (1)–(4) are listed in [4, 5]. 2.2
Inclusion Model and Boundary Conditions
Integral Eqs. (1)–(4) are derived from the extended Somigliana identity for thermoelastic material [4] and relate given and unknown boundary conditions at the boundary @B of the solid B; e.g. when the traction vector is given on @B the sought function is displacement vector and vice versa. Consequent usage of extended Somigliana identity allow determination of the stress ﬁeld in the entire solid B. When cracks orPshelllike inclusions are considered, the sought functions are ﬁeld discontinuities Dh, hn , Dui , P ti at the surface C. The same functions are convenient to use as sought functions in the problems of partially debonded inclusions. Therefore, boundary conditions should P be rewritten through Df and f. Prior to consideration of the boundary conditions at the discontinuity surface C consider the model of a rigid perfectly conducting nondeformable inclusion, which is derived in [5]: ZZ h
incl
ð xÞ ¼ h ;
0 hincl n ðxÞdSðxÞ H ¼ 0
0
ð5Þ
S 0 0 uincl i ðxÞ ¼ ui þ eijm xj xm ; ZZ tiincl ðxÞdSðxÞ P0i ¼ 0; S
ZZ
eijm xj tmincl ðxÞdSðxÞ Mi0 ¼ 0;
ð6Þ
S
where h0 is a temperature of the inclusion; H 0 is the constant heat (actually heat generation rate) applied to the inclusion; u0i is a rigid displacement of the inclusion and x0j is its rigid rotation about the origin; eijm is the permutation tensor; S is a surface of the inclusion; P0i and Mi0 are resultants of forces and couples applied to the inclusion, respectively.
Boundary Element Analysis of Partially Debonded ShellLike Rigid Inclusions
245
Now consider the following types of the boundary conditions at the discontinuity surface: a. b. c. d.
perfect thermal and mechanical contact at Sa C; partial debonding at Sb C þ ; partial debonding at Sc C ; bilateral debonding at Sd C.
Also assume that Sa [ Sb [ Sc [ Sd ¼ C and Si \ Sj ¼ 0 for i 6¼ j, i.e. the domains of different type of boundary conditions do not intersect. Accounting for inclusion models (5), (6), these boundary conditions can be written in terms of temperature, heat flux, displacement and traction on the faces C þ and C of the cut as follows, 0 0 h þ ðxÞ ¼ h ðxÞ ¼ h0 ; uiþ ðxÞ ¼ u i ðxÞ ¼ ui þ eijm xj xm ; 8x 2 Sa ; 0 0 þ h ðxÞ ¼ h0 ; hnþ ðxÞ ¼ 0; u i ðxÞ ¼ ui þ eijm xj xm ; ti ðxÞ ¼ 0; 8x 2 Sb ; þ 0 0 h þ ð xÞ ¼ h0 ; h n ðxÞ ¼ 0; ui ðxÞ ¼ ui þ eijm xj xm ; ti ðxÞ ¼ 0; 8x 2 Sc ; þ hnþ ðxÞ ¼ h n ðxÞ ¼ 0; ti ðxÞ ¼ ti ðxÞ ¼ 0; 8x 2 Sd ;
ð7Þ ð8Þ ð9Þ ð10Þ
In this case inclusion equilibrium equations do not depend on the type of boundary conditions and can be written through the sought functions on the cut as ZZ X hn ðxÞdSðxÞ H 0 ¼ 0; S
ZZ X
ZZ ti ðxÞdSðxÞ P0i ¼ 0;
S
eijm xj
X
ð11Þ tm ðxÞdSðxÞ Mi0 ¼ 0:
S
Since fþ ¼
1 X 1 X f þ Df ; f ¼ f Df 2 2
ð12Þ
boundary conditions (7)–(10) on the cut C can be rewritten through the sought discontinuity functions as 1X 1X hðxÞ ¼ h0 ; DhðxÞ ¼ 0; ui ðxÞ ¼ u0i þ eijm x0j xm ; Dui ðxÞ ¼ 0; 8x 2 Sa ; 2 2 ð13Þ
246
H. Sulym et al.
1X
hð xÞ ¼ h0 þ
1 DhðxÞ; 2
Dhn ðxÞ ¼
2 1X 1 ui ðxÞ ¼ u0i þ eijm x0j xm þ Dui ðxÞ; 2 2
X
hn ðxÞ;
Dti ðxÞ ¼
X
ti ðxÞ
8x 2 Sb ;
X 1X 1 hðxÞ ¼ h0 DhðxÞ; Dhn ðxÞ ¼ hn ðxÞ; 2 2 X 1X 1 ui ðxÞ ¼ u0i þ eijm x0j xm Dui ðxÞ; Dti ðxÞ ¼ ti ðxÞ 8x 2 Sc ; 2 2 X X Dhn ðxÞ ¼ hn ðxÞ ¼ 0; Dti ðxÞ ¼ ti ðxÞ ¼ 0; 8x 2 Sd
ð14Þ
ð15Þ
ð16Þ
Boundary conditions (13)–(16) are readily substituted into Eqs. (1)–(4) to obtain the of boundary integral equations for the sought discontinuity functions Dh, P system P hn , Dui , ti at the surface C, which model debonded shelllike inclusion. To reduce the number of equations one can use only Eqs. (1) and (3) with boundary conditions (13) (Type a) and Eqs. (2) and (4) with boundary conditions (16) (Type d).
3 Boundary Element Approach At the ﬁrst step (preprocessing) of the boundary element solution of derived boundary integral equations for a particular problem the surface @B of the solid along with the discontinuity surface C (which model partially debonded inclusion) is meshed with quadrilateral quadratic discontinuous boundary elements. The local curvilinear coordinate system Ong is associated with each boundary element, moreover, 1 n 1, 1 g 1. The collocation points are placed at nodes n ¼ ð2=3; 0; 2=3Þ; g ¼ ð2=3; 0; 2=3Þ. Therefore, there are 9 collocation points associated with each boundary element. Boundary conditions along with unknown boundary and discontinuity functions are interpolated within the collocation points at each boundary element CN as bN ðn; gÞ ¼
3 X 3 X i¼1 j¼1
where b ¼ ðh; Dh; hn ; are given as [4] / 1 ð nÞ ¼ n
P
hn ; ui ; Dui ; ti ;
P
bi;j N /i ðnÞ/j ðgÞ;
ð17Þ
ti ÞT , and the discontinuous shape functions
9 3 3 3 9 3 n ; /2 ðnÞ ¼ 1 n 1 þ n ; /3 ðnÞ ¼ n n þ ð18Þ 8 4 2 2 8 4
If the side of the boundary element models the inclusion front, which is perfectly bonded, special shape functions are used for heat flux and traction to capture the square root singularity arising at its front [5]
Boundary Element Analysis of Partially Debonded ShellLike Rigid Inclusions
/Ri ðnÞ
! 3 X 1 j1 R R ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Ui1 þ Uij ð1 nÞ : 1n j¼2
247
ð19Þ
Constants URij are determined from the system of equations /i nj ¼ dij , where nj ¼ ð2=3; 0; 2=3Þ. Substituting (17) along with appropriate boundary conditions (13)–(16) into the boundary integral Eqs. (1)–(4) one obtains the system of linear algebraic equations for unknown nodal values of the boundary and discontinuity functions. Evaluation of kernels, regular, singular and hypersingular integrals is the same as in the case of cracks and perfectly bonded inclusions and is discussed in details in Refs [4, 5].
4 Discussion and Further Studies Obtained boundary element approach was programmed to objectoriented C ++ code, which was used in calculation of solids with debonded nondeformable shelllike inclusions. Veriﬁcation was made through comparison of the numerical results with analytic solution of Selvdurai et al. [1]. Good agreement was observed. Further studies are assumed to be concerned with smooth or frictional contact conditions on the surfaces of the inclusion, since it is essential to account for these conditions in the cases of nonplanar shapes of inclusions.
References 1. Selvadurai, A.P.S., Singh, B.M., Au, M.C.: Axial loading of a rigid disc inclusion with a debonded region. Int. J. Solids Struct. 25(7), 783–795 (1989) 2. Shahmohamadi, M., Khojasteh, A., Rahimian, M.: Frictionless contact of a rigid disk with the face of a pennyshaped crack in a transversely isotropic solid. Int. J. Solids Struct. 106, 274– 283 (2017) 3. Nategh, S., Khojasteh, A., Rahimian, M.: Bonded contact of a rigid disk inclusion with a pennyshaped crack in a transversely isotropic solid. J. Eng. Math. 110, 123–146 (2018) 4. Pasternak, I.A., Pasternak, R., Pasternak, V., Sulym, H.: Boundary element analysis of 3D cracks in anisotropic thermomagnetoelectroelastic solids. Eng. Anal. Bound Elem 74, 70–78 (2017) 5. Pasternak, I.A., Sulym, H., Ilchuk, N.: Boundary element analysis of 3D shelllike rigid electrically conducting inclusions in anisotropic thermomagnetoelectroelastic solids. Z Angew Math Mech, e201800319 (2019)
The Transmission of an Acoustic Wave Through a Composite Plate with Energy Dissipation in a Material Taken into Account Based on ThreeDimensional Equations of Elasticity Theory V. N. Paimushin1,2
and R. K. Gazizullin1(&)
1
Kazan National Research Technical University named after A. N. Tupolev  KAI, Kazan, Russia [email protected], [email protected] 2 Kazan Federal University, Kazan, Russia
Abstract. The problem of a plane monoharmonic sound wave passage through a thin composite rectangular plate hinged in the opening of an absolutely stiff dividing wall has been considered on the basis of twodimensional in spatial coordinates motion equations. These equations have been constructed by the reduction of threedimensional equations on the basis of the discrete layered model of a multilayer plate deformation at small displacements and deformations with account of the internal damping of layers according to the Kelvin– Voight model. Behavior of acoustic media has been described by the classical wave equations based on the model of an ideal compressible fluid. The exact analytical solutions of the formulated problem have been constructed. The dependence of sound insulation properties and parameters of the stressstrain state of a composite plate reinforced with carbon ﬁber textile on the incident sound wave frequency was studied. It is shown that under highfrequency acoustic impact, the deformation mechanics of the structures made of ﬁber reinforced composite must be described by reﬁned equations of motion as they have a high degree of accuracy and intensionality since the formation of the stressstrain state in them is almost threedimensional with components of the same order. Keywords: Multilayer plate Discrete layered model Internal friction of the material Kelvin–Voigt model Acoustic medium Sound wave Analytical solution
1 Introduction The sound waves passage through thin plates, including composite ones, has been studied in numerous scientiﬁc works [1–5 et al.]. However, in these works the simplest relations of plate theory are used to describe the plate deformation mechanics. As a rule, these models are based on the introduction of a number of wellknown simplifying hypotheses and the assumption that only the tangential components of the stress tensor © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 248–253, 2020. https://doi.org/10.1007/9783030478834_45
The Transmission of an Acoustic Wave Through a Composite Plate
249
are formed in the plate during the sound wave passage. In order to further develop the results obtained earlier [6] and to study the influence of the incident sound wave frequency on the parameters of a dynamic stressstrain state forming in a plate, we use the developed earlier [6] discrete layered model to formulate the considered problem of sound waves passage through multilayer thin plates. This model makes it possible to obtain solutions that are practically approaching a solution based on the equations of the threedimensional elasticity theory.
2 Statement of the Problem and the Construction of its Solution Let us consider a multilayer rectangular plate having dimensions a, b and consisting of M ¼ N 1 layers of thickness h½k (here k ¼ 1; M is the layer number). For dis½k
½k
placement components Ui ði ¼ 1; 2Þ and U3 approximations ½k
Ui ¼
ðk þ 1Þ
ui
2
þ
z½k ðk þ 1Þ ðk Þ ui ui ; h½k
½k
U3 ¼
z½k ðk þ 1Þ wðk þ 1Þ þ w wðkÞ : 2 h½k
are accepted within the thickness of each layer (h½k 2 h½k 2). We assume that the plate is placed in the opening of an absolutely stiff dividing wall separating two adjacent spaces V1 and V2 . This plate is overrun by a flat harmonic wave of pressure p and frequency x. As a result of it interaction with the plate, acoustic waves are excited in the halfspaces V1 and V2 around the plate, which are reflected in the ﬁrst medium and are radiated in the second medium. To determine the pressures p ; p1 applied to the boundary plane of the 1st layer of the plate and the pressure p2 applied to the boundary plane of the Nth layer of the plate, it is necessary to ﬁnd solutions of the wave equations € U;zz c2 1 U ¼ 0;
€ Us;xx þ Us;yy þ Us;zz c2 s Us ¼ 0; s ¼ 1; 2
ð1Þ
written in the potentials U ; U1 and U2 of velocities. Here, c1 and c2 are sound velocities. The pressure p ; ps and the velocity components vz ; vsx ; vsy ; vsz in the spaces V1 and V2 are determined in terms of the functions U and Us : p ¼ q1 U_ ;
ps ¼ qs U_ s ;
vz ¼ U;z ; vsx ¼ Us;x ;
vsy ¼ Us;y ;
vsz ¼ Us;z
where qs are the densities of acoustic media in the spaces. Solutions to the equations of plate motion and Eqs. (1) have to satisfy the kinematic conjugation conditions w_ ð1Þ ¼ vz þ v1z z¼0 ; w_ ðNÞ ¼ v2z z¼0 ;
ð2Þ
where w_ ð1Þ and w_ ðNÞ are the deflections of the boundary planes of the 1st and ½N 1th layers, respectively.
250
V. N. Paimushin and R. K. Gazizullin
The process of dynamic deformation of a plate is described by the equations of the multilayer plate theory taking into account transverse shear and transverse compression in each layer obtained in [6]. The internal friction of the material in each layer of the plate is taken into account according to the Kelvin–Voigt hysteresis model. For such a ½k ½k ½k ½k model, the stresses raa ; rab ; a 6¼ b; a ¼ 1; 3; b ¼ 1; 3 and strains ea ; cab arising in the plate can be connected by the relationships (da and dab are logarithmic decrements of vibrations under axial and shear deformations, respectively; s is time): ½k ½k
½k ½k
½k ½k
k r½aa ¼ ~ga1 e1 þ ~ga2 e2 þ ~ga3 e3 ;
½k ~ ½k c½k ; rab ¼ G ab ab
where ! ! k ½k ½k ~ 1½k 1 m½23 E m32 d d½ak @ @ ½k ~ ½k ¼ G½k 1 þ ab ~11 ¼ 1þ ; ; G ; g ab ab px @s px @s D½k
~ a½k ¼ Ea½k E
g12[ ] = k
E1[
k]
(ν [ ] +ν [ ]ν [ ] ) ; k 21
Δ
k 23
k 31
[k ]
k k [k ] [k ] [k ] ν 32 −ν 31[ k ]ν 13[ k ] − 2ν 12[ k ]ν 23[ k ]ν 31[ k ] . −ν 23 1, 2,3, Δ[ ] = 1 −ν 12[ ]ν 21
ðk Þ
ðk Þ
The components of the displacements u1 ; u2 and wðkÞ of the points of ﬁrst and last layers’ front planes as well as the points of the conjugation planes of inner layers are accepted as unknowns. For the case of hinged support of the plate in the opening of an absolutely stiff dividing wall under the action of a monoharmonic sound pressure on it, for these functions we take the representations ðk Þ
u1 ¼ eixs w
ðk Þ
¼e
ixs
X m;n¼1;3;...
X
m;n¼1;3;...
ðk Þ
ðk Þ
~u1mn cos km x sin kn y; u2 ¼ eixs kÞ ~ ðmn w
X m;n¼1;3;...
ðk Þ
~ u2mn sin km x cos kn y;
sin km x sin kn y; km ¼ mp=a; kn ¼ np=b;
: ð3Þ
In view of the conditions of (2) and representations (3), for solutions of two latter Eqs. (1) representations have to be in the form Us ¼ eixs
X m;n¼1;3;...
~ mn ðzÞ sin km x sin kn y: U s
ð4Þ
Based on the accepted representations (3)–(4), the analytical solution to the formulated problem is found. This solution should be considered as exect for N ! 1; M ! 1. Thesolution found allows us to calculate the sound transmission loss R0p ¼ 20 lg~p2 jz¼0 ð~p þ ~p1 Þjz¼0 of the plate and determine the amplitude values of all stressstrain state parameters. Let us note that at ~ p ¼ 0 the formulated problem
The Transmission of an Acoustic Wave Through a Composite Plate
251
becomes homogeneous. Its solution determines the eigenfrequencies and the corresponding eigenmodes of vibration for the hingedly supported composite plate, taking into account the internal energy dissipation in the plate material and its aerodynamic interaction with surrounding acoustic media.
3 Calculation Results and Their Analysis On the basis of the solutions found, studies of a rectangular composite plate of thickness t ¼ 3 mm, length a ¼ 480 mm and width b ¼ 560 mm, made of carbon ﬁber textile Porcher 3692 and a binder EDT69NM were carried out. Such material under dynamic deformation processes has the following mechanical characteristics and logarithmic decrements of vibrations [7]: E1;d ¼ E2;d ¼ 40 GPa, E3;d ¼ 5:9 GPa, G12;d ¼ G13;d ¼ G23;d ¼ 4 GPa, m12 ¼ 0:163; m13 ¼ m23 ¼ 0:3; q ¼ 1500 kg/m3, d1 ¼ d2 ¼ d3 ¼ 0:012, d12 ¼ d13 ¼ d23 ¼ 0:03. The plate is surrounded on both sides by air characterized by the parameters q1 ¼ q2 ¼ q ¼ 1:225 kg/m3, c1 ¼ c2 ¼ c ¼ 340 m/s. Table 1 represents the results of the calculation of the real parts of eigenfrequencies fmn ¼ xrmn ð2pÞ (here xrmn is the real part of the circular frequency) for the hingedly supported composite plate taking into account the internal energy dissipation. Furthermore, the parameters nmn characterizing the imaginary parts of the complex vibration frequencies determined by the formula nmn ¼ ximn xrmn (ximn is the imaginary part of the circular frequency) are also presented in the table. Let us note that the results are given for a plate in vacuum, i.e. excluding interaction with acoustic media. Such results, as was shown in [8], practically do not differ from the results obtained by taking into account the influence of acoustic media, if the behavior of the media is described on the basis of threedimensional wave equations. Table 1. Real parts of eigenfrequencies fmn and the parameters nmn of the composite plate. No of tone fmn , Hz
nmn
M n
1 2 3 4 5 6 7 8 9 10
0,0023 0,00219 0,00209 0,00231 0,00207 0,00229 0,002 0,00219 0,00201 0,00232
1 1 2 2 1 2 3 3 1 3
44,4 105,81 133,314 177,465 217,008 273,609 286,483 321,336 374,493 398,778
1 2 1 2 3 3 1 2 4 3
To establish the effect of the incident sound wave frequency on the sound transmission loss and the characteristics of stressstrain state of the plate, computational experiments were also carried out. The data in Fig. 1a illustrates dependence of the
252
V. N. Paimushin and R. K. Gazizullin
sound transmission loss R0p values in the center of the plate at frequency f ¼ x=ð2pÞ. ~ show the dependence Moreover, Fig. 1b and 1c on a logarithmic scale along the axis r ~11 (line 1 in Fig. 1b and 1c), of the maximum amplitude values of the normal stresses r ~33 (line 2 in Fig. 1b) and tangential stresses r ~13 (line 3 in Fig. 1c) on the frequency f . r As is seen, there are frequencies f R of sound wave at which signiﬁcant drop in sound ~11 and r ~13 arise. By transmission loss R0p as well as signiﬁcant splashes of stresses r R comparing such frequencies f obtained through analysis of Fig. 1 with the data represented in the Table 1 we can see that in case of a plane sound wave action, the plate exhibits forced vibrations only with resonant frequencies corresponding to the eigenmodes with odd numbers of harmonics m and n in each direction. Along this, the harmonics with even number at least in one direction, do not objectify.
a
b
c
~11 , r ~33 and r ~13 (b, c) on Fig. 1. Dependences of sound transmission loss R0p (a) and stresses r frequency.
It is important to note that at low frequencies of the sound wave, the main in the plate are the tangential components of the stress tensor (~ r33 values are by three orders ~11 values) and the description of the dynamic stressstrain state of magnitude less than r
The Transmission of an Acoustic Wave Through a Composite Plate
253
of the plate by classical twodimensional equations of plate theory is quite acceptable. ~33 formed in the plate are of the same magHowever, at high frequencies, stresses r ~11 (~ ~11 values). Furthermore, stresses r ~33 nitude as stresses r r33 values is 25 30% of r ~11 values in narrow frequency ranges in the spectrum of medium can even exceed the r and high frequencies. Consequently, a correct description of the plate deformation mechanics at high frequencies setting the problem of the class in question is possible only on the basis of reﬁned equations with the necessary allowance for transverse compression. This is especially important studying the acoustic effects on thinwalled structural elements made of ﬁbrous reinforced composite materials. Such materials, as a rule, have elastic and strength characteristics in the transverse direction on several orders of magnitude less than similar characteristics in the tangential directions. It also ~13 ¼ r ~13 ð f Þ and r ~11 ¼ r ~11 ð f Þ have the should be noted that the obtained dependences r same character of change (Fig. 1c). The analysis of the calculation results showed that ~13 values of shear stresses are an order of magnitude less than the the maximum r ~11 values of stresses. maximum r Acknowledgment. This research was supported by a grant from the Russian Science Foundation (project № 191900058).
References 1. Pretlove, A.J.: Free vibrations of a rectangular panel backed by a closed rectangular cavity. J. Sound Vib. 2(3), 197–209 (1965) 2. Pretlove, A.J.: Forced vibrations of a rectangular panel backed by a closed rectangular cavity. J. Sound Vib. 3(3), 252–261 (1966) 3. Jeyaraj, P., Ganesan, N., Padmanabhan, C.: Vibration and acoustic response of a composite plate with inherent material damping in a thermal environment. J. Sound Vib. 320(1), 322– 338 (2009) 4. Li, X., Yu, K., Han, J., Song, H., Zhao, R.: Buckling and vibroacoustic response of the clamped composite laminated plate in thermal environment. Int. J. Mech. Sci. 119, 370–382 (2016) 5. D’Alessandro, V., Petrone, G., Franco, F., De Rosa, S.: A review of the vibroacoustics of sandwich panels: models and experiments. J. Sandwich Struct. Mater. 15(5), 541–582 (2013) 6. Paimushin, V.N., Gazizullin, R.K.: Static and monoharmonic acoustic impact on a laminated plate. Mech. Compos. Mater. 53(3), 283–304 (2017) 7. Paimushin, V.N., Firsov, V.A., Gyunal, I., Shishkin, V.M.: Identiﬁcation of the elastic and damping characteristics of carbon ﬁberreinforced plastic based on a study of damping flexural vibrations of test specimens. J. Appl. Mech. Tech. Phys. 57(4), 720–730 (2016) 8. Paimushin, V.N., Tarlakovskii, D.V., Firsov V.A., Gazizullin, R.K.: Free and forced bending vibrations of a thin plate in a perfect compressible fluid with energy dissipation taken into account. Zeitschrift für Angewandte Mathematik und Mechanik, e201900102 (2020)
Vibration of the Plate with Integral Layer Damping: Experimental and Theoretical Studies V. N. Paimushin1,2 , V. A. Firsov1 , V. M. Shishkin3 and R. K. Gazizullin1(&)
,
1
Kazan National Research Technical University named after A. N. Tupolev  KAI, Kazan, Russia [email protected], [email protected] 2 Kazan Federal University, Kazan, Russia 3 Vyatka State University, Kirov, Russia
Abstract. The paper discusses the classical methods of surface damping of bending vibrations in thinwalled structures. Furthermore, the perspective integral version of a damping coating has been proposed. Such coating consists of two layers of material with pronounced viscoelastic properties with a thin reinforcing layer of high modulus material between them. Dynamic tests of cantilevered duralumin specimens under the damped bending vibrations were carried out using the created experimental setup. The purpose of these tests is to compare the effectiveness of the known and proposed methods of surface vibration damping. The influence of aerodynamic drag forces on the vibration damping of specimens is noted. A reﬁned ﬁnite element model of an elongated plate with an integral layer damping is constructed on the basis of the fourlayer ﬁnite element. This model allows taking into account the effect of transverse compression of damping layers under highfrequency deformation. The analysis of the stressstrain state of the damping layers of a simply supported elongated plate under resonance vibrations in several lower eigenmodes has been carried out. The analysis showed a signiﬁcant increase in the transverse compression stresses of the damping layers with frequency increasing. Keywords: Plate Damping coating Experiment Logarithmic decrement of vibrations Finite element model
1 Introduction Traditional structural materials (metals and metal alloys) are characterized by large values of elastic and strength parameters, but, as a rule, they have low damping properties. In this connection, various types of coatings made of viscoelastic materials [1–3] are used to reduce the vibration activity and dynamic stress of thinwalled structures. The relevance of the problem and the constant attention of researchers to it are reflected in the fundamental monograph [4]. In this monograph authors discuss the
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 254–260, 2020. https://doi.org/10.1007/9783030478834_46
Vibration of the Plate with Integral Layer Damping
255
effect on damping of various physical factors such as temperature, vibration frequencies, layer thicknesses, loading level, etc. The results of these studies formed the basis of the American standard for an experimental method of material damping properties measurement [5]. According to [4], surface damping devices are divided into two classical methods depending on the dominant deformations in the damping layer. The ﬁrst method is the freelayer damping. In accordance with this method, the damping layer of the viscoelastic material is ﬁxedly connected to the damped thinwalled structure. In this case the bending under transverse vibrations causes cyclic tensilecompression deformations in the damping layer. However, this damping method has a very low efﬁciency [4], as the damping forces are maximum only in the areas of greatest curvature of the damping layer. The second method is constraining damping layer. In accordance with this method the layer of damping material is additionally covered with a thin reinforcing layer which under cyclic bending of the structure mainly experiences transverse shear deformations. In this case, the maximum damping forces arise only in the areas of the maximum shift of the damping layer. Therefore this method does not allow you to effectively damp vibrations throughout the design area. In view of this, the integral damping coating consisting of two viscoelastic layers with thin reinforcing layer of high modulus material between them (Fig. 1a) seems more effective. In case of bending vibrations of a thinwalled structure the lower layer of the damping coating undergo a shear and acts as a constraining layer damping, and the upper layer undergo tensilecompression deformations and acts as a free damping layer (Fig. 1b). This allows you to integrate the area of active vibration damping, practically getting rid of the ballast coating areas for any form of bending vibrations in a wide range of operating frequencies. So, for the simply supported beam under second bending vibrations mode the active damping regions (marked in dark on the ﬁgure) cover almost the entire surface of the damped structure (Fig. 1c). Moreover, the outer layer protects the thin reinforcing layer from buckling and delamination in the phase of cyclic compression of bending vibrations, as such destruction is possible in the reinforcing layer in case of the use of constraining layer damping method. In turn, the presence of a thin reinforcing layer having an insigniﬁcant mass and bending stiffness practically does not increase the weight characteristics of the damping coating and does not reduce the possibility of the proposed method using for damping of curved surfaces structures.
(a)
(b)
(c)
Fig. 1. The physical picture of surface vibration damping of the structure with an integral damping coating. (a) shows an undeformed state; (b) shows an deformed condition; (c) illustrates active damping areas.
256
V. N. Paimushin et al.
2 Experimental Studies Dynamic tests of cantilevered duralumin specimens under the damped bending vibrations were carried out using the created experimental setup [6]. The purpose of these tests is to compare the effectiveness of the known and proposed methods of surface vibration damping. Some calculation results for specimens with lengths of 500 (a), 300 (b) and 200 (c) mm are shown in Fig. 2 as relations between the logarithmic decrements of vibration d(A) and the vibration amplitude A of specimens’ free ends. Here, line 1 correspond to basic specimens without a damping coating; line 2 correspond to specimens with a free layer damping; line 3 correspond to specimens with constraining layer damping; line 4 correspond to specimens with integral layer damping. In order to more contrastly evaluate the effectiveness of the studied damping coatings, they were applied on both sides of the basic specimens. An oilresistant rubber with a low static elastic modulus E 5.3 MPa and manufactured in the form of plates 2H1MBSS (GOST 733890) with a thickness of 1.8 mm and a density of q = 1345 kg/m3 was used as a damping material. The damping properties of rubber are characterized by logarithmic decrements of vibration d 1.2.
Fig. 2. Relation dð AÞ. Explanations in the text.
The above results indicate that in all the cases considered, the effectiveness of the proposed integral method of vibration damping is higher than the most effective of the previously known methods by an average of 20% even under conditions of the lowest modes of vibration. We should note that, in addition to the damping properties of the material, dependence d(A) can be signiﬁcantly affected by the air drag [6]. For duralumin basic specimens the aerodynamic component of damping is approximately 85– 90% of the total (experimental) logarithmic decrements of vibration [7]. For specimens with a damping coating this effect becomes signiﬁcantly less. The calculations showed that for specimens with a free layer damping the aerodynamic component of the damping does not exceed 12% of the total logarithmic decrements of vibration (at the maximum amplitude of oscillations). Moreover, for specimens with a constraining and integral layer damping this component becomes even signiﬁcantly smaller.
Vibration of the Plate with Integral Layer Damping
257
3 Reﬁned Finite Element Model of an Elongated Plate with Integral Layer Damping Under static and lowfrequency deformations of a plate with an integral damping coating, one can adopt the classical model in which the constraining layer is in a state of homogeneous transverse shear and the free layer is in a state of inhomogeneous tensioncompression. However, in case of resonant vibrations at higher frequencies, the stressstrain state of the damping layers can be qualitatively different due to the influence of inertia forces on it. This leads to the necessity of taking into account all components of the stress state when determining the energy dissipation in damping layers. To analyze the stressstrain state of the marked layers under cyclic deformation in a wide frequency range, a reﬁned ﬁnite element model of an elongated plate with an integral layer damping is constructed. This model is based on the developed fourlayer compound ﬁnite element (Fig. 3) and uses the following models to describe the mechanics of layer deformation: the plate undergo a tensioncompression and bending; both damping layers are in a plane stress state; the reinforcing layer undergo a tensioncompression only. Independent nodal parameters of the element are displacements ui ; wi (i ¼ 1; 2; . . .; 6) as well as rotation angles /1 ; /4 of the cross sections of layer 1. They can be represented by a vector rðeÞ ¼ fu1 w1 u1 u2 w2 u3 w3 u4 w4 u4 u5 w5 u6 w6 g.
Fig. 3. The ﬁnite element of the elongated plate with integral layer damping.
The elastic and damping properties under cyclic deformation of the damping layer material are taken into account by the physical dependence r ¼ De þ Dg e_
ð1Þ
representing a generalization of the wellknown KelvinVoigt model under tensioncompression of the material in the case of a complex stress state. Vectors r, e contain components of the stress and strain states; D, Dg are the stiffness matrix and the matrix
258
V. N. Paimushin et al.
of viscous damping of the material, respectively. For an isotropic viscoelastic material in a plane stress state, the matrices D and Dg will be as follows: 2
3 E ð1 m2 Þ Em ð1 m2 Þ 0 D ¼ 4 Em ð1 m2 Þ E ð1 m2 Þ 0 5; Dg 0 G 2 0 3 2 Ed Þ Ede m ð1 m2 Þ 0 ð1 m e 1 4 ¼ Ede m ð1 m2 Þ Ede ð1 m2 Þ 0 5 px 0 0 Gdc Here E, G, de , dc are the dynamic moduli of elasticity and the logarithmic decrements of vibrations of the material, respectively, under tensioncompression and shear, x is the deformation frequency, m is the Poisson’s ratio. In the dynamic analysis of structures based on the FEM, usually, the task is to synthesize elastic, damping and inertial forces, which requires stiffness matrices KðeÞ , damping matrices CðeÞ and mass matrices MðeÞ constituting the ﬁnite element structure. To construct the matrices KðeÞ и CðeÞ we used dependence (1) and geometric relations which connect deformations e with the vector of nodal displacements rðeÞ of the ﬁnite element. To construct the matrix MðeÞ , we supposed that the kinetic energy of an _ element is determined only by the velocities w. For numerical experiments, we chose an elongated simply supported plate with an integral damping coating. Geometrical parameters of the plate are following: length L = 200 mm; width b = 20 mm; thickness h1 = 1 mm. The thickness of the damping layers are h2 = h4 = 1.8 mm. The reinforcing layer has a thickness h3 = 0.1 mm. The plate material is aluminum alloy D16AT with a dynamic elastic modulus E = 5.54 104 MPa and density q = 2700 kg/m3. The material of the damping layers is technical rubber. Dynamic elasticity moduli of rubber under tensioncompression and shear are E = 20.1 MPa, G = 2.6 MPa. Density of rubber is q = 1345 kg/m3, logarithmic decrement of vibrations under tensilecompression and shear are de = 1.2, dc = 1.1, respectively. The reinforcing layer is made of unidirectional ﬁber composite based on carbon tape ELURP and binder HT118 (dynamic elastic modulus E = 10.5 104 MPa, density q = 1200 kg/m3). The plate is divided into 100 ﬁnite elements of the same length. We studied stressstrain state of damping layers under resonance vibrations of a plate by several lower eigenmodes with an amplitude of the normal coordinate q0 ¼ 0:01. Figure 4 and 5 illustrates the amplitudes of the normal and shear stresses rx ; rz and sxz in the middle surface of the constraining and free damping layers, respectively, under resonance vibrations of the plate by the ﬁrst, ﬁfth, and seventh modes. The frequencies corresponding to these modes were as follows: f1 = 69.43 Hz; f5 = 856.43 Hz; f7 = 1588.66 Hz.
Vibration of the Plate with Integral Layer Damping
259
Fig. 4. Stresses in a constraining damping layer under resonance vibrations of the plate by the ﬁrst (a), ﬁfth (b) and seventh (c) modes.
Fig. 5. Stresses in a free damping layer under resonance vibrations of the plate by the ﬁrst (a), ﬁfth (b) and seventh (c) modes.
An analysis of the obtained stresses shows that the transverse shear stresses sxz dominate (Fig. 4a) in the constraining damping layer when the plate vibrates in the ﬁrst (main) mode as well as only normal stresses rx mainly act (Fig. 5a) in the free damping layer. As the shape number and, correspondingly, the frequency f increase, stresses rx ; rz increasing appear against the background of stresses sxz in the constraining damping layer. Thus, on the seventh mode (Fig. 4c) stress rx is approximately 65% of the sxz value and stress rz even slightly exceeds the shear stress sxz . With increasing frequency f in the free damping layer (Fig. 5) in addition to stress rx two other stresses rz and sxz appear, of which the stress rz is the most signiﬁcant. Acknowledgment. This research was supported by a grant from the Russian Science Foundation (project № 191900058).
References 1. Oberst, H., Becker, G.W., Frankenfeld, K.: Über die Dampfung der Biegeschwingunden dunner Bleche durch fest haftende Belage. Acustica 4(2), 181–184 (1952) 2. Kerwin, E.M.: Damping of flexural waves by a constrained viscoelastic layer. J. Acoust. Soc. Am. 31(7), 952–964 (1959) 3. Ross, D., Ungar, E.E., Kerwin, E.M.: Damping of plate flexural vibrations by means of viscoelastic laminate. In: Structural Damping. Section 3, pp. 49–88. ASME, New York (1959)
260
V. N. Paimushin et al.
4. Nashif, A.D., Johnes, D.I.G., Henderson, J.P.: Vibration Damping. Wiley, New York (1984) 5. ASTM E75605: Standard test method for measuring vibrationdamping properties of materials. S. I.: ASTM Intern. (2017) 6. Paimushin, V.N., Firsov, V.A., Gyunal, I., Egorov, A.G.: Theoreticalexperimental method for determining the parameters of damping based on the study of damped flexural vibrations of test specimens. 1. Experimental basis. Mech. Compos. Mater. 50(2), 127–136 (2014) 7. Paimushin, V.N., Firsov, V.A., Gyunal, I., Shishkin, V.M.: Theoreticalexperimental method for evaluating the elastic and damping characteristics of soft materials based on studying the resonance flexural vibrations of test specimens. Mech. Compos. Mater. 52(5), 571–582 (2016)
Thermomagnetoelectroelasticity of Bimaterial Solids with High Temperature Conducting Interface and Thin Internal Inhomogeneities Andrii Vasylyshyn1(&) , Iaroslav Pasternak2 and Heorhiy Sulym3
,
1
Ivan Franko National University of Lviv, Universytetska Str. 1, Lviv 79000, Ukraine [email protected] 2 Lutsk National Technical University, Lvivska Str. 75, Lutsk 43018, Ukraine [email protected] 3 Pidstryhach Institute for Applied Problems of Mechanics and Mathematics of NASU, Naukova Str. 3b, Lviv 79060, Ukraine [email protected] Abstract. This work studies the problem of a thermomagnetoelectroelastic anisotropic bimaterial with imperfect high temperatureconducting coherent interface, which components contain thin inclusions. Using the extended Stroh formalism and complex variable calculus the Somigliana type integral formulae and corresponding boundary integral equations for the anisotropic thermomagnetoelectroelastic bimaterial with high temperatureconducting coherent interface are obtained. These integral equations are introduced into the modiﬁed boundary element approach. The numerical analysis of new problems is held and results are presented. Keywords: Bimaterial Thermomagnetoelectroelasticity Boundary element method Coherent imperfect interface
Thin inclusion
1 Introduction Modern advanced hightech industries, especially precision mechanics, are increasingly using multiﬁeld (thermomagnetoelectoelastic) materials in the manufacture of various devices. The latter are smart composites based on the mechanical combination of pyroelectric (ferroelectric) and magnetostrictive (piezomagnetic) materials. When creating such materials, a thin intermediate layer is usually formed that affects the stress and temperature ﬁelds. The influence of this layer is reduced to the conditions of imperfect thermal and magnetoelectromechanical contact of the bimaterial components. In general, in the scientiﬁc literature [1, 2] there are two types of imperfect thermal conditions and two types imperfect mechanical conditions of contact of a thin layer with the medium. Thus, there arises the scientiﬁc problem of development integral mathematical models and methods of analysis of bimaterial thermomagnetoelectroelastic solids, which can contain both defects of structure and purposefully introduced thin layers that change the properties of these bodies. © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 261–267, 2020. https://doi.org/10.1007/9783030478834_47
262
A. Vasylyshyn et al.
At present, methods of analyzing the interaction of mechanical, electrical and magnetic ﬁelds in anisotropic smart materials are intensively being developed. An effective method for solving such problems is an approach based on methods of the complex variable function theory and the Stroh formalism. Thus, in [3], the Somigliana type boundary integral equations along with the explicit closed form of expressions for the kernels were obtained and for the boundary element analysis of the anisotropic thermoelectroelastic bimaterial with holes, cracks and thin inclusions. This approach was also applied in [4] for a bimaterial solid with a Kapitsa type interface. The paper [5] obtained a twodimensional Green’s function for anisotropic bimaterials with imperfect thermal and springtype mechanical contact. In this work a mathematical model of a thermomagnetoelectroelastic bimaterial solid with high temperature conductive coherent interface, which parts can contain thin deformable inclusions, is developed. The boundary integral equations of the formulated problem are constructed in a closed form. The boundary element method for their fast and accurate numerical solution is developed.
2 Governing Equations of Thermomagnetoelectroelasticity In a ﬁxed rectangular system of coordinates Ox1 x2 x3 the balance equations for stress, electric displacement, magnetic induction and heat flux, and constitutive laws in absence of volumetric loading can be written in the following compact form ~ ijkm ~uk;jm þ ~fi ¼ 0; ~ij;j þ ~fi C r ~ h; ~ ijkm ~uk;m b ~ij ¼ C r ij
hi;i fh ¼ 0;
hi ¼ kij h;j :
ð1Þ ð2Þ
The nomenclature is the same as in Refs. [3, 4]. According to the extended Stroh formalism, the general homogeneous solution of Eqs. (1) and (2) can be expressed in terms of complex analytic functions as follows h ¼ 2Refg0 ðzt Þg; # ¼ 2kt Im fg0 ðzt Þg
ð3Þ
~ ¼ 2Re½Bfðz Þ þ dgðzt Þ; ~ ¼ 2Re½Afðz Þ þ cgðzt Þ; u u
ð4Þ
f ðz Þ ¼ ½F1 ðz1 Þ; F2 ðz2 Þ; F3 ðz3 Þ; F4 ðz4 Þ; F5 ðz5 ÞT :
ð5Þ
~ is where # is a heat flux function; h is a change in temperature compared with actual; u ~ is an extended stress function; gðzt Þ and Fa ðza Þ are an extended displacement vector; u complex analytic functions with respect to their arguments.
Thermomagnetoelectroelasticity of Bimaterial Solids
263
Based on Eqs. (3), (4) one can derive the following relation between the function gðzt Þ and temperature and heat flux function: g0 ð z t Þ ¼
1 # hþi : 2 kt
ð6Þ
3 Problem Statement Consider an anisotropic bimaterial medium consisting of two thermomagnetoelectroelastic anisotropic halfspaces x1 [ 0 and x2 \0 (which in terms of 2D problem are modeled as two halfplanes S1 ðx1 [ 0Þ and S2 ðx2 \0Þ as depicted in Fig. 1), and which are connected along the boundary x2 ¼ 0. On the boundary, the conditions of imperfect thermal contact are satisﬁed, and can be written as follows: #ð1Þ ðx1 ; x2 Þx2 ¼0 ¼ #ðx1 Þ þ l0 h;1 ðx1 Þ; 8x2 ¼ 0; #ð2Þ ðx1 ; x2 Þx2 ¼0 ¼ #ðx1 Þ; hð1Þ ðx1 ; x2 Þ
x2 ¼0
¼ hð2Þ ðx1 ; x2 Þ
x2 ¼0
¼ hðx1 Þ;
where l0 is constant thermal conductivity of the interface.
Fig. 1. The sketch of the problem
ð7Þ ð8Þ
264
A. Vasylyshyn et al.
Also, the conditions of perfect mechanical contact of bimaterial components at the interface are as follows: ~ð2Þ ðx1 ; x2 Þx ¼0 ¼ u ~ðx1 Þ; 8 x2 ¼ 0 ~ð1Þ ðx1 ; x2 Þx ¼0 ¼ u u 2 2
~ ð1Þ ðx1 ; x2 Þ u
x2 ¼0
~ ð2Þ ðx1 ; x2 Þx ¼0 ¼ u ~ ðx1 Þ; 8 x2 ¼ 0: ¼ u 2
ð9Þ ð10Þ
Here, indices (1) and (2) are used to denote the magnitudes of the ﬁelds acting in halfspaces S1 and S2 respectively. It is considered that each of the halfspaces contains S ð1Þ S ð2Þ a system of smooth closed contours C1 ¼ i Ci and C2 ¼ i Ci on which we can set different thermal or mechanical and electric conditions. To derive integral formulas of Stroh complex potentials, the Cauchy integral formula is used [5]: 1 2pi
Z @S
/ðsÞds ¼ sz
/ðzÞ 0
8z 2 S; 8z 62 S:
ð11Þ
It relates values of an arbitrary analytic function /ðsÞ at the boundary @S of the domain S with its value /ðzÞ inside this domain. Here s; z 2 C are complex variables, which deﬁne the position of the source and ﬁeld points, respectively. Herewith, if the domain S is inﬁnite it is assumed that the function /ðsÞ vanishes at z ! 1. ðiÞ
Thus, the expressions for complex temperature functions g0i zt
can be written as
follows: Z g0 sð1Þ dsð1Þ Zþ 1 g0 xð1Þ dxð1Þ t t t 1 1 1 1 1 ð1Þ ð1Þ þ ; 8 Im zt ¼ [ 0; g01 zt ð1Þ ð1Þ ð1Þ ð1Þ 2pi 2pi st z t x 1 zt C
Z g0 sð2Þ dsð2Þ Zþ 1 g0 xð2Þ dxð2Þ t t t 2 2 1 1 1 ð2Þ ð2Þ þ ; 8 Im zt \0 ¼ g02 zt ð2Þ ð2Þ ð2Þ ð2Þ 2pi 2pi st z t x1 z t C
ð12Þ
1
ð13Þ
1
ðiÞ Similarly, the expressions for the vectors of Stroh complex potentials f ðiÞ z can be written. The procedure of obtaining boundary integral equations of the problem is in elimination of integral over the interface, which is done using complex variable calculus.
Thermomagnetoelectroelasticity of Bimaterial Solids
265
4 Numerical Examples Using the obtained Somigliana type integral formulae incorporated with the boundary element approach [4] consider several problems for a thermoelectroelastic bimaterial with imperfect thermal and perfect electromechanical contact of its components. The considered material contains internal thin inclusion. Only 20 threenode boundary elements, including two special tip elements, were used to mesh the inclusion. Consider a thermoelastic anisotropic bimaterial consisting of two halfplanes. It contains a rectilinear isotropic thermally insulated deformable permeable inclusion of length 2a. It is not subject to thermal deformation and it does not undergo thermal expansion. It is located in halfplane x2 \0 at a distance d parallel to the interface. The thickness of inclusion is h ¼ 0:01a. The relative rigidity of inclusion is k ¼ Gi =C11 , where Gi is inclusion shear modulus and C11 is material 2 elastic moduli. Halfplane x2 [ 0 contains two heat sources of equal intensity. They are located at a distance d0 to the boundary. Figure 2 and Fig. 3 show the relationship between the generalized stress intensity factors (SIF) and the parameter of thermal conductivity of the interface l0 ; ðl0 ¼ ak11 Þ when the relative rigidity is k ¼ 1010 . Figure 2 illustrates the case when bimaterial components are made of different materials. Namely, component x2 [ 0 is made of BaTiO3 and component is x2 \0 made of CdSe. Figure 3 illustrates the case when bimaterial components are made of BaTiO3, and have the same properties.
Fig. 2. The relationship between SIF K21 =K0 (a), K11 =K0 (b) and l0 =l0
266
A. Vasylyshyn et al.
Fig. 3. The relationship between SIF K21 =K0 (a), K11 =K0 (b) and l0 =l0
5 Conclusions This paper extends the possibilities of an approach, methods of the theory of function of complex variable and Stroh formalism, to obtain integral formulas and equations for structurally heterogeneous bimaterial solids with imperfect thermal contact of its components. A mathematical model of a thermomagnetoelectroelastic bimaterial solid with a high thermal conductivity interface and perfect electromagnetomechanical contact of components, which in turn can contain thin deformable inclusions, is developed. In closed form, the boundary integral equations of the formulated problem are constructed, as well as the boundary element method, which makes it possible to solve it effectively(accurate and fast). All this makes it possible to solve with high precision the problems of thermomagnetoelectroelasticity for bimaterial solids with hightemperature conductivity interface containing thin ribbonlike deformable inclusions or cracks that have not yet been achieved using traditional numerical approaches, including boundary or ﬁnite element methods.
References 1. Kaessmair, S., Javili, A., Steinmann, P.: Thermomechanics of solids with general imperfect coherent interfaces. Arch. Appl. Mech. 84(9–11), 1409–1426 (2014) 2. Benvensite, Y.: A general interface model for a threedimensional curved thin anisotropic interface between two anisotropic media. J. Mech. Phys. Solids 54, 708–734 (2006) 3. Pasternak, I., Pasternak, R., Sulym, H.: Boundary integral equations and Green’s functions for 2D thermoelectroelastic bimaterial. Eng. Anal. Boundary Elem. 48, 87–101 (2014)
Thermomagnetoelectroelasticity of Bimaterial Solids
267
4. Pasternak, I., Pasternak, R., Sulym, H.: 2D boundary element analysis of defective thermoelectroelastic bimaterial with thermally imperfect but mechanically and electrically perfect interface. Eng. Anal. Boundary Elem. 61, 194–206 (2015) 5. Wang, X., Pan, E.: Thermal Green’s functions in plane anisotropic bimaterials with springtype and Kapitzatype imperfect interface. Acta Mechanica et Automatica 209, 115–128 (2010)
Fracture of Composite Materials Under Compression Along Cracks Mykhailo Dovzhyk(&), Viacheslav Bogdanov, and Vladimir Nazarenko S.P. Timoshenko Institute of Mechanics, National Academy of Sciences of Ukraine, Nesterov Str. 3, Kyiv 01057, Ukraine [email protected]
Abstract. The axisymmetrical problems of fracture of bodies with nearsurface pennyshaped cracks and two parallel pennyshaped cracks under compressive loads directed along cracks are considered. In the situation examined the start of the process of material fracture is determined by the local loss of stability of the equilibrium of the material surrounding cracks. There are two approaches that are used to investigate such problems, namely, socalled “beam approximation” based on applied theories of mechanics of thinwalled structures and the approach in the framework of the rigorous threedimensional linearized theory of stability of deformable bodies. According to the second approach we reduce the problems to systems of integral Fredholm equations and then to system of algebraic linear equations with use the BubnovGalerkin method and numerically analytic technique. As an example we present the numerical calculation for a composite material. The values of critical loads corresponding to the start of fracture are obtained for small and large distance between the cracks (or between the crack and the body surface). Keywords: Composite materials cracks Parallel coaxial cracks
Compression along cracks Nearsurface
1 Compression Along Cracks Fracture of material at compression along cracks is one of the nonclassical problems of fracture mechanics. In this case, the classical approaches of fracture mechanics such as GrifﬁthsIrwin approach do not work. In this situation, destruction process is identiﬁed as the moment of local stability loss of the equilibrium of a part of material in the vicinity of cracks. Currently, there are two general approaches used to investigate such problems [1]. The ﬁrst of them is based on the use of approximate design diagrams and approximate theories of mechanics of thinwalled structures [2]. Within the framework of this approach, has the greatest application the “beam approximation”, when the part between the crack and the free surface (between the cracks) is replaced by a thinwalled element: beam, plate or shell, which are investigated in the framework of the applied theory of stability of thin systems. However, this method has signiﬁcant drawbacks: it is necessary to carry out separate investigations to determine the possibilities of its application depending on the distance between the cracks, but even having determined this distance, © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 268–272, 2020. https://doi.org/10.1007/9783030478834_48
Fracture of Composite Materials Under Compression Along Cracks
269
there remains the question of choosing the conditions for ﬁxing of thinwalled element. The second approach is based on the basic relationships and methods of rigorous threedimensional linearized theory of stability of deformable bodies for ﬁnite and small subcritical strains [3]. In [4] using the second approach the conditions of applicability of the “beam approximation” was found for isotropic elastic materials containing nearsurface cracks. It is interesting to ﬁnd such conditions for composite materials. 1.1
Problem Formulation
We considered two geometric schemes of cracks disposition in composites: a halfspace with pennyshaped crack of radius a which is situated in the plane x3 ¼ 0 with center on Ox3 (Fig. 1a) and unbounded body with two parallel pennyshaped cracks of radius a which are situated in the plane x3 ¼ 0 and x3 ¼ 2h with center on Ox3 (Fig. 1b). The initial stresses that operated along cracks correspond to biaxial uniform compression.
x3
x3
2h
r
a
r
h
a b) material with two parallel cracks
a) halfspace with a nearsurface crack
Fig. 1. Compression of cracked bodies along cracks
Within the limits of the second approach the both problems were reduced to the solution of system of integral Fredholm equations with a side condition [5] 1 f ðnÞ þ pk gðnÞ þ
1 pk
Z1 0
1 M1 ðn; gÞf ðgÞdg þ pk
Z1 M2 ðn; gÞgðgÞdg þ 0
1 pk
Z1 N1 ðn; gÞgðgÞdg ¼ 0; 0
Z1
~ 1 ¼ 0; N2 ðn; gÞf ðgÞdg þ C
0
Z1 gðnÞdn ¼ 0
ð0 n 1; 0 g 1Þ;
0
f ðnÞ uðanÞ;
gðnÞ wðanÞ:
ð1Þ
270
1.2
M. Dovzhyk et al.
Exploratory Procedure
We used the procedure based on the BubnovGalerkin method to solve integral Eqs. (1) and search of critical shortening and stress correspond to start of the fracture process. Power functions were used as a system of coordinate functions. For further calculations we use the numerical analytical procedure proposed in [4]. This procedure allows to obtain results for elastic materials. The procedure allows to calculate analytically the integrals for the chosen system of coordinate functions using a package of symbolic computations. It is allowed to achieve at the further numerical calculations higher exactitude of evaluations at the expense of a numerical integration lapse exclusion. The recurrence relations were used to accelerate of integrals solutions. Using the method offered in [4], Fredholm integral Eqs. (1) for both problems was transformed to systems of the equations with corresponding factors F1ji , G1ji and ~ 1 , i; j 2 ½0; N. variables Fi , Gi , C N X
Fi F1ji þ
N X
i¼0 N X i¼0
Fi F2ji þ
Gi G1ji ¼ 0;
i¼0 N X
~ 1 ¼ 0; Gi G2ji þ C
ð2Þ
i¼0
N X 1 Gi ¼ 0; 0 j N: i þ 1 i¼0
1.3
Results
Table 1. Critical compressive stress for small dimensionless distance between a crack and free surface in halfspace with pennyshaped crack. b 1 1 1 1 1 1
−2
10 10−3 10−4 10−5 10−6 10−9
Critical compressive stress (r011 =E) A
−1.268 10−4 −1.290 10−6 −1.287 10−8 −1.285 10−10 −1.1284 10−12 −1.284 10−18
−1.268 −1.290 −1.287 −1.285 −1.284 −1.284
Fracture of Composite Materials Under Compression Along Cracks
271
Table 2. Critical compressive stress for small dimensionless distance between cracks in material with two parallel cracks. b 1 1 1 1 1 1
10−2 10−3 10−4 10−5 10−6 10−9
Critical compressive stress (r011 =E) A
A
−5.01367 −5.16309 −5.15527 −5.14160 −5.13770 −5.13672
−1,25342 −1,29077 −1,28882 −1,28540 −1,28443 −1,28418
10−4 10−6 10−8 10−10 10−12 10−18
−5.01367 −5.16309 −5.15527 −5.14160 −5.13770 −5.13672
As an example, we considered a laminate composite with isotropic layers. In macrovolumes such composite may be considered as transverselyisotropic medium. In the case considered, cracks are located in plane x3 ¼ const, parallel to interface boundary of layers. Dependence of critical dimensionless compressive stress r011 =E on ratio of the dimensionless distance between a crack and free surface b ¼ h=a are given in Figs. 2, Table 1 and Table 2 (for m ¼ m1 ¼ m2 , ﬁber concentration c1 is 0.7 and ﬁber aspect ratio is 10).
a)
0.1
0.1

11
0/E

11
0/E
0.08
0.08
0.06
0.06
0.04
0.04
0.02
0.02
β
0 0.1
0.6
1.1
1.6
2.1
β
0 0.1
0.6
1.1
1.6
2.1
2.6
2.6
a) a halfspace with nearsurface crack
b) a body with two parallel cracks
Fig. 2. Dependence of critical dimensionless compressive stress on ratio of the dimensionless distance between the crack and free surface of composite
For both problems the critical values of r011 =E at b ! 1 go asymptotically to values 0.0965, which are equal to respective critical values at surface instability of halfspace. For a thin plate critical stress can be found as rcr ¼ Acr b2 . For small dimensionless distance between the crack and the free surface the values of coefﬁcient A are presented in Table 1 and Table 2. At both case b ¼ h=a. For nearsurface crack h is three distance between crack and free surface – plate thickness in the “beam approximation”. For material with two cracks h is the halfdistance between cracks – half of plate thickness in the “beam approximation”. For a thin plate we can found critical stress as
272
M. Dovzhyk et al.
rcr ¼ Acr t2 =a2 , where t is thickness of plate. At the case of nearsurface crack Acr ¼ Acr , for material with two parallel crack Acr ¼ Acr =4 (A in Table 2). Values of A for halfspace with nearsurface crack are given in Table 1 and values of A for material with two parallel crack at b ! 0 go to same value −1.284. Critical compressive stress was obtained for composite materials for large and small distances between the crack and free surface (between cracks). Analysis of the results allows to determine the conditions of applicability of the “beam approximation”. Beam approximation good work for small distance between the crack and the free surface (when b \ 0:01 computing error less than 1%) and bad work in else case (when b [ 0:1 computing error more than 5%).
References 1. Guz, A.N.: Establishing the foundations of the mechanics of fracture of materials compressed along cracks (review). Int. Appl. Mech. 50, 1–57 (2014) 2. Obreimoff, I.W.: The splitting strength of mica. Proc. R. Soc. London 127, 290–297 (1930) 3. Guz, A.N.: On one criterion of fracture of solids in compression along the cracks. Plane problem. Docl. Akad. Nauk SSSR. 259, 1315–1318 (1980). (in Russian) 4. Guz, A.N., Dovzhik, M.V., Nazarenko, V.M.: Fracture of a material compressed along a crack located at a short distance from the free surface. Int. Appl. Mech. 47(6), 627–635 (2011) 5. Guz, A.N., Nazarenko, V.M.: Mechanics of fracture of materials in compression along the cracks (review) highly elastic materials. Sov. Appl. Mech. 25(9), 3–32 (1989)
Development of Welded Elements of the Railway Freight Car Bogie with Increased Characteristics of Fatigue Resistance and Survivability L. Lobanov, O. Makhnenko(&), A. Pustovoy, and S. Solovey E.O. Paton Electric Welding Institute, NAS of Ukraine, Kiev, Ukraine [email protected]
Abstract. In last years in the railroad territory of 1520 mm accidents have often occurred due to the destruction (failure) of the casting elements of threeelement freight car bogie. The quality and durability of loadbearing elements, which is traditionally produced by casting technology, is insufﬁcient. The development of new welded designs of the loadbearing elements were carried out on the basis of wide use of mathematical modeling to determine the stressstrain state of the welded elements under the action of regulated loads and to make the assessment of strength according to Ukrainian standards and current world approaches. The accelerated fatigue tests on prototypes were carried out, which showed that the service life of the welded structure of the side frame is ten times longer than the service life of the cast structure, and its survivability is longer in several times. Keywords: Railway freight car bogie Low alloy steel Side frame Welded joints Fatigue Test Service life
In recent years, on the area of 1520 mm gauge railways the accidents involving the destruction of the casting elements of threeelement bogie of freight car has often had. The quality and durability of bogie elements such as the side frame and the beams traditionally made by casting technology are of insufﬁcient level, so it is advisable to look for an alternative  the possibility of using welding technology in the manufacture of these parts to improve the characteristics of fatigue resistance [1]. In the E.O. Paton Electric Welding Institute of the NAS of Ukraine a work on the development of a new allwelded design of the side frame of a threeelement bogie of a freight car was carried out on the basis of widespread use of mathematical modeling to determine the stressstrain state of the welded elements of the bogie under the influence of regular loads and the assessment of (fatigue) strength according to current standards [2] and modern approaches [3]. Calculation of the fatigue resistance of the developed welded structure of side frame of the bogie in accordance with the Standard [2] considering the coefﬁcients of fatigue resistance for different evaluation zones (base metal and welds) taking into account the distribution of the coefﬁcient of vertical dynamics over the operating speed ranges (range of operating speeds) taking into account the additional load spectrum © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 273–279, 2020. https://doi.org/10.1007/9783030478834_49
274
L. Lobanov et al.
from the longitudinal compressive forces through the clutch, showed that the developed welded structure is workable with variable loading and rear frees the requirements of Standard [2] with the coefﬁcient of fatigue resistance [n] = 2, both under the condition of not exceeding the calculated stresses of the magnitudes of the allowed stress amplitudes and under the condition of damage accumulation. The fatigue resistance of the structure is estimated by the formula: n¼
ra;N ½n; ra;3
ð1Þ
where ra,N is the endurance limit (in amplitude) for a symmetric loading cycle on the base N0 = 107 cycles; ra,e  the calculated value of the amplitude of the dynamic stress of the conditional symmetric cycle, equivalent to the damaging effect of the real mode of operational stresses for the life of the part; [n]  the permissible minimum value of the fatigue resistance factor is taken in accordance with the Standard [2] for the new structure element of bogie  [n] = 2,0. The endurance limit (in amplitude) for a symmetrical load cycle is determined by [2]: ra;N ¼
r1 1 z p vr ; Kr
ð2Þ
where r1 is the average endurance limit of a smooth standard specimen; zp is a quantile of the distribution ra,N as a random variable; vr is the coefﬁcient of variation of the endurance limit; Kr  the average value of the reduction factor of the endurance limit of a part relative to the endurance limit of a smooth standard pattern. The calculated value of the dynamic stress amplitude of the conditional symmetric cycle, equivalent to the damaging effect of the real mode of operational stresses over the life of the structure element, is calculated taking into account the distribution of the vertical dynamics coefﬁcient over the 10 speed ranges [2]: ra;e
rﬃﬃﬃﬃﬃﬃﬃﬃ 10 X m T p fe ¼ maxðra Þ Pðvi Þkim ; N0 i¼1
ð3Þ
where m is the slope of the fatigue strength curve in the amplitudes; Tp  the total time of dynamic load over the estimated life of the element; fe  the effective frequency of pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ the process of changing dynamic loads for the trimmed parts fe ¼ 4c=mk , where c is the vertical rigidity of the spring kit under the gross weight of the car; mk  weight of the loaded car body; N0 is the base number of cycles of dynamical stresses; i  a speed range counter; P(vi)  the fraction of time in operation in the ith speed range, vi  the average value of the speed in the ith range; ki  the coefﬁcient of vertical dynamics in the ith speed range; max(ra)  the maximum stress amplitude during a symmetrical load cycle.
Development of Welded Elements of the Railway Freight Car Bogie
275
From the formulas given above, the maximum permissible stress amplitude of the fatigue resistance criterion would be expressed as follows:
½maxðra Þ ¼
ra;N sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ : 10 m Tp f 0 P ½n N03 Pðmi Þkim
ð4Þ
i¼1
In the case of a welded structure of the side frame, the values of fatigue strength (stress amplitudes) are calculated for the several evaluation zones according to the fatigue resistance criterion. To assess the fatigue strength of the side frame the loads were applied corresponding to the mode of normal movement of the car in the train: – vertical force reduced by the gross weight of the car body; – transverse component of longitudinal quasistatic force. The amplitudes of loads are determined by the coefﬁcient of vertical dynamics in the range of speeds till the speciﬁed 120 km/h. The coefﬁcient of vertical dynamics is assumed to be the same for the straight and curve sections of the rail path. Additionally, the assessment of fatigue strength of the welded structure of the bogie side frame in accordance with Recommendations of the International Institute of Welding (IIW) [3] was carried out. The assessment is based on the fatigue fracture (macro crack) observation in different zones of the structure (zones of welded joints), taking into account the speciﬁed stress spectrum of load during longterm operation [2]. Results of assessment showed that the developed welded design of the side frame has a sufﬁcient level of fatigue resistance with a safety factor cM = 1,1–1,4. The Recommendations of IIW summarize a large amount of experimental research for typical welded joints, which allowed for each type of joint and load direction to formulate a methodology for determining the fatigue strength at regular loading in the form: ½Dr ¼
FAT f1 ðRÞ f2 ðNÞ f3 ð@Þ f4 ðTÞ ; cM
ð5Þ
where FAT – fatigue class or fatigue strength of classiﬁed welded joint at 2 ∙ 106 cycles of regular loading (constant parameters of load cycle) at f1 = f2 = f3 = f4 = cM = 1, cM – safety factor. There is a table of FAT values for different classiﬁed welded joints [3]. Fatigue enhancement factor f1(R) depends on the stress ratio in a particular stress cycle and the level and direction of residual stresses. For stress relieved welded components with negligible residual stresses ( 0,5.
276
L. Lobanov et al.
Fig. 1. Fatigue resistance SN curves [3] for different classes FAT of welded joints (material – steel) for normal nominal stress at N < 109 cycles
For complex two or threedimensional components, components with global residual stresses, thick walled components like a welded side frame of railcar bogie f1(R) = 1,0 and no enhancement is considered. In the range of 104 < N < 108 cycles the factor f2(N) (Fig. 1) is deﬁned by equation: f2 ðNÞ ¼
m1 C ; N
where N – the number of cycles to failure, C = 2∙106, m = 3 for 104 < N < 107 cycles and C = 5,8∙106, m = 5 for 107 < N < 108 cycles. The influence of plate thickness on fatigue strength should be taken into account in cases where plates thicker than 25 mm. For weld joints of side frame with thickness of elements till 25 mm the correction factor can be taken equal f3(d) = 1,0. The reduction factor f4(T) is taken in consideration at elevated operation temperatures T. For T < 100 °C can be taken f4(T) = 1,0. The safety factor is recommended to take in the range cM = 1…1,4 [3]. In most cases for normal fabrication quality and regular inspection in service, cM = 1 might be adequate. Safety factor value cM = 1,4 corresponds to the consequence of failure – loss of human life. The load spectrum for the calculation of fatigue resistance is determined by the coefﬁcient of vertical dynamics and the probability of movement in the range of speeds up to the maximum design (120 km/h). Therefore, for the welded joints of the side frame the dependence (5) for determining the fatigue strength at regular loading can be represented as: ½Dr ¼
1 FAT C m : cM N
ð6Þ
Development of Welded Elements of the Railway Freight Car Bogie
277
Accordingly, the ultimate durability [N] at regular loading with a stress range Dr is expressed as follows
FAT ½N ¼ C Dr cM
m
:
ð7Þ
At variable amplitude loading (stress spectrum), linear damage calculation by “PalmgrenMiner” summation is appropriate. Table 1 summarizes the allowable amplitudes of the stresses (fatigue strength) in accordance with the National Standard [2] and IIW Recommendations [3] in the different zones of the side frame welded structure, taking into account the speciﬁed [2] stress spectrum of load at 107 cycles during longterm operation. Comparison shows insufﬁcient conservatism of the Standard in assessment of fatigue strength of welded joints.
Table 1. Fatigue strength (stress amplitudes) in accordance with the current Standard and IIW Recommendations, and calculated static stresses in different zones of the welded side frame Zone of the side frame structure
1 Base material of bottom belt in R55 of axle box pedestal 2 Longitudinal ﬁllet weld joint of sidewall and coil springs support plate 3 Transverse ﬁllet weld joint of axle box support 4 Longitudinal ﬁllet weld joint of sidewall and bottom belt in R55 of axle box pedestal 5 Transverse butt weld joint of sidewall
Standard [2]
Reduction factor of endurance limit Kr 1,5
Calculation IIW Recommendations [3] Fatigue strength Maximum Fatigue (in amplitude) [ra], principal strength stresses (in amplitude) MPa ra, MPa max(ra), MPa cM = 1/1,4 150
–
81
3,0
78
40/50
56
3,0
78
40/50
37
3,0
78
40/50
53
4,7
51
44/56
33
Also in Table 1 the calculated static stresses in the different zones of the side frame due to acting of maximum design operational load 23,5 tf are presented. In the most loaded areas of the side frame welded structure to provide the enough level of fatigue resistance it is advisable to apply additional improvement of residual stress conditions
278
L. Lobanov et al.
(stress relieving thermal treatment, hammerpeening) in the transition zone of the longitudinal welds (pos.2 and 4). The prototypes of welded side frames were manufactured and accelerated fatigue testing were carried out (Fig. 2) with a cycle stress amplitude increased in 2 times. After N = 8.8 million cycles of vertical loading (amplitude Pai = 245 kN = 25 tf, constant average cycle load Pm = 363 kN = 37 tf), a macro crack formed on the side wall of the frame between the lower belt and the support plate of the springs. The prototypes of the welded side frame showed a high value of durability, which is ten times greater than the design life of the cast structure of the side frame with an axial load of 23.5 tons. After N = 13 million cycles the failure along the transverse weld joint of the sidewall occurred (Fig. 2).
Fig. 2. Distribution of maximum principal stresses in the structure of welded side frame under the action of maximum design operational load 23,5 tf
A prototype of the welded side frame demonstrated a high value of the relative survivability (NiNi_cr)/Ni = 0,32, and in absolute value survivability of welded structure exceeds several times the service life of the cast structure of the side frame (Fig. 3).
Fig. 3. Prototype of side frame during accelerated fatigue test (a) and failure in the weld zone (b)
Development of Welded Elements of the Railway Freight Car Bogie
279
1 Conclusions 1. Welded structures of loadbearing elements of freight rail cars bogie designed within the requirements of the National Standard may not have sufﬁcient durability, because the exist Standard are not sufﬁciently conservative. The design of new welded structures must be carried out in accordance with the current Recommendations of the International Welding Institute for fatigue design of welded joints and components. 2. The results of the accelerated tests of the prototypes of the developed side frame welded structure of a threeelement rail freight car bogie with an axial load of 23,5 ts showed a signiﬁcant increase in service life and survivability, higher in tens time in comparison with a side frame of cast design at operational cyclic loads.
References 1. Makhnenko, O.V., Saprykina, G.J., Mirzov, I.V., Pustovoi, A.D.: Prospects for the creation of welded structures of loadbearing elements of a freight car bogie. J. Autom. Weld. 3(3), 36–42 (2014). (in Russian) 2. GosNIIV – VNIIGT, M.: Standards for the calculation and design of railroad cars of the Ministry of Railways of 1520 mm gauge (nonselfpropelled), p. 317 (1995). (in Russian) 3. Recommendations for Fatigue Design of Welded Joints and Components. IIW Doc XIII1965к1403/XV1127к1403, p. 147, 10 July 2006
Electron Beam Additive Technology Optimization Using Mathematical Modeling Oleh Makhnenko1(&), Nikita Ananchenko1, Stepan Kandala1, and Andriy Babenko2 1
2
E.O. Paton Electric Welding Institute of NASU, Kyiv 03680, Ukraine [email protected] Igor Sikorsky Kyiv Polytechnic Institute, NTUU, Kyiv 02056, Ukraine
Abstract. Additive manufacturing technology are developing fast these days. Economical proﬁt of manufacturing parts with complex geometry which have either hollow section or complex threedimensional curvature, using 3D printers are higher than using standard manufacturing methods. Which means that 3D printer could be an alternative to traditional ways of manufacturing. This technology used in aerospace and medicine right now, and have a future in other industries. Currently the technology of wire electron xBeam 3D Metal Printer of parts with complex geometry from titanium alloy has been developing in Ukraine. Using of mathematical modeling for optimization of the technology parameters is very promising. Keywords: Additive technology Mathematical modelling Residual stresses and deformations Thermal ﬁelds
Microstructure
1 Introduction Additive manufacturing is becoming an alternative to traditional manufacturing methods for titanium parts and structural components these days, in aerospace and medicine industries ﬁrst of all. Additive technology makes manufacturing of parts with complex threedimensional surface curvature or limited edition parts with nonstandard dimensions much cheaper and easier. Using of ﬁller wire makes additive manufacturing process much faster, electron beam heating sources are efﬁcient in vacuum condition that also is advisable for preventing titanium alloy from oxidation. But using of wire in the manufacturing process leads to a high level of residual stresses and distortions in structure element. Samples, made on 3D printer, could be seen on Fig. 1 [1]. Optimization of additive manufacturing process, using mathematical modeling and FEM analysis, makes sense these days.
2 Microstructure Mechanical properties of titanium alloy Ti6Al4V depends on its microstructure: grain size [2, 3] and percentage of a″ phase in a + b structure [4]. Grain size deﬁned by cooling rate during polymorphic transformation [5]: the higher cooling rate, the less © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 280–286, 2020. https://doi.org/10.1007/9783030478834_50
Electron Beam Additive Technology Optimization Using Mathematical Modeling
281
Fig. 1. Samples, formed by xBeam 3D metal printer technology, with small (a) and large (b) substrates.
grain size (Eq. 1) [2]. Percentage of martensitic a″ phase also deﬁned by cooling rate: when cooling rate is 410 °C/s and higher – fully a″ structure formed; in interval from 20°C/s to 410°C/s – a″ + a+b structure formed, and percentage of a″ phase linearly decreases, with decreasing of cooling rate from 410 °C/s to 20 °C/s; when cooling rate is 20 °C/s and less – a + b structure formed [4]. Mechanical properties of material, such as yield strength and elongation, deﬁned by grain size and percentage of a″ phase in titanium alloy Ti6Al4V. Yield strength of material deﬁned, mostly, by grain size: increasing of cooling rates, which means decreasing of grain size, leads to growth of yield strength [3, 6]; but, as it mentioned above, too high cooling rates leads to a″ phase formation, which reduces yield strength a little bit (Eq. 2) [4]. Though, impact of a″ phase percentage, on strength characteristics much less, than grain size. Elongation of material mostly deﬁned by quantity of martensitic a″ phase in titanium alloy: increasing of a″ phase percentage in alloy from 0% to 100% leads to linear decreasing of elongation from 11% to 2% (Eq. 3) [4]. dgrain ¼
0;58 ; lm where Vcooling 6 C=s 8220 Vcooling 2500; lm where Vcooling \6 C=s
ð1Þ
1;724 100 ma0 ; MPa ry ¼ 905 þ 8; 757 106 dgrain
ð2Þ
d ¼ 9 ma0 þ 11; %
ð3Þ
3 Mathematical Model 3.1
Mathematical Model for Temperature Fields
Finite element model of printed samples with small and large substrate was created, to calculate thermal ﬁelds during layer surfacing of a sample, using heat equation (Eq. 4) and heat sink boundary conditions (Eq. 5).
282
O. Makhnenko et al.
ccðT Þ @T ¼ kðT Þ @n
@T ¼ r½kðT Þ rT @t
aT ðT Tout Þ; heat transfer with machining attachment 4 e rSF T 4 Tout q; thermal radiation from surfaces
ð4Þ ð5Þ
Also, was created the thermo elastic plastic FE analysis model to calculate residual stresses and distortions after ﬁnish of forming and complete cooling of a sample. 3.2
Comparing of 2D and 3D Thermal Field Models
Two dimensional thermal ﬁeld model can be used for assumption of the fast moving heat source, which allows to reduce time of calculation sufﬁciently. Calculation’s accuracy is, from one side, increasing because of smaller mesh size, but from other side decreasing, because 2D thermal ﬁeld model don’t consider terminal effects on the beginning and end of surfaced layer. Results of 2D and 3D solution for typical example of titanium alloy Ti6Al4V sample forming (electron beam power 4,5 kW, wire diameter 1,6 mm, cladding speed 14 mm/s, dimensions of substrate 8 30 70 mm, wall width 3,2 mm), are compared on Fig. 2.
Fig. 2. Comparing of 3D (a, b) and 2D (c, d) thermal ﬁeld models on example of 5th (a, c), and 25th (b, d) layer surfacing.
Electron Beam Additive Technology Optimization Using Mathematical Modeling
3.3
283
Results for Residual Stresses and Distortions
Residual stresses and displacements in printed structure elements could limit usage of additive technology. After surfacing of 25 layers and complete cooling of a sample, residual deflection on a 70 mm long sample with large substrate are less than 0,4 mm, when its height 21 mm; and for sample with small substrate  are more than 3 mm, when its height 16 mm (Fig. 3a, b). Longitudinal component has the highest level of residual stresses. For large substrate sample, maximum residual tensile stress reach’s 480 MPa, and for small substrate sample – 280 MPa (Fig. 3c, d). Because of small substrate sample has less transverse stiffness than the large substrate one, residual stresses in it is less almost in two times, but residual deflection almost in ten times more, which can lead to culling this kind of samples.
Fig. 3. Residual deflections (a, b) and longitudinal stresses (c, d) of samples with large (a, c) and small (b, d) substrate.
4 Optimization of Technology, Varying Time Dt and Temperature Because of irregular heat sink from each formed layer, which related to cladding ﬁrst layers on a cold substrate, and last ones – on heated metal, high cooling rates received on ﬁrst layers, and as a result – small grain size with big percentage of a″ phase; and on the last layers received low cooling rates and large grain size (about 2500 µm). Which causes low plasticity of material on ﬁrst layers, and low strength characteristics on last layers. Delay time Dt between cladding of each layer is one of factors to change for getting efﬁcient technology parameters. Heat sink on last layers, comes on stationary mode with increasing of time Dt, on example of sample with large substrate. So, grain size and yield strength distribution becomes more regular on the last layers, with increasing
284
O. Makhnenko et al.
of Dt (Fig. 4a, b). Considering, that Dt = 24 s mode will be optimal, because Dt = 60 s mode leads to higher level of residual stresses and deformations.
Fig. 4. Relation between grain size (a, c), yield strength (b), elongation (d) and layer number for different delay time Dt (a, b) and preheat temperature (c, d).
Substrate preheat is also one of process parameters to change, for getting optimal microstructure. Increasing of preheat temperature until 600 °C, with combination of delay time Dt = 24 s, leads to stationary heat sink mode on ﬁrst layers, which means more regularly distribution of a″ phase, grain size, and elongation of material (Fig. 4c, d). Comparing of Residual Stresses and Distortions for Different Technology Parameters. In Table 1 shown modeled residual stresses and deflections of samples with large and small substrates, with using different delay time Dt between layer cladding. Results shows that too long delay time Dt affects on residual deflection negatively.
Electron Beam Additive Technology Optimization Using Mathematical Modeling
285
Table 1. Residual stresses and deflections of samples, made with different delay time Dt.
Small substrate Large substrate
Delay time Dt, s
Residual deflection, mm
Residual stresses, MPa Mises Longitudinal
Transverse
5 24 60 5 24 60
3.07 3.81 4.11 0.39 0.43 0.48
302 622 844 778 875 872
83/−115 98/−142 149/−222 350/−189 360/−286 420/−288
258/−166 472/−245 642/−410 483/−325 505/−364 423/−411
On height 87/−102 91/−94 117/−98 175/−180 193/−183 190/−160
Fig. 5. Macrosection of manufactured sample (a), modeled grain size (b), residual deflection of manufactured sample (c) and modeled residual deflection (d).
5 Comparing with Experiment Grain size was compared on a samples with large substrate, using initial technology parameters, i.e. without extra delay time (Dt = 0 s) and without substrate preheat. In result of experiment, macrosection analysis gives grain size 200–300 µm on ﬁrst layers, and 400–600 µm on middle layers (Fig. 5a) [1]. Modeled grain size on ﬁrst layers is 150–250 µm and 400–700 µm on middle layers (Fig. 5b). Also, residual deflection of manufactured sample with small substrate was compared with modeled deflection. Modeled residual deflection of sample with small substrate equals to 1,5 mm (Fig. 5d) and shows adequately correlation with deflection of manufactured sample – about 2 mm (Fig. 5c).
286
O. Makhnenko et al.
References 1. Kovalchuk, D., Melnyk, V., Melnyk, I.: New capabilities of additive manufacturing with xBeam 3D Metal Printing technology. In: College of Works of Eight International Conference on Beam Technology in Welding and Material Handling, Kiev, Ukraine, p. 51 (2017) 2. Polkin, I.: Progressive technologies and new processes. In: Progressive Technologies of Light and Special Alloys, Fizmatlit, Moscow, pp. 66–73 (2006) 3. Lutjering, G., Williams, J.C.: Microstructure and properties of materials V.2. In: Li, J.C.M.: Microstructure and Mechanical Properties of Titanium Alloys, pp. 26–29 (2000) 4. Liu, S.: Additive manufacturing of Ti6Al4V alloy: a review. Mater. Des. 164, 1–23 (2018) 5. Sieniawski, J., Ziaja, W., Kubiak, K.: Microstructure and mechanical properties of high strength twophase titanium alloys. In: Sieniawski, J.: Titanium Alloys, pp. 69–79 (2013) 6. Grabin, V.: Structure and Properties of Welded Joints from Titanium Alloys, p. 59. Naukova Dumka, Kiev (1964)
Nonstationary Contact Problems for Thin Shells and Solids Grigory Fedotenkov1,2(&) 1
2
and Dmitry Tarlakovskii2
Moscow Aviation Institute, National Research University, Moscow, Russia [email protected] Institute of Mechanics, Lomonosov Moscow State University, Moscow, Russia
Abstract. A spatial nonstationary contact problem with moving boundaries of the interaction region for a thin elastic cylindrical shell and an absolutely rigid indenter bounded by a smooth convex surface is considered. A closed mathematical formulation is given and a system of resolving equations is constructed. The system of resolving equations is based on the spatialtemporal integral equation resulting from the principle of superposition and contact conditions. The core of this equation is the transient function for the cylindrical shell. To a closed system of resolving equations, it is supplemented by a kinematic relation for determining the moving boundary of the contact area and the equation of motion of the indenter as an absolutely rigid body. An algorithm for solving the spatial nonstationary contact problem for an inﬁnitely long cylindrical shell and absolutely rigid indenter in the case of a normal impact on the side surface of the shell is constructed and implemented. Examples of calculations are given. Keywords: Spatial nonstationary contact problems Cylindrical shell Superposition method Fourier series Integral transforms Transient functions Numericalanalytical algorithms
1 Problem Formulation At the initial instant of time, an absolutely rigid indenter, moving with a given initial velocity V0 , comes into contact with the lateral surface of the inﬁnitely long thin elastic circular cylindrical shell. The indenter is bounded with a smooth convex surface, the vector of its initial velocity is directed normal to the side surface of the shell (Fig. 1). The equations of motion of the model S.P. Timoshenko in displacements recorded in the main orthogonal coordinates associated with the directions of the main curvatures of the middle surface are used to describe the motion of the shell [1, 2]: @2W ¼ LW þ P; @s2 T L ¼ Lij 55 ; W ¼ u; v; w; va ; vz ; P ¼ ð0; 0; p; 0; 0ÞT ;
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 287–292, 2020. https://doi.org/10.1007/9783030478834_51
ð1Þ
288
G. Fedotenkov and D. Tarlakovskii
Fig. 1. Problem formulation.
2 @2 @ @2 2 @ 2 ; ; L13 ¼ 1 þ kg2 þ g k ; L12 ¼ 1 g2 2 2 @a @a @z @a@z @2 @2 @2 @2 L14 ¼ c2 2 þ g2 k2 ; L15 ¼ c2 1 2g2 ; L21 ¼ L12 ; L22 ¼ 2 þ g2 2 ; @a @a@z @z @a 2 2 @ @ @ ; L24 ¼ c2 g2 ; L25 ¼ c2 g2 2 ; L31 ¼ L13 ; L23 ¼ 1 2g2 @z @a@z @a 2 @ @2 @ @ 2 2 ; L35 ¼ g2 k 2 ; þ 2 1; L34 ¼ g2 k 2 L32 ¼ L23 ; L33 ¼ g k 2 @a @z @a @z 2 2 @ @ 2 2 2 2 2 2 L41 ¼ c L14 ; L42 ¼ c L24 ; L43 ¼ c L34 ; L44 ¼ 2 þ g k c ; @a @z2 L11 ¼
L45 ¼ L12 ; L51 ¼ c2 L15 ; L52 ¼ c2 L25 ; L53 ¼ c2 L35 ; 2 @2 @ 2 2 2 L54 ¼ L12 ; L55 ¼ 2 þ g k c : @z @a2 u, v – tangential displacements of the shell in the direction of the coordinate lines a (angular coordinate) and z (longitudinal coordinate) respectively, w – normal displacement of the shell va , vz – angles of rotation of the normal ﬁber, p – normal pressure, s – dimensionless time, L – matrixoperator, k2 ¼ 5=6 – shear coefﬁcient. Here and further all functions, variables, and parameters are reduced to a dimensionless form using a system of dimensionless quantities (primed variables correspond to dimensional ones): u¼
u0 v0 w0 u0 c z0 c1 t 2 c22 2 k þ 2l ; g ¼ 2 ; c1 ¼ ; ; v ¼ ; w ¼ ; uc ¼ ;z ¼ ;s ¼ R q R R R R R c1
NonStationary Contact Problems for Thin Shells and Solids 0
0
289
m0u c21
l h pR V0 ; V0 ¼ : c22 ¼ ; c2 ¼ ;p ¼ ; mu ¼ 2 2 q hðk þ 2lÞ 12R c1 R hðk þ 2lÞ 2
q – density of the shell material, k; l – Lame parameters of the shell material, R and h – radius and thickness of the shell, uc – displacement of the center of mass of the indenter, c1 and c2 – speed of the tensioncompression waves and shear waves in the shell material, mu – the mass of the indenter, t – dimensional time. The equation of motion of the striker as an absolutely rigid body has the following form: ZZ pðn; f; sÞdndf; uc ð0Þ ¼ 0; u_ c ð0Þ ¼ V0 : ð2Þ mu €uc ðsÞ ¼ PðsÞ ¼ XðsÞ
P – the resulting force of contact pressure p, XðsÞ – the contact area, the boundary of which depends on time. We assume that the contact between the shell and the striker occurs under conditions of free slippage. Let P1 and P2 be the surfaces bounding the shell and the striker at the moment of time s [ 0. With respect to an inertial Cartesian rectangular coordinate system whose axis coincides with the axis of the shell, they are given by the equations Pk : x ¼ fk ðy; z; sÞ; ðy; zÞ 2 Xk ; k ¼ 1; 2; where Xk – projections of surfaces P1 and P2 on a plane Oyz. Then the true contact area is deﬁned by the following conditions: P : Dðy; z; sÞ ¼ f1 ðy; z; sÞ f2 ðy; z; sÞ ¼ 0; pðy; z; sÞ\0; ðy; zÞ 2 Xk ;
ð3Þ
where D – is the gap between the boundary surfaces P1 and P2 . The equations that implicitly deﬁne the boundary @P of the contact area follow from (3): @P : Dðy; z; sÞ ¼ 0; pðy; z; sÞ ¼ 0 In the linearized formulation of the problem, the true contact area P is replaced by a ﬁctitious area XðsÞ belonging to the plane that is a common tangent to the surfaces P1 and P2 at the initial time of contact interaction (Fig. 2). Suppose that the position of the surface bounding the striker at the current time s is given by an explicit equation in the coordinate system Oxyz: x ¼ f ðy; zÞ þ uc ðsÞ:
ð4Þ
290
G. Fedotenkov and D. Tarlakovskii
Fig. 2. Contact area.
The boundary @XðsÞ of the area XðsÞ is determined from the condition of intersection of the surface bounding the striker with the plane P: @XðsÞ : f ðy; zÞ þ uc ðsÞ ¼ 1:
ð5Þ
Taking into account (4), the contact conditions of the indenter and the shell have the form f ðy; zÞ þ uc ðsÞ ¼ wða; z; sÞ; pða; z; sÞ\0; y; z 2 XðsÞ; y ¼ sin a:
ð6Þ
At the initial time, the shell is in an unreformed state, which corresponds to zero initial conditions _ s¼0 ¼ v_ js¼0 ¼ wj _ s¼0 ¼ v_ a js¼0 ¼ v_ z s¼0 ujs¼0 ¼ vjs¼0 ¼ wjs¼0 ¼ va js¼0 ¼ vz s¼0 ¼ uj ¼ 0: ð7Þ Equations and relations (1), (2), (4)–(7) are a closed mathematical formulation of the nonstationary contact problem with movable boundaries for a cylindrical shell and an absolutely rigid indenter.
2 Calculation Examples To solve the system of resolving equations, we use a numericalanalytical algorithm based on the method of mechanical quadratures [3–6]. As an example, consider the nonstationary contact interaction of a circular cylindrical shell (R ¼ 1, h ¼ 0:025), with an absolutely rigid indenter bounded by a surface that has the shape of rotating paraboloid: f ðy; zÞ ¼ y2 þ z2 þ 1: As the shell material, we use steel with the following parameters: g ¼ 0:53, c ¼ 1:3 106 . In Fig. 3a–3c shows the dependence of the movement of the center of mass of the striker on time (Fig. 3a), the radius of the contact area from time (Fig. 3b) and the
NonStationary Contact Problems for Thin Shells and Solids
291
Fig. 3. Dependences of the movement of the center of mass of the indenter, the radius of the contact area and the resulting contact force on time.
resulting contact force from time (Fig. 3c). Here, the solid curves correspond to V0 ¼ 0:01, dashed V0 ¼ 0:05, dashdotted – V0 ¼ 0:1. In Fig. 4a–4c shows the distribution of contact pressure in the angular coordinate a at the time s ¼ 0:3. Figure 4a corresponds to the coordinate value z ¼ 0, 4b – z ¼ 0:15, 4c – z ¼ 0:3. Solid curves correspond to V0 ¼ 0:01, dashed V0 ¼ 0:05, dashdotted – V0 ¼ 0:1.
Fig. 4. Distribution of contact pressure by angular coordinate at a time.
Figure 5a and 5b represent distributions of normal displacements along the angular coordinate (Fig. 5a) and along the longitudinal coordinate (Fig. 5b). Here, the results correspond to the time s ¼ 0:6 and the initial speed V0 ¼ 0:1. In Fig. 5a, the solid curves correspond to z ¼ 0, dashed z ¼ 0:15, dashdotted – z ¼ 0:3. Solid curves in Fig. 5b correspond to a ¼ 0, dashed a ¼ 0:15, dashdotted – a ¼ 0:3.
Fig. 5. The distribution of normal displacements along the angular and longitudinal coordinates.
292
G. Fedotenkov and D. Tarlakovskii
Acknowledgments. This work was ﬁnancially supported by the Russian Foundation for Basic Research (RFBR), project 190800438 A.
References 1. Fedotenkov, G.V., Kalinchuk, V.V., Mitin, A.Y.: Threedimensional nonstationary motion of Timoshenkotype. Lobachevskii J. Math. 40(3), 311–320 (2019) 2. Fedotenkov G.V., Tarlakovskii D.V., Mitin A.Y.: Transient spatial motion of cylindrical shell under influence of nonstationary pressure. In: Gdoutos E. (eds) Proceedings of the Second International Conference on Theoretical, Applied and Experimental Mechanics. ICTAEM 2019. Structural Integrity, vol. 8, pp. 264–269. Springer, Cham (2019) 3. Tarlakovskii, D.V., Fedotenkov, G.V.: Twodimensional nonstationary contact of elastic cylindrical or spherical shells. J. Mach. Manuf. Reliab. 43(2), 145–152 (2014) 4. Tarlakovskii, D.V., Fedotenkov, G.V.: Fedotenkov nonstationary 3D motion of an elastic spherical shell. Mech. Solids 50(2), 208–217 (2015) 5. Fedotenkov, G.V., Mikhailova, E.Y., Kuznetsova, E.L., Rabinskiy, L.N.: Modeling the unsteady contact of spherical shell made with applying the additive technologies with the perfectly rigid stamp. Int. J. Pure Appl. Math. 111(2), 331–342 (2016) 6. Mikhailova, E.Yu., Tarlakovskii, D.V., Fedotenkov, G.V.: The unsteady contact interaction problem of an absolutely rigid body and a membrane. In: Gdoutos E. (eds) Proceedings of the Second International Conference on Theoretical, Applied and Experimental Mechanics. ICTAEM 2019. Structural Integrity, vol. 8, pp. 289–293. Springer, Cham (2019)
Shear Buckling Mode and Failure of Sandwich Specimen Facing Layer Under FourPoint Bending V. N. Paimushin1,2(&) , M. V. Makarov1,2 , S. A. Kholmogorov1 , and M. A. Shishov1 1
Kazan National Research Technical University named after A.N. Tupolev, K. Marks Str. 10, 420111 Kazan, Russia [email protected] 2 Kazan Federal University, Kremlyovskay Str. 18, 420008 Kazan, Russia
Abstract. The geometrically and physically nonlinear problem of fourpoint bending of a sandwich specimen with a transversally flexible core and facing layers from ﬁber reinforced plastic, characterized by a nonlinear relationship between transverse shear stresses and the corresponding shear strains, is formulated. The statement of the problem is given taking into account the contact interaction of the facing layers with the support and loading rollers, a numerical method for solving it is developed based on the ﬁnite sum method (method of integrating matrices). Equations based on the reﬁned kinematic model of S. P. Tymoshenko taking into account the transverse compression of the facing layers and the equations of elasticity theory for the core, simpliﬁed in the framework of the model of the transversally flexible layuer. The latter allow integration along the transverse coordinate when introducing as unknown transverse shear stresses in the core, constant in thickness. An investigation of the prebuckling and postbuckling behavior of the specimen was carried out, based on the method of continuing the solution with respect to the parameter, when the transverse shear strain in the loaded facing layer was chosen as the parameter. It was shown that during tests for fourpoint bending of specimens of the class under consideration, their failure can be due to the implementation of transverseshear buckling modes of the facing layer in the vicinity of the loading roller. Keywords: Sandwich specimen Transversely soft core Facing layer Fiber reinforced plastic Fourpoint bending Integration matrices method Iterative process Geometrically and physically nonlinearity Parameter continuing method Shear buckling mode Postbuckling behaviour
1 Introduction The most rational use of ﬁber reinforced plastics (FRP) is possible in structural elements of a sandwich structure. Their facing (loaded) layers made of FRP have, as a rule, low transverse shear stiffness. If compressive stresses are formed in them during loading, then one of the mechanisms of their failure is the transverseshear buckling © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 293–300, 2020. https://doi.org/10.1007/9783030478834_52
294
V. N. Paimushin et al.
mode. In the mechanics of composites, theoretical studies of this buckling mode, which is realized in standard specimens under compression, were carried out in different approximations in many works [1, 2, etc.]. In accordance with the results of these works, in order to identify the described buckling mode, which can also be realized in sandwich structures with facing layers of ﬁbrous composites, the construction of the corresponding theory requires taking into account the transverse shear strains in the facing layers. Such reﬁned geometrically and physically nonlinear equations of the theory of sandwich plates and shells with facing hard layers of ﬁbrous composites and a medium transversely flexible layer were constructed in [3]. Tests of specimens for fourpoint bending according to the scheme shown in Fig. 1 are one of the types of experimental studies of sandwich structural elements with facing rigid layers of ﬁbrous composites.
2.5
G13, GPa
2 1.5 1 0.5 0 0.1
0.05
0 2ε13
0.05
0.1
Fig. 1. Installing diagram of sandwich speci Fig. 2. Relationship of shear modulus from men on fourpoint bending test shear strain
These tests are carried out, as a rule, in order to determine the value of the ultimate compressive stress that is formed in the bottom facing layer within the area L of the working length a of the specimen, upon reaching which the speciﬁed layer is failure. It can be assumed that one of the causes of such failure is the buckling of the compressed facing layer in one of the possible modes, the classiﬁcation of which is given in [4, 5]. As will be shown below, using the equations constructed in [3], it is possible to identify both bending and bendingshear and purely shear buckling modes of the lower facing layer of the specimen under compression under its fourpoint bending according to the diagram in Fig. 1.
2 Statement of the Problem In accordance with [3], a reﬁned kinematic model of S.P. Tymoshenko UzðkÞ ¼ uðkÞ e1 þ wðkÞ m þ zðkÞ cðkÞ e1 þ uðkÞ m was adopted to describe the mechanics of the deformation of facing layers at small and medium bends of the plate, and for the core a
Shear Buckling Mode and Failure of Sandwich Specimen Facing Layer
295
model of a transverse flexible layer was used. After integrating the simpliﬁed equations of theory of elasticity, written for the core along the transverse coordinate z, and introducing an unknown function q into consideration, the equilibrium equations corresponding to the accepted model and the kinematic condition for the interface of the facing layers with the core were derived in [3]. With fourpoint bending of the plate in a cylindrical shape, they have the form (dð1Þ ¼ dð2Þ ¼ 1) 11 ðk Þ Tð13 T w þ hq=2 þ dðkÞ r033 þ Xð3kÞ ¼ 0; kÞ ðkÞ ;x ;x 0 3 Mð11kÞ;x Tð13 Mð13kÞ þ dðkÞ htq=4 Tð33 k Þ þ tq=2 ¼ 0; kÞ þ r33 t=2 dðkÞ XðkÞ t=2 ¼ 0; ;x uð2Þ uð1Þ ðcð1Þ þ cð2Þ Þt=2 þ wð;x1Þ þ wð;x2Þ h=2 þ uð;x1Þ uð;x2Þ ht=4
Tð11 kÞ;x þ dðkÞ q ¼ 0;
hq=G013 þ q;xx h3 =ð12E30 Þ ¼ 0; ð1Þ where, with the linearly elastic behavior of the material of the facing layer in the x; z ðk Þ directions and the physically nonlinear dependence between the shear stresses r13 and ðk Þ
the corresponding shear strain 2e13 , the internal forces and moments introduced into the analysis and the desired functions uðkÞ ; wðkÞ ; cðkÞ , uðkÞ are related by the dependences ðk Þ ðk Þ 2 ðk Þ ðk Þ ðk Þ 2 ðk Þ Tð11 ; Tð33 ; kÞ ¼ B1 u;x þ ðw;x Þ =2 þ m31 u k Þ ¼ B3 m13 ðu;x þ ðw;x Þ =2Þ þ u ðk Þ ðk Þ 0 ð2Þ wð1Þ tðuð1Þ þ uð2Þ Þ=2 E30 =h; Tð13 kÞ ¼ B13 ðw;x þ c Þ; r33 ¼ w Mð11kÞ ¼ D1 cð;xkÞ ; B13 ¼ G13 t;
Mð13kÞ ¼ D13 uð;xkÞ ; B1 ¼ E1 t=ð1 m13 m31 Þ; D1 ¼ B1 t =12; 2
B3 ¼ E3 t=ð1 m13 m31 Þ;
D13 ¼ B13 t =12: 2
For Eqs. (1) for x ¼ l; l we formulate the boundary conditions for free edges (2l – plate length) 11 13 Tð11 ðxÞ ¼ 0; M ðxÞ ¼ 0; M þ d qht=4 ðxÞ ¼ 0; qðxÞ ¼ 0; ð k Þ kÞ ðk Þ ðk Þ 11 ðk Þ Tð13 k Þ Tðk Þ w;x þ hq=2 ðxÞ ¼ 0;
ð2Þ
for x ¼ 0 – symmetry conditions with respect to the central section, and for x ¼ a=2 – condition in the form of equal to zero of transverse displacement of the upper facing layer in the center of the support roller: uðkÞ ð0Þ ¼ 0; cðkÞ ð0Þ ¼ 0; Mð13kÞ þ dðkÞ htq=4 ð0Þ ¼ 0; qð0Þ ¼ 0; 11 ðk Þ T w þ hq=2 ð0Þ ¼ 0; wð2Þ ða=2Þ þ uð2Þ ða=2Þt=2 ¼ 0: Tð13 kÞ ðkÞ ;x
ð3Þ
296
V. N. Paimushin et al.
3 To simulate external loading (see Fig. 1), the distributed load Xð1Þ applied to the bottom layer at the contact area of the loading roller with the facing layer and it is speciﬁed by a cosine function with an amplitude value p. To simulate the contact interaction between the support and the top facings layer in the support section x ¼ a=2, the condition was set in the form of the last equation of system (3), and the 3 unknown reaction Xð2Þ from the support roller was approximated by the cosine function with an amplitude value pz , that can be determined from the solution of the problem. For an approximate solution of the formulated boundary value problem (1)–(3), the ﬁnite sum method (the method of integrating matrices) was used [6, 7]. In accordance with this method, we reduce the initial differential equations to Volterratype integral equations of the second kind with additional relations for determining unknown integration constants. Such a reduction is carried out by integrating Eqs. (1) and satisfying conditions (2)–(3). Note that the initial boundaryvalue problem has the form of a secondorder differential problem, while integral equations will contain only derivatives of the desired functions. In [7], a method of collocation by Gaussian nodes and a method for constructing integrating matrices were proposed, and in [8, 9] a constructive application of the method of integrating matrices in version [7] for problems of the theory of plates and shells was described in detail. Therefore, we restrict ourselves to the ﬁnal discrete statement of the problem in the operator form, which is obtained by replacing the integral operators in the problem with integrating matrices: ð1Þ ð2Þ ð1Þ ð2Þ ð1Þ ð2Þ ð1Þ AðUÞ ¼ A1 U þ A2 ðUÞ ¼ F, where U ¼ ðw;x ; w;x ; u;x ; u;x ; q;x ; wl ; wl ; ul ; ð2Þ
ul ; qa;1 ; pz Þ 2 Hh5 R6 , A1 – linear, A2 – nonlinear operators; the vector function F 3 of the righthand sides depends only on the transverse load function Xð1Þ ðpÞ applied to the bottom facing layer. Experimental investigations were carried out in [10, 11] to determine the shear modulus of ﬁbrous composite materials used for facing layers of a sandwich plate. As a ðkÞ ðkÞ result of the studies, averaged experimental dependences r13 ¼ G13 ð2e13 Þ2e13 of shear stresses on shear strains were obtained, on the basis of which the dependences of the secant shear modulus on the corresponding shear strains were constructed (see Fig. 2). The last dependences in the used mathematical model of deformation are included as terms, which are taken into account in the form of a physically nonlinear dependence ðkÞ G13 ð2e13 Þ ¼ G13 ðwð;xkÞ þ cðkÞ Þ during piecewise linear interpolation of the experimental dependence G13 ðwð;xkÞ þ cðkÞ Þ obtained in [11]. The described numerical method for solving the formulated nonlinear problem is implemented on the basis of a modiﬁed Newton’s iterative process ðnÞ
ðnÞ
A0ðnÞ ðU ðnÞ Þ ðU ðn þ 1Þ U ðnÞ Þ þ ðA1 þ A2 Þ U ðnÞ ¼ F:
ð4Þ
The nonlinear dependence of the transverse shear modulus G13 on the shear strain ðkÞ 2e13 ¼ wð;xkÞ þ cðkÞ , obtained by the experimental method in [11], is included in the ðnÞ
ðnÞ
problem as the dependence of the operators A0ðnÞ , A1 , A2 on U ðnÞ , where U ð0Þ – is the given initial approximation, i.e. at each nth iterative step, it is necessary to recalculate
Shear Buckling Mode and Failure of Sandwich Specimen Facing Layer
297
the stiffness matrix depending on the nth approximation of the solution ðkÞ ðU ðnÞ ; ð2e13 ÞðnÞ Þ; A0ðnÞ ðU ðnÞ ÞDU is the differential of the operator AðnÞ at the point U ðnÞ . Calculations according to the iteration process (4) were carried out until the norms of the residual and the difference between the iterations remained greater than the speciﬁed accuracy. In the calculations, the elastic characteristics of the facing layers are taken to be E1 ¼ 103 GPa, E3 ¼ 5; 9 GPa, m13 ¼ 0; 3; transversely flexible core – E30 ¼ 80 MPa, G013 ¼ 30 MPa, and geometric parameters equal to t ¼ 0; 3 cm, h ¼ 1 cm, L ¼ 7 cm, a ¼ 25 cm, 2l ¼ 27 cm. To describe the desired functions having large gradients on very short regions (in particular, in the loading roller zone), the region was decomposed using piecewise Lagrangian interpolation to construct integrating matrices. To this end, we divide the region ½0; l into three segments e1 ¼ ½0; L=2, e2 ¼ ½L=2; L=2 þ R, e3 ¼ ½L=2 þ R; l, introduce a global grid xh ¼ fxi : 0\x1 \x2 \. . .xN \lg on the segment ½0; l as follows: on each segment e1 , e2 , e3 we introduce independent Gaussian nodes associated with the roots of the Legendre polynomial; the number of nodes on these segments were taken equal N1 ¼ 40, N2 ¼ 81, N3 ¼ 130 respectively.
3 Results of Numerical Experiments ð1Þ
By tabulating the parameter of the amplitude value p of the transverse load X3 , an analysis was made of the sequence of equilibrium states (solutions of the problem) at various loading levels, including the maximum values of deflections and shear strains of the bottom loaded facing layer. It is worth noting that the “loaddeflection” relationship is linear in nature, therefore it is not of particular interest. Figure 3 shows the dependence of the load on the maximum modulus of the shear strain, where, Rl 3 ð1Þ ð1Þ P ¼ b Xð1Þ , b ¼ 2:5 cm, e13 ¼ max je13 ðxi Þj. l
i¼1;...N
Note that in Fig. 3 dashed line represents the solution of a geometrically nonlinear problem without taking into account physical nonlinearity, the solid line represents the solution of a geometrically and physically nonlinear problem. In the vicinity of some load value P ¼ P indicated in Fig. 3 by triangle, the iterative process ceases to converge. To search for the unstable equilibrium positions indicated in Fig. 3 by a dashed line, the parameter continuation method was implemented (see, for example, [8, 9], which describes in detail the constructive implementation of the parameter continuation method [12]), which is one of the versions of the modiﬁed globally incremental Lagrange theory (the problem regarding increments, in contrast to the classical incremental Lagrange theory, is solved in a nonlinear formulation).
298
V. N. Paimushin et al. 6 5
P, kN
4 3 2 1 0 0
0.005
0.01
0.015 0.02 2ε(1)  13
0.025
0.03
0.035
Fig. 3. “Loadshear transversal strain” curve
The shear strains at the point n was used as loading parameter in the method, where n – the point at which the shear strains reach the maximum value in absolute value. The Fig. 4a shows the distribution along the length of the specimen of the transverse shear strains of the bottom facing layer at various load values P; Fig. 4b shows a plot of Fig. 4a on an enlarged scale, indicating the corresponding values P of the applied force for each of the solutions shown in the form of shear strains. The load values P in Fig. 4b are also marked with black round markers in the diagram “load – transverse shear strain” (see Fig. 3). Figure 5 shows the distribution of the transverse shear modulus along the length of the bottom compressed facing layer, corresponding to the shear strain at the point indicated in Fig. 3 by triangle marker, at P ¼ P . It should be noted that the maximum modulus values of the transverse shear strains and shear stresses, as well as the minimum absolute values of the transverse shear moduli, are reached at the edge of the loading roller (see Fig. 4, 5, 6). It can be seen that in its vicinity localized zones of concentration of shear stresses and corresponding
1.65 kN
0.005
2.77 kN 3.55 kN
(1)
0
0.01
4.13 kN
2ε13
2ε13
(1)
0.01
4.56 kN
0.015
0.01
4.91 kN 5.12 kN
0.02
0.02
5.26 kN
0.025 0.03 0
2
4
6
8 x, cm
a
10
12
5.28 kN
3.6
3.8
x,cm
b
Fig. 4. Shear transversal strain for different load values
4
4.2
Shear Buckling Mode and Failure of Sandwich Specimen Facing Layer
299
shear strains are formed, and, consequently, a sharp drop in the values of secant shear moduli. Figure 6 shows the increments of the transverse shear strains of the bottom facing layer in the postbuckling region, which were obtained as a solution to the problem with respect to the increment functions using the parameter continuation method. The analysis showed that they characterize the buckling by the transverseshear mode, which is realized when the transverse shear stresses in the facing layer reach a certain limiting value. This buckling mode is similar to the transverseshear mode [10], which is realized in the specimen of ﬁber reinforced plastic at threepoint bending and is the cause of their failure during testing.
x 10
2.2 0
2
2 2Δε13
(1)
G13 , GPa
1.8 (1)
1.6 1.4
4 6
1.2
8
1 0.8 0
4
5
x, cm
10
15
Fig. 5. The distribution of transverse shear modulus along the length
10 0
5
x, cm
10
15
Fig. 6. The distribution of increments of transverse shear strains along the length
Acknowledgments. The research results were obtained in the framework of the fulﬁllment of the state task of the Ministry Science and High Education of Russia (evaluation of mechanical characteristics of CFRP), supported by Russian Science Foundation (project No. 197910018, Section 2 and 3) and by Russian Foundation for Basic Research (project No. 190800073, development of numerical method).
References 1. Naik, N.K., Kumar, R.S.: Compressive strength of unidirectional composites: evaluation and comparison of prediction models. Compos. Struct. 46, 299–308 (1999) 2. Budiansky, B., Fleck, N.A.: Compressive failure of ﬁbre composites. J. Mech. Phys. Solids 41(1), 183–211 (1993) 3. Badriev, I.B., Paimushin, V.N., Shihov, M.A.: Reﬁned equations of the sandwich shells theory with composite external layers and a transverse soft core at average bending. Lobachevskii J. Math. 40(11), 1094–1914 (2019) 4. Paimushin, V.N.: A stability theory of sandwich structural elements analysis of the current state and a reﬁned classiﬁcation of buckling forms. Mech. Compos. Mater. 35(6), 465–470 (1999) 5. Paimushin, V.N.: Theory of stability for threelayer plates and shells: stages of development, stateoftheart, and prospects. Mech. Solids 36(2), 127–137 (2001)
300
V. N. Paimushin et al.
6. Vakhitov, M.B.: Integration matrices: apparatus for numerical solving of differential equations of structural mechanics. Russ. Aeronaut. 3, 50–61 (1966). (In Russian) 7. Dautov, R.Z., Paimushin, V.N.: On the method of integrating matrices for the solution of boundary value problems for fourthorder ordinary equations. Russ. Math. 40(10), 11–23 (1996) 8. Badriev, I.B., Makarov, M.V., Paimushin, V.N.: Solvability of physically and geometrically nonlinear problem of the theory of sandwich plates with transversallysoft core. Russ. Math. 59(10), 57–60 (2015) 9. Badriev, I.B., Makarov, M.V., Paimushin, V.N.: Geometrically nonlinear problem of longitudinal and transverse bending of a sandwich plate with transversally soft core. Lobachevskii J. Math. 39(3), 448–457 (2018) 10. Paimushin, V.N., Kholmogorov, S.A., Makarov, M.V., Tarlakovskii, D.V., Lukaszewicz, A.: Mechanics of ﬁber composites: forms of loss of stability and fracture of test specimens resulting from threepoint bending tests. Zeitschrift fur Angewandte Mathematik und Mechanik 99(1), 1–25 (2019) 11. Paimushin, V.N., Kholmogorov, S.A.: Physicalmechanical properties of a ﬁberreinforced composite based on an ELURP carbon tape and XT118 binder. Mech. Compos. Mater. 54 (1), 2–12 (2018) 12. Grugoluk, E.I., Shalashilin, V.I.: Nonlinear Deformation Problems: Method of Parameter Continuation in Nonlinear Problems of Mechanics of Rigid Bodies. Nauka, Moscow (1988)
Model of LowCycle Deformation of Stainless Steel Under Soft Loading Vasilii Gorokhov(&) , Sergei Kapustin, Yuriy Churilov, Dmitriy Kazakov, and Dmitriy Zhegalov Research Institute for Mechanics, National Research Lobachevsky State University of Nizhny Novgorod, Gagarin Avenue 23, Nizhny Novgorod 603950, Russia [email protected] Abstract. A variant of the plasticity model is proposed that allows describing the kinetics of plastic deformation of materials under different modes of lowcycle loads. In the model, the radius of the flow surface is represented as a function depending on temperature and accumulated plastic deformation, and the coordinates of the center are described by two ArmstrongFrederickKadashevichtype evolutionary equations, the ﬁrst of which additionally introduces corrective material functions. Changes in plastic deformations in the model are determined based on the associated flow law. Receiving material functions of the model and testing it was carried out on the basis of the results of experimental study of the deformation of a cylindrical sample under soft cyclic loading with maximum control and minimum effort in the cycle. The experiments were carried out on the Amsler HA 100 servohydraulic fatigue testing machine. Comparative analysis of the results of numerical simulation and experiment shows that the proposed model allows us to describe the main effects of plastic deformation of the material under consideration under soft asymmetric loads (displacement of the plastic hysteresis loop and reduction of its width) quite well. Keywords: Plasticity
Soft loading Lowcycle deformation Yield surface
1 Introduction Currently, there are a number of mathematical models proposed to describe the processes of plastic deformation under lowcycle loads. In [1], it was found that the variants of the models proposed in [2, 3] do not allow us to correctly describe the quantitative dependence of the displacement and change in the loop width on the number of cycles under soft cyclic loads. In [1], it is also shown that for these types of loads, the models [4–6] satisfactorily describe the laws of displacement of the plastic deformation loop, but there is practically no information about the possibility of describing the kinetics of the plastic hysteresis loop width within these models, which actually determine the cyclic component of the fracture energy. A variant of the plasticity model with combined hardening is considered below to describe the main effects of deformation under soft, hard, symmetric and asymmetric lowcycle loads, which is a development of the model variant [3], supplemented with reﬁned relations for describing kinematic hardening [1, 4, 6]. © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 301–304, 2020. https://doi.org/10.1007/9783030478834_53
302
V. Gorokhov et al.
2 Constitutive Equations of the Plasticity Model In the proposed version of the model, the radius of the yield surface Cp is represented as a function depending on the temperature T and the accumulated plastic deformation characterized by parameter kp  plastic strain path length: Cp ¼ Cp ðT; kp Þ; rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ 2 p p Deij Deij : kp ¼ kp þ Dkp ; Dkp ¼ 3
ð1Þ ð2Þ
The components of the qij tensor are the functional of the plastic deformation process: qij ; qij ¼ qij þ D
ð3Þ
where Dqij is the change in qij at the elementary step of changing external influences, which is the sum of two types of backstress described by evolutionary equations of the ArmstrongFredericKadashevich type [7, 8]: Dqij ¼
2 X m¼1
Dqm ij ;
ð4Þ
Dq1ij ¼ G11 Depij G12 q1ij Dkp þ gpT q1ij hDT i;
ð5Þ
Dq2ij ¼ G21 Depij G22 q2ij Dkp þ gpT q2ij hDT i:
ð6Þ
hDT i ¼ DT at DT 0; hDT i ¼ 0 at DT\0;
ð7Þ
G11 ¼ G01 ð1 n1 ðT; kp ÞÞ; G12 ¼ G02 ð1 n2 ðT; epu ÞÞ:
ð8Þ
In ratios (3):
In the above ratios (5), (6) and (8): G01 ðTÞ; G02 ðTÞ; G21 ðTÞ; G22 ðTÞ; gpT ðTÞ – temperature – dependent T material functions; n1 ðT; kp Þ; n2 ðT; epu Þ – corrective material functions (epu – intensity of plastic deformations).
3 Results of the Experiment and Numerical Simulation Obtaining the material parameters of the model and checking its operability was carried out on the basis of the results of an experimental study of the deformation of a sample made of material of the 12Kh18N10T type with a cylindrical working part, under soft cyclic loading with control of the maximum and minimum values of forces in the cycle.
Model of LowCycle Deformation of Stainless Steel
303
In Fig. 1 and Fig. 2 shows graphs of the dependence of the displacement of the loop DlðnÞ ¼ lðnÞ lð50Þ (Fig. 1) and the magnitude of the total deformations of the loop in the hðnÞ cycle (Fig. 2) versus the number of cycles n. The results of numerical simulation are shown by solid lines in the ﬁgure, and the experimental results by dots.
Fig. 1. Loop offset depending on the number of loading cycles. Solid line  numerical modeling, points – experiment.
Fig. 2. The range of total deformations in the cycle depending on the number of loading cycles. Solid line  numerical modeling, points – experiment.
304
V. Gorokhov et al.
4 Conclusion A variant of the plasticity model is proposed that allows describing the kinetics of plastic deformation of materials under soft modes of lowcycle loading. A good agreement between the results of numerical simulation of plastic deformation of stainless steel and experimental data is demonstrated. Acknowledgements. This work was supported by the Ministry of Science and Higher Education of the Russian Federation (Agreement No. 075112019050).
References 1. Bondar, V.S., Abashev, D.R., Petrov, V.K.: Comparative analysis of variants of plasticity theories under cyclic loading. PNRPU Mech. Bull. 2, 23–44 (2017) 2. Kazakov, D.A., Kapustin, S.A., Korotkikh, Y.: Modeling of Deformation and Fracture Processes of Materials and Structures. Publishing house of Nizhny Novgorod state University, Nizhny Novgorod (1999) 3. Kapustin, S.A., Churilov, Y., Gorokhov, V.A.: Modeling of Nonlinear Deformation and Fracture of Structures Under MultiFactor Influences on the Basis of FEM. Publishing house of Nizhny Novgorod state University, Nizhny Novgorod (2015) 4. Bondar, V.S.: Inelasticity: Variants of the Theory. Fizmatlit, Moscow (2004) 5. Chaboche, J.L.: A review of some plasticity and viscoplasticity constitutive theories. Int. J. Plast. 24, 1642–1692 (2008) 6. Bondar’, V.S., Danshin, V.V., Makarov, D.A.: Mathematical modeling of deformation processes and damage accumulation under cyclic loading. PNRPU Mech. Bull. 2, 125–152 (2014) 7. Amstrong, P.J., Frederick, C.O.: A mathematical representation of the multiaxial Bauscinger effect. CEGB Report No. RD/B/N/731 (1966) 8. Kadashevich, Y.: On various tensorlinear relations in the theory of plasticity. Stud. Elast. Plast. 6, 39–45 (1967)
Creep and LongTerm Strength of Structures Ivan Volkov, Leonid Igumnov(&), and Svetlana Litvinchuk Research Institute for Mechanics, National Research Lobachevsky State University of Nizhny Novgorod, Gagarin Avenue 23, Nizhny Novgorod 603950, Russia [email protected] Abstract. The issue of evaluating strength and service life is discussed as applied to structures performance of which is characterized by multiparametric nonstationary thermalmechanical effects. The major degradation mechanisms of structural materials are considered. In the framework of mechanics of damaged media, a mathematical model describing the processes of viscoplastic deformation and damage accumulation due to creep is developed. The results of numerical simulation of the carrying capacity of a power plant reactor vessel in the event of a hypothetical emergency are presented. A number of characteristic features accompanying the deformation and failure processes connected with the time and place of macrocrack nucleation, the stressstrain state history and damage degree are given. By comparing numerical and experimental results we can conclude that the proposed constitutive relations of MDM adequately describe degradation of the initial strength properties of the material in terms of creep and longterm strength. Keywords: Longterm strength Mechanics of damaged media
Modeling Constitutive relations
1 Introduction To guarantee safe exploitation of critical engineering facilities and to prolong their standard service life, it is necessary to monitor damage growth rates in the most hazardous zones of structural elements and predict the development of such processes up to the limit state [1]. The currently available methods for evaluating service life of structural elements do not account for actual processes taking place in materials. Elastic analysis used in the standard approach does not enable us to consider actual characteristics of viscoplastic deformation, on which the service life of structural elements depends [1]. In this connection, it becomes vital to develop new methods for evaluating service life of structural elements based on equations of thermal viscoplasticity, equations of damage accumulation and failure criteria with their comprehensive substantiation by conducting the related fullscale and numerical experiments on laboratory specimens and numerically analyzing the deformation and failure processes of structural elements under service conditions [1–6]. The most effective tool for these purposes is mathematical modeling of degradation processes of structural materials, using modern models and methods of mechanics of © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 305–308, 2020. https://doi.org/10.1007/9783030478834_54
306
I. Volkov et al.
damaged media and fracture mechanics. Obtained by modeling, the values of damage degree of the material in accessible zones must be updated with the help of modern physical methods using periodic nondestructive control [7]. In the framework of MDM, a mathematical model has been developed that describes the processes of damage accumulation in structural materials due to degradation mechanisms, determined by growing creep strains under multiaxial stress and arbitrarily complex regimes of thermalmechanical loading.
2 Technique and Numerical Results The main assumptions of the introduced version of MDM are as follows: – the material is initially isotropic and free of damage (only the anisotropy caused by deformation processes is accounted for, whereas damageinduced anisotropy of material elastic properties is not taken into account); – the components of strain tensors and strain rates are the sum of momentary and time components; – the evolution of equipotential creep surfaces is described by the change of its radius and displacement of its center; – the volume change of the body element is elastic; – small deformation processes are considered; – the only structural parameter characterizing the material damage degree at the macrolevel is scalar parameter – damage degree; – the accumulated damage degree affecting the deformation process of the material is taken into account by introducing effective stresses. The relation between tensor components of stresses and elastic strains is established on the basis of the equations of thermal elasticity. To describe creep processes, a family of equipotential creep surfaces (surfaces with a constant creep strain rate) is introduced in the stress space, which has a common center and different radii deﬁned by a current stressed state [8–10]. Tensor components of creep strain rates are deﬁned on the basis of the associated flow law and gradientality principle. At the stage of the development of defects scattered over the volume, the damage degree effect on the material physical mechanical properties is observed. In the ﬁrst approximation, this effect can be taken into account based on the concept of a degrading continuum, by introducing effective stresses [2, 7, 11]. The rate of damage accumulation during creep is determined by the evolutionary equation accounting for the volumetric stressed state, the level of accumulated damage, accumulated relative damage energy, spent on the nucleation of defects and the rate of change of damage energy [3, 5, 6, 12]. The condition when damage degree reaches its critical value is taken as the criterion of termination of the growth phase of scattered macrodefects. The results of numerically analyzing the carrying capacity of a NPP reactor vessel made of 15X2NMFA steel in the event of a hypothetical emergency for the longterm strength mechanism are presented.
Creep and LongTerm Strength of Structures
307
The calculation scheme is represented by an axisymmetric structure of a reactor vessel, consisting of a cylindrical wall and an elliptic bottom. An emergency was simulated by applying internal hydrostatic pressure, varying from zero at a height of h = 1,5 m from the bottom lowest point and modeling the force effect of meltdown, internal pressure and temperature, varying in the limits of the considered part of the reactor vessel within 184° to 1510 °C. The reliability of the developed MDM model was numerically assessed prior to emergency simulation and material parameters of 15X2NMFA steel were determined within the temperature range of 20 °C to 1200 °C. The problem of evaluating longterm strength of a NPP reactor vessel under thermal dynamical loading was numerically solved in two steps. At the ﬁrst step, the stage when the pressure and temperature increase up to their maximal values during a short period was analyzed. At the second step, the pressure and temperature were kept constant. A number of calculations were carried out which differ in the value of internal pressure. The numerical analyses proved that, for all the versions of the computations from the viewpoint of longterm strength, the second stage (with the constant pressure and temperature) accompanied by the intensive development of creep strains and growth of defects is the most important. The maximum allowable pressure that doesn’t give rise to macrocrack nucleation has been deﬁned. The obtained numerical results on determining the maximum allowable pressure agrees with the results presented in [13].
3 Conclusion The numerical computations conducted and their comparison with the available experimental data make it possible to make the conclusion about the adequacy of the constitutive relations of MDM in modeling degradation of materials according to the longterm strength mechanism and the possibility of effectively using the developed constitutive relations of MDM for evaluating longterm strength of materials and structures. The mathematical model of MDM has been developed, that describes the processes of inelastic deformation and damage accumulation in structural materials (metals and their alloys) during the degradation of initial strength properties of materials according to the longterm strength mechanism. Using the numerical modeling method and comparing the obtained results with experimental data, the reliability of the constitutive relations of MDM for creep has been assessed. This made it possible to make the conclusions about the reliability of the developed modeling representations and the accuracy of the developed method for determining the material parameters included into these relations. The results of numerically analyzing the carrying capacity of a NPP reactor vessel in the event of a hypothetical accident are presented proving the validity of the carrying capacity failure of such facilities.
308
I. Volkov et al.
Acknowledgements. This work was supported by the Ministry of Science and Higher Education of the Russian Federation (Agreement No. 075112019050).
References 1. Mitenkov, F.M., Kaidalov, V.F., Korotkikh, Y., et al.: Methods of Justifying the Resource of Nuclear Power Plants. Mashinostroenie, Moscow (2007) 2. Volkov, I.A., Кorotkikh, Y.: The Equations of State of Viscoelastoplastic Media with Damage. Fizmatlit, Moscow (2008) 3. Lemaitre, J.: Damage modelling for prediction of plastic or creep fatigue failure in structures. In: Trans. 5th International Conference on SMRiT, Paper no. L5/1b, North Holland (1979) 4. Muracami, S., Imaizumi, T.: Mechanical description of creep damage and its experimental veriﬁcation. J. Mech. Theor. Appl. 1, 743–761 (1982) 5. Lemaitre, J.: Continual damage model used to calculate plastic damage. In: Proceedings of the American Society of Mechanical Engineers, vol. 107, pp. 90–98 (1985) 6. Chaboche, J.L.: Constitutive equation for cyclic plasticity and cyclic viscoplasticity. Int. J. Plast 5(3), 247–302 (1989) 7. Volkov, I.A., Igumnov, L.A.: Introduction to the Continuum Mechanics of the Damaged Environment. Fizmatlit, Moscow (2017) 8. Nikitenko, A.F.: Experimental substantiation of the hypothesis of existence of a creep surface under complex loading. Probl. Strength 8, 3–11 (1984). Report 1, 2 9. Volkov, I.A., Igumnov, L.A., Korotkih, Y.: Applied Theory of Viscoplasticity. Publishing House of Nizhny Novgorod State University, Nizhny Novgorod (2015) 10. Volkov, I.A., Igumnov, L.A., Kazakov, D.A., Shishulin, D.N., Smetanin, I.V.: Constitutive relations of nonstationary creep under a complex stress state. Probl. Strength Plast. 78(4), 436–451 (2016) 11. Volkov, I.A., Igumnov, L.A., Kazakov, D.A., Mironov, A.A., Tarasov, I.S., Shishulin, D.N., Smetanin, I.V.: The damage media model for describing service life of structural materials. Probl. Strength Plast. 79(3), 285–300 (2017) 12. Bodner, S.R., Lindholm, U.S.: An incremental criterion for timedependent failure of materials. J. Eng. Mater. Technol. ASME 100(2), 51–58 (1976) 13. Semishkin, V. P., et al.: Thermomechanical behavior of the VVR corps in a severe accident, In: Proceedings, 5th International Scientiﬁc and Technical Conference, Podolsk, Russia (2007)
Mathematical Modeling of Nonlinear Dynamic Deformation and Failure of MetalPlastic Shells of Revolution Leonid Igumnov(&) , Nikolai Abrosimov , Nadezhda Novoseltseva , and Vasilii Gorokhov Research Institute for Mechanics, National Research Lobachevsky State University of Nizhni Novgorod, 23, bldg. 6, Prospekt Gagarina (Gagarin Avenue), Nizhny Novgorod 603950, Russia [email protected]
Abstract. A technique for numerical analysis of nonlinear dynamic deformation and progressive failure of multilayered metalplastic shells of revolution is developed with account for their strainrate dependent strength characteristics. The geometric dependencies are formulated on the basis of quadratic version of the nonlinear theory of elasticity. The relationship between stress and strain tensors in a composite macrolayer is based of Hooke’s law for an orthotropic body combined with the theory of effective modules. The process of progressive layerbylayer failure is described in the framework of the degradation model of stiffness characteristics. The strain rate dependent stiffness and strength characteristics are accounted for. An energetically consistent system of equations of motion is constructed using the principle of possible displacements. A numerical method for solving the problem is based on an explicit variationaldifference scheme. The proposed technique was veriﬁed on the problem of unsteady deformation of a cylindrical shell subjected to pulse pressure. Keywords: Composite materials Shells of revolution Numerical methods Explosive loading
Strength Failure
Due to their effective energy absorption, increased crackresistance and nonsplintering character of possible failure, composite materials are widely used in constructing protective structures subjected to intense pulse loadings. In this connection, experimental and theoretical studies of strain rate effect of composite materials on their strength and stiffness characteristics appear to be highly topical since the material of structural elements subjected to pulse loading exhibits stressstrain behavior with a high degree of variability over time. In a number of experimental and theoretical works [1– 3], the strain rate dependence of elastic and strength characteristics of composite materials is noted. However, the determination of the parameters characterizing the properties of composite materials at high strain rates is associated with certain difﬁculties due to the necessity to measure the effect of dynamic pressure on a specimen as a function of time. The paper presents analytical results of the strain rate effect on dynamic behavior and progressive failure of shells of revolution made of hybrid metalplastic materials. © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 309–311, 2020. https://doi.org/10.1007/9783030478834_55
310
L. Igumnov et al.
We considered both homogeneous glassﬁberreinforced plastic shells formed by double alternating winding of spiral and annular layers with a thickness ratio of 1:1, and inhomogeneous ones fabricated by spiral cross winding of unidirectional glassﬁberreinforced plastic (according to the scheme of reinforced homogeneous shells) on a steel cylindrical mandrel made of mild steel. Since the shells of revolution made from composite materials are inhomogeneous, have low shear stiffness and, in some cases, are rather thick, thus, in order to describe their stressstrain state, it is necessary to use nonclassical shell theories [4]. Geometrical dependencies are constructed using the relations of the simplest quadratic version of the nonlinear elasticity theory [4]. The stressstrain tensors in a homogeneous composite macrolayer are related by Hooke’s law for an orthotropic body in combination with the theory of effective moduli [4]. The process of progressive layerbylayer damage of layered shells of revolution is described in the framework of the model of degradation of their stiffness characteristics [5]. And furthermore, the strainrate dependent strength characteristics of composite materials are taken into account. In particular, for unidirectional ﬁberglass, the material stiffness and strength characteristics can be described by the regression function [3] F ðe_ Þ ¼ a þ b_ec
ð1Þ
where F and e_ are strength characteristics and strain rate; a, b, c are experimentally determined material constants. The constitutive relations in the isotropic steel layer of the shell are formulated on the basis of the differential theory of plasticity with linear hardening [4]. In order to derive the equations of motion of an inhomogeneous shell of revolution, the principle of virtual displacements is used [6]. The equations derived are universal enough, because they allow one to describe nonlinear nonstationary deformation processes and to estimate the limiting deformability and dynamic strength of twolayered metalplastic shells of revolution, and their geometrical and structural parameters changing over a wide range. The numerical method for solving the problem formulated was based on the explicit variationaldifference scheme [4, 7]. The calculations were carried out on a “Lobachevsky” supercomputer. A numerical analysis of the effect of the strain rate on the dynamic strength of twolayered metalplastic cylindrical shells was considered on the problem of their deformation under the action of a pressure pulse caused by a blast in a center of a shell of an explosion charge (EC), which describes the pressure proﬁle in the incident shock wave by an empirical relation [8]. The physicomechanical characteristics of unidirectional glassﬁberreinforced plastic shells were determined from the results of quasistatic tests on ring and plane unidirectional specimens by standard techniques for identifying the corresponding stiffness and strength characteristics [9]. The strain rate dependence of the strength characteristics of glassﬁberreinforced plastics is described by function (1). The results obtained attest that the account of strain rate dependence of strength characteristics for all the reinforcement schemes considered lead to a qualitative difference in the character and size of failure zones of the binder and ﬁbers and to a
Mathematical Modeling of Nonlinear Dynamic Deformation
311
signiﬁcant increase in the loadcarrying capacity of the shells compared with the calculations of constant strength characteristics. Calculation models allowing one to analyze the processes of progressive failure of pulseloaded metalplastic cylindrical shells of revolution both with account of the strain rate dependence of their strength characteristics (dynamic model) and with constant characteristics (static model) have been proposed. A comparative analysis of calculation results with experimental data testiﬁes their better agreement in dynamic model. For various reinforcement schemes of composite macrolayer, the qualitative differences in character and size of failure zones calculated by both the methods were revealed. The results obtained can be used in the design and evaluation of the dynamic strength of loadcarrying elements. This work was supported by a grant from the Government of the Russian Federation (contract No. 14.Y26.31.0031).
References 1. Aseev, A.V., Makarov, G.E., Stepanenko, S.V.: An experimental study of the dynamic behavior of tubular samples of ﬁber composite materials at the limit of their bearing capacity. Prikl. Mekh. Tekhn. Phys. 3, 140–147 (1992) 2. Aseev, A.V., Gorshkov, N.N., Demeshkin, A.G., Makarov, G.E., Plastinin, A.V., Sil’vestrov, V.V., Stepanenko, S.: Experimental investigation of the deformability of ﬁberglass and organic plastics as a function of strain rate. Mech. Compos. Mater. 2, 188–195 (1992). (in Russian) 3. Shokrieh, M.M., Karamnejad, A.A.: Investigation of strain rate effects on the dynamic response of a glass/epoxy composite plate under blast loading by using the ﬁnitedifference method. Mech. Compos. Mater. 50(3), 295–310 (2014) 4. Abrosimov, N.A., Bazhenov, V.G.: Nonlinear Problems of Dynamics of Composite Structures, 400 p. N. Novgorod: Publishing House NNGU (2002). (in Russian) 5. Abrosimov, N.A., Novosel’tseva, N.A.: Numerical simulation of the levelbylevel destruction of cylindrical shells under explosive loading. Mech. Compos. Mater. 51(4), 579–594 (2015) 6. Vasidzu, K.: Variational Methods in the Theory of Elasticity and Plasticity. M., Mir, 512 p. (1987). (Russian translation) 7. Abrosimov, N.A., Elesin, A.V., Lazarev, L.N., Novosel’tseva, N.A.: Numerical analysis of the strength of glassﬁberreinforced plastic cylindrical shells of different structure at a pulse loading. Probl. Prochn. Plastychn. Mezhvuz. Sborn. 4(75), 288–295 (2013). N. Novgorod: Publishing House NNGU 8. Adishchev, V.V., Kornev, V.M., Talzi, L.A.: Estimates of maximum stresses in closed cylindrical vessels under axisymmetric explosive loading. Institute of Hydrodynamics SB AS Russia, Novosibirsk. Department in VINITI, № 658883 Dep. (1983) 9. Rusak, V.N., Fedorenko, A.G., Syrunin, M.A., et al.: Ultimate strain and strength of basaltﬁberreinforced shells under internal explosive loading. Prikl. Mekh. Tekhn. Phys. 43(1), 186–195 (2002)
Impact of Transient Pressure on a HalfSpace with Membrane Type Coating Elena Mikhailova1(&) , Grigory Fedotenkov1,2 and Dmitry Tarlakovskii1,2 1
2
,
Moscow Aviation Institute (National Research University), Moscow, Russia [email protected] Institute of Mechanics, Lomonosov Moscow State University, Moscow, Russia
Abstract. The unsteady influence of an external load on the base, which is an elastic halfspace with a membranetype coating is investigated. The load acting on the “halfspacemembrane” system is directed normally to the surface of the membrane and is a function that depends on the coordinate and time. A system of resolving equations is built. Its basic equation follows from the boundary condition, which corresponds to the equality of normal displacements on the surface of the halfspace to the deflections of the membrane. The normal displacements of halfspace and deflections of the membrane are connected with contact pressure and stresses by integral relations based on the principle of superposition. The basic equation is supplemented by initial conditions to a closed system of resolving equations. To solve the system of resolving equations, a numericalanalytical algorithm based on the method of quadratures is used. The results of calculations for the external load speciﬁed by various functions are presented. Keywords: Membrane analytical algorithm
Elastic halfspace Transient load Numerical
1 Problem Formulation The transient impact of normal pressure pðs; xÞ on the elastic halfspace with a membranetype coating is considered. We assume that the halfspace is occupied by a homogeneous isotropic linearly elastic medium with constants k; l and density. A rectangular Cartesian coordinate system Oxyz is introduced. In it, the coordinate plane z ¼ 0 coincides with the undeformable free surface of the halfspace, and the axis Oz is directed deep into the halfspace. Mathematical model of the problem contains [1–4]
© Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 312–315, 2020. https://doi.org/10.1007/9783030478834_56
Impact of Transient Pressure on a HalfSpace with Membrane Type Coating
313
– equations of motion of an elastic medium in displacement potentials u and w € ¼ Dw; D¼ € ¼ Du; g2 w u
@2 @2 þ 2 2 @x @z
ð1Þ
– relation between elastic displacement potentials and nonzero components of the displacement vectors u (along the axis Ox), w (along the axis Oz) u¼
@/ @w @/ @w ;w¼ þ ; @x @z @z @x
ð2Þ
– relation between the components of the displacement vectors and the stress tensor rij r11 r13
@u @w @u @w @u @w þj ; r22 ¼ j þ þ ; ¼ ; r33 ¼ j @x @z @x @z @x @z 1 j @u @w þ ¼ 2 @z @x
ð3Þ
– membrane motion equation (v – deflection, a – the speed of the waves of tensioncompression in the membrane) €vðs; xÞ ¼ a2
@2v þ p þ r330 ; r330 ¼ r33 jz¼0 @x2
ð4Þ
– initial conditions _ s¼0 ¼ 0 vjs¼0 ¼ v_ js¼0 ¼ wjs¼0 ¼ w_ s¼0 ¼ ujs¼0 ¼ uj
ð5Þ
– boundary adhesionfree conditions between the membrane and the surface of the halfspace r13 jz¼0 ¼ 0; v ¼ wjz¼0
ð6Þ
All variables and parameters are presented in a dimensionless form (the prime indicates the dimensional values):
314
s¼
E. Mikhailova et al.
c1 t v0 u0 w0 x0 z0 p0 L a0 k þ 2l ; v ¼ ; u ¼ ; w ¼ ; x ¼ ; z ¼ ; p ¼ 2 ; a ¼ ; c21 ¼ L qp L L L L L c1 c1 qm c22 ¼
l c2 u0 w0 r0 ij k ;j¼ ; g2 ¼ 12 ; u ¼ 2 ; w ¼ 2 ; rij ¼ qp k þ 2l L L k þ 2l c2 ð7Þ
Here t  dimensional time, qm ; qp  density of the membrane and the halfspace material, c1 ; c2  speed of the tensioncompression waves and shear waves in halfspace material, L  the characteristic linear parameter.
2 Method of Solution of Problem The resolving equation is based on the principle of superposition and follows from the boundary condition (6) Gm p ¼ r330 ðGp Gm Þ:
ð8Þ
Here Gm ; Gp  transient function for a for a membrane and halfspace, respectively [2–4]. The left side of Eq. (8) can be represented as follows: 1 Gm p ¼ 2
Zs
xZ þ st
dt 0
pdn
ð9Þ
xs þ t
This integral for a given function is calculated analytically. To solve Eq. (8), a numericalanalytical algorithm based on the quadrature method is used. For the hyperbolic type of equations of motion of the halfspace and the membrane an explicit integration scheme is used. The spacetime domain is covered with a grid with a constant step in time and coordinate. The grid functions correspond to the required functions. A discrete analogue is constructed for the equation. Moreover, the kernel of convolution has the form Gp ðx; sÞ ¼ ½Gr ðx; sÞ þ Gs ðx; sÞHðs j xjÞ:
ð10Þ
Here Gr ; Gs  the regular and singular components of the transient function for halfspace, Hðs; xÞ  Heaviside function. The integrals from the ﬁrst component are calculated using Gauss method, the integrals from the second are calculated using the weighting method and are understood in the meaning of a regularized value. Acknowledgment. This work was ﬁnancially supported by the Russian Foundation for Basic Research (RFBR), project 200801099 A.
Impact of Transient Pressure on a HalfSpace with Membrane Type Coating
315
References 1. Gorshkov, A.G., Medvedsky, A.L., Rabinsky, L.N., Tarlakovsky, D.V.: Waves in Continuum Media. Fizmatlit, Moscow (2004). (in Russian) 2. Gorshkov, A.G., Tarlakovsky, D.V.: Dynamic Contact Problems with Moving Boundaries. Fizmatlit, Moscow (1995). (in Russian) 3. Mikhailova, E.Yu., Fedotenkov, G.V.: Nonstationary axisymmetric problem of the impact of a spherical shell on an elastic halfspace (initial stage of interaction). Mech. Solids 46(2), 239– 247 (2011) 4. Mikhailova, E.Yu, Tarlakovskii, D.V., Fedotenkov, G.V.: The unsteady contact interaction problem of an absolutely rigid body and a membrane. In: Proceedings of the Second International Conference on Theoretical, Applied and Experimental Mechanics, ICTAEM 2019. Structural Integrity, vol. 8, pp. 289–293. Springer, Cham (2019)
Fracture Nanomechanics, Fatigue and Fracture at Small Scales (experiments and simulations) by Pasquale Gallo
Some Considerations on Stress Intensity Factor at Atomic Scale Pasquale Gallo(&) Aalto University, P.O. Box 14100, 00076 Espoo, Finland [email protected]
Abstract. This work reviews recent molecular statistics (MS) numerical experiments of cracked samples, and discusses the cracktip region stress ﬁeld of ideal brittle materials. Continuumbased linear elastic fracture mechanics, indeed, breaks down at extremely small scale, where the discrete nature of atoms is considered. Surprisingly, recent results have shown that the concept of stress intensity factor (SIF) is still valid. In this work, by means of MS simulations on singleedge cracked samples of ideal brittle silicon, it is shown that the stress intensity factor derived from the virial stress may be useful to describe the fracture at extremely small dimensions and to quantify the breakdown of continuumbased linear elastic fracture mechanics. However, it is still debated whether a continuumbased concept such as the “stress” should be applied to a system made of atoms. Keywords: Virial stress
Atom Crack Stress intensity factor
1 Introduction With recent developments in miniaturization of electronics devices such as nano and microelectromechanical systems (NEMS/MEMS), issues usually addressed at the macroscale, i.e. fatigue and fracture, have been brought into a completely new “scale” [1, 2]. At the same time, developments in nanotechnology give nowadays a completely new way at which the fatigue and fracture can be studied with a remarkable potential impact in several ﬁelds of engineering [3–10]. At such small scales, where discrete nature of atoms can’t be ignored, the continuum concepts largely used at the macroscale become questionable [11–13]. While methods based on energy have shown good potential to be extended from continuum to discrete system [12, 14–18], it is still debated whether the concept of “stress” should be applied to a system made of atoms [19, 20]. Stress is, indeed, a continuum concept, originated from the study of strength and failure of solid, and commonly deﬁned as the quantity that represents the internal forces on a deﬁned plane of a continuous material. Thus, questions arise on the deﬁnition of “atomic stress”. When investigating fracture at the atomic scale, the virial stress tensor is commonly employed to derive mechanical stresses acting on atoms [20–22]. Setting aside the debate on the validity of the virial stress as a representation of mechanical stress at atomic scale, in the present work the focus is on the applicability of classic continuum concepts in the presence of defects, such as the stress intensity factor (SIF). By © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 319–324, 2020. https://doi.org/10.1007/9783030478834_57
320
P. Gallo
reviewing recent molecular statistics (MS) analyses on singleedged cracked samples loaded under mode I [23], and representative of ideal brittle fracture, it is demonstrated that the virial stress shows the trend of inverse square root singularity and that computation of the SIF according to Irwin’s concept is possible. Furthermore, the breakdown of continuum linear elastic fracture mechanics, recently deﬁned by means of energy concepts [11–13], is here quantiﬁed by using merely the stress ﬁelds. It is concluded that the SIF from atomic stress may be useful in characterizing fracture at atomic scale, provided that the virial stress is accepted as representative of atomic mechanical stress. On the other hand, energy concepts should be anyway preferred for future developments, since they can provide a direct equivalence between continuum, discrete systems and among different scales.
2 Review of Recent Molecular Statistics Simulations on Cracked Samples Recently, fracture tests by means of MS simulations were conducted by using opensource code LAMMPS [24]. While details can be found in [23], important aspects are presented hereafter. The modiﬁed StillingerWeber (SW) interatomic potential [25] was employed. The SW potential is representative of ideal brittle fracture, and often used when studying single crystal silicon. The focus was on singleedge cracked sample, loaded under mode I. Figure 1 depicts an example of the samples and orientation.
Fig. 1. Cracked samples employed in the molecular statistics analyses and orientation [23]. The thickness of the simulation cell is indicated as t.
Several specimens where considered, scaling their size until few nanometers: the width of the sample W varied from 198 nm to 9.8 nm, while the crack length a was kept equal to W/3. The mechanical properties were given by the following material constants: C11 = 201 GPa, C12 = 51.4 GPa and C44 = 90.5 GPa. Along the direction [111], an ideal material strength rIS of 35 GPa at critical strain eC = 0.3 was obtained. A stepwise increment of strain e is applied at the upper and lower layers of atoms according to Fig. 1, and the strain is increased until ﬁnal fracture. At fracture, the critical displacement dC (maximum displacement before failure) is obtained. The mechanical stress is obtained dividing the virial stress (stress volume quantity) by
Some Considerations on Stress Intensity Factor at Atomic Scale
321
the peratom volume at eC = 0.3, i.e. 24.44 Å3. This value is, indeed, a more reliable estimation of the atomic volume in regions that are highly deformed, such as close to the crack tip at failure conditions. Analyses were conducted at 0 K and fully included the lattice trapping.
3 Results and Discussion The crack tip stress ﬁelds of some selected considered geometries are presented in Fig. 2a for the sake of clarity. The values of the atoms at the crack tip are plotted at r = 0.1 Å for convenience, since as well known the loglog scale does not allow the value of 0. The depicted stress is the mechanical atomic stress, i.e. virial stress divided by the peratom volume as explained in the previous section.
Fig. 2. (a) Near cracktip atomic stress distribution for selected geometries; atomistic stress is derived from virial stress/peratom volume. The stress values of the atoms at the crack tip are plotted for r = 0.1 Å rather than 0 Å in order to summarize in a single loglog scale graph both stress distribution and cracktip values. (b) Critical stress intensity factors versus the variation of the specimen width W.
The ﬁgure shows two very important results: • The MS analyses do not predict the inﬁnite stress at the cracktip but rather a ﬁnite value, i.e. the ideal material strength rIS, regardless of the specimen size. This indicates that the fracture, in the case of ideal brittle materials, is ultimately governed by atoms at crack tip. • Even if the stress singularity is missing, near the crack tip region the stress still varies with 1/r0.5 as expected from continuum LEFM. Figure 2a depicts only selected geometries for the sake of clarity, but same results are obtained for all the considered samples. The results allow the quantiﬁcation of the SIF at failure KIf (i.e. at critical displacement dC), according to the classic Irwin’s deﬁnition [26, 27]:
322
P. Gallo
pﬃﬃﬃﬃﬃﬃﬃﬃ KIf ¼ rV 2pr ;
ð1Þ
where rV is the atomistic mechanical stress, perpendicular to the crack plane; r is the distance from the cracktip along the crack plane. The results are presented in Fig. 2b and compared with other experimental and numerical works by other authors [16, 17, 28]. KIf 0.97 MPam0.5 is constant for all the geometries, and it agrees well with the fracture toughness of single crystal silicon, including bulk samples [29].
Fig. 3. Normalized SIF at failure versus the ratio of singular stress ﬁeld length KK and fracture process zone length RFPZ. Numerical values are reported in [23].
Finally, the comparison with continuumbased linear elastic solutions conducted in [23] is summarized in Fig. 3. The stress intensity factors at failure are normalized vs the KIf of the largest sample W = 198.41 nm, and plotted versus the length of the singular stress ﬁeld KK normalized by the fracture process zone RFPZ. KK is the distance from the cracktip at which the stress deviates more than 5% from the expected 1/r0.5, while the RFPZ is a constant value taken from the literature [12, 13]. When continuum and atomistic simulations are overlapped, the continuumbased formulation breaks down when the ratio between KK and RFPZ is approximately 45, in agreement with [12, 13]. The atomistic simulations, instead, show a clearly scaleindependence, conﬁrming that ideal brittle fracture is ultimately governed by atomic bond breaking [7, 17]. Concluding, the concept of SIF is still surprisingly valid if the atoms are modeled, and static crack and ideal brittle material containing no other defects are considered. This result also agrees well with conclusions made by other authors [30]. Provided that the virial stress is affectively accepted as representative of atomic stress, crack tip region stress ﬁeld of molecular system may be described by continuumbased SIF concept.
Some Considerations on Stress Intensity Factor at Atomic Scale
323
References 1. Kitamura, T., Sumigawa, T., Shimada, T., Van Lich, L.: Challenge toward nanometer scale fracture mechanics. Eng. Fract. Mech. 187, 33–44 (2018) 2. Kitamura, T., Sumigawa, T., Hirakata, H., Shimada, T.: Fracture Nanomechanics, 2nd edn. Pan Stanford Publishing, Singapore (2016) 3. Xu, K., Li, B., Li, S., Luo, M., Gao, X., Jiang, C., Song, L.: In situ observation for the fatigue crack growth mechanism of 316L stainless steel fabricated by laser engineered net shaping. Int. J. Fatigue 130, 105272 (2019). https://doi.org/10.1016/j.ijfatigue.2019.105272 4. Andric, P., Curtin, W.A.: Atomistic modeling of fracture. Model. Simul. Mater. Sci. Eng. 27 (1), 013001 (2018). https://doi.org/10.1088/1361651x/aae40c 5. Ghayesh, M.H., Farajpour, A.: A review on the mechanics of functionally graded nanoscale and microscale structures. Int. J. Eng. Sci. 137, 8–36 (2019). https://doi.org/10.1016/j. ijengsci.2018.12.001 6. Taloni, A., Vodret, M., Costantini, G., Zapperi, S.: Size effects on the fracture of microscale and nanoscale materials. Nat. Rev. Mater. 3, 211–224 (2018). https://doi.org/10.1038/ s4157801800294 7. Shimada, T., Kitamura, T.: Fracture mechanics at atomic scales. In: Altenbach, H., Matsuda, T., Okumura, D. (eds.) Advanced Structured Materials, pp. 379–396. Springer International Publishing, Cham (2015) 8. Kumar, S., Curtin, W.A.: Crack interaction with microstructure. Mater. Today 10, 34–44 (2007). https://doi.org/10.1016/S13697021(07)702079 9. Wang, Y.Q., Fritz, R., Kiener, D., Zhang, J.Y., Liu, G., Kolednik, O., Pippan, R., Sun, J.: Fracture behavior and deformation mechanisms in nanolaminated crystalline/amorphous microcantilevers. Acta Mater. 180, 73–83 (2019). https://doi.org/10.1016/j.actamat.2019. 09.002 10. Pippan, R., Wurster, S., Kiener, D.: Fracture mechanics of micro samples: fundamental considerations. Mater. Des. 159, 252–267 (2019). https://doi.org/10.1016/j.matdes.2018.09. 004 11. Gallo, P., Sumigawa, T., Shimada, T., Yan, Y., Kitamura, T.: Investigation into the breakdown of continuum fracture mechanics at the nanoscale: synthesis of recent results on silicon. In: Gdoutos, E.E. (ed.) Proceedings of the First International Conference on Theoretical, Applied and Experimental Mechanics, pp. 205–210. Springer International Publishing, Cham (2019) 12. Gallo, P., Hagiwara, Y., Shimada, T., Kitamura, T.: Strain energy density approach for brittle fracture from nano to macroscale and breakdown of continuum theory. Theor. Appl. Fract. Mech. 103, 102300 (2019). https://doi.org/10.1016/j.tafmec.2019.102300 13. Shimada, T., Ouchi, K., Chihara, Y., Kitamura, T.: Breakdown of continuum fracture mechanics at the nanoscale. Sci. Rep. 5, 8596 (2015). https://doi.org/10.1038/srep08596 14. Gallo, P., Sumigawa, T., Kitamura, T., Berto, F.: Static assessment of nanoscale notched silicon beams using the averaged strain energy density method. Theor. Appl. Fract. Mech. 95, 261–269 (2018). https://doi.org/10.1016/j.tafmec.2018.03.007 15. Gallo, P., Sumigawa, T., Kitamura, T.: Experimental characterization at nanoscale of single crystal silicon fracture toughness. Frat ed Integrità Strutt 13, 408–415 (2019). https://doi.org/ 10.3221/IGFESIS.47.31 16. Gallo, P., Yan, Y., Sumigawa, T., Kitamura, T.: Fracture behavior of nanoscale notched silicon beams investigated by the theory of critical distances. Adv. Theory Simul. 1, 1700006 (2018). https://doi.org/10.1002/adts.201700006
324
P. Gallo
17. Sumigawa, T., Shimada, T., Tanaka, S., Unno, H., Ozaki, N., Ashida, S., Kitamura, T.: Grifﬁth criterion for nanoscale stress singularity in brittle silicon. ACS Nano 11, 6271–6276 (2017). https://doi.org/10.1021/acsnano.7b02493 18. Huang, K., Shimada, T., Ozaki, N., Hagiwara, Y., Sumigawa, T., Guo, L., Kitamura, T.: A uniﬁed and universal Grifﬁthbased criterion for brittle fracture. Int. J. Solids Struct. 128, 67– 72 (2017). https://doi.org/10.1016/j.ijsolstr.2017.08.018 19. Zhou, M.: A new look at the atomic level virial stress: on continuummolecular system equivalence. Proc. R. Soc. Math. Phys. Eng. Sci. 459, 2347–2392 (2003). https://doi.org/10. 1098/rspa.2003.1127 20. Cheng, S.H., Sun, C.T.: Convergence of local atomistic stress based on periodic lattice. Int. J. Solids Struct. 51, 2027–2035 (2014). https://doi.org/10.1016/j.ijsolstr.2014.02.023 21. Subramaniyan, A.K., Sun, C.T.: Continuum interpretation of virial stress in molecular simulations. Int. J. Solids Struct. 45, 4340–4346 (2008). https://doi.org/10.1016/j.ijsolstr. 2008.03.016 22. Zimmerman, J.A., Webblll, E.B., Hoyt, J.J., Jones, R.E., Klein, P.A., Bammann, D.J.: Calculation of stress in atomistic simulation. Modell. Simul. Mater. Sci. Eng. 12(4), S319– S332 (2004). https://doi.org/10.1088/09650393/12/4/S03 23. Gallo, P.: On the cracktip region stress ﬁeld in molecular systems: the case of ideal brittle fracture. Adv. Theory Simul. 2, 1900146 (2019). https://doi.org/10.1002/adts.201900146 24. Plimpton, S.: Fast parallel algorithms for shortrange molecular dynamics. J. Comput. Phys. 117, 1–19 (1995). https://doi.org/10.1006/jcph.1995.1039 25. Sillinger, F.H., Weber, T.A.: Computer simulation of local order in condensed phases of silicon. Phys. Rev. B 31, 5262–5271 (1985). https://doi.org/10.1103/PhysRevB.31.5262 26. Irwin, G.R.: Linear fracure mechanics, fracture transition, and fracture control. Eng. Fract. Mech. 1(2), 241–257 (1968) 27. Irwin, G.R.: Analysis of stresses and strains near the end of a crack traversing a plate. J. Appl. Mech. 24, 361–364 (1957) 28. Sumigawa, T., Ashida, S., Tanaka, S., Sanada, K., Kitamura, T.: Fracture toughness of silicon in nanometerscale singular stress ﬁeld. Eng. Fract. Mech. 150, 161–167 (2015). https://doi.org/10.1016/j.engfracmech.2015.05.054 29. Stan, G., Krylyuk, S., Davydov, A.V., Cook, R.F.: Bending manipulation and measurements of fracture strength of silicon and oxidized silicon nanowires by atomic force microscopy. J. Mater. Res. 27, 562–570 (2011). https://doi.org/10.1557/jmr.2011.354 30. Le, M.Q., Batra, R.C.: ModeI stress intensity factor in single layer graphene sheets. Comput. Mater. Sci. 118, 251–258 (2016). https://doi.org/10.1016/j.commatsci.2016.03.027
Initial Intergranular Cracking of NiBase Superalloys Due to the Degradation of the Crystallinity of Grain Boundaries Under CreepFatigue Loading Wataru Suzuki1, Yifan Luo1, Kenta Ishihara1, Kens Suzuki2, and Hideo Miura2(&) 1
2
Department of Finemechanics, Graduate School of Engineering, Tohoku University, Sendai, Miyagi 9808579, Japan Fracture and Reliability Research Institute, Graduate School of Engineering, Tohoku University, Sendai, Miyagi 9808579, Japan [email protected]
Abstract. The mechanism of the drastic decrease in the lifetime of Nibase superalloy, Alloy 617 under creepfatigue loading at elevated temperatures was clariﬁed by using EBSD (Electron BackScatter Diffraction) analysis. The degradation process was monitored by using an intermittent creepfatigue test and EBSD analysis. The change of the crystallinity of grains and grain boundaries was quantitatively analyzed by using the image quality (IQ) value obtained from the EBSD analysis. The IQ value indicated the density of defects such as vacancies, dislocations, local strain, and so on. The decrease in the IQ value corresponded to the decrease in the crystallinity of the observed area. The accumulation of ﬁne voids was found to be accelerated under the creepfatigue loading, and it caused the drastic decrease of not only the IQ value, but also the strength of the grain boundaries. Intergranular cracking started to occur when the crystallinity of grain boundaries decreased to the critical value due to the degradation of the crystallinity caused by the local accumulation of dislocations and voids around the grain boundaries. Keywords: Creepfatigue damage Nibase superalloy cracking. EBSD analysis EBSD analysis
Intergranular
1 Introduction Nibase superalloys are strong candidate for the various components used in advanced thermal and chemical plants and jet engines, such as pressure vessels, pipes, turbine blades, and so on, because of their high strength at elevated temperatures higher than 700 °C. In order to minimize the emission of CO2 during their operations, it is very important to improve their thermal efﬁciency by elevating their operating temperatures. In the case of thermal power plants, the frequent random change of output is required to compensate the unexpected changes of the outputs of renewable energies, comparing with the constant output of the conventional plants. Thus, the creepfatigue loads are applied to the components used in the advanced plants at the elevated temperatures. © Springer Nature Switzerland AG 2020 E. Gdoutos and M. KonstaGdoutos (Eds.): ICTAEM 2020, STIN 16, pp. 325–331, 2020. https://doi.org/10.1007/9783030478834_58
326
W. Suzuki et al.
It was reported that the effective lifetime of Nibase superalloys dropped down drastically under the creepfatigue loading at elevated temperatures [1–3]. The main reason for the drastic decrease was attributed to the change of the crack propagation path from conventional transgranular to intergranular. The mechanism of the change, however, is not clariﬁed yet. Therefore, in this study, the degradation process of the strength of grain boundaries in Alloy 617, one of the representatives of Nibase superalloy, was investigated in detail by using an intermittent creepfatigue test and EBSD analysis. The degradation of the local crystallinity of grains and grain boundaries was continuously monitored in the same area.
2 Experimental Methods Table 1 shows the chemical composition of Alloy 617 used in this study. This alloy consists of two phases, c phase (Ni) and c’ phase (Ni3Al). The alloy was heattreated by solution annealing at 1150 °C for 1.12 h after hot rolling. After that a small specimen was cut into the dumbbell shape as shown in Fig. 1. This size was good for the continuous observation of the change of its crystallinity by EBSD in SEM. The intermittent creepfatigue test was applied to the specimen at 800 °C in an inert gas of Ar. The test conditions were as follows: The maximum applied stress was 100 MPa, and the stress ration was 0.03. The loading rate was 100 N/s and the holding time at the maximum stress was 10 min. The test was frequently stopped at certain plastic strains because all the fractured specimen showed the almost the same normalizedtime dependency of plastic strain. Table 1. Chemical composition of Alloy 617 (wt%).
C 0.06 Ti 0.4
S